This Page Intentionally Left Blank
D. Demus, J. Goodby, G. W. Gray, H.W. Spiess, V. Vill
Physical Properties of Liquid Crystals
@3WILEYWCH
Related Reading from WILEYVCH D. Demus, J. Goodby, G.W. Gray, H.W. Spiess, V Vill (Eds.) Handbook of Liquid Crystals ISBN 352729502X (4Volume Set)
J. L. Serrano (Ed.) Metallomesogens ISBN 3527292969
D. Demus, J. Goodby, G.W. Gray, H.W. Spiess, V Vill
Physical Properties of Liquid Crystals
6BWILEYVCH Weinheim  New York Chichester Brisbane  Singapore  Toronto
Prof. Dietrich Demus Veilchenweg 23 06 1 18 Halle Germany Prof. John W. Goodby School of Chemistry University of Hull Hull, HU6 7RX U.K. Prof. George W. Gray Merck Ltd. Liquid Crystals Merck House Poole BH IS 1 TD U.K.
Prof. HansWolfgang Spiess MaxPlanckInstitut fur Polymerforschung Ackermannweg 10 5 5 128 Mainz Germany Dr. Volkmar Vill Institut fur Organische Chemie Universitat Hamburg MartinLutherKingPlatz 6 20 146 Hamburg Germany
This book was carefully produced. Nevertheless, authors, editors and publisher do not warrant the information contained therein to be free of errors. Readers are advised to keep in mind that statements, data, illustrations, procedural details or other items may inadvertently be inaccurate.
Library of Congress Card No. applied for. A catalogue record for this book is available from the British Library.
Deutsche Bibliothek CataloguinginPublication Data:
Physical properties of liquid crystals I ed. by Dietrich Deinus ...  1 Aufl.  Weinheim ; New York ; Chichester ; Brisbane ; Singapore ; Toronto : WileyVCH, 1999 ISBN 3527297472
0 WILEYVCH Vcrlag GmbH. D60469 Weinheim (Federal Republic of Germany), 1999 Printed on acidfree and chlorinefree paper. All rights reserved (including those of translation in other languages). No part of this book may be reproduced i n any form  by photoprinting, microfilm, or any other means  nor transmitted or translated into machine language without written permission from the publishers. Registered names, trademarks, etc. used in this book, even when not specifically marked as such, are not to be considered unprotected by law. Composition, Printing and Bookbinding: Fa. Konrad Triltsch Druck und Verlagsanstalt GmbH, D97070 Wiirzburg. Printed in the Federal Republic of Germany.
The Editors
’
D.Dernus studied chemistry at the MartinLutherUniversity, Halle, Germany, where he was also awarded his Ph. D. In 1981 he became Professor, and in 1991 Deputy ViceChancellor of Halle University. From 19921994 he worked as a Special Technical Advisor for the Chisso Petrochemical Corporation in Japan. Throughout the period 19841 99 I he was a member of the International Planning and Steering Commitee of the International Liquid Crystal Conferences, and was a nonexecutive director of the International Liquid Crystal Society. Since 1994 he is active as a Scientific Consultant in Halle. He has published over 3 10 scientific papers and 7 books and he holds 170 patents.
J. W. Goodby studied for his Ph. D. in chemistry under the guidance of G. W. Gray at the University of Hull, UK. After his postdoctoral research he became supervisor of the Liquid Crystal Device Materials Research Group at AT&T Bell Laboratories. In 1988 he returned to the UK to become the ThornEMI/STC Reader in Industrial Chemistry and in 1990 he was appointed Professor of Organic Chemistry and Head of the Liquid Crystal Group at the University of Hull. In 1996 he was the first winner of the G. W. Gray Medal of the British Liquid Crystal Society.
G. W. Gray studied chemistry at the University of Glasgow, UK, and received his Ph. D. from the University of London before moving to the University of Hull. His contributions have been recognised by many awards and distinctions, including the Leverhulme Gold Medal of the Royal Society (l987), Commander of the Most Excellent Order of the British Empire (1991), and Gold Medallist and Kyoto Prize Laureate in Advanced Technology (1995). His work on structure/property relationships has had far reaching influences on the understanding of liquid crystals and on their commercial applications in the field of electrooptical displays. In 1990 he became Research Coordinator for Merck (UK) Ltd, the company which, as BDH Ltd, did so much to commercialise and market the electrooptic materials which he invented at Hull University. He is now active as a Consultant, as Editor of the journal “Liquid Crystals” and as author/editor for a number of texts on Liquid Crystals.
VI
The Editors
H. W. Spiess studied chemistry at the University of Frankfurt/Main, Germany, and obtained his Ph. D. in physical chemistry for work on transition metal complexes in the group of H. Hartmann. After professorships at the University of Mainz, Munster and Bayreuth he was appointed Director of the newly founded MaxPlanckInstitute for Polymer Research in Mainz in 1984. His main research focuses on the structure and dynamics of synthetic polymers and liquid crystalline polymers by advanced NMR and other spectroscopic techniques.
V. Vill studied chemistry and physics at the University of Munster, Germany, and acquired his Ph. D. in carbohydrate chemistry in the group of J. Thiem in 1990. He is currently appointed at the University of Hamburg, where he focuses his research on the synthesis of chiral liquid crystals from carbohydrates and the phase behavior of glycolipids. He is the founder of the LiqCryst database and author of the LandoltBornstein series Liquid crystal.^.
List of Contributors
Barois, P. (IV:6.1) Centre de Recherche P. Pascal Ave. A. Schweitzer 33600 Pessac Cedex France
Goodby, J. W. (11) School of Chemistry University of Hull Hull, HU6 7RX U.K.
Blinov, L. M. (IV:9) Institute of Crystallography Russian Academy of Sciences Leninsky prosp. 59 117333 Moscow Russia
Gray, G. W. (I and 11) Merck Ltd. Liquid Crystals Merck House Poole BH15 1TD U.K.
Bouligand, Y. (IV:7) Histophysique et Cytophysique Ecole Pratique des Hautes Etudes 10, rue A. Bocquel 49 100 Angers France
JkrGme, B. (IV:10) FOMInstitute for Atomic and Molecular Physics Kruislaan 407 1098 SJ Amsterdam The Netherlands
Cladis, P. E. (IV:6.3 and IV:6.4) Advanced Liquid Crystal Technologies, Inc. P.O. Box 1314 Summit, NJ 07902 USA
Kapustina, 0. (IV: 1 1) Shvernik St. 4 117036 Moscow Russia
Dunmur, D. A.; Toriyama, K. (IV: 15) Department of Chemistry University of Southampton Southampton SO 17 1 BJ U.K.
Leslie, F. M. (111: I ) University of Strathclyde Dept. of Mathematics Livingstone Tower 26 Richmond Street Glasgow GI 1XH U.K.
VIII
List of Contributors
Noack, F.' (IV:13) IV. Physikalisches Institut Universitat Stuttgart Pfaffenwaldring 57 70550 Stuttgart Germany Osipov, M. (III:2) Institute of Crystallography Academy of Science of Russia Leninski pr. 59 Moscow 117333 Russia PalffyMuhoray, P. (IV: 12) Kent State University Liquid Crystal Institute Kent, OH 44242 USA Pollmann, P. (IV:6.2.4) Universitat GH Paderborn FB 13, Chemie u. Chemietechnik FG Physikal. Chemie 33095 Paderborn Germany Schneider, F.; Kneppe, H. (IV:8) Universitat GH Siegen Physikal. Chemie 57068 Siegen Germany
Thoen, J. (IV:6.2.1) Katholieke Universiteit Leuven Departement Natuurkunde Laboratorium voor Akoestiek en Thermische Fysica Celstijnenlaan 200 D 3001 Leuven (Heverlee) Belgium Wedler, W. (IV:6.2.2 and IV:6.2.3) Tektronix, Inc.; CPID MIS 63424 26600 SW Parkway Wilsonville, OR 970701000 USA Wilson, M. R. (III:3) Department of Chemistry University of Durham South Road Durham, DHI 3LE U.K.
Contents
Chapter I: Introduction and Historical Development . . . . . . . . . . . . . . . . 1 George W Gray 1
Introduction. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
1
2
The Early Years up to About 1925 . . . . . . . . . . . . . . . . . . . . . . .
2
3
The Second Phase from 1925 to 1959 . . . . . . . . . . . . . . . . . . . . .
5
4 4.1 4.2 4.3 4.4
The Third Phase from 1960 to the Present Time . . . . . . . . . . . . . . . . 8 Lyotropic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 Polymer Dispersed Liquid Crystals (PDLCs) and Anchoring . . . . . . . . . 12 Materials and New Phases . . . . . . . . . . . . . . . . . . . . . . . . . . . 13
5
Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
14
6
References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
14
Chapter 11: Guide to the Nomenclature and Classification of Liquid Crystals . . . 17 John W Goodby and George W Gruy 1
Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
17
2
General Definitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
18
3
Structural Features . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
19
4
Polymeric Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . .
20
5 5. I 5.1.1 5.2 5.2.1 5.2.2 5.2.3 5.2.4 5.2.5
Notation of Thermotropic Liquid Crystalline Properties . . . . . . . . . . . . 20 Description of the Solid State . . . . . . . . . . . . . . . . . . . . . . . . . . 20 Description of Soft Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . 20 Description of the Liquid Crystalline Phases . . . . . . . . . . . . . . . . . . 21 21 Nematic and Chiral Nematic Phases . . . . . . . . . . . . . . . . . . . . . . Smectic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21 Chiral Smectic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . 21 Columnar Phases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 22 Plastic Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23
X
Contents
23 23 23 23
6
Condis Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Cubic . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Reentrants . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Description of the Clearing Parameters . . . . . . . . . . . . . . . . . . . . . Stereochemistry . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
7
References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
23
5.2.6 5.2.7 5.2.8 5.3
23
Chapter 111: Theory of the Liquid Crystalline State . . . . . . . . . . . . . . . . . 25 1 1.1 1.2 1.2.1 1.2.2 1.2.3 1.2.4 1.2.5 1.2.6 1.3 1.3.1 1.3.2 1.4 1.4.1 1.4.2 1.4.3 1.4.4 1.5 2 2.1 2.2 2.2.1 2.2.2 2.2.3 2.3 2.3.1 2.3.2 2.3.3 2.4 2.4.1 2.4.2
Continuum Theory €or Liquid Crystals . . . . . . . . . . . . . . . . . . . . . Frank M . Leslie Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Equilibrium Theory for Nematics . . . . . . . . . . . . . . . . . . . . . . . . The FrankOseen Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . A Virtual Work Formulation . . . . . . . . . . . . . . . . . . . . . . . . . . Body Forces and Moments . . . . . . . . . . . . . . . . . . . . . . . . . . . The Equilibrium Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . Boundary Conditions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Proposed Extensions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Equilibrium Theory for Smectic Liquid Crystals . . . . . . . . . . . . . . . An Energy Function for SmC Liquid Crystals . . . . . . . . . . . . . . . . Equilibrium Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Dynamic Theory for Nematics . . . . . . . . . . . . . . . . . . . . . . . . . Balance Laws . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A Rate of Work Hypothesis . . . . . . . . . . . . . . . . . . . . . . . . . . . The Viscous Stress . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Equations of Motion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Molecular Theories of Liquid Crystals . . . . . . . . . . . . . . . . . . . . . M . A . Osipov Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Microscopic Definition of the Order Parameters for Nematic and Smectic Phases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Uniaxial Nematic Phase . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Biaxial Nematic Phase . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Smectic A and C Phases . . . . . . . . . . . . . . . . . . . . . . . . . . . . Anisotropic Intermolecular Interactions in Liquid Crystals . . . . . . . . . Hardcore Repulsion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Electrostatic and Dispersion Interactions . . . . . . . . . . . . . . . . . . . . Model Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Molecular Theory of the Nematic Phase . . . . . . . . . . . . . . . . . . . . Meanfield Approximation and the MaierSaupe Theory . . . . . . . . . . Shortrange Orientational Correlations . . . . . . . . . . . . . . . . . . . . .
25 25 26 26 27 28 29 30 31 . 32 . 32 33 35 35 36 36 37 38 40 40 41 41 42 43 . 44 44 44 46 47 . 47 51
Contents
XI
2.4.3 2.4.4 2.4.5 2.4.6 2.5 2.5.1 2.5.2 2.5.3 2.5.4 2.6 2.7
Excluded Volume Effects and the Onsager Theory . . . . . . . . . . . . . . Packing Effects in Thermotropic Nematics . . . . . . . . . . . . . . . . . . The Role of Molecular Biaxiality . . . . . . . . . . . . . . . . . . . . . . . Density Functional Approach to the Statistical Theory of Liquid Crystals . . Molecular Models for Simple Smectic Phases . . . . . . . . . . . . . . . . Meanfield Theory of the NematicSmectic A Transition . . . . . . . . . . Phase Diagram of a Hardrod Fluid . . . . . . . . . . . . . . . . . . . . . . The Role of Intermolecular Attraction . . . . . . . . . . . . . . . . . . . . Smectic ASmectic C Transition . . . . . . . . . . . . . . . . . . . . . . . Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
3
Molecular Modelling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 72 Mark R. Wilson Techniques of Molecular Modelling . . . . . . . . . . . . . . . . . . . . . . 72 Molecular Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 72 Molecular Dynamics and Monte Carlo Simulation . . . . . . . . . . . . . . 74 Quantum Mechanical Techniques . . . . . . . . . . . . . . . . . . . . . . . 78 Applications of Molecular Modelling . . . . . . . . . . . . . . . . . . . . . 78 Determination of Molecular Structure . . . . . . . . . . . . . . . . . . . . . 78 Determination of Molecular Properties . . . . . . . . . . . . . . . . . . . . 80 Determination of Intermolecular Potentials . . . . . . . . . . . . . . . . . . 81 LargeScale Simulation of Liquid Crystals . . . . . . . . . . . . . . . . . . 82 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 85
3.1 3.1.1 3.1.2 3.1.3 3.2 3.2.1 3.2.2 3.2.3 3.2.4 3.3
Chapter I V Physical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1.1 1.2 2 2.1 2.2 2.2.1 2.2.2 2.2.3 2.3 2.4 2.5 2.6 2.7
52 54 56 58 60 60 63 65 65 69 69
87
Tensor Properties of Anisotropic Materials . . . . . . . . . . . . . . . . . . 87 David Dunmur and Kazuhisa Toriyama Macroscopic and Microscopic Properties . . . . . . . . . . . . . . . . . . . 92 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 100 Magnetic Properties of Liquid Crystals . . . . . . . . . . . . . . . . . . . . David Dunmur and Kazuhisa Toriyama Magnetic Anisotropy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Types of Magnetic Polarization . . . . . . . . . . . . . . . . . . . . . . . . Diamagnetism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Paramagnetism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Ferromagnetism . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Diamagnetic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . Paramagnetic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . Ferromagnetic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . Applications of Magnetic Properties . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
102 102 104 104 104 106 106 108 110 110 112
XI1 3 3.1 3.2 3.3 3.4 3.5 3.6
Contents
Optical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 113 David Dunmur and Kazuhisa Toriyama Symmetry of Liquid Crystal Phases and the Optical Indicatrix . . . . . . . . 115 115 Molecular Theory of Refractive Indices . . . . . . . . . . . . . . . . . . . . Optical Absorption and Linear Dichroism . . . . . . . . . . . . . . . . . . . 119 Refractive Indices and Liquid Crystal Phase Structure . . . . . . . . . . . . 121 Optics of Helicoidal Liquid Crystal Structures . . . . . . . . . . . . . . . . 124 127 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Dielectric Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 129 David Dunmur and Kazuhisa Toriyama 129 Dielectric Response of Isotropic Fluids . . . . . . . . . . . . . . . . . . . . 4.1 Dielectric Properties of Anisotropic Fluids . . . . . . . . . . . . . . . . . . 133 4.2 4.2.1 The Electric Permittivity at Low Frequencies: The Static Case . . . . . . . . 133 4.2. I .1 Nematic Phase . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 133 138 4.2.1.2 The Smectic Phases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.2 Frequency Dependence of the Electric Permittivity: Dielectric Relaxation . . 143 4.3 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 149
4
Elastic Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 151 David Dunmur and Kazuhisa Toriyama Introduction to Torsional Elasticity . . . . . . . . . . . . . . . . . . . . . . 151 5.I 5.2 Director Distribution Defects and Fluctuations . . . . . . . . . . . . . . . . 157 158 Defects in Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 5.2.2 Fluctuations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 160 Curvature Elasticity of Liquid Crystals in Three Dimensions . . . . . . . . . 161 5.3 Electric and Magnetic Fieldinduced Deformations . . . . . . . . . . . . . . 163 5.4 Director Distribution in Magnetic Fields . . . . . . . . . . . . . . . . . . . 164 5.4.1 5.4.2 Director Distribution in Electric Fields . . . . . . . . . . . . . . . . . . . . 167 5.4.3 FrCedericksz Transitions as a Method for Measuring Elastic Constants . . . 168 5.4.3.1 Capacitance Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 168 5.4.3.2 Birefringence Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 169 5.4.4 Frkedericksz Transition for Chiral Nematics . . . . . . . . . . . . . . . . . 170 5.4.5 FrCedericksz Transitions for Smectic Phases . . . . . . . . . . . . . . . . . 171 5.5 Molecular Aspects of Torsional Elasticity . . . . . . . . . . . . . . . . . . . 172 5.5.1 van der Waals Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 172 175 5.5.2 Results from Lattice Models . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5.3 Mean Field and Hard Particle Theories . . . . . . . . . . . . . . . . . . . . 175 176 5.5.4 Computer Simulations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Experimental Aspects of Elastic Constants and Comparison 5.6 177 with Theoretical Predictions . . . . . . . . . . . . . . . . . . . . . . . . . . 5.7 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 178 6 Phase Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 179 6.1 Phase Transitions Theories . . . . . . . . . . . . . . . . . . . . . . . . . . 179 Philippe Barois 179 6.1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
5
Contents
6.1.2 6.1.2. I 6.1.2.2 6.1.2.3 6.1.3 6.1.3.1 6.1.3.2 6.1.3.3 6.1.3.4 6.1.3.5 6.1.3.6 6.1.4 6.1.4.1 6.1.4.2 6.1.5 6.1.6 6.1.6.1 6.1.6.2 6.1.6.3 6.1.7 6.1.7.1 6.1.7.2 6.1.7.3 6.1.7.4 6.1.7.5 6.1.8 6.1.9 6.2 6.2.1 6.2. I . 1 6.2.1.2 6.2.1.3 6.2.1.4 6.2.1.5 6.2.1.6 6.2.1.7 6.2.2 6.2.2.1 6.2.2.2 6.2.2.3 6.2.2.4 6.2.2.5 6.2.2.6
XI11
179 The IsotropicNematic Transition . . . . . . . . . . . . . . . . . . . . . . . Mean Field Approach (Landaude Gennes) . . . . . . . . . . . . . . . . . . 179 182 Fluctuations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . IsotropicNematic Transition in Restricted Geometries . . . . . . . . . . . . 182 The NematicSmectic A Transition . . . . . . . . . . . . . . . . . . . . . . 183 183 Definition of an Order Parameter . . . . . . . . . . . . . . . . . . . . . . . Mean Field Description (McMillan, de Gennes) . . . . . . . . . . . . . . . 184 Analogy with Superconductors . . . . . . . . . . . . . . . . . . . . . . . . 184 Critical Exponents and Scaling . . . . . . . . . . . . . . . . . . . . . . . . 187 Renormalization Group Procedures . . . . . . . . . . . . . . . . . . . . . . 188 188 Dislocation Loops Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . The Smectic ASmectic C Transition . . . . . . . . . . . . . . . . . . . . . 189 The Superfluid Helium Analogy . . . . . . . . . . . . . . . . . . . . . . . . 189 The NSmASmC Point . . . . . . . . . . . . . . . . . . . . . . . . . . . . 189 The Smectic AHexatic Smectic B Transition . . . . . . . . . . . . . . . . 191 Phase Transitions in Chiral Liquid Crystals . . . . . . . . . . . . . . . . . . 192 Chirality in Nematic and Smectic Liquid Crystals . . . . . . . . . . . . . . 192 Mean Field Chiral NSmASmC model . . . . . . . . . . . . . . . . . . . 193 194 Twist Grain Boundary Phases . . . . . . . . . . . . . . . . . . . . . . . . . Frustrated Smectics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 196 196 Polar Smectics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Model of Frustrated Smectics (Prost) . . . . . . . . . . . . . . . . . . . 197 199 The Mean Field Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . Critical Properties of the Isolated SmASmA Critical Point . . . . . . . . . 202 204 The Reentrant Phenomenon . . . . . . . . . . . . . . . . . . . . . . . . . Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 205 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 206 Experimental Methods and Typical Results . . . . . . . . . . . . . . . . . . 208 208 Thermal Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Jun Thoen Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 208 Theoretical Background . . . . . . . . . . . . . . . . . . . . . . . . . . . . 208 Experimental Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 212 Calorimetric Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 221 Photoacoustic and Photopyroelectric Results . . . . . . . . . . . . . . . . . 229 230 Acknowledgements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 230 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Density . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 232 Wolfgang Wedler Instrumentation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 232 General Conclusions from Density Studies on Liquid Crystals . . . . . . . . 232 236 Studies of Calamitic Compounds . . . . . . . . . . . . . . . . . . . . . . . 241 Discotics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Lyotropics and Anhydrous Soaps . . . . . . . . . . . . . . . . . . . . . . . 241 Polymeric Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . 241
XIV
Contents
6.2.2.7 Further Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 6.2.2.8 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 242 6.2.3 Metabolemeter . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 248 Wolfgang Wedler 6.2.3.1 Thermobarograms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 250 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.3.2 References 253 High Pressure Investigations . . . . . . . . . . . . . . . . . . . . . . . . . 253 6.2.4 P. Pollmann 6.2.4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 253 254 6.2.4.2 Phase transitions at High Pressures . . . . . . . . . . . . . . . . . . . . . . 6.2.4.3 Critical Phase Transitions Under Pressure . . . . . . . . . . . . . . . . . . . 266 6.2.4.4 PressureVolumeTemperature Behavior . . . . . . . . . . . . . . . . . . . 269 6.2.4.5 Appendix . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 273 6.2.4.6 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 274 Fluctuations and Liquid Crystal Phase Transitions . . . . . . . . . . . . . . 277 6.3 P. E . Cladis 6.3.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 277 The NematicIsotropic Transition . . . . . . . . . . . . . . . . . . . . . . . 278 6.3.2 6.3.3 The UniaxialBiaxial Nematic Transition . . . . . . . . . . . . . . . . . . . 279 6.3.4 Type I Smectic A's: NematicSmectic A Transition . . . . . . . . . . . . . 279 6.3.5 Type I1 Smectic A's: CholestericSmectic A Transition . . . . . . . . . . . 281 6.3.6 Transitions between Tilted and Orthogonal Smectic Phases . . . . . . . . . 282 6.3.7 BSmBSmA Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . 283 6.3.8 Fluctuations at Critical Points . . . . . . . . . . . . . . . . . . . . . . . . . 284 6.3.8.1 BPI,, Isotropic . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 284 284 6.3.8.2 SmA, and SmA, . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.8.3 NAC Multicritical Point . . . . . . . . . . . . . . . . . . . . . . . . . . . . 285 285 6.3.9 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.10 References and Notes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 285 6.4 Reentrant Phase Transitions in Liquid Crystals . . . . . . . . . . . . . . . 289 P. E . Cladis 289 6.4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 291 6.4.2 R 1 : Reentrance from Frustration . . . . . . . . . . . . . . . . . . . . . . . 6.4.3 Reentrance from Geometric Complexity . . . . . . . . . . . . . . . . . . . 298 6.4.4 R3: Reentrance from Competing Fluctuations . . . . . . . . . . . . . . . . 300 6.4.5 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 301 6.4.6 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 301 Defects and Textures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 304 Yves Bouligand 304 Definitions. Conventions and Methods . . . . . . . . . . . . . . . . . . . . 7.1 Local Molecular Alignment . . . . . . . . . . . . . . . . . . . . . . . . . . 304 7.1 . 1 7.1.2 Microscopic Preparations of Liquid Crystals . . . . . . . . . . . . . . . . . 304 7.1.2.1 Thermotropic Textures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 305 7.1.2.2 Lyotropic Textures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 307 7
Contents
XV
7.1.2.3 7.1.3 7.1.4 7.2 7.2.1 7.2.2 7.2.3 7.2.4 7.2.5 7.3 7.3.1 7.3.2 7.3.3 7.3.4 7.3.5 7.3.6 7.3.7 7.4 7.4.1 7.4.2 7.4.3 7.4.4 7.4.4. I 7.4.4.2 7.4.4.3 7.4.4.4 7.4.4.5 7.4.4.6 7.4.5 7.4.6 7.4.7 7.4.7.1 7.4.7.2 7.4.7.3 7.4.7.4 7.4.7.5 7.4.7.6 7.4.7.7 7.4.7.8 7.5
Liquid Monocrystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 308 Images of Liquid Crystals in Polarizing Microscopy . . . . . . . . . . . . . 308 Other Microscopic Methods . . . . . . . . . . . . . . . . . . . . . . . . . . 311 Strong Deformations Resulting in Defects . . . . . . . . . . . . . . . . . . 311 Singular Points . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 311 Singular Lines . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 312 Walls . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 313 Interface Defects (Points and Lines) . . . . . . . . . . . . . . . . . . . . . 313 The Nature of Thick and Thin Threads . . . . . . . . . . . . . . . . . . . . 316 Topological Structure of Defects . . . . . . . . . . . . . . . . . . . . . . . 316 The Volterra Process . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 316 The Volterra Process in Nematic. Smectic A and Cholesteric Phases . . . . . 316 A Different Version of the Volterra Process . . . . . . . . . . . . . . . . . . 318 Continuous and Discontinuous Defects in Cholesteric Phases . . . . . . . . 321 Core Disjunction into Pairs of Disclinations . . . . . . . . . . . . . . . . . 325 Optical Contrast . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 326 Classification of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 327 Geometrical Constraints and Textures . . . . . . . . . . . . . . . . . . . . . 328 Parallel Surfaces and Caustics in Liquid Crystals . . . . . . . . . . . . . . . 328 Dupin’s Cyclides and Focal Conics . . . . . . . . . . . . . . . . . . . . . . 328 Slight Deformations of Dupin’s Cyclides . . . . . . . . . . . . . . . . . . . 331 Textures Produced by Parallel Fluid Layers . . . . . . . . . . . . . . . . . . 332 Planar Textures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 332 Focal Conics and Polygonal Textures . . . . . . . . . . . . . . . . . . . . . 333 Fan Textures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 334 Texture Distribution in Lamellar Mesophases . . . . . . . . . . . . . . . . . 335 Illusory Conics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 337 Walls, Pseudowalls and Broken Aspects . . . . . . . . . . . . . . . . . . . 337 Origin of Spirals in Chiral Liquid Crystals . . . . . . . . . . . . . . . . . . 340 Defects and Mesophase Growth . . . . . . . . . . . . . . . . . . . . . . . . 341 Defect Energies and Texture Transformations . . . . . . . . . . . . . . . . . 342 Disclination Points . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 342 Disclination Lines . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 343 Focal Curves . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 344 Translation Dislocations . . . . . . . . . . . . . . . . . . . . . . . . . . . . 345 Simulations of Defects and Textures . . . . . . . . . . . . . . . . . . . . . 345 Defect Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 346 Textures and Defect Associations . . . . . . . . . . . . . . . . . . . . . . . 347 Crystals of Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 348 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 348
8
Flow Phenomena and Viscosity . . . . . . . . . . . . . . . . . . . . . . . . 352 E Schneider and H . Kneppe Nematic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . 353 Shear Viscosity Coefficients q,. q2. q3.and q I 2 . . . . . . . . . . . . . . . 353
8.1 8.1.1
XVI
Contents
8.1.2 8.1.3 8.1.4 8.1.5 8.1.6 8.1.7 8.1.8 8.1.9 8.2 8.2.1 8.2.2 8.2.3 8.2.4 8.3 8.3.1 8.3.2 8.3.3 8.4 8.4.1 8.4.2 8.4.3 8.4.4 8.5 8.6
Rotational Viscosity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 354 Flow Alignment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 356 Viscous Flow under the Influence of Elastic Torques . . . . . . . . . . . . . 358 Transverse Pressure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 360 Backflow . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 361 Discotic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . 362 Influence of Temperature and Order Parameter on the Viscosity Coefficients 362 Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 363 Cholesteric Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . 364 Helical Axis Parallel to the Shear Gradient (Case I) . . . . . . . . . . . . . 364 Helical Axis Parallel to the Flow Direction (Case 11) . . . . . . . . . . . . . 365 Helical Axis Normal to v and grad v (Case 111) . . . . . . . . . . . . . . . . 365 Torque Generation Under Flow . . . . . . . . . . . . . . . . . . . . . . . . 366 Biaxial Nematic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . 366 Shear Viscosity Coefficients . . . . . . . . . . . . . . . . . . . . . . . . . . 367 Rotational Viscosity Coefficients . . . . . . . . . . . . . . . . . . . . . . . 368 Flow Alignment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 368 SmCPhase . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 368 Shear Flow with a Fixed Director Orientation . . . . . . . . . . . . . . . . 369 Rotational Viscosity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 370 Flow Alignment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 371 SmC* Phase . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 371 SmAPhase. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 372 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 373
9
Behavior of Liquid Crystals in Electric and Magnetic Fields . . . . . . . . . 375 Lev M . Blinov Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 375 Direct Influence of an Electric or Magnetic Field on Liquid Crystal Structure . 376 Shift of Phase Transition Temperatures . . . . . . . . . . . . . . . . . . . . 376 SecondOrder Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . 376 Strong FirstOrder Transitions . . . . . . . . . . . . . . . . . . . . . . . . . 377 Weak FirstOrder Transitions . . . . . . . . . . . . . . . . . . . . . . . . . 379 Influence of the Field on Order Parameters . . . . . . . . . . . . . . . . . . 380 Changes in Symmetry . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 381 Induced Biaxiality in Nematics . . . . . . . . . . . . . . . . . . . . . . . . 381 The Kerr Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 382 Specific Features of Twisted Phases and Polymers . . . . . . . . . . . . . . 383 Bluephases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 383 Twist Grain Boundary Phases . . . . . . . . . . . . . . . . . . . . . . . . . 385 Comment on Polymer Liquid Crystals . . . . . . . . . . . . . . . . . . . . 386 Distortions due to Direct Interaction of a Field with the Director . . . . . . . 386 Nematics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 386 Classical Frederiks Transition . . . . . . . . . . . . . . . . . . . . . . . . . 386 FieldInduced Periodic Structures . . . . . . . . . . . . . . . . . . . . . . . 390
9.1 9.2 9.2.1 9.2.1.1 9.2.1.2 9.2.1.3 9.2.2 9.2.3 9.2.3.1 9.2.3.2 9.2.4 9.2.4.1 9.2.4.2 9.2.4.3 9.3 9.3.1 9.3.1.1 9.3.1.2
Contents
XVII
9.3.1.3 9.3.2 9.3.2.1 9.3.2.2 9.3.2.3 9.3.2.4 9.3.3 9.3.3.1 9.3.3.2 9.4 9.4.1 9.4.1.1 9.4.1.2 9.4.1.3 9.4.2 9.4.2.1 9.4.2.2 9.4.2.3 9.5 9.6
FlexoElectric Phenomena . . . . . . . . . . . . . . . . . . . . . . . . . . . 391 Twisted Nematics and Cholesterics . . . . . . . . . . . . . . . . . . . . . . 395 395 Twist and Supertwist Structures . . . . . . . . . . . . . . . . . . . . . . . . Instability of the Planar Cholesteric Texture . . . . . . . . . . . . . . . . . 397 Field Untwisting of the Cholesteric Helix . . . . . . . . . . . . . . . . . . . 399 Flexoelectric Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 401 403 Smectics and Discotics . . . . . . . . . . . . . . . . . . . . . . . . . . . . Field Behavior of Achiral Smectics . . . . . . . . . . . . . . . . . . . . . . 403 Chiral Ferroelectrics and Antiferroelectrics . . . . . . . . . . . . . . . . . . 406 Eiectrohydrodynamic Instabilities . . . . . . . . . . . . . . . . . . . . . . . 413 413 Nematics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 413 Classification of Instabilities . . . . . . . . . . . . . . . . . . . . . . . . . 414 Isotropic Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 419 Anisotropic Modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Cholesterics and Smectics . . . . . . . . . . . . . . . . . . . . . . . . . . . 424 Cholesterics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 424 425 Smectics A . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 426 Smectics C . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 427 427 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
10
433 Surface Alignment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Blandine JkrBme 433 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Macroscopic Alignment of Nematic Liquid Crystals . . . . . . . . . . . . . 434 434 Definitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 435 Anchoring Directions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 436 Anchoring Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Microscopic Surface Order of Nematic Liquid Crystals . . . . . . . . . . . 438 Surface Orientational Order . . . . . . . . . . . . . . . . . . . . . . . . . . 438 Microscopic Anchoring Mechanisms at Solid Substrates . . . . . . . . . . . 439 The Nematic/Isotropic and NematicNapor Interfaces . . . . . . . . . . . . . 441 442 Orientation of Other Liquid Crystals . . . . . . . . . . . . . . . . . . . . . 442 Smectic and Chiral Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . 444 Polymer Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . 444 Lyotropic Liquid Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . 445 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
10.1 10.2 10.2.1 10.2.2 10.2.3 10.3 10.3.1 10.3.2 10.3.3 10.4 10.4.1 10.4.2 10.4.3 10.5
Ultrasonic Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 447 Olga A . Kapustina Structural Transformation in Liquid Crystals . . . . . . . . . . . . . . . . . 447 1 1.1 1I . I . 1 Orientation Phenomena in Nematics . . . . . . . . . . . . . . . . . . . . . 448 11.1.1.1 Homogeneous Distortion Stage . . . . . . . . . . . . . . . . . . . . . . . . 448 1 1.1.1.2 Spatially Periodic Distortion Stage . . . . . . . . . . . . . . . . . . . . . . 452 453 11.1.1 .3 Inhomogeneous Distortion Stage . . . . . . . . . . . . . . . . . . . . . . . 11
XVIII
Contents
455 11.1.2 Cholesterics in an Ultrasonic Field . . . . . . . . . . . . . . . . . . . . . . 1 1.1.2.1 Periodic Distortion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 455 11.1.2.2 Storage Mode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 455 1 1.1.2.3 FocalConic to Planar Texture Transition . . . . . . . . . . . . . . . . . . . 456 11.1.2.4 Bubble Domain Texture . . . . . . . . . . . . . . . . . . . . . . . . . . . . 456 1 1.1.2.5 Fingerprint Texture Transition . . . . . . . . . . . . . . . . . . . . . . . . . 457 457 1 1.1.3 Smectic Phase in an Ultrasound Field . . . . . . . . . . . . . . . . . . . . . 11.2 Wave Interactions in Nematics . . . . . . . . . . . . . . . . . . . . . . . . 457 Acoustoelectrical Interactions in Nematics . . . . . . . . . . . . . . . . . . 460 11.3 461 Ultrasound Studies of Liquid Crystals . . . . . . . . . . . . . . . . . . . . . 1 I .4 461 1 1.4.1 Ultrasonic Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . I I .4.2 Photoacoustic Spectroscopy 463 11.4.3 Acoustic Emission . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 463 463 11.4.4 Monitoring Boundary Effects . . . . . . . . . . . . . . . . . . . . . . . . . 11.4.5 Acoustic Microscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 464 464 11.5 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 12.1 12.2 12.2.1 12.2.2 12.3 12.3.1 12.4 12.5 12.5.1 12.5.2 12.5.3 12.5.4 12.6 12.6.1 12.6.2 12.6.3 12.7 12.8
Nonlinear Optical Properties of Liquid Crystals . . . . . . . . . . . . . . . 467 P. Pa l&Mu horu y Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 467 Interaction between Electromagnetic Radiation and Liquid Crystals . . . . . 467 467 Maxwell’s Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Nonlinear Susceptibility and Hyperpolarizability . . . . . . . . . . . . . . . 468 Nonlinearities Originating in Director Reorientation . . . . . . . . . . . . . 469 D . C . Kerr Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 469 470 Optical FieldInduced Reorientation . . . . . . . . . . . . . . . . . . . . . Nonlinearities without Director Reorientation . . . . . . . . . . . . . . . . 472 OpticalFieldInduced Orientational Order . . . . . . . . . . . . . . . . . . 472 Thermal Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 473 Conformational Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . 473 Electronic Response . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 474 475 Optical Harmonic Generation . . . . . . . . . . . . . . . . . . . . . . . . . Bulk Second Harmonic Generation . . . . . . . . . . . . . . . . . . . . . . 475 Surface Second Harmonic Generation . . . . . . . . . . . . . . . . . . . . . 476 Third Harmonic Generation . . . . . . . . . . . . . . . . . . . . . . . . . . 476 Materials and Potential Applications . . . . . . . . . . . . . . . . . . . . . 476 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 477
Diffusion in Liquid Crystals . . . . . . . . . F: Nouck f 13.1 Introduction . . . . . . . . . . . . . . . . . 13.2 Theoretical Concepts . . . . . . . . . . . . 13.2.1 The Diffusion Tensor . . . . . . . . . . . . 13.2.2 Basic Models . . . . . . . . . . . . . . . . 13.2.3 Model Refinements . . . . . . . . . . . . .
13
.................
480
. . . . .
480 480 480 481 483
. . . . .
............... . . . . . . . . . . . . . . . ............... . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Contents
13.3 13.3.1 13.3.2 13.3.3 13.4 13.4.1 13.4.2 13.4.3 13.4.4 13.4.5 13.4.6 13.4.7 13.5
Experimental Techniques . . . . . . . . . . . . . . . . . . . . . . . . . . . Tracer Techniques . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quasielastic Neutron Scattering . . . . . . . . . . . . . . . . . . . . . . . . Magnetic Resonance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Selected Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Experimental Dilemma . . . . . . . . . . . . . . . . . . . . . . . . . . Nematic Mesophase . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Nematic Homologues . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Smectic Mesophases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Solute Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Lyotropic Mesophases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Selected Diffusion Constants . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
XIX 483 483 484 484 485 486 486 487 488 488 489 490 490
This Page Intentionally Left Blank
Chapter I Introduction and Historical Development George W Gray
1 Introduction It is with a sense of responsibility that I begin this summary of the historical development of liquid crystals, because one of the two authors of the original Handbook of Liquid Crystals of 1980 [ 11 was Professor Hans Kelker, a friend and a very well informed authority on the history of the subject and the personalities involved in the earlier stages of its emergence. Those who attended the Twelfth International Liquid Crystal Conference in Freiburg in 1988, which marked the centenary of the discovery of liquid crystals, and heard Professor Kelker’s plenary lecture  Some Pictures of the History of Liquid Crystals [2]  which was part of a conference session devoted to a historical review of the field, will know this. Here he demonstrated that he was in possession of a very wonderful collection of manuscripts and photographs relating to the scientists who, in the latter part of the nineteenth century and the early part of the twentieth century, laid the foundations of our presentday knowledge of liquid crystals. I am not in that privileged situation, but I have worked in the field for 50 years, beginning my first experiments on aromatic carboxylic acids in October 1947. I have therefore worked through approaching half of the historical span of the subject, including the most recent years during which the subject has expanded and deepened so markedly. I hope this firsthand experience will counterbalance my lack of detailed his
torical knowledge of the earlier years, as possessed by Professor Kelker. Were he alive today, I hope he would not disapprove of what I write in this chapter. The history of the development of liquid crystals may be divided into three phases: 1. The period from their discovery in the latter part of the nineteenth century through to about 1925, the years during which the initial scepticism by some that a state of matter was possible in which the properties of anisotropy and fluidity were combined, through to a general acceptance that this was indeed true, and publication of a first classification of liquid crystals into different types. 2. The period from 1925 to about 1960, during which general interest in liquid crystals was at a fairly low level. It was a niche area of academic research, and only relatively few, but very active, scientists were devoted to extending knowledge of liquid crystals. Two world wars and their aftermaths of course contributed greatly to the retardation of this field during this period. Taking the aftermaths of the wars into account, probably at least 15 years were effectively lost to progress during this second phase. 3 . The period from 1960 until today is by contrast marked by a very rapid development in activity in the field, triggered of course by the first indications that technological applications could be found for liquid crystals. These early indications
2
I
Introduction and Historical Development
were justified, and led to today’s strong electrooptical display industry. The quest for new applications stimulated research and the flow of financial support into the involved areas of chemistry, physics, electrical and electronic engineering, biology, etc. As a marker of this activity, the numbers of papers and patents published in 1968 was about 2000 and this had risen to 6500 in 1995.
2 The Early Years up to About 1925 The question as to when liquid crystals were discovered must now be addressed. In pinpointing a discovery, it is necessary to distinguish simple observations of an unusual phenomenon or effect from observations that develop into an understanding of the meaning and significance of that phenomenon or effect. If we accept that the latter criteria must be met to justify the word discovery, then the credit for the discovery of liquid crystals must go to Friederich Reinitzer, a botanist of the Institute for Plant Physiology of the German University of Prague, who in a paper submitted on May 3, 1888 [3], described his observations of the colored phenomena occurring in melts of cholesteryl acetate and cholesteryl benzoate. In addition, he noted the “double melting” behavior in the case of cholesteryl benzoate, whereby the crystals transformed at 145.5 “C into a cloudy fluid, which suddenly clarified only on heating to 178.5 “C. Subsequent cooling gave similar color effects (but see later) to those observed on cooling the melt of cholesteryl acetate. Today of course we know that the colored phenomena reported by Reinitzer are characteristic of many cholesteric or chiral nematic (N*) liquid crystal phases.
In his article [ 3 ] , Reinitzer acknowledges that other workers before him had observed curious color behavior in melts of cholesteryl systems. He mentions that Planar in Russia and Raymann in Paris had noted violet colors reflected from cholesteryl chloride and that Lobisch in Germany had observed a bluishviolet flourescence in the case of cholesteryl amine and cholesteryl chloride. Two things distinguish these earlier observations from those of Reinitzer. These are Reinitzer’s recording of the “double melting” property of cholesteryl benzoate, and the fact that Reinitzer carried out preliminary studies on thin films of cholesteryl benzoate and noted the range of spectral colors reflected as the temperature decreased until crystallization occurred and the complementary nature of the colored light when the sample was viewed in transmission. Moreover, Reinitzer knew of the excellent work of the German physicist Professor Otto Lehmann, then at the Polytechnical School at Aachen, in designing and developing polarization microscopes, and recognized that Lehmann could advise on the optical behavior of his cholesteryl esters. The approach to Lehmann was made in March 1888 and the correspondence is excellently documented in Kelker and Knoll’s article [2]. This interaction led to agreement that Reinitzer’s materials were homogeneous systems of which Lehmann wrote in August 1889: “It is of high interest for the physicist that crystals can exist with a softness, being so considerable that one could call them nearly liquid.” This led quickly to the submission by Lehmann, by then at the University of Karlsruhe, of his paper Uber fliessende Kristalle to the Zeitschrift f u r Physikalische Chemie [4]. Significantly, this uses for the first time the term liquid crystal. As a consequence of the above events and the development of our understanding of liquid crystals which
2
stemmed from them, we must clearly acknowledge Reinitzer as the true discoverer of liquid crystals and the date of the event as March 14, 1888. It should be noted that the discovery related exclusively to materials we now class as thermotropic liquid crystals, wherein the liquid crystal phases form either on heating crystals or on cooling isotropic liquids, that is, as a consequence of thermal effects. In addition to thermotropic liquid crystals, a second class of fluid anisotropic materials is known, namely, lyotropic liquid crystals where the disruptive effect on the crystal lattice involves a solvent (often water), coupled where necessary with thermal change. Here, the order of the crystal is broken down by the solvent and the molecules form micelles which then arrange themselves in an ordered way, while allowing fluidity. Excess of solvent completes the decrease in order and an isotropic solution is formed. Observations of anisotropy and optical birefringence in such systems were indeed made well before Reinitzer’s discovery, but like the observations of Planar, Raymann, and Lobisch, there was no followthrough to a realization of the full significance of what was being seen. These observations were made by Mettenheimer [ 5 ] ,Valentin [6], and Virchow [7] in the period 18341861, and involved studies of biological samples derived from nerve tissue, for example, myelin, a complex lipoprotein which can be separated into fractions and which forms a sheath round nerve cells. In watercontaining sodium oleate, these sheaths develop what have been called myelinic forms visible microscopically, especially in polarized light, as fluid, birefringent entities. Progress on these anisotropic systems was however impeded by the complexity and lack of reproducibility of the biological systems involved, and whilst predating the studies of Reinitzer and Lehmann are not generally re
The Early Years up to About 1925
3
garded as marking the discovery of liquid crystals. Following publication of his paper in 1889 [4], Lehmann continued work with liquid crystals and indeed dominated the scene in the late 1800s and the early part of the twentieth century, continuing to publish on liquid crystals until the year of his death in 1922. Turning to purely synthetic materials, unlike the cholesteryl esters which were of natural origin, examples of liquid crystal behavior were found in these by Lehmann in 1890. The materials were azoxy ethers prepared by Gattermann and Ritschke [8]. The next ten years or so saw studies of pmethoxycinnamic acid and in 1902 the synthesis by Meyer and Dahlem [9] of the first smectogen, ethyl pazoxybenzoate, although not recognized structurally for what it was at that time. Through studying such materials, Lehmann did however recognize that all liquid crystals are not the same, and indeed in 1907 he examined the first liquid crystal material exhibiting two liquid crystal phases. This material had what was later shown to be a smectic A (SmA) and a cholesteric (N*) phase. Significantly in the context of much later work in the field of applications, he also reported on the aligning effects of surfaces on liquid crystals. Despite the growing number of compounds shown to exhibit liquid crystal phases (and in a short number of years Vorlander contributed about 250), the acceptance of liquid crystals as a novel state of matter was not universal. Tammann in particular [ 101 persisted in the view that liquid crystals were colloidal suspensions, and was in bitter argument with Lehmann and Schenk who upheld the view that they were homogeneous systems existing in a new state distinct from the crystalline solid and isotropic liquid states. Nernst [ 1 I] too did not subscribe to the latter view and believed that liquid crystals were mixtures of tautomers.
4
I
Introduction and Historical Development
There was however a steadily growing body of evidence supporting the view that liquid crystals represent a true state of matter and acceptance of this slowly grew, aided by the excellent reviews of 1905 by Schenk (Kristalline Fliissigkeiten und flussige Kristalle) [ 121 and Vorlander (KristalZinischfliissige Substanzen) [ 131. There then followed the important review of optical effects by Stumpf [14] and, much later, an important paper was that by Oseen [15] on a kinetic theory of liquid crystals. The real seal of acceptance of liquid crystals for what they are, i.e., a fascinating and distinct state of matter, was however given in 1922 in the famous publication by G. Friedel [16] in the Annales de Physique, entitled Les Etats Mesomorphes de la Matidre. Here, in connection with Friedel’s article and on a personal note, I well remember my research supervisor, Professor and later Sir Brynmor Jones, sending me to the library to find the appropriate journal, requiring that I produce a complete translation from French of all 273 pages in order to be “fully familiar with all that had been written”. This I dutifully did in the fullness of time, and on taking my translation to show my supervisor, he then reached up to a shelf and withdrew a black notebook saying “now you can compare the quality of your translation with mine!” I learned much from that exercise, as will anyone who repeats it today. In addition to containing a wealth of information on microscopic techniques and materials, Friedel’s article represented in 1922 the first classification of liquid crystals into types, i.e., nematic, smectic and cholesteric. Today, of course, cholesterics are known simply as chiral nematics with no need that they be derived from cholesterol, and we recognize the existence of several polymorphic smectic forms, whereas Friedel allowed for only one (today’s smectic A; S mA).
Friedel did however understand the layered nature of smectics, firstly through the stepped edges possessed by smectic droplets with a free surface, and secondly through his detailed studies of the optical microscopic textures of thin films of smectic phases. He understood the optical discontinuities, i.e., the defects, of the smectic focalconic texture and saw the relationship of the black lines delineating ellipses of different eccentricities and their associated hyperbolae in terms of focalconic “domains” which may be divided into a series of parallel, curved surfaces known as Dupin cyclides. He also understood that the optically extinct homeotropic textures of smectics of the type he studied gave positive uniaxial interference figures consistent with systems of layers lying flat to the surface. His microscopic studies demonstrated the immense value of the optical microscope as a precise scientific instrument in studies of all types of liquid crystal phases. Friedel’s article, coupled with the publications on synthesis and studies of new liquid crystal materials by organic chemists in Germany, notably Vorlander (see, for example, his monograph Chemische Kristallographie der Flussigkeiten of 1924 [17]), firmly cemented in place all the earlier observations, providing a firm basis on which to build the future structure of the subject. Before moving on to phase two of the history, we might just return to Reinitzer, the discoverer of liquid crystals, and recognize the quality of his powers of observation, for not only did he focus on the color effects and double melting, but also he noted the blue color appearing in the isotropic melt just before the sample turned into the cloudy cholesteric phase. About this, he said the following: “there appeared (in the clear melt) at a certain point a deep blue colour which spread rapidly through the whole mass and almost as quickly disappeared,
3 The Second Phase from 1925 to 1959
again leaving in its place a uniform turbidity. On further cooling, a similar colour effect appeared for the second time to be followed by crystallisation of the mass and a simultaneous disappearance of the colour effect.” The turbid state and the second color effect were of course due to the cholesteric phase, but the first transient blue color we now know was associated with the optically isotropic ‘blue phases’ we are familiar with today. Although Lehmann believed that this transient effect represented a different state, the full significance of Reinitzer’s observations had to wait until the 1980s when these isotropic cubic phases became a focus of attention in condensed matter physics. A further point concerning the first phase of our history of liquid crystals is about nomenclature, a matter about which scientists of today still love to argue. In the early years, however, the debate was sparked by Friedel who strongly objected to Lehmann’s term liquid crystal, on the basis that liquid crystals were neither true liquids nor true crystals. The term does of course remain in widespread use today, simply because the juxtaposition of two contradictory terms carries an element of mystery and attraction. Friedel preferred the term mesomorphic to describe the liquid crystal state, and the associated term mesophase, reflecting the intermediate nature of these phases between the crystalline and isotropic liquid states. These terms are again widely used today and coexist happily with the Lehmann terminology. A useful term springing from Friedel’s nomenclature is the word mesogen (and also nematogen and smectogen), used to describe a material that is able to produce mesophases. The associated term mesogenic is used by some to indicate that a material does form liquid crystal phases and by others to indicate that a compound is structurally suited to give mesophases, but may not, if, for
5
example, the melting point of the crystalline state is too high. Then the isotropic liquid is produced directly from the crystal, and, on cooling, crystallization may occur too quickly for even a monotropic liquid crystal phase to form. Yet this compound may show strong tendencies to be mesomorphic if binary phase diagrams of state are examined using a standard material as the second component. My view is that the term mesogenic should be used to describe a structural compatibility with mesophase formation, without the requirement that a phase is actually formed. After all, if the compound does really form a mesophase, the description of it as mesomorphic is perfectly adequate. Finally, on the subject of nomenclature, Friedel of course gave us today’s terms smectic and nematic with their wellknown Greek derivations.
3 The Second Phase from 1925 to 1959 In the first part of this period, Vorlander and his group in Halle contributed strongly to the growing number of compounds known to form liquid crystal phases, some showing up to three different mesophases. Based upon his work came the recognition that elongated molecular structures (lath or rodlike molecules) were particularly suited to mesophase formation. His work also showed that if the major axis of a molecule were long enough, protrusions could be tolerated without sacrifice of the liquid crystal properties. Thus 1,4disubstituted naphthalenes with a strong extension of the major axis through the I ,4substituents were liquid crystalline, despite the protruding second ring of the naphthalene core. It is interesting that Vorlander records that the mate
6
I
Introduction and Historical Development
rials behaved as liquid crystallline resins or lacquers (an early thought perhaps about the potential of liquid crystals for applications). In his book Nature’s Delicate Phase of Matter, Collings [ 181 remarks that over 80 doctoral theses stemmed from Vorlander ’s group in the period 19011934. Further evidence of Vorlander’s productivity is found in the fact that five of the 24 papers presented at the very important and first ever symposium on liquid crystals held in 1933 under the auspices of the Faraday Society in London, Liquid Crystals and Anisotropic Fluids  A General Discussion [ 191, were his. Perhaps the most important consequence of Vorlander’s studies was that in laying down the foundations of the relationship between molecular structure and liquid crystal properties, attention was focused upon the molecules as the fundamental structural units of the partially ordered phases. Up to then, even Lehmann had been uncertain about the units involved in the ordering and what occurred at the actual transitions. The Faraday Meeting of 1933 was of great importance in bringing together the small number of active, but often isolated, scientists involved at that time in liquid crystal research. This propagated knowledge and understanding, but, as we shall see, it also generated some dispute. As early as 1923, de Broglie and E. Friedel (the son of G. Friedel) had shown [20] that Xray reflections could be obtained from a system of sodium oleate containing water, and that the results were consistent with a lamellar or layered structure. This Xray work was extended [21] in 1925 to Vorlander’s thermotropic ethyl pazoxybenzoate, confirming G. Friedel’s conclusions of a layered structure stemming from his microscopic studies of smectic defect structures. Further, in the period 19321935, Herrmann [22], who also contributed to the 1933 Faraday Discussion, was deci
sive in confirming the lamellar nature of smectics by Xray studies which included Vorlander’s material exhibiting more than one smectic phase. The latter work substantiated a change from a statistical order in the layers of one srnectic to a hexagonal ordering in the lower temperature phase. A tilted lamellar structure was also found by Herrmann for some thallium soaps [23]. Amongst other names of historical interest featured on the Faraday Discussion program were, for example, Frkedericksz and Zolina (forces causing orientation of an anisotropic liquid), Zocher (magnetic field effects on nematics), Ostwald, Lawrence (lyotropic liquid crystals), Bernal, Sir W. H. Bragg (developing the concept of Dupin cyclides in relation to Friedel’s earlier studies of focalconics), and also Ornstein and Kast who presented new arguments in favor of the swarm theory, which was first put forward in 19071909 by Bose [24]. This theory had proposed that the nematic phase consisted of elongated swarms of some 1Oh molecules, and in the 1930s much effort was given to proving the existence of these swarms, which were used to explain some, but not all, of the physical properties of nematics. However, at the 1933 Faraday Meeting, the presentation of Oseen [25] and the strong reservations expressed by Zocher during the discussions were already casting shadows of doubt on the swarm theory. Today of course we accept that definitive proof of the existence of swarms was never obtained, and by 1938 Zocher was expressing further strong reservations about the theory [26], proposing alternatively that the nematic phase is a continuum, such that the molecular orientation changes in a continuous manner throughout the bulk of the mesophase. This was called the distortion hypothesis and together with Oseen’s work marked the beginning of the modern continuum theory of liquid crystals. However, de
3 The Second Phase from 1925 to 1959
velopments here had to wait until after the second world war when Frank [27], at a further Faraday discussion in 1958, and consequent upon his reexamination of Oseen’s treatment, presented it as a theory of curvature elasticity, to be advanced in the next historical phase by names such as Ericksen, Leslie, de Gennes, and the Orsay Group in France. The period following the war up until the 1950s is also significant for the work of Chatelain [28], in collaboration with Falgueirettes. Using surface alignment techniques, they measured the refractive indices of different nematics, and Chatelain produced his theoretical treatment of the values of the ordinary and extraordinary indices of refraction of an oriented nematic melt. Following Vorlander, other chemists were now becoming interested in new liquid crystal materials, and in the early 1940s we find publications on structure/property relations by Weygand and Gabler [29]. Later, in the 1950s, Wiegand [30] in Germany and the author in the UK were also making systematic changes in the structures of mesogens to establish the effects on liquid crystal behavior. The author’s work included not only systematic modifications to aromatic core structures, but also studies of many homologous series, establishing clearly that within series systematic changes in transition temperature always occur, within the framework of a limited number of patterns of behavior. In the period 19511959, the author published some 20 papers on structure/property relations in liquid crystals. These are rather numerous to reference here, but in the account of the third historical phase from 1960 until today, reference to relevant reviews and books is given. Lyotropic liquid crystals also progressed during this second phase. Lawrence’s paper at the 1933 Faraday meeting discussed the pb,ase diagrams for different compositions
7
of fatty acid salts, recognizing the different phase types involved and the transitions undergone with change of temperature and/or water content. Examples of aromatic materials, including dyes, giving lyotropic phases were also found, and solvents other than water as the lyophase were explored. The early work of Robinson et al. [31] was also done in this period. This involved solutions of polyybenzylLglutamate in organic solvents. These solutions exhibited the selective light reflecting properties of thermotropic cholesteric liquid crystals. This period of history also saw the publication of work by Eaborn and Hartshorne [32] on diisobutylsilandiol, which generated a mesophase. This was a puzzling result at the time, as the molecular shape was inconsistent with views of the time that liquid crystal formation required rodshaped molecules. Light would be shed on this only after the discovery of liquid crystal phases formed by discshaped molecules in the early 1970s. Finally, it should be noted that in this period, in 1957, a very important review on liquid crystals was published by Brown and Shaw [33]. This did much to focus the attention of other scientists on the subject and certainly contributed to the increase in liquid crystal research, which was to herald the strong developments in the early 1970s. The period 19251959 may be usefully summarized now. Although the level of activity in the field was limited, important developments did occur in relation to: the influence of external fields (electric and magnetic) on liquid crystals;  the orienting influences of surfaces;  measurements of the anisotropic physical properties of aligned liquid crystals;  the range of new liquid crystal materials and structure/property relationships; 
8
I
Introduction and Historical Development
the development of theories of the liquid crystal state ranging from the swarm theory to the emerging continuum theory;  increased awareness of the value of polarizing optical microscopy for the identification of mesophases, the determination of transition temperatures, and reaching a fuller understanding of defect textures. 
4 The Third Phase from 1960 to the Present Time The first ten years of this period saw several important developments which escalated interest and research in liquid crystals. Among these, there was the publication by Maier and Saupe [34] of their papers on a mean field theory of the nematic state, focusing attention on London dispersion forces as the attractive interaction amongst molecules and upon the order parameter. This theory must be regarded as the essential starting point for the advances in theoretical treatments of the liquid crystal state which followed over the years. There was also much activity in the field of new liquid crystal materials, notably by Demus et al. [35] in Germany and by the author who, in 1962, produced his monograph Molecular Structure and the Properties of Liquid Crystals [36], published by Academic Press, Also, further Xray studies began to advance knowledge of the structure of liquid crystal phases, particularly smectics. The work of de Vries and Diele should be mentioned, and later on, notably that by Levelut and coworkers in France and Leadbetter in England (see, for example, [37, 38]), work which culminated in the 1980s in a clear structural elucidation and classification of smetic liquid crystals. This distin
guished the true lamellar smectics with little or no correlation between layers from lamellar systems, previously regarded as smectics, which possess threedimensional order and are really soft crystals. Today, the true smectics are labeled SmA, for example, and the crystal phases are referred to simply by a letter such as K, or by CrK. The phase once known as SmD and first observed by the author and coworkers in laterally nitro substituted biphenyl carboxylic acids [39] is now recognized [40] as a cubic liquid crystal phase. Several other examples of cubic thermotropic liquid crystal phases are now known [4 1, 421. Such studies focused attention on the microscopic textures of liquid crystal phases. The defects characterizing these textures are now well understood through rather beautiful studies by workers such as Klkman [43], and from textures it is now possible to go a long way towards characterizing the phase behavior of new materials. A great deal of work on phase characterization has been done, and two reference sources are important [44,45]. Through such detailed studies of phase behavior, new phenomena were often recognized and explained, for example, the reentrance phenomenon through the work of Cladis [46], and the existence of the blue phases (BPI, BPII, and BPIII) through the work of several groups [47]. We should remember of course that Reinitzer did observe blue phases many years earlier and knew, without understanding the situation, that something occurred between the isotropic liquid and the N* phase on cooling many chiral materials. Reflectance microscopy played a big part in the eventual elucidation of these phases as cubic phases involving double twist cylinders. The widened interest in liquid crystals exemplified above had its origins in a number of events, such as the publication of the Brown and Shaw review [ 3 3 ] and the
4
The Third Phase from 1960 to the Present Time
author's monograph [36], but a very big part was played by the launch of the now regular International Liquid Crystal Conferences (ILCCs). We owe these now biennial conferences to Glenn Brown, the first one being organised by him in 1965 in Kent State University in Ohio. Attended by some 90 delegates from different countries, this meeting was most important in providing that small group of research workers with an identity and the opportunity to meet and discuss problems and new ideas. Glenn Brown was indeed successful in obtaining funding for the second ILCC, held again in Kent State University, in 1968. The liquid crystal community owes a great deal to Glenn Brown for his vision in making these meetings possible. He created for liquid crystals a community of scientists within which the vigorous development of new research results and the technological innovation of the 1970s was to generate and continue unabated to the present time. At the 1965 ILCC Meeting, the focus on applications was on Fergason's presentations on thermography using cholesteric liquid crystals, but in 1968, the meeting was attended by a group of researchers from Radio Corporation of America (RCA) in Princeton, where work under Heilmeier, Castellano, Goldmacher, and Williams was being done on display devices based on liquid crystals. The liquid crystal community was having its eyes opened to the potential of liquid crystals for application in electrooptical displays. The seminal work of the RCA group, initially on dynamic scattering displays, cannot be overstressed for its importance to the field. Two years later, at the 1970 ILCC in Berlin, display applications of liquid crystals were being discussed freely, and later when the patents of Schadt and Helfrich and of Fergason on the twisted nematic liquid crystal electrooptical display mode came into the public domain, activity
9
intensified. At the fourth ILCC in 1972, again at Kent State, display applications dominated the meeting, and two years later at the 1974 ILCC in Stockholm, the author's presentation was on materials for use infive different display types, i.e., dynamic scattering, Frkedericksz, twisted nematic, cholesteric memory, and cholestericnematic phase change display devices. Electrooptical liquid crystal display devices were now well established, and the twisted nematic device was obviously the superior one, based as it was upon a field effect in a pure nematic of positive dielectric anisotropy rather than upon the conductivity anisotropy, generated by ionic dopants in nematics of negative dielectric anisotropy, as in dynamic scattering displays. In 1970, the author and coworkers obtained a research grant from the UK Ministry of Defence for work on room temperature liquid crystal materials that would function well in electrooptic displays. When our attention was directed to liquid crystal materials of positive dielectric anisotropy rather than negative dielectric anisotropy, we were able to make rapid progress, drawing on the store of fundamental knowledge relating molecular structure to liquid crystal properties, and, as a consequence, following patenting, the synthesis and behavior of the 4alkyl and 4alkoxy4'cyanobiphenyls, designed for twisted nematic displays, were published in 1973 [48]. The history of the events leading up to the discovery of the cyanobiphenyls has been nicely documented by Hilsum [49], the originator of the research program under the author at the University of Hull and the coordinator of the associated programs on physics/devices at DRA, Malvern, and eventually on commercial production at BDH Ltd (now Merck UK Ltd). The advent of the cyanobiphenyls made available the materials for the manufacture
10
I
Introduction and Historical Development
of high quality, reliable liquid crystal displays, and in so doing provided the secure basis upon which today’s burgeoning electrooptical liquid crystal display device industry rests. The availability of these materials also spawned intense interest in other related families of materials, and during the later 1970s, the cyclohexane analogs of the biphenyls [50] and the pyrimidine analogs [S 11 became available, widening the choice of physical properties available to device engineers. The market place welcomed the first simple, direct drive twisted nematic liquid crystal (LC) displays, but in so doing, created a demand for devices capable of portraying more complex data, particularly important for the display of Chinese/Japanese characters. Multiplex driven liquid crystal displays with some capability in this direction required the exploration of more complex mixtures incorporating ester components. However, the limitations of multiplex addressing were quickly exposed, encouraging interest in new device forms and addressing techniques. One development was the discovery of the supertwisted nematic display [52, 531 and of addressing methods for twisted nematic displays using thin film transistors. These two possibilities have progressed forwards successfully, each having to overcome its own particular problems. For a survey, see the review by Schadt [S4]. As a result, in the late 1980s and early 1990s really excellent full color LC displays for direct view and for projection, involving where necessary high definition resolution, have come to the fore and dominate today’s marketplace. The devices have steadily improved in viewing angle, brightness, definition, and color quality, and the most up to date displays (supertwisted nematic and active matrix twisted nematic) are technological products of great quality which lead the liquid crystal display device
industry into the new millennium in a most confident mood. Work in other display areas has of course occurred. Through the seminal work of R. B. Meyer and the research of Clark and Lagerwall [ S 5 ] on surface stabilized ferroelectric liquid crystal devices based on chiral smectic C liquid crystal materials, the potential for ferroelectric devices has been fully explored in recent years. With their faster switching capability, they are attractive, and the difficulties over addressing schemes and the manufacture of ferroelectric displays will perhaps soon be overcome to give the marketplace a further liquid crystal device. In the search for novel materials, particularly new ferroelectric materials, new phase types were also discovered, notably the antiferroelectric phase [56] which, with tristable switching characteristics, also has potential for display use, possibly overcoming some of the difficulties with ferroelectric systems and providing a further display device of high quality. A further development in the display area concerns liquid crystal devices using inplaneswitching techniques, giving much improved viewing angle of the display [57, 581. Here the molecules switch across the surface of the display cell, and this technology is now being adopted by three companies. Plasma switching of other types of liquid crystal display is another interesting technology awaiting further development [591. Going back to the earlier 1970s, with the advent of the cyanobiphenyls and later the cyclohexane and pyrimidine analogs, not only was the display device industry provided with a wealth of novel, useful materials, but also those in fundamental research were given a range of stable, room temperature liquid crystal materials for study by a growing panoply of experimental and theoretical
4
The Third Phase from 1960 to the Present Time
techniques. Fundamental research therefore moved forward rapidly with very good readily available materials and the funding for such work that was released by the potential for technological applications. Publications of research papers and patents escalated, as mentioned earlier, and in the journals Molecular Crystals and Liquid Crystals and Liquid Crystals the field now has its own dedicated literature shop windows. The knowledge base in fundamental science was also extended greatly by the discovery in Chandrasekhar’s group [60] of liquid crystals formed by discshaped molecules. Capable of forming discotic nematic phases and a range of columnar phases, these materials currently attract much interest and technological applications for them are possible. This period also saw the growth of work on liquid crystal polymers both of the main chain and the side group varieties, and amongst others, the names of Blumstein and Finkelmann are associated with the first advances in this field which attracts many workers today (see [61,62]). Main chain liquid crystal polymers became known for their ability to form high tensile strength fibers and moldings, and side group liquid crystal polymers also have applications in optical components such as brightness enhancement films for display devices. Anisotropic networks, elastomers, and gels are also intriguing systems that have been reviewed by Kelly [63]. Fundamental studies of liquid crystals have also opened up much interest in metallomesogens, i.e., materials incorporating metal centers and capable of giving liquid crystal phases. Many materials ranging from the calamitic (rodlike) type to the disclike metallophthalocyanines are now known and with appropriate metal centers have interesting magnetic characteristics. Indeed, such have been the developments in
11
this area that a text devoted to the subject has been published [64]. If this section of this chapter hardly reads as a chronological history, this is because the last 15 years have seen so many developments in different directions that a simple pattern of evolution does not exist. Instead, developments have occurred in an explosive way, emanating outward from the core of fundamental knowledge acquired up to the end of the 1970s. We have already looked briefly at display applications, liquid crystals from discshaped molecules, liquid crystal polymers, and metallomesogens, but to follow all the developments of recent years radiating out from the central core is hardly possible in a short chapter like this. Only a few topics can be selected for brief mention, and if some areas of development are excluded through shortness of space, the author can at least feel confident that justice is done to them in the four volume Handbook of Liquid Crystals.
4.1 Lyotropic Liquid Crystals Activity here may have been less intense than i n the thermotropic liquid crystal area. Important developments began, however, through the work of the Swedish group under Ekwall, Fontell, Lawson, and Flautt, and the 1970s saw the publication by Winsor of his Rtheory of fused micellar phases [65] and of Friberg’s valuable book Lyotropic Liquid Crystals [66]. The importance of lyotropic liquid crystals in the oil industry, the food industry, and the detergent industry is high because of the need to know the exact behavior of amphiphile/water/oil systems and the role played by the micellar phases in the context of ef
12
I
Introduction and Historical Development
ficient extraction of oil from natural rocks and whether a system will flow, the processes of baking and the uses of emulsifiers, and the general efficiency of soaps and detergents. Especial mention should be made of the work of Tiddy and his studies of the complex phase relations involving lamellar, hexagonal, and viscous isotropic (cubic) micellar phases and his extension of the field to include zwitterionic systems (see, for example, [67]), as well as cationic and anionic amphiphiles. The importance of lyotropic liquid crystal concepts in relation to biological systems and the role played therein by liquid crystals must also be noted. A recent review of lyotropic liquid crystals by Hiltrop is to be found in [68].
4.2 Theory Theoretical treatments of liquid crystals such as nematics have proved a great challenge since the early models by Onsager and the influential theory of Maier and Saupe [34] mentioned before. Many people have worked on the problems involved and on the development of the continuum theory, the statistical mechanical approaches of the mean field theory and the role of repulsive, as well as attractive forces. The contributions of many theoreticians, physical scientists, and mathematicians over the years has been great  notably of de Gennes (for example, the Landaude Gennes theory of phase transitions), McMillan (the nematicsmectic A transition), Leslie (viscosity coefficients, flow, and elasticity), Cotter (hard rod models), Luckhurst (extensions of the MaierSaupe theory and the role of flexibility in real molecules), and Chandrasekhar, Madhusudana, and Shashidhar (pretransitional effects and nearneighbor correlations), to mention but some. The devel
opment of these theories and their significance are fully documented in the second edition of Chandrasekhar’s excellent monograph [69] entitled simply Liquid Crystals, and supported by earlier reviews in [70]. In many of the above studies, the GayBerne potential describing the interactions between anisotropic particles has been used, and this can be separated into repulsive and attractive parts, enabling studies of the roles played by each in mesophase formation. Computer simulation has been used to investigate GayBerne fluids, and phase diagrams giving isotropic, nematic, smectic, and crystalline phases have been produced (see, for example, Hashim et al. [71]). Simulations aimed ultimately at the prediction of the phase behavior of compounds of given molecular structure (the molecular dynamics approach), avoiding synthesis, is another area of growth, supported by the increasing power of computers, and results from studies of molecular mechanics, used in the determination of molecular structure and lowest energy conformations, are proving to be increasingly useful (see Chap. 111, Sec. 3 of this volume [72]).
4.3 Polymer Dispersed Liquid Crystals (PDLCs) and Anchoring The behavior of liquid crystals at surfaces is of course of great importance in normal flat panel electrooptical displays, and the subject of anchoring is an area of strong research activity, where the work of Barber0 and Durand is particularly noteworthy 1731. In recent years, PDLCs have attracted much attention because sheets consisting of droplets of nematic liquid crystal in an amorphous polymer matrix can be made by a number of techniques. The orientation in
4
The Third Phase from 1960 to the Present Time
the nematic droplets can be manipulated by electric fields, changing the appearance of the sheet from cloudy to clear, and opening up possibilities for electrically switchable windows and panels, and for large area signs and advertising boards. The high voltages initially required for the operation of such systems have been reduced considerably and problems of offaxis haze in the viewing panels have been diminished. The full impact of such switchable panels has not yet been realized, and some of the problems have focused attention on the fact that in such systems the liquid crystal is constrained in a confined geometry, and the ratio of surface contact area to bulk volume is high. This has led to important research on liquid crystals in confined geometries and a text on this subject by Crawford and Zumer was published in 1996 [74]. This valuable book embraces other important aspects of confinement than that in PDLC systems, and includes porous polymer network assemblies in nematic liquid crystals, polymer stabilized cholesterics with their implications for reflective cholesteric displays, liquid crystal gel dispersions, filled nematics, and anisotropic gels.
4.4 Materials and New Phases The applications of liquid crystals have unquestionably added incentive to the quest for new liquid crystal materials with superior properties such as viscosity, elastic constants, transition temperatures, and stability. In recent years this has catalyzed work on chiral materials as dopants for ferroelectric displays and for antiferroelectric materials with structures avoiding the number of potentially labile ester groups that were present in the original materials in which
13
antiferroelectric properties were discovered. The quest for new materials, whether driven by their potential for applications or simply by natural scientific curiosity about structure/property relations (i.e., as part of fundamental research programs) has always been and is today a vital part of the liquid crystal scenario. Indeed, it is often the case that the freethinking fundamental research on new materials opens the door to new applications or improvements in existing device performance. The fascination of the liquid crystal field in fact derives from this continuing materialsknowledgeapplications knockon effect. Importantly, it can occur in both directions. Thus studies of the significance of the position of the location of the double bond in a terminal alkyl chain led to the alkenylbicyclohexane systems [75],which today provide excellent materials for supertwisted nematic devices, and the work on ferroelectric materials led to the discovery of the antiferroelectric phase. A notable example of phase discovery was that of the twist grain boundary smectic A* phase (TGBA") by Goodby et al. in 1989 [76]. This new liquid crystal phase is a frustrated smectic in which the opposing tendencies to twist and be lamellar are accommodated through a regular array of dislocations, the possibility of which was predicted by de Gennes [77] in 1972 when he saw the analogous roles played by the director in an SmA phase and the magnetic vector potential in a superconductor. The analogous TGBC* phase is also now known. In the field of natural products, there is growing interest in the increasing range of carbohydrates that are being found to be liquid crystalline [78801, swinging interest back to the role of liquid crystals in biological systems, where recent studies of lyotropic mesomorphism in deoxyguanosine
14
I
Introduction and Historical Development
cyclic monophosphates [8 11 and of the significance of hydrogen bonding [82] and charge transfer [83] in low molar mass liquid crystals may be of further relevance. Studies of the liquid crystal properties of terminally [84] and laterally [85] connected di, tri and tetramesogens are probing the behavior in the area between monomeric liquid crystals and liquid crystal polymers. The intercalated smectic phase (SmA,,J has been found [84] and the somewhat related organosiloxanes [86] are proving to be most interesting materials with properties intermediate between low molar mass and polymeric liquid crystals, developed apparently through a microsegregation of the siloxane parts of the molecules into layers, leaving the organic moieties as appendages. Materials with both ferroelectric and antiferroelectric properties are provided and, significantly for applications, have almost temperature insensitive tilt angles and polarizations. Finally, a breakdown of the division between calamitic liquid crystals and the columnar phases formed by discshaped molecules has occurred through the discovery of materials that give both types of mesophase in single compounds. For example, some sixring, double swallowtailed mesogens reported by Weissflog et al. [87] exhibit the very interesting phase sequence SmCoblique columnarSmCnematic, combining not only calamitic and columnar phases, but also a reentrant SmC phase.
5
Conclusions
Thus in the above selected areas and in many others that cannot be mentioned specifically here, the development of knowledge and understanding of liquid crystal systems goes on in a manner that is quite prolific.
It remains to be said that much has happened in the short history of liquid crystals and that the field is vigorous in research today, both in the areas of fundamental science and application driven investigations. Saying that the position is healthy today may lead to the question: “What of the future?” Fortunately, the author is acting here in the capacity of historian, and it is not in the historian’s job description to predict the future. It will only be said that the future prospects for liquid crystals look healthy, but they will only be maintained so if fundamental research by scientists of imagination is adequately funded to enable the exploration of new ideas, new aspects, and new possibilities, because history does demonstrate that many of the discoveries significant for applications and technology derive from sound basic science or a sound knowledge of established basic science.
References H. Kelker, W. Hatz, Handbook of Liquid Crystals, VCH, Deerfield Beach, FL 1980. H. Kelker, P. M. Knoll, Liq. Cryst. 1989, 5 , 19. F. Reinitzer, Monatsh. Chem. 1888, 9, 42 1 ; for an English translation see Liq. Cryst. 1989,5,7. 0. Lehmann, Z. Phys. Chem. 1889,4,462. C . Mettenheimer, Corr: Blatt Verein gem. Arb. Forderung wissenschaftl. Heilkunde 1857, 24, 331. G. Valentin, Die Untersuchung der Pflanzenund der Tiergewebe im polarisierten Licht, Engelmann, Leipzig 1861. R. Virchow, VirchowsArch. path. Anat. Physiol. 1853, 6 , 57 1. L. Gattermann, A. Ritschke, Ber. Dtsch. Chem. Ges. 1890, 23, 1738. F. Meyer, K. Dahlem, Liebigs Ann. 1902, 320, 122. G. Tammann, Ann. Physik. 1901, 4 , 524; 1902, 8, 103; 1906, 19,421. W. Nernst, Z. Elektrochem. 1906, 12,431. R. Schenk, Kristalline Fliissigkeiten und piissige Kristalle, Engelmann, Leipzig 1905. D. Vorlander, Kristallinisch~iissige SubstanZen, Enke, Stuttgart 1905.
6 [14] F. Stumpf, Radioakt. Elektron. 1918, XV, 1 . 1151 C. W. Oseen, Die anisotropen Flussigkeiten, Borntrager, Berlin 1929. [I61 G. Friedel, Ann. Physique 1922, 18, 273. [ 171 D. Vorlander, Chemische Kristallographie der Flussigkeiten, Akadem. Verlagsanstalt, Leipzig 1924. [I81 P. J. Collings, Nature5 Delicate Phase o f M a t ter, Princeton U. P., 1990. [I91 General Discussion Meeting held by the Faraday Society, April 1933. [20] M. de Broglie, E. Friedel, C. R. 1923, 176, 738. [21] E. Friedel, C. R. 1925, 180, 269. [22] K. Herrmann, A. H. Krummacher, Z. Kristallogr. 1932, 81, 31; 1935, 92, 49. [23] K. Herrmann, Trans. Faraday Soc. 1933,29,27. 1241 E. Bose, Phys. Z. 1907, 8, 513; 1908, 9, 708; 1909,10,230;E. Bose, F. Conrat, Phys. Z. 1908, 9, 916. [25] C. W. Oseen, Trans. Faraday Soc. 1933,29,883. [26] H. Zocher, Trans. Faraday Soc. 1933,29, 1062; H. Zocher, G. Ungar, Z. Phys. Chem. 1938,110, 529; see also H. Zocher in Liquid Crystals and Plastic Crystals, Vol. I (Eds.: G. W. Gray, P. A. Winsor), Ellis Horwood, Chichester 1974, Chap. 3.1, p. 64. [27] F. C. Frank, Discuss. Faraday Soc. 1958, 59, 958. [28] P. Chatelain, C. R. 1948, 227, 136; Bull. Soc. Franc. Mineral. Crist. 1954, 77, 353; 1955, 78, 262; P. Chatelain, 0. Pellet, Bull. Soc. Franc. Mineral. Crist. 1950, 73, 154; J. Falgueirettes, C. R. 1952, 234, 2619. [29] C. Weygand, R. Gabler, J. Prakt. Chem. 1940, 155,332; C. Weygand, R. Gabler, J. Hoffmann, Z. Phys. Chem. 1941, 50B, 124; C. Weygand, R. Gabler, N. Bircon, J. Prakt. Chem. 1941,158, 26. [30] C. Wiegand, Z. Naturforsch. 1954, 3b, 313; 1955, Yb,5 16. [31] C. Robinson, Trans. Faraday Soc. 1956, 52, 571; C. Robinson, J. C. Ward, R. B. Beevers, Discuss. Faraday Soc. 1958,25,29. [32] C. Eaborn, N. H. Hartshorne, J. Chem. Soc. 1955,549. [33] G. H. Brown, W. G. Shaw, Chem. Rev. 1957,57, 1097. [34] W. Maier, A. Saupe, Z. Naturforsch. 1958, 13a, 564; 1959,14a, 882; 1960, 15a, 287. [35] D. Demus, L. Richter, C. E. Rurup, H. Sackmann, H. Schubert, J. Phys. (Paris) 1975, 36, C1349. [36] G. W. Gray, Molecular Structure and the Properties qf Liquid Crystals, Academic, London 1962. [37] J. Doucet, A . M . Levelut, M. Lambert, Phys. Rev. Lett. 1974,32, 30 1 ; J. Doucet, A. M. Levelut, M. Lambert, M. Liebert, L. Strzelecki, J. Phys. (Paris) 1975, 36, C113; J . J. Benattar,
References
15
A. M. Levelut, L. Liebert, F. Moussa, J. Phys. (Paris) 1979,40, C3115. [38] A. J. Leadbetter in The Molecular Physics of Liquid Crystals (Eds.: G. W. Gray, G. R. Luckhurst), Academic, London 1979, Chap. 13 and references therein and later in Thermotropic Liquid Crystals (Ed.: G. W. Gray), Wiley and Sons, New York 1987, Chap. 1 and references therein. [39] G. W. Gray, B. Jones, F. Marson, J. Chem. Soc. 1957, 393; D. Demus, G. Kunicke, J. Neelson, H. Sackmann, Z. Naturforsch. 1968,23a, 84; S . Diele, P. Brand, H. Sackmann, Mol. Cryst. Liq. Cryst. 1972,17, 84 and 163. [40] G. E. Etherington, A. J. Leadbetter, X. J. Wang, G. W. Gray, A. R. Tajbakhsh, Liq. Cryst. 1986, 1, 209. [41] D. Demus, A. Gloza, H. Hartung, I. Rapthel, A. Wiegeleben, Cryst. Res. Technol. 1981, 16, 1445. [42] A. M. Levelut, B. Donnio, D. W. Bruce, Liq. Cryst. 1997, 22, 753. [43] M. KICman, Liquid Crystals and Plastic Crystals, Vol. 1 (Eds.: G. W. Gray, P. A. Winsor), Ellis Horwood, Chichester 1974, Chap. 3.3, p. 76. [44] D. Dernus, L. Richter, Textures ofLiquid Crystals, VEB Deutscher Verlag fur Grundstoffindustrie, 1978. [45] G. W. Gray, J. W. Goodby, Smectic Liquid Crystals, Textures and Structures, Leonard Hill, Glasgow 1984. [46] P. E. Cladis, Phys. Rev. Lett. 1975, 35,48; P. E. Cladis, R. K. Bogardus, W. B. Daniels, G. N. Taylor, Phys. Rev. Lett. 1977,39,720. [47] D. Coates, G. W. Gray, Phys. Lett. 1973, 45A, 115; D. Armitage, F. P. Price, J. Appl. Phys. 1976,47,2735; H. Stegemeyer, K. Bergmann in Liquid Crystals of One and TwoDimensional Order (Eds.: W. Helfrich, A. Heppke), Springer, Berlin 1980, p. 161; H. Stegemeyer, T. H. Blumel, K. Hiltrop, H. Onusseit, F. Porsch, Liq. Cryst. 1986, I, 3; P. P. Crooker, Liq. Cryst. 1989, 5, 751. [48] G. W. Gray, K. J. Harrison, J. A. Nash, Electron. Lett. 1973, 9, 130; G. W. Gray, K. J. Harrison, J. A. Nash, J. Constant, J. S. Hulme, J. Kirton, E. P. Raynes, Liquid Crystals and Ordered Fluids, Vol. 2 (Eds.: R. S . Porter, J. F. Johnson), Plenum, New York 1973, p. 617. [49] C. Hilsurn in Technology of Chemicals and Materials f o r Electronics (Ed.: E. R. Howells), Ellis Horwood, Chichester 1991, Chap. 3. [50] R. Eidenschink, D. Erdmann, J. Krause, L. Pohl, Angew. Chem., lnt. Ed. Engl. 1977, 16, 100. [51] A. Boller, M. Cereghetti, M. Schadt, H. Scherrer, Mol. Cryst. Liq. Cryst. 1977, 42, 215. [52] C. M. Waters, E. P. Raynes, V. Brimmel, S.1. D. Proc. Jpn. Display 1983, 396.
16
I
Introduction and Historical Development
[53] T. J. Scheffer, J. Nehring,Appl. Phys. Lett. 1984, 45, 1021. [54] M. Schadt in Liquid Crystals (Eds.: H. Baumgartel, E. U . Frank, W. Grunbein; Guest Ed.: H. Stegemeyer), Springer, N. Y.1994, Chap. 6, p. 195. [55] N. A. Clark, S . T. Lagerwall, Appl. Phys. Lett. 1980,36, 899. [56] A. D. L. Chandani, E. Gorecka, Y.Ouchi, H. Takezoe, A. Fukuda, Jpn. J . Appl. Phys. 1988, 27, L729. [57] Society for Information Display, information Display 1996, 12 ( I 2), 13. [58] Eurodisplay '96 1997, 26 ( I ) , 16. 1591 S . Kataoka, International Lecture, Institute of Electrical and Electronic Engineers, Savoy Place, London, March 1997. [60] S . Chandrasekhar, B. K. Sadashiva, K. A. Suresh, Pramana 1977, 9 , 4 7 1. [61] Side Chain Liquid Crystal Polymers (Ed.: C. B. McArdle), Blackie, Glasgow 1989. [62] Liquid Crystalline Polymers (Ed.: C. Carfagna), Pergamon, Oxford 1994. [63] S . M. Kelly, Liq. Cryst. Today 1996, 6 (4), 1. [64] Metallomesogens (Ed.: J. L. Serrano), VCH, Weinheim 1996. [65] P. A. Winsor in Liquid Crystals and Plastic Crystals, Vol. 1 (Eds.: G. W. Gray, P. A. Winsor), Ellis Horwood, Chichester 1974, Chap. 5, p. 199. [66] S . Friberg, Lyotropic Liquid Crystals (Ed.: R. F. Could), Advances in Chemistry Series, American Chemical Society, Washington, DC 1976. [67] H. Morgans, G. Williams, G. J. T. Tiddy, A. R. Katritzky, G. P. Savage, Liq. Cryst. 1993, 15, 899. [68] K. Hiltrop in Liquid Crystals (Eds.: H. Baumgartel, E. U. Frank, W. Grunbein; Guest Ed.: H. Stegemeyer), Springer, N. Y.1994, Chap. 4, p. 143. [69] S . Chandrasekhar, Liquid Crystals, 2nd ed., Cambridge U. P., Cambridge 1992. [70] The Molecular Physics of Liquid Crystals (Eds.: G. R. Luckhurst, G. W. Gray), Academic, London 1979. [71] R. Hashim, G. R. Luckhurst, S . Romano, J. Chem. Soc., Furaday Trans. 1995, 21, 2141; G. R. Luckhurst, R. A. Stephens,R. W. Phippen, Liq. Cryst. 1990, 8, 45 1. [72] M. R. Wilson in Handbook qfLiquid Crystals, Vol. 1 (Eds.: D. Demus, J. W. Goodby, G. W. Gray, H. W. Spiess and V. Vill), WileyVCH, Weinheim 1998, p. 53.
1731 G. Barbero, G. Durand in Liquid Crystals in Complex Geometries (Eds.: G. P. Crawford, S . Zumer), Taylor and Francis, London 1996, Chap. 2, p. 21. [74] Liquid Crystals in Complex Geometries (Eds.: G. P. Crawford, S . Zumer), Taylor and Francis, London 1996. 1751 M. Schadt, R. Buchecker, K. Muller, Liq. Cryst. 1989, 5, 293. [76] J. W. Goodby, M. A. Waugh, S . M. Stein, E. Chin, R. Pindak, J. S . Patel, Nature, Lond. 1989, 337, 449; J. Am. Chem. Soc. 1989, 111, 8119; G. Strajer,R. Pindak,M. A. Waugh, J. W. Goodby, J. S . Patel, Phys. Rev. Lett. 1990, 64, 1545. [77] P. G. de Gennes, Solid State Commun. 1972, 10, 753. [78] J . W. Goodby, Mol. C y s t . Liq. Cryst. 1984, 110, 205; J. W. Goodby, J. A. Haley, G. Mackenzie, M. J. Watson, D. Plusquellec, V. Ferrieres, J . Muter. Chem. 1995, 5,2209. [79] H. Prade, R. Miethchen, V. Vill, J. Prakt. Chem. 1995,337,427;J . W. Goodby, J. A. Haley, M. J. Watson, G. Mackenzie, S . M. Kelly, P. Letellier, P. Code, G. Goethals, G. Ronco, B. Harmouch, P. Martin, P. Villa, Liq. Cryst. 1997, 22, 497. [80] M. A. Marcus, P. L. Finn, Liq. Cryst. 1988, 3, 38. [Sl] G. P. Spada, S . Bonazzi, A. Gabriel, S . Zanella, F. Ciuchi and P. Mariani, Liq. Cryst. 1997, 22, 341. 1821 K. Willis, J. E. Luckhurst, D. J. Price, J. M. Frechet, H. Kihara, T. Kato, G. Ungar, D. W. Bruce, Liq. Cryst. 1996, 21, 585 and references therein. 1831 K. Praefcke, D. Singer, A. Eckert, Liq. Cryst. 1994, 16, 53; B. Neumann, D. Joachimi, C. Tschierske, Liq. Cryst. 1997, 22, 509. [84] A. E. Blatch, I. D. Fletcher, G. R. Luckhurst, Liq. Cryst. 1995, 18, 80 1. [SS] J. Anderesch, C. Tschierske, Liq. Cryst. 1996, 21, 51; J. Anderesch, S . Diele, D. Lose, C. Tschierske, Liq. Cryst. 1996, 21, 103. 1861 M. IbnElhaj, A. Skoulios, D. Guillon, J. Newton, P. Hodge, H. J. Coles, Liq. Cryst. 1995, 19, 373. [87] W. Weissflog, M. Rogunova, I. Letkos, S . Diele, G. Pelzl, Liq. Cryst. 1995, 19, 541.
Chapter I1 Guide to the Nomenclature and Classification of Liquid Crystals John W Goodby and George W Gray
1 Introduction Nomenclature in liquid crystal systems is a nonsystematic language that is still, like any modern language, very much alive. Thus, many changes to currently acceptable terms, introductions of new notations, and deletions of outmoded notation have been made since the conception of the currently used nomenclature system. As the nomenclature system is in somewhat of a fluxional state it is not wise to assume that all definitions and accompanying notations are sacrosanct. Nevertheless, in some areas the topic of nomenclature has settled down into an internationally accepted, but unrecognized (by Scientific Societies) notation system, while in other areas, where research is still very active, changes to notation are still common. Members of the International Liquid Crystal Society (ILCS) and the International Union of Pure and Applied Chemists (IUPAC) are, however, attempting to create the first widely accepted naming system for liquid crystals. The descriptions and notations that follow are in agreement with the current proposals of the ILCS and IUPAC. Notation for liquid crystals really started with the naming of the nematic and smectic phases in the early 1920s by Friedel [l]. However, it was the discovery of the existence of a variety of smectic phases in the 1950s60s which lead Sackmann and Demus to propose the current lettering scheme for smectic liquid crystals [2]. Originally
only three smectic phases were defined, SmA, SmB and SmC, but more followed rapidly as new phases were discovered. The notation introduced by Sackmann and Demus was dependent on the thermodynamic properties of mesophases and their ability to mix with one another, thus the miscibility of a material of undefined phase type with a standard material of knowddefined mesophase morphology became the criterion for phase classification. Immiscibility, on the other hand has no special significance. Consequently all materials should have become standardized with those labelled by Sackmann and Demus. Shortly after the introduction of the notation system, confusion set in with the notations for the phases G and H becoming interchanged (which was later resolved by agreement between the Hull and Halle Research Groups [ 3 ] . In addition, the D phase had been introduced as a smectic phase but later it turned out to be cubic; the B phase was split into two, the tilted B and orthogonal B phases, which were later to be redefined as the B and G phases; two E phases were thought to exist, one being uniaxial and the other biaxial, that were later defined as all being biaxial; and of course there was the perennial problem as to whether or not a phase was a soft crystal or a real smectic phase. This latter debate finally gave rise to a change in notation for soft crystal phases, the Sm notation being dropped, but with the hangover of the B notation being used in both smectic and soft crystal phases.
18
I1
Guide to the Nomenclature and Classification of Liquid Crystals
As our understanding of smectic phases increased, and structural studies using Xray diffraction became more prevalent, there was an attempt to use crystallographic notation to describe the structures of smectic phases and, in addition, subscripts and superscripts were introduced to describe certain structural features, for example the subscript 2 was introduced to describe bilayer structures. By and large, however, there has been a general resistance to moving over to a full blown crystallographic notation system simply because there is a general feeling that a small change in structure within a miscibility class would lead to an unnecessary change in notation, consequently leading to complications and confusion. To some degree problems of notation did arise with the naming of columnar mesophases. Originally they were called discotic liquid crystals, and indeed they also acquired a crystallographic notation. Both of these notations have, however, fallen out of favor and the naming of the state has been redefined. As research in disclike systems remains relatively active, it is to be expected that further phases will be discovered, and as our understanding of the structures of these phases increases changes may be made to our current notation. Notation in chiral phases is in flux basically because many new phases have been recently discovered, for example, antiferroelectric phases, blue phases and twist grain boundary phases. Even the use of an asterisk to indicate the presence of chirality is a hotly debated topic because chiral systems have broken symmetries and sometimes helical structures. Thus the debate is an issue over which aspect of chirality does the asterisk represent  broken symmetry or helicity. Thus further developments and changes in notation may be expected to occur in this area in the future.
Another problem that exists in notation is the relationship between thermotropic and lyotropic nomenclature. In some cases continuous behavior has been seen between thermotropic and lyotropic mesophases suggesting that they should share the same notation; however, at this point in time this has not occurred. The notation scheme given below will be used wherever possible in the Physical Properties of Liquid Crystals; however for the reasons given above, readers should take care in its implementation, and they should also remember that the literature has suffered many changes over the years and so nomenclature used years ago may not tally with today’s notation.
2 General Definitions Liquid crystal state recommended symbol LC  a mesomorphic state having longrange orientational order and either partial positional order or complete positional disorder. Mesomorphic state  a state of matter i n which the degree of molecular order is intermediate between the perfect threedimensional, longrange positional and orientational order found in solid crystals and the absence of longrange order found in isotropic liquids, gases and amorphous solids. Liquid crystal crystal state.

a substance in the liquid
Crystal phase phase with a longrange periodic positional/translational order. Liquidphase  phase with no longrange periodic or orientational order. Mesophase or liquid crystal phase  phase that does not possess longrange positional ordering, but does have longrange
3 Structural Features
19
orientational order. A phase occurring over a defined range of temperature or pressure or concentration within the mesomorphic state.
core with a flexible chain attached at one end and a branched flexible chain, with branches of about the same length at the other.
Thermotropic mesophase  a mesophase formed by heating a solid or cooling an isotropic liquid, or by heating or cooling a thermodynamically stable mesophase.
Mesogenic dimers, trimers etc.  a mesogen consisting of molecules with two, three, or more linked mesogenic units usually of identical structure.
Lyotropic mesophase  a mesophase formed by dissolving an amphiphilic mesogen in suitable solvents, under appropriate conditions of concentration and temperature.
Sanidic mesogen  a mesogen composed of molecules with boardlike shapes.
Calamitic mesophase  a mesophase formed by molecules or macromolecules with rod or lathlike molecular structures. Columnar phase  phase that is formed by stacking of molecules in columns. Note that sugars, etc. are not necessarily discotic; discotic reflects a disclike molecular shape. Also phasmids are columnar, but not necessarily discotic. Mesogen (mesomorphic compound)  a compound that under suitable conditions of temperature, pressure and concentration can exist as a mesophase. Calamitic mesogen  a mesogen composed of molecules or macromolecules with rod or lathlike molecular structures. Discotic mesogen  a mesogen composed of relatively flat, disc or sheetshaped molecules. Pyramidal or bowlic mesogen  a mesogen composed of molecules derived from a semirigid conical core. Polycatenary mesogen  a mesogen composed of molecules having an elongated rigid core with several flexible chains attached to the end(s). Swallowtailed mesogen  a mesogen composed of molecules with an elongated rigid
Amphiphilic mesogen  a compound composed of molecules consisting of two parts with contrasting character, which may be hydrophilic and hydrophobic, that is lipophobic and lipophilic. Amphotropic material  a compound which can exhibit thermotropic as well as lyotropic mesophases.
3
Structural Features
Molecules of liquid crystalline compounds are subdivided into the central core (mesogenic group), the linking groups, and lateral groups as well as terminal groups, depending on whether or not the groups lie along the long axis of the molecule. In relation to disclike molecules, the central rigid region is called the core and the outer region the periphery; linking groups have the same definition as for calamitic rodlike systems. The term mesogenic means that the structure is generally compatible with mesophase formation. A compound that forms real mesophases is however mesomorphic.
20
I1 Guide to the Nomenclature and Classification of Liquid Crystals
4 Polymeric Liquid Crystals Liquid crystalline polymers are classified either as mainchain liquid crystalline polymers (MCLCP), as polymers with mesogenic side groups (SGLCP), or as liquid crystalline elastomers.
5 Notation of Thermotropic Liquid Crystalline Properties To denote one phase transition, the abbreviation T together with an index is used (for example, TNIfor a nematicisotropic transition; TcA for a smectic Csmectic A transition). The complete transition sequence is characterized by the description of the solid state (Sec. 5. l ) , the liquid crystalline transitions (Sec. 5.2) and the clearing parameter (Sec. 5.3). The phase symbol is followed by the upper temperature limit as measured during the heating and not during the cooling cycle. Crystal types should be arranged in an ascending order of transition temperature. If a transition temperature of a liquid crystalline phase is lower than the melting point, this phase only occurs monotropically. Monotropic transitions appear in round brackets.
In this context, square brackets mean virtual transitions. Examples:
Cr 34 N 56 I designates a compound melting at 34 "C into the nematic phase; at 56 "C
it changes into the isotropic phase; normal behavior.
Cr 56.5 (SmA 45) I designates a compound melting at 56.5 "C into the isotropic phase. Below 45 "C, a monotropic A phase exists. Cr 120 B 134 I [N 56 I,] designates a compound melting at 120 "C into the crystal B phase. At 134°C the isotropic phase is formed. The virtual nematic clearing point of 56°C is one obtained by extrapolation from mixtures. Cr, 78 Cr, 212 N ? Idecompdesignates a compound with a crystal to crystal transition at 78 "C and a melting point of 212 "C to a nematic phase. The clearing point is unknown because decomposition takes place. Cr, 112 (Cr, 89) I designates a material with a metastable crystal phase formed on cooling the isotropic melt slowly and having a lower melting point than the stable crystal phase.
5.1 Description of the Solid State Cr Cr, g Tg
crystalline phase second crystalline phase glassy state glasstransition temperature
5.1.1 Description of Soft Crystals The following phases should just be called B, E, etc. (i.e. retaining their historic classification, but losing their smectic code letter Sm) because they are no longer regarded as true smectics as they have long range positional order. In fact they are soft or dis
5
Notation of Thermotropic Liquid Crystalline Properties
ordered crystals. The single letter notation (B, E, etc.) is preferred to B,,, E,, etc. B crystal B E crystal E Emod crystal E phase with modulated inplane structure G crystal G H crystal H J crystal J K crystal K
Tilted Chiral Soft Crystal Phases A superscript asterisk (*) is used throughout to denote the presence of chirality.
J*
tilted chiral crystal H* tilted chiral crystal G* tilted chiral crystal K* tilted chiral crystal
J H G K
Chiral Orthogonal Soft Crystal Phases A superscript asterisk (*) is used throughout to denote the presence of chirality. B* chiral orthogonal crystal B phase
E* chiral orthogonal crystal E phase
5.2 Description of the Liquid Crystalline Phases 5.2.1 Nematic and Chiral Nematic Phases n N N* Nu N, also NZ
21
BP blue phases. These are designated BPI, BP,,, BP,,, or BP,,, and BPS.
5.2.2
Smectic Liquid Crystals
Use Sm for smectic instead of S (unless spelt out), this avoids subscripts and double subscripts SmA
Smectic A SmA, monolayer SmA, bilayer SmA, interdigitated bilayer SmA modulated bilayer SmB or Smectic B; hexatic B SmB,,, (SmB preferred) SmC Smectic C SmC monolayer SmC, bilayer SmC, interdigitated bilayer S m c modulated bilayer SmC,,, alternating tilt phase see smectic 0 SmF Smectic F SmI Smectic I SmM Smectic M  not found common use so far SmO Smectic 0  not found common use so far. Use carefully in relation to smectic Calt and antiferroelectric smectic C* phase SmO and SmM should be defined in the text Intercalated mesophases take the subscript c, e.g., SmA,. Biaxial variants of uniaxial smectic phases take the subscript b, e.g., SmA,.
director nematic chiral nematic (cholesteric) uniaxial nematic phase biaxial nematic phase (sanidic phase)
5.2.3 Chiral Smectic Liquid Crystals
infinite pitch cholesteric, i.e. at a helix inversion or compensation point
Usually given the notation * to indicate the presence of chirality, e.g., SmA*, SmC*.
22
I1 Guide to the Nomenclature and Classification of Liquid Crystals
Twist Grain Boundary Phases (TGB) Orthogonal TGB Phases TGBA* structure based on the smectic A phase. The phase can be either commensurate or incommensurate depending on the commensurability of the helical structure with respect to the rotation of the smectic A blocks in the phase. TGBB* proposed structure based on a helical hexatic B phase.
Tilted TGB Phases TGBC phase poses the following problems for nomenclature: TGBC where the normal smectic C* helix is expelled to the screw dislocations. TGBC* phase where the blocks have a local helix associated with the out of plane structure. Possibly too early to define notation yet; therefore spell out notation in text.
Tilted Chiral Phases SmC* chiral C phase SmC2 infinite pitch smectic C*  ferroelectric SmCg unwound antiferroelectric phase occurring at higher temperature, and above a ferroelectric SmC* phase in a phase sequence SmC: ferrielectric phases that occur on cooling ferroelectric C* phases S m C i antiferroelectric C* phase Try not to use a, p and y notations, simply spell out the phase type, e.g. ferrielectric SmC* phase, or SmC* (ferri). The above notations may also be applied to SmI* and SmF* phases as and when required  for example, S m I i is an antiferroelectric I* phase.
Orthogonal Phases SmA* SmB*/ SmBte,
chiral orthogonal smectic A chiral orthogonal hexatic smectic B phase (SmB* preferred)
Analogous Achiral Systems Here, antiferroelectriclike structures are often observed, i.e. zigzag layer ordering. The following designation should be used and reference to antiferroelectriclikeordering should be suppressed: SmC,,, alternating tilt smectic C phase see also smectic 0 for crossreferencing
Unknown Phases Label as SmX,, SmX,, etc.
5.2.4
Columnar Phases
nematic discotic phase hexagonal discotic ordered hexagonal columnar phase cO1ho disordered hexagonal columnar cO1hd phase COlro ordered rectangular columnar phase disordered rectangular columnar cO1rd phase Colt tilted columnar phase phasmidic phase, but Col is preferred 4J
ND
Col,
For nematic phases  spell out positive and negative birefringent situations in the text. In addition spell out if the nematic phase is composed of single molecular entities or short columns which exist in a disordered nematic state. Care should be taken when using the term discotic; columnar is preferred.
Unknown Discotic Phases Col,, Col,, etc.
7
5.2.5 Plastic Crystals Rotationally (3D) disordered crystals that may be derived from globular molecules leading to isotropic phases. This classification does not apply to crystal smectic phases composed of elongated molecules, although these could be described as anisotropic plastic crystals.
5.2.6 Condis Crvstals
References
23
6 Stereochemistry unknown chirality
(#>
One Chiral Centre ( R or s,
(S) chiral (S) (R) chiral (R) (S)/(R) racemate
Two Chiral Centres
I
Crystals in which the positional and conformational order in the packing of molecules arranged in parallel is lost to some degree.
5.2.7
Cubic
Cubic thermotropic liquid crystalline phases are designated Cub. CubD
Cubic D phase
5.2.8 Reentrants Use the same notation as for nematic or other appropriate phase with subscript reentrant, i.e., N,, or SmC,, or Col,,,.
5.3 Description of the Clearing Parameters I isotropic, standard case Idecomp decomposition at clearing temperature Ie extrapolated temperature
This situation is more complex and depends upon whether the two centres are the same or different. If they are the same the notation should be: chiral (S,S or R,R); or for racemic materials (S,S or R,R); mesocompounds (optically inactive by internal compensation should be denoted as (S,R Or
7
RyS)*
References
[ I ] G. Friede1,Ann. Physique 1922, 18, 272. [2] H. Sackmann, D. Demus, Mol. Cryst. Liq. Cryst. 1966, 2, 8 1 . [3] D. Demus, J. w. Goodby, G. W. Gray, H. Sackmann, Mnl. Cryst. Liq. Cryst. Lett. 1980,56,311.
This Page Intentionally Left Blank
Chapter I11 Theory of the Liquid Crystalline State
1 Continuum Theory for Liquid Crystals Frank M. Leslie
1.1 Introduction Continuum theory for liquid crystals has its origins in the work of Oseen [ 11 and Zocher [2] i n the 1920s. The former essentially derived the static version of the theory for nematics that has been used extensively in device modelling, while the latter successfully applied it to Frkedericksz transitions [3]. Later Frank [4] gave a more direct formulation of the energy function employed in this theory, and stimulated interest in the subject after a period of relative dormancy. Soon thereafter Ericksen [5] set the theory within a mechanical framework, and generalized his interpretation of static theory to propose balance laws for dynamical behaviour [6]. Drawing upon Ericksen’s work, Leslie [7] used ideas prevalent in continuum mechanics to formulate constitutive equations, thus completing dynamic theory. This continuum theory models many static and dynamic phenomena in nematic liquid crystals rather well, and various accounts of both the theory and its applications are available in the books by de Gennes and Prost [8], Chandrasekhar [9], Blinov [ 101 and Virga [ 1 I], and also in the reviews by Stephen and Straley [12], Ericksen [13], Jenkins [14] andLeslie [15]. Given this suc
cess of continuum theory for nematics, much current interest in continuum modelling of liquid crystals now centres upon appropriate models for smectic liquid crystals, liquid crystalline polymers and (to a lesser extent) lyotropics. Otherwise, interest in nematics is largely confined to studies of behaviour at solid interfaces, this including discussions as to whether or not one should include an additional surface term in the FrankOseen energy as proposed by Nehring and Saupe [ 161, although there has also been some activity into the modelling of defects, particularly using a modified theory proposed recently for this purpose by Ericksen [ 171. In this section I aim to describe in some detail continuum theory for nematics, and also to draw attention to some points of current interest, particularly surface conditions and surface terms. At this juncture it does seem premature to discuss new developments concerning smectics, polymers and lyotropics, although a brief discussion of an equilibrium theory for certain smectics seems appropriate, given that it relates to earlier work on this topic. Throughout, to encourage a wider readership, we endeavour to employ vector and matrix notation, avoiding use of Cartesian tensor notation.
26
1
Continuum Theory for Liquid Crystals
1.2 Equilibrium Theory for Nematics
tions (Eq. 2) and (Eq. 3 ) lead to
1.2.1 The FrankOseen Energy Continuum theory generally employs a unit vector field n(x) to describe the alignment of the anisotropic axis in nematic liquid crystals, this essentially ignoring variations in degrees of alignment which appear to be unimportant in many macroscopic effects. This unit vector field is frequently referred to as a director. In addition, following Oseen [ 11 and Frank [4], it commonly assumes the existence of a stored energy density W such that at any point W = W(n, Vn)
(1)
the energy is therefore a function of the director and its gradients at that point. Since nematic liquid crystals lack polarity, n and n are physically indistinguishable and therefore one imposes the condition that W(n, Vn) = W(n, Vn)
(2)
and invariance to rigid rotations requires that W(n, Vn) = W(fn, f V n e T )
(3)
e
where is any proper orthogonal matrix, the superscript denoting the transpose of the matrix. While the above suffices for chiral nematics or cholesterics, for nonchiral nematics, invariably referred to simply as nematics, material symmetry requires that (Eq. 3) be extended to W(n, Vn) = W(Qn, QVnQT) I


(4)
where the matrix Q belongs to the full orthogonal group, t6e function is therefore isotropic rather than hemitropic. Oseen and Frank both consider an energy function that is quadratic in the gradients of the director n, in which case the condi
2W = Kl(div n)2 + K2(n curl n + q)2 + K, I n x curl n I + (K2+ K4) . div[(n . grad)n  (div n)n] (5 1 where the K s and q are constants. The above is the form appropriate to cholesterics or chiral nematics, q being related to the natural pitch of the characteristic helical configurations found in these materials, through p =2dq.
(6)
For ordinary nematics, however, the conditions (Eq. 2) and (Eq. 4) yield 2W = K,(div n)2 + K2(n curl n)2 + K3 I n x curl n l + (K2+ K4) . div[(n . grad)n  (div n)n] +
(7)
the coefficient q necessarily zero for such materials. This latter energy can alternatively be expressed as 2W = (K,  K2  K4)(div n)2 + K2tr(VnVnT)+ K , t ~ ( v n ) ~ (8) + ( K 3  K,)(n. grad)n. (n . grad)n
trb and 4 denoting the trace and transpose of the matrix 4, respectively. This latter form can be more convenient for some purposes. It is common to refer to the constants K,, K2 and K3 as the splay, twist and bend elastic constants, respectively, while the K4 term is sometimes omitted since the last term in the form (Eq. 7) can clearly be expressed as a surface integral. Given that nematics tend to align uniformly with the anisotropic axis everywhere parallel, Ericksen [ 181 argues that this must represent a state of minimum energy, and thus assumes that W(n, Vn) > W(n, 0), Vn
f
0
(9)
and as a consequence the coefficients in (Eq. 7) or (Eq. 8) must satisfy
> 0, K2 > 0, K , > 0, 2K, > K2 + K4 > 0, K2 > K4 Kl
(10)
1.2 Equilibrium Theory for Nematics
Jenkins [ 191 discusses the corresponding restrictions placed upon the energy (Eq. 5 ) by assuming that the characteristic twisted helical configuration represents a minimum of energy. To conclude this section we note an identity derived by Ericksen [6] from the condition (Eq. 3) by selecting
p=l
+&R, RT=R
being the unit matrix and E a small parameter. With this choice one can quickly show that
27
straint div 6x = 0
(15)
and of course the variations 6n and An are constrained by
( 1 6)
Gn.n=An.n=O
due to n being of fixed magnitude. Through consideration of an arbitrary, infinitesimal, rigid displacement in which An is zero, it quickly follows from (Eq. 13) that
I Fdv +
t ds = 0
(17)
S
V
which of course expresses the fact that the resultant force is zero in equilibrium. Similarly, consideration of an arbitrary, infinitesimal, rigid rotation o,in which a result required below. In the above, the notation a * b represents the 3 x 3 matrix with (i, j)thelement ai bj.
6 Wdv = ( F .6x + G . An) dv V
(13)
S
where An = 6n + (6x . grad)n
(18)
yields from (Eq. 13) following rearrangement of the triple scalar products V
The approach adopted by Ericksen [5] to equilibrium theory for both nematic and cholesteric liquid crystals appeals to a principle of virtual work, which for any volume V of material bounded by surface S takes the form
+I (t.6x+s.An)ds
An=oxn
j(x x F +n xG)dv+j(x x t +nxs)ds =0
1.2.2 A Virtual Work Formulation
V
6x=oxx,
(14)
F denotes body force per unit volume, t surface force per unit area, and G and s are generalized body and surface forces, respectively. With the common assumption of incompressibility the virtual displacement 6x is not arbitrary, but is subject to the con
S
(19) which one interprets as a statement that the resulting moment is zero in equilibrium. Hence (Eq. 19) relates the generalized forces G and s to the body and surface moments K and 1, respectively, through K=nxG,
1=nxs
(20)
which allows the determination of the generalized body force. By first expressing the left hand side of the statement of virtual work (Eq. 13) as using (Eq. 15)
6 j Wdv=j(6W+(6x.grad)W)dv V
(21)
V
this taking account of the change of volume in the virtual displacement, and then reorganizing the resultant volume integral so that it has a similar format to the right hand side of (Eq. 13), it is possible to obtain expressions for the surface force t and the gen
28
1
Continuum Theory for Liquid Crystals
eralized surface force s , and also two equations required to hold in equilibrium [5]. Denoting by v the unit outwards normal to the surface S and bearing in mind the constraints (Eq. 15) and (Eq. 16), one finds from the surface integrals
aw + T"v, TS = Vn T aVn s = pn + S"v, Sx= aw aVn
t = pv
In an isotropic material the induced magnetization is necessarily parallel to the field and the couple is zero, but for a nematic or cholesteric liquid crystal the magnetization can have an anisotropic contribution of the form
x,land xLdenoting the diamagnetic suscept
~
ibilities when n and H are parallel and perpendicular, respectively. As a consequence a body moment can occur given by
~
and also from the volume integrals
F  grad p + divTx=0,
K = xan Hn x H
aw G  + div Ss= yn, an
and it immediately follows from the first of equations (Eq. 20) that
with p an arbitrary pressure due to incompressibility, and p and y arbitrary scalars due to the director having fixed magnitude. In equations (Eq. 23) the divergence applies to the second of the indices of the matrices _T" and S". The former of (Eq. 23) clearly represents the point form of the balance of forces (Eq. 17), while the latter can be shown to be the point form of the balance of moments (Eq. 19), this requiring some manipulation involving the identity (Eq. 12).
G =xo,n.HH
While the action of gravity upon a liquid crystal is identical to that on other materials, external magnetic and electric fields have a rather different effect upon these anisotropic liquids than they do on isotropic materials. Both can give rise to body forces and moments as is to be expected from rather simple arguments common in magnetostatics and electrostatics. To fix ideas, consider a magnetic field H which induces a magnetization M in the material, and this in turn gives rise to a body force F and a body moment K, given by
F = (M . grad)H, K = M x H
(24)
(27)
any contribution parallel to the director being simply absorbed in the scalar y in equations (Eq. 23). In general the anisotropy of the diamagnetic susceptibility is positive, but it is also rather small. Consequently one can ignore the influence of the liquid crystal upon the applied field. Similar expressions arise for an electric field E, this creating an electric displacement D of the form
xa
D = E ~ +E&,n . En,
1.2.3 Body Forces and Moments
(26)
E, =

(28)
and denoting the corresponding dielectric permittivities, which gives rise to similar body forces and moments. However, as Deuling [20] points out, there can be one important difference between the effects of magnetic and electric fields upon liquid crystals, in that an electric field can give rise to significant permittivities, and thus one must allow for the influence of the liquid crystal upon the applied field by employing the appropriate reduced version of Maxwell's equations. Associated with a magnetic field there is an energy y =  1M . H (29) 2
1.2 Equilibrium Theory for Nematics
and if one regards the energy Was simply a function of the director n and position x, then one can write
the former using the fact that in equilibrium the magnetic field is irrotational. However, if the field applied is dependent upon the director, as can occur for an electric field, then (Eq. 30) are not valid.
1.2.4 The Equilibrium Equations The equations (Eq. 23) representing balance of forces and moments constitute six equations for four unknowns, two components of the unit vector n and the scalars p and ’/. However, this apparent overdeterminacy does not materialize if the external body force and moment meet a certain requirement [5]. To see this combine the two equations as follows
29
which can be written in forms more convenient for particular problems as discussed by Ericksen [21]. Frequently one selects a particular form for the director n so that it is immediately a unit vector, this representation invariably involving two angles 8 and $ so that
Initially for purposes of illustration it is convenient to restrict 8 and $ to be functions of a single Cartesian coordinate, say z, and consider the application of an external magnetic field H, so that (Eq. 30) holds. In this event
where the prime denotes differentiations with respect to z. Employing the chain rule, one obtains (37) and thus
F + VnTG grad p + div T S +VnrdivSs Vn r a w  0 _____
an
(31)
and by appeal to equations (Eq. 22) this reduces to
F + VnTG =
[email protected] + W)
w
w=po

~
an
~
an
r
(33)
where p o is an arbitrary constant pressure, and thus the equation for the balance of forces integrates to give the pressure, removing the potential overdeterminacy. Also the balance of moments becomes d i v 9  aw + av yn
ef.
(32)
clearly limiting the body force and moment. However, when (Eq. 30) applies, the above at once yields
P+
with similar expressions for the derivatives with respect to $ and Combining the above it follows that
(34)
and similarly
7
30
I
Continuum Theory for Liquid Crystals
Hence, employing Eqs. (34) and (35) the former can be rewritten as
For the general case when 8 and @ are arbitrary functions of Cartesian coordinates, essentially a repetition of the above leads to
which are clearly more convenient to use than (Eq. 34). In addition, as Ericksen [21] also shows, the above reformulation can be extended to include curvilinear coordinate systems (y , y2, y 3 ) introduced by
,
x = X ( Y l ? Y 2 ,Y 3 ) .
(43)
Denoting the Jacobian of this transformation by
(44)
W = JV = j ? ( y i , 8, $1
(45)
where yi is short for y l , y2, and y 3 , and similarly for the partial derivatives, one can show that (Eq. 34) can be recast as
where
(47) and the repeated index is summed over the values 1, 2 and 3. Rather clearly Eqs. (41), (42) and (46) are appropriate forms of the EulerLagrange equations for the integral
/<w  v)dv
(48)
V
this the formulation of equilibrium theory initially adopted by, for example, Oseen [ 11 and Frank [4]. For electric fields, certainly for the special cases generally considered, the outcome is rather similar in that the equation for the balance of forces integrates to give the pressure, and one can recast that for balance of moments in the same way as above. However, a general treatment does not appear to be available.
1.2.5 Boundary Conditions In general the choice of boundary conditions for the alignment at a liquid crystalsolid interface is one of two options, either strong or weak anchoring [8]. Strong anchoring as the term suggests implies that the alignment is prescribed at the boundary by a suitable prior treatment of the solid surface and remains fixed in the presence of competing agencies to realign it. Most commonly this fixed direction is in the plane of the surface (planar) or it is perpendicular (homeotropic), but it need not be so. Weak anchoring, first proposed by Papoular and Rapini [22] assigns an energy to the liquid crystalsolid interface, and assumes a balance between the moment or torque in the liquid crystal from the FrankOseen energy and that arising from the interfacial energy. Denoting by w this latter energy per unit area, the sim
1.2
plest assumption is a dependence upon the director n and a fixed direction n , at the interface, so that w = w(n,
n,)
(49)
Equilibrium Theory for Nematics
31
than previously in order to model these effects adequately, and they measure some relevant parameters, Sergan and Durand [28] describing further measurements.
but equally one can have
w = w(n, Y ,z)
(50)
where Y is again the unit normal and z a fixed unit vector on the surface. By essentially a repetition of the approach of section 2, Jenkins and Barratt [23] show that this leads to the boundary condition
aw + aw = An an
Y
aVn
1.2.6 Proposed Extensions Some 25 years ago, Nehring and Saupe [ 161 proposed that one should add terms linear in second gradients of the director to the FrankOseen energy, this ultimately entailing the inclusion of a single additional term, namely

K , div((div n)n)
W again denoting the FrankOseen energy and A an arbitrary scalar. If one introduces the representation (Eq. 35), it follows that W = W(0, $, V0, V$>,
w = ~ ( 8$1, (52)
and using the methods of the previous section the boundary condition (Eq. 51) becomes
Frequently these boundary conditions can be reduced to equations for 8 and $ at the interface by eliminating the derivatives of 8 and $, after they have been obtained from the equilibrium equations. More recently, however, it has become apparent that the situation can be more complex with the realization that surface anchoring in nematics can be bistable, as found by Jerome, Pieranski and Boix [24] and Monkade, Boix and Durand [25]. Shortly thereafter, Barberi, Boix and Durand [26] showed that one can switch the surface alignment from one anchoring to the other using an electric field. As Nobili and Durand [27] discuss, one must consider rather more complex forms for the surface energy
(54)
which clearly proves to be a surface term in the sense that the volume integral integrates to give a surface integral over the boundary. On the grounds of a microscopic calculation they argue that the coefficient in (Eq. 54) is comparable in magnitude to the other coefficients in the FrankOseen energy, and so the term should be added. More recently Oldano and Barbero [29] include such a term and consider the variational problem for static solutions to conclude that in general there are no continuous solutions to this problem, since it is not possible to satisfy all of the boundary conditions that arise in the variational formulation. These are of two types, one corresponding to weak anchoring as described in the previous section, but the other lacking a physical interpretation. This has given rise to some controversy, initially with Hinov [30], but later with contributions from Barbero and Strigazzi [31], Barbero, Sparavigna and Strigazzi [32], Barbero [33], Pergamenshchik [34] and Faetti 135,361. In general the arguments rest solely upon a resolution of the variational problem, and mostly favour the inclusion of higher order derivatives in the bulk elastic energy in different ways to overcome this difficulty. More
32
1 Continuum Theory for Liquid Crystals
recently Barbero and Durand [37] relate this additional term to temperatureinduced surface transitions in the alignment, and Barberi, Barbero, Giocondo and Moldovan [38] attempt to measure the corresponding coefficient. Also Lavrentovich and Pergamenshchik [39] argue that such a term explains their observations of stripe domains in experiments with very thin films, and also provide a measurement of the coefficient. While these latter developments relating to experimental observations are of interest, it is rather early to draw any conclusions. A further recent innovation is due to Ericksen [ 171 who proposes an extension to the FrankOseen theory in order to improve solutions modelling defects. To this end he incorporates some variation in the degree of alignment or the order parameter, and therefore proposes an energy of the form
W = W(s,n, Vs, Vn)
(55)
where n is again a unit vector describing alignment and s is a scalar representing the degree of order or alignment. By allowing this scalar to tend to zero as one approaches point or line defects, it is possible to avoid the infinite energies that can occur with the FrankOseen energy. Some account of analyses based on this development are to be found in the book by Virga [ 111.
1.3 Equilibrium Theory for Smectic Liquid Crystals 1.3.1 An Energy Function for SmC Liquid Crystals The first to give serious thought to continuum theory for smectics appears to have been de Gennes’ group at Orsay [8]. Amongst other things they present an ener
gy function for SmC liquid crystals [40], albeit restricted to small perturbations of planar layers. More recently, however, Leslie, Stewart, and Nakagawa [41] derive an energy for such smectics which is not limited to small perturbations, but which is identical to the Orsay energy when so restricted [42]. Below our aim is to present this energy, and show its relationship to that proposed by the Orsay group. One can conveniently describe the layering in smectic liquid crystals by employing a density wave vector a, which following Oseen [43] and de Gennes [8] is subject to the constraint curl a = 0
(56)
provided that defects or dislocations in the layering are absent. To describe SmC configurations de Gennes adds a second vector c perpendicular to a and in the direction of inclination of the tilt of alignment with respect to a. Leslie, Stewart and Nakagawa [41] invoke two simplifications to reduce mathematical complexity that clearly restrict the range of applicability of their energy, but equally appear very reasonable in many cases. They firstly assume that the layers, although deformable, remain of constant thickness, and also that the angle of tilt with respect to the layer normal remains constant, the latter excluding thermal and pretransitional effects. With these assumptions there is no loss of generality in choosing both a and c to be unit vectors, identifying a with the layer normal, the constraint (Eq. 56) still applying. As in nematic theory one assumes the existence of an elastic energy W which here is a function of both a and c and their gradients, so that
W = W(a, c, Va, Vc)
(57)
The absence of polarity in the alignment implies that the energy is independent of a si
33
I .3 Equilibrium Theory for Smectic Liquid Crystals
multaneous change of sign in a and c, and thus W(a, c, Va, Vc) = W(a, c, Va, Vc) (58) Invariance to rigid rotations adds the requirement that W(a, c, Va, VC) = W(ca, pc, pVaeT,i_'VcpT)
(59)
c.
for all proper orthogonal matrices While these conditions suffice for chiral materials, for nonchiral materials symmetry requires that (Eq. 59) is extended to include all orthogonal matrices. Assuming a quadratic dependence upon gradients one finds for nonchiral materials that [44] 2W = K:(trVa), + K;(c . Vat), + 2K",trVa)(c . Vac) + K?(trVc), + KStr(VcVcT) + KS(VCC.VCC) + 2Ki(Vcc. Vca) + 2Krc(trVc)(c . Vac) + 2K,""(trVc)(trVa)

(60)
(trva)',
(61)
partly on the grounds that the above suffices for present purposes. For chiral materials Carlsson, Stewart and Leslie [45] show that one must add two terms 2K,"b. Vac,
2Kgb. Vca
(62)
plus an additional surface term associated with div b, where b completes the orthonorma1 triad with the vectors a and c, so that b=axc
2 W = A, ( b . curl c ) +~A2 (c .curl b)* + 2AII (b . curl c)(c . curl b)
+ B1(div b), + B2(div c),
I'
b+c.curlc)
[:
+2B13(divb) (b.curl b + c . c u r l c ) +2Cl(div c)(b.curl c ) +2C2(div c)(c.curl b)
1
(64)
As Carlsson, Stewart and Leslie [42] discuss, the terms associated with the coefficients A *, A, ,, B I , B, and B, represent independent deformations of the uniformly aligned planar layers, the remaining terms being coupling terms. Also, as the notation for the coefficients anticipates, this expression reduces to the Orsay energy [40] when one considers small perturbations of uniformly aligned planar layers. The coefficients in the two energies (Eq. 60) and (Eq. 64) are related by
,
the coefficients being constants. This expression omits three surface terms associated with tr(Vc),  (trVcl2, tr(Va)' tr(VcVa)  (trVa)(trVc),
normal, while the former implies a nonplanar equilibrium configuration, and consequently is generally omitted. One can of course employ any two members of the orthonormal triad a, b and c to describe smectic configurations, and employing b and c the energy (Eq. 60) becomes [44]
(63)
The latter of (Eq. 62) describes the characteristic twist of the c director about the layer
K;=A,,, K,"=2AI, +AIz+A21 +B,BI, 2Kz=(2A1,+2A,l+B,) K;'= B2  B,, K$ = B,, Kg = B ,  B,, K$ = B I 3 Kr'= C , + Cz, K,"'= C2 (65) as Leslie, Stewart, Carlsson and Nakagawa [44] demonstrate.
1.3.2 Equilibrium Equations Adopting a similar approach to that by Ericksen for nematics, Leslie, Stewart and Nakagawa [41] assume a principle of virtu
34
Continuum Theory for Liquid Crystals
1
a1 work for a volume V of smectic liquid crystal bounded by a surface S of the form
6 Wdv = ( F . 6 x + G U.Aa+G' .Ac) dv V
V
+ j (t .6x + s" . Aa + sc . Ac) ds S
(66)
where
t = pv
Aa = 6a + (6x . grad)a, Ac = 6c + (6x . grad)c
div 6x = 0
(68)
and the variation 6a must satisfy curl 6a = curl(Aa  Va6x) = 0
(69)
on account of (Eq. 56). In addition of course
a . 6a = c . 6 c = a . Aa = c . Ac = 0 a . 6c + c . 6 a = a . Ac + c A a = O
(70)
t ds = 0 S
j ( x x F + a x G" + c x G")dv V
=j(x x t
+ a x sa + c x s")ds = 0
(71)
S
representing balance of forces and moments, respectively. Hence, as above, it is possible to relate the generalized forces to a body moment K and surface moment t as follows K = a x G" + c x G",
where v denotes the unit surface normal, p an arbitrary pressure due to the assumed incompressibility, /3 an arbitrary vector arising from the constraint (Eq. 69), and a, A and p arbitrary scalars stemming from the constraints (Eq. 70). In addition one obtains the balance laws
F  grad p  VaT(curlp) + div T" = 0 div S"
given that a and c are mutually orthogonal unit vectors. By a repetition of the arguments for a nematic regarding an infinitesimal, rigid displacement and rotation, one deduces that
j Fdv +
+ VaT(pxv) + T'v,
(67)
F denotes external body force per unit volume, G" and G' generalized external body forces per unit volume, t surface force per unit area, and sa and sc generalized surface forces per unit area. As before, on account of the assumed incompressibility, the virtual displacement is not arbitrary, but is subject to
V
essentially allowing the determination of the generalized body forces. By rewriting the left hand side of (Eq. 66) just as before, it follows that the surface force and generalized surface forces are given respectively by [4 11
e = a x S" + c x s(' (72)
~

div Sc

~
aw + G" + ya + icc + curlp= 0 aa
aw + G" + zc + ica = 0
ac
(74)
y, ic and z being arbitrary scalars again arising from the constrains (Eq. 70). The first of equations (Eq. 74) is clearly the point form of the balance of forces, the first of equations (Eq. 71), and the remaining two are equivalent to the second of (Eq. 7 1) representing balance of moments, this requiring the generalization of the identity (Eq. 12). Also one can show that the surface moment 4 is given by
aw
+'av? this combining Eqs. (72) and (73).
(75)
1.4 Dynamic Theory for Nematics
If external forces and moments are absent, it is possible to combine equations (Eq. 74) to obtain the integral P + W=Po
(76)
where p o is an arbitrary constant pressure. With certain restrictions on the external body force and moment, a similar result follows when these terms are present. Hence as for a nematic, the balance of forces need not concern us except possibly to compute surface forces, and we therefore have two EulerLagrange type equations representing balance of moments. Boundary conditions for the above theory tend to be very similar to those employed in nematics, with little so far emerging by way of genuine smectic boundary conditions.
1.4 Dynamic Theory for Nematics 1.4.1 Balance Laws To derive a dynamic theory one can of course extend the above formulation of equilibrium theory employing generalized body and surface forces as in the initial derivation [7,15]. Here, however, we prefer a different approach [46], which, besides providing an alternative, is more direct in that it follows traditional continuum mechanics more closely, although introducing body and surface moments usually excluded, as well as a new kinematic variable to describe alignment of the anisotropic axis. As above we assume that the liquid crystal is incompressible, and thus the velocity vector v is subject to the constraint
(77) with the result that conservation of mass reduces to the statement that the density p is divv = 0
35
constant in a homogeneous material. As before the director n is constrained to be of unit magnitude. Since thermal effects are excluded, our two balance laws are those representing conservation of linear and angular momentum, which for a volume Vof liquid crystal bounded by surface S take the forms
+I
~
~
d j p v d v = j F d v t ds dt v V S d jpx x vdv dt v = j(x x F + K)dv x t +t)ds
+I(x
(78)
S
V
where F and K are body force and moment per unit volume, t and e surface force and moment per unit area, respectively, x the position vector, and the time derivative the material time derivative. The inertial term associated with the director in the latter of equations (Eq. 78) is omitted on the grounds that it is negligible. The force and moment on a surface with unit normal v are given by
t = pv + ~ v ,e = c.v (79) wherep is an arbitrary pressure arising from the assumed incompressibility, and T and & are the stress and couple stress matrices or tensors, respectively. As a consequence one can express (Eq. 78) in point form
pdv = F  g r a d p + d i v T , dt 0 = K +T+divC
(80)
where T is the axial vector associated with the asymmetric matrix T, so that
T, = Tzy T,,,,
T, = Txz T,,,
A
T, = Tyx T,,,,
(81)
and the divergence is with respect to the second index of both T and L. Finally we remark that for isotropic liquids K and & are generally assumed to be absent, so that angular momentum reduces to T being zero,
36
1
Continuum Theory for Liquid Crystals
or equivalently that the stress matrix symmetric.
T is
1.4.2 A Rate of Work Hypothesis Somewhat analogous to our earlier principle of virtual work, we here assume that the rate of working of external forces and moments either goes into increasing the kinetic and elastic energies, or is dissipated as viscous dissipation. Thus for a volume V of liquid crystal bounded by surface S
I(
j(F. v + K . w)dv + t . v + C w)ds S
V
i n which w denotes the local angular velocity, Wis the FrankOseen energy, and D represents the rate of viscous dissipation. With the aid of equations (Eq. 79) the above can be expressed in point form, and following some simplification through use of equations (Eq. 80) one obtains tr(TVT)+tr(LWT)W.T=+D dW (83) _ _ dt where the velocity and angular velocity gradient matrices yand W take the forms I
_
angular velocity gradients and the angular velocity. Also by appeal to the identity (Eq. 12), the resultant expression cancels the contributions from the static terms on the left hand side of (Eq. 83), given by Eqs. (20) and ( 2 2 ) ,and thus the rate of work postulate reduces to tr(TdYr)
+ tr(LdWT)  w . Td = D > 0
(87)
the superscript d denoting dynamic contributions, and noting that the rate of viscous dissipation is necessarily positive. Alternatively of course one can argue from the linearity of these terms in the velocity and angular velocity gradients that the static contributions are indeed given by our earlier expressions. To complete our dynamic theory, it is necessary to prescribe forms for the dynamic stress and couple stress. The simplest choice consistent with known effects appears to be that at a material point
Td and Ld are functions of y , n and w
(88)
all evaluated at that point at the given instant. However, since dependence upon the gradients of the angular velocity is excluded, it follows at once from the inequality (Eq. 87), given that these gradients occur linearly, that Ld
=0
(89)
respectively. Noting that the material time derivative of the director n is given by
in agreement with the earlier formulation [7]. Hence the rate of viscous dissipation inequality reduces to
dn = w x n dt
D = tr(TdyT)  w . T > 0
(90)
and also that one can show that
which we employ below to limit viscous coefficients.
dt
1.4.3 The Viscous Stress
it is possible by using the chain rule to express the material derivative of the energy Win a form linear in the velocity gradients,
Invariance at once requires that the assumption (Eq. 88) for the dynamic part of the
1.4 Dynamic Theory for Nematics
stress matrix be replaced by
Td is a function of 4, n and w
(91)
all evaluated at that point at that instant, where 1 2A = V+ V T , a=w  curl v 2 I
^
_
(92)
4 being the familiar rate of strain tensor or matrix, and w the angular velocity relative to the background rotation of the continuum. While it is possible to derive the viscous stress from the above assumption [46], we opt here for a more direct approach, and replace (Eq. 91) by
Td is a function of 4, n and N
(93)
all evaluated at that point at that instant, where using (Eq. 85) d N =wxn = n
 1( V 
T
V )n (94) 2  this restricting the dependence upon the relative rotation, essentially discounting the component parallel to the director n, which can be shown to be zero in any event [46]. Nematic symmetry requires that (Eq. 93) be an isotropic function and independent of a change of sign in the director n. Thus assuming a linear dependence upon 4 and N one finds that dt
Td= a , n Ann * n + a,N * n + a,n * N + a44 + as& * n + a6n * An, (95) where again a * b denotes the matrix with +
(i,j)‘h element aibj,and the as are constants. Ignoring thermal effects, the above is also the form that one obtains for cholesterics or chiral nematics. Somewhat straightforwardly it follows from the above that
P = n x g
Y2=
a5
D = tr(TdA) 0 . Td = tr(Td4) g N > o (98) The above of course restricts possible values for the viscous coefficients and one can readily deduce from it that [47]
a,$> 0, 2a4 + as + a6 > 0,
301, + 2a5 + 201, + 2 a , > 0
fi>O,
(99)
(a,+a,+Y2)2(a2'U12)
+ 35(a1
W
I
I
20° 3
;
m
16
I
0.1 0.7
(b)
I
0.8
0.9
1.0
TITAG?
Figure 8. Temperature dependence of the tilt angle in the SmC phase near the secondorder AC transition (a) and near the firstorder NC transition (b) (after Van der Meer and Vertogen [79]).
'U,2
(a2 'U,d21
(92)
The last three terms of the potential (Eq. 90) have the same mathematical form as the corresponding terms in Eq. (85). This means that the quadrupolartype potential appears to be a good model potential for the theory of smectic Asmectic C transition. The interaction potentials (Eqs. 85 and 90) essentially depend on a coupling between the molecular orientation and the intermolecular vector. We note that this coupling could be neglected in the first approximation in the theory of the nematicsmectic A transition, as it is done, for example, in the McMillan theory. At the same time this coupling just determines the effect in the theory of transition into the smectic C phase. Finally we note that both theories, discussed above, neglect the biaxiality of the
2.1
L
1
2
4
3
References
69
Figure 9. Biaxiality order parameter B as a function of the tilt angle in the SmC phase. The curves (3)(I) correspond to the increasing strength of the biaxial part of the interaction potential [ 8 ] .
5
10 0 2
smectic C phase. In real systems some biaxiality is always induced by the tilt and it is only a question of how large the corresponding contribution is to the free energy. In Fig. 9 we present the value of the biaxiality order parameter B (that determines the nonpolar ordering of molecular short axes in the smectic C phase) as a function of the tilt angle. This dependence has been calculated theoretically in [8] using a simple model. The value of the biaxiality order parameter seems to be overestimated. However, even if the actual value is several times smaller, the problem of interaction between biaxiality and the tilt in the smectic C phase deserves further attention.
2.6 Conclusions The literature on the molecular theory of liquid crystals is enormous and in this chapter we have been able to cover only a small part of it. We have mainly been interested in the models for the nematicisotropic, nematicsmectic A and smectic Asmectic C phase transitions. The existing theory includes also extensive calculations of the various parameters of the liquid crystal phases: Frank elastic constants, dielectric susceptibility, viscosity, flexoelectric coefficients and so
on. This part of the molecular theory of liquid crystals remains completely beyond the scope of this review. We also did not consider the theory of more complex liquid crystalline phases including the cholesteric phase, the ferroelectric smectic C* phase, reentrant phases, bilayer and incommensurate smectic phases and phases with hexatic ordering. The majority of these theories, however, employ the same general ideas and approximations that have been discussed above. Thus the present review presents some basic information necessary for the understanding of the existing molecular theory of liquid crystals. Acknowledgements The author would like to acknowledge interesting and stimulating discussions on the molecular theory of liquid crystals with T. J. Sluckin, D. A. Dunmur, G. R. Luckhurst, S . Hess, E. M. Terentjev, B. Mulder, A. Somoza and P. I. C. Teixeira.
2.7
References
[ I ] B. Berardi, S. Orlandi, C. Zannoni, Chem. Phys. Lett. 1996, 261, 363. [2] A. Ferrarini, G. J. Moro, P. L. Nordio, G. R. Luckhurst, Mol. Phys. 1992, 77, 1. [3] P. G. de Gennes, The Physics ofLiquid Crystals, Oxford University Press, Oxford, 1974. [4] E. M. Averjanov, M. A. Osipov, Sov. Phys. Uspihi 1990, 161, 93.
70
2 Molecular Theories of Liquid Crystals
[S] S.C. McGrother, D. C. Williamson, G. Jackson, J. Chem. Phys. 1996,104,6755. [6] D. A. Dunmur, P. PalffyMuhoray, Mol. Phys. 1992,76,1015;A. G. Vanakaras, D. J. Photinos, Mol. Phys. 1995, 85, 1089. [7] A. Perera, G. N. Patey, J . Chem. Phys. 1989,91, 3045. [S] M. A. Osipov, S . A. Pikin, J . Phys. (France) 1995,11/5, 1223. [9] S. A. Pikin, M. A. Osipov in Ferroelectric Liquid Crystals (Ed.: G. W. Taylor), Gordon and Breach, New York, 1992. [ 101 L. Onsager, Ann. N. k: Acad. Sci. 1949,51,627. [ I I ] W. Maier, A. Saupe, Z. Naturforsch. 1959, 14a, 882. [I21 W. Maier, A. Saupe, Z. Nuturforsch. 1960, 15a, 287. [I31 B. W. Van der Meer, G. Vertogen in Molecular Physics of Liquid Crystals (Eds.: G. R. Luckhurst, G. W. Gray), Academic Press, New York, 1979. [ 141 B. W. Van der Meer, Thesis, Groningen, 1979. [IS] L. Pohl, R. Eidenschink, J. Krause, G. Weber, Phys. Lett. A 1978, 65, 169. [ 161 W. M. Gelbart, A. Gelbart, Mol. Phys. 1977,33, 1387. 1171 A. Kloczkowski, J. Stecki, Mol. Phys. 1985,55, 689. [I81 M. A. Osipov, H. Stegemeyer, A. Sprick, Phys. Rev. E 1996,54,6387. [ 191 R. L. Humphries, P. G. James, G. R. Luckhurst, J. Chem. Soc., Faraday Trans. 11 1972, 68, 1031. [20] R. G. Priest, J. Phys. (France) 1975,36,437;J. Chem. Phys. 1976,65,408. [21] B. W. Van der Meer, G. Vertogen, Phys. Lett. A 1979, 71, 488. [22] J. G. Gray, B. J. Berne, J. Chem. Phys. 1981, 74, 31 16. 1231 G. R. Luckhurst in The Molecular Physics of Liquid Crystals (Eds.: G. R. Luckhurst, G. W. Gray), Academic Press, London, 1979. [24] H. Toriumi, E. T. Samulski, Mol. Cryst. Liq. Cryst. 1983, 101, 163. [25] W. H. de Jeu, J. van der Veen, Mol. Cryst. Liq. Cryst. 1977, 40, 1. [26] J. G. T. Ypma, G. Vertogen, H. T. Koster, Mol. Cryst. Liq. Cryst. 1976, 37, 57. [27] N. V. Madhusudana, S. Chandrasekhar, Solid. State Commun. 1973, 13, 377. [28] S. Chandrasekhar, N. V. Madhusudana, Acta Crystallogr. 1971, 27, 303. [29] J. P. Straley, Mol. Cryst. Liq. Cryst. 1973, 24, 7. [30] G. Lasher, J. Chem. Phys. 1970, 53,4141. [31] H. N. W. Lekkerkerker, Ph. Coulon, R. van der Haegen, R. Deblieck, J. Chem. Phys. 1984, 80, 3247. [32] SinDoo Lee, R. B. Meyer, J. Chem. Phys. 1986, 84, 3443.
[33] G. J. Vroege, H. N. W. Lekkerkerker, Rep. Progr. Phys. 1992,55, 124I. [34] A. N. Semenov,A. R. Khokhlov,Sov. Phys. Usp. 1988, 31, 988. [35] T. Odjik, Macromolecules 1986, 19, 2313. [36] T. Sato, A. Teramoto in Advances in Polymer Science, Vol. 126, SpringerVerlag, Berlin, Heidelberg, 1996. [37] M. A. Cotter in Molecular Physics of Liquid Crystals (Eds.: G. R. Luckhurst, G. W. Gray), Academic Press, New York, 1979. [38] SinDoo Lee, J . Chem. Phys. 1987,87, 4972. [39] A. R. Khokhlov, A. N. Semenov, J . Stat. Phys. 1985, 38, 161. [40] J. G. J. Ypma, G. Vertogen, Phys. Rev. A 1978, 17, 1490. [41] J. D. Parsons, Phys. Rev. A 1979, 19, 1225. [42] W. M. Gelbart, B. Barboy, Acc. Chem. Rex 1980, 13, 290. [43] W. M. Gelbart, J. Phys. Chem. 1982, 86, 4298. [44] B. Barboy, W. M. Gelbart, J . Stat. Phys. 1980, 22, 709. [45] J. A. C. Veerman, D. Frenkel, Phys. Rev. A 1990,41,3237;D. Frenkel, J. Phys. Chem. 1988, 92, 3280. [46] G. R. Luckhurst in Recent Advances in Liquid Crystalline Polymers (Ed.: L. L. Chapoy), Elsevier, London, 1986, p. 105. 1471 G. R. Luckhurst, C . Zannoni, P. L. Nordio, U. Segre, Mol. Phys. 1975,330, 1345. [48] C. S.Shih, R. Alben, J. Chem. Phys. 1972, 57, 3055. [49] J. P. Straley, Phys. Rev. A 1974, 10, 1881. [SO] B. Mulder, Phys. Rev. A 1989, 39, 360. [51] B. M. Mulder, D. Frenkel, Mal. Phys. 1985, 55, 1171. [52] T. J. Sluckin, P. Shukla, J. Phys. A: Math. Gen. 1983, 16, 1539. [53] Y. Singh, Phys. Rev. A 1984, 30, 583. 1541 T. J. Sluckin, Mol. Phys. 1983,49, 221. 1551 M. P. Allen et al., Phys. Rev. E 1995, 52, R95. [56] A. Poniwierski, J. Stecki, Mol. Phys. 1979, 38, 1931. [57] M. A. Osipov, Chap. 1 in Liquid Crystalline and Mesomorphic Polymers (Eds.: V. P. Shibaev, L. Lam), SpringerVerlag, New York, 1994. [58] M. A. Osipov, S . A. Pikin, E. M. Terentjev, Sov. Scientific Rev.,harwood acad. publ. 1989,11,19 1, [59] W. L. McMillan, Phys. Rev. A 1971, 4, 1238; 1972, 6, 936. [60] C. Kobayashi, Mol. Cryst. Liq. Cryst. 1971, 13, 137. [61] S. Chandrasekhar, Liquid Crystals, 2nd edn., Cambridge University Press, 1992. [62] L. Shen,H. K. Sim,Y. M. Shin,C. W. Woo,Mol. Cryst. Liq. Cryst. 1977, 39, 299. [63] H. T. Tan, Phys. Rev. A 1977, 16, 1715. [64] P. J. Photinos, A. Saupe, Phys. Rev. A 1975, 13, 1926.
2.7 References [65] A. Poniwierski, Phys. Rev. A 1992,45, 5605. [66] B. Mulder, Phys. Rev. A 1987,35, 3095. [67] A. Stroobants, H. N. W. Lekkerkerker, D. Frenkel, Phys. Rev. Lett. 1986,57,1452;Phys. Rev. A 1987,36,2929. [68] P. Tarazona, Phys. Rev. A 1985,41,2672;W. A. Curtin, N. W. Ashcroft, Phys. Rev. A 1985, 32, 2909; T. F. Meister, D. M. Kroll, Phys. Rev. A 1985,31,4055. [69] A. Poniwierski,T. J. Sluckin,Phys. Rev. A 1991, 43, 6837. I701 A. Poniwierski, T. J. Sluckin, Mol. Phys. 1991, 73, 199. [71] A. M. Somoza, P. Tarazona, Phys. Rev. A 1990,41, 965. [72] A. M. Somoza, P. Tarazona, Phys. Rev. Lett. 1988, 61, 2566; J. Chem. Phys. 1989, 91, 517. [73] A. Poniwierski, R. Holyst, Phys. Rev. Lett. 1988, 61, 2461. [74] L. Senbetu, C.W. Woo, Phys. Rev. A 1978, 17, 1529. [75] M. D. Lipkin, D. W. Oxtoby, J. Chem. Phys. 1983, 79, 1939. [76] L. Mederos, D. E. Sullivan, Phys. Rev. A 1989, 39, 854.
71
[77] B. TjiptoMargo, D. E. Sullivan, J. Chem. Phys. 1988,88,6620. [78] C. G. Gray, K. E. Gubbins, Theory of Molecular Fluids, Clarendon Press, Oxford, 1984. [79] B. W. Van der Meer, G. Vertogen, J. Phys. Colloq. (France) 1979,40, C3222. [80] A. Wulf, Phys. Rev. A 1975, 11, 365. [81] A. Meyer, W. L. McMillan, Phys. Rev. A 1974, 9, 899. [82] D. Cabib, L. Benguigui, J. Phys. (France) 1977, 38,419. [83] A. M. Somoza, P. Tarazona, Phys. Rev. Lett. 1988,61,2566. [84] A. Poniwierski, T. J. Sluckin, Mol. Phys. 1991, 73, 199. [85] H. Hervet, F. Volino et al., J. Phys. (Lett.) France 1974,35, L151; Phys. Rev. (Lett.) 1975, 34, 451; P.4. Bos, J. Pirs et al., Mol. Cryst. Liq. Cryst. 1977,40, 59. [86] L. Blum, A. J. Torruella, J. Chem. Phys. 1972, 56, 303. [87] J. W. Goodby, G. W. Gray, D. G. McDonnell, Mol. Cryst. Liq. Cryst. (Lett.) 1977, 34, 183. [88] W. H. de Jeu, J. Phys. (France) 1977,38, 1263. (891 G. Barbero, G. Durand, Mol. Cryst. Liq. Cryst. 1990, 179, 57.
3 Molecular Modelling Mark R. Wilson Over the past 10 years, rapid progress has been made in the field of molecular modelling. Advances have been led by two important factors: the increase in speed and reduction in cost of modern computers, and an accompanying improvement in the accuracy and ease of use of molecular modelling software. Modelling packages are now commonly available in many laboratories. Their ability accurately to predict molecular structures of simple organic molecules makes them a useful tool in the study of liquid crystals. In this article developments in molecular modelling are discussed in the context of liquid crystal systems. The article is divided into two main sections: Sec. 3.1 covers the main molecular modelling techniques that are currently available; whilst Sec. 3.2 covers specific applications of these techniques in the study of liquid crystal molecules.
3.1 Techniques of Molecular Modelling 3.1.1 Molecular Mechanics Molecular mechanics is the simplest and most commonly used molecular modelling
technique. It is concerned with the determination of molecular structure, and is of particular relevance to liquid crystal chemists concerned with the design of appropriate molecular structures, or to physicists interested in calculating molecular properties. The molecular mechanics approach has been reviewed in a number of places [ 141, and so here only the basics of the technique are described. The standard approximation employed in molecular mechanics is to consider a molecule as a collection of atoms held together by elastic restoring forces. These forces are described by simple functions that characterise the distortion of each structural feature within a molecule. Usually separate functions exist for each bond stretch, bond bend, and dihedral angle; as well as for each nonbonded interaction. Together these functions make up the molecular mechanics force field for a particular molecule. The steric energy E can then be defined with reference to the force field. E has no physical meaning in itself, but can be thought of as measuring how the energy of a particular molecular conformation varies from a hypothetical ideal geometry where all bonds, bond angles, etc. have their ideal (or natural) values.
3.1 Techniques of Molecular Modelling
=
c
Ebond
+
bond lengths
c
(1)
&ngle
bond angles N
2 Etorsion dihedral
41x1
N
c
(&bij
+
J are the components in the new axis system. If the quantities aaP are the nine direction cosines between the axes of the two coordi
nate frames, the transformation law for the vector property becomes:
Ph = a, P,+a,, P,+ acYz Pz = aap Pp
(1)
where the repeated suffix p implies summation over all values of P=x, y , z. A consequence of the transformation law Eq. ( I ) , is that under inversion all the components change sign, &=pa: this is a polar vector. There are some quantities (axial or pseudo
2
X
Figure 1. Change i n vector Components on rotating axes.
88
1
Tensor Properties of Anisotropic Materials
vectors) which transform according to:
4iY = asp iug These are usually associated with magnetic phenomena (angular momentum, magnetic moments and magnetic fields are axial vectors) and related properties. The nine direction cosines can conveniently be represented as a 3 x 3 matrix, but the components of this matrix (aap)are not independent, since for orthogonal axes the sums of squares of components in columns or rows are unity, while the sums of products of components in adjacent rows or columns are zero. It is clear that one set of orthogonal axes can be rigidly related to another by just three angles, and Euler angles (8, @, y) provide a consistent definition of three such angles which are frequently used. The Euler angles are defined as follows. Assuming that the axes (x, y , z ) and ( X , Y ,Z) are initially coincident, rotation around Z=z, by an angle y gives X + x ’ , Y+y’, rotation about the new axis y’ by 8 gives Z+z, X’JX’’, and finally rotation about z by an amount $ gives d ’ j x and y’+y, see Fig. 2 [2]. The direction cosine matrix represented by asp, can now be expressed in terms of Euler angles by:
Figure 2. Euler angles.
sor quantity depends on another vector or tensor quantity. A simple example of importance to liquid crystals is the second rank tensor property electric susceptibility which relates electric polarization (vector) to an applied electric field (vector). Neglecting nonlinear effects, the electric polarization Pa is proportional to the magnitude of the applied electric field E, but for anisotropic materials it may not be in the same direction. Consider a linear (onedimensional) array of charges aligned at an angle
x,
1
cos8cos$cos y  sin $sin y cosBsin $ c o s y  cos$ sin y sin
[email protected] [email protected] + sin$cos y cos Bsin @siny +
[email protected] sin 8 sin @  sin 8 cos y sin 8 sin y cos 8 Having established the transformation law Eq. ( I ) , first rank tensor quantities (i.e. vectors) may be defined as those properties which transform according to Eq. (1). Higher order tensors can be defined i n terms of different transformation laws, and they arise in a general sense when one vector or ten
(3)
to an applied electric field (see Fig. 3). A separation of charge will be induced by the field resulting in a polarization necessarily along the direction of the array of charges: the electric field has induced a component of the polarization in a direction orthogonal
1 Z
Tensor Properties of Anisotropic Materials
89
where, as before, the repeated suffixes yand 6 indicate a summation over all possible values (x, y , z). Thus the expression for each component of the transformed property, for example contains nine terms, although in practice symmetry usually reduces this number. It is possible to use an alternative transformation rule for second rank tensor properties, equivalent to Eq. (6), but which can be expressed in terms of the matrix of direction cosines, such that:
xx,,
E
I
X
(7)
Figure3. The polarization of a linear array of charges by a field.
to the field. Such a result cannot be described in terms of a simple proportionality between the polarization and the field (Pa Em),because a field along the xaxis has induced a polarization along the zaxis. Obviously the susceptibility also depends on direction, and for the example given, the relationship between polarization and electric field can be written as (for the configuration depicted in Fig. 3 , Ez=O):
#x
px = x x x Ex + x x z Ez pi = x z x Ex + x z z Ez
(4)
This is readily extended to three dimensions, and using the notation introduced above:
where xaprepresents nine coefficients or a 3x3 matrix of nine quantities. The electric susceptibility of an anisotropic material can be represented by a matrix of nine components, and we can now consider how such a second rank tensor property changes as a result of rotation with respect to an orthogonal axis system. The transformation rule for second rank tensor properties is:
where A' is the transpose of the direction cosine matrix. Although the simplest directiondependent property is a vector, most physical properties of liquid crystals are higher order tensors. All tensor properties can be categorized by their transformation properties under rotation of the coordinate frame, and the transformation law for a third rank tensor such as the piezoelectric tensor Papyis:
The tensor rank of a property is also established by the number of components it has: first rank (vector) 3 , second rank 9, third rank 27 and so on. This definition is correct for three dimensions, but in two dimensions the number of components for a tensor property of rank n becomes 2". It must be emphasized that not all the components are necessarily independent, and symmetry can provide relationships between them, thereby reducing the number that have to be separately measured. Many physical properties can be described in terms of the response of a system to an external force or perturbation. This force might be an electric field or a magnetic field, a mechanical force (stress), a torque or a combination of these. The effect of an external perturbation may be described in
90
1
Tensor Properties of Anisotropic Materials
terms of a new tensor property, or a modification to an existing one; polarization by an electric field results in an induced polarization which adds to any permanent polarization already present. To lowest order, the induced polarization is linear in the applied field, but nonlinear terms can be important for strong fields, as in nonlinear optics. The nonlinear contributions represented in Eq. (9) below are described in terms of third xap and fourth rank tensors
,
xap
Pa =pj*O)+
c XapEp c Xapy Ep E y c XapysEpE, E8
p=n,\,z
+
xap,
(9)
P,y,G=x,\,:
This equation includes a number of pairs of repeated suffixes, and each pair indicates a summation over all possible values. Having understood this convention (the Einstein summation convention) it is no longer necessary to write the summation signs explicitly in an equation. It is sometimes useful to represent the physical properties in terms of their contribution to the internal energy, since all types of energies are scalar quantities. Thus the energy of a polarized body in an electric field becomes:
This manipulation is a simple application of tensor calculus, and illustrates the simplification of the summation convention (summation signs have been omitted). The intrinsic symmetry of a property can reduce the number of independent components;
xaDr6 xap,
j a = %p Ep
p,Y=X,,,Z
+
thus neglecting complications that may arise if electric fields of more than one frequency are present, the order of the field components in Eq. (10) is immaterial. xapyand Hence the properties must be symmetric with respect to interchange of suffixes, and this immediately reduces the number of independent components of the tensor properties to six for ten for Xapyand 15 for xapyS. Another example of a second rank tensor property is electrical conductivity oapwhich relates the current flow j , in a particular direction to the electric field: ( 1 1)
This may also be written in terms of resistivity pap as:
Ea = pap j p
(12)
and the Joule heating which a current generates in a sample is a scalar given by: u = j . E = j , E,
=papj , j p
(13)
Each tensor property has an intrinsic symmetry, which relates to the interchangeability of suffixes. However, the number of independent tensor components for a property also depends on the symmetry of the system it is describing. Thus the properties of an isotropic liquid, which has full rotational symmetry, can be defined in terms of a single independent coefficient. The number of independent components for a particular tensor property depends on the point group symmetry of the phase to which it refers. This is expressed by Neumann’s principle which states that the symmetry elements of any physical property of a crystal must include the symmetry elements of the point group of the crystal. Many properties of interest for liquid crystals are second rank tensors, and these have some special properties, since they
1
can be represented as 3 x 3 matrices. Those second rank tensor properties which have an intrinsic symmetry with respect to interchange of suffixes are called symmetric and only have six independent components. A symmetric 3x3 matrix can always be diagonalized to give three principal components, which is equivalent to finding an axis system for which the offdiagonal components are zero. The principal axis system requires three angles to define it with respect to an arbitrary axis frame, so there is no loss of variables: three principal components and three angles being equivalent to the six independent components. However, if the material being described (i.e. the liquid crystal) has some symmetry, then the principal axes will be defined, and so it is possible to reduce the number of independent components of a second rank tensor to three (the principal values). For uniaxial liquid crystal phases of symmetry D,, such as N and SmA, as well as SmB and Col,, and Col,, phases, a unique symmetry axis can be defined, parallel to the director, and there are just two independent components of any second rank tensor property xap: (par(perpendicular) to the symmeallel) and try axis:
x,,
x1
where the zaxis is defined as the symmetry axis. The values of the components in any other axis system can be obtained from the transformation law Eqs. (6) or (7). Two useful quantities defined in terms of these independent components are the anisotropy A x and the mean
Tensor Properties of Anisotropic Materials
Another special feature of second rank tensor properties in three dimensions is that they can be represented by a property ellipsoid, such that the value of the property in a particular direction is represented by the length of the corresponding radius vector of the property ellipsoid. A three dimensional surface representing an ellipsoid can be defined by
c,, x 2 + c,, y 2+ czzz 2 + 2C,,
xy + 2CXzxz + 2CVzyz = I
(16)
where the coefficients Cap behave as the components of a second rank tensor. If the ellipsoid is expressed in terms of principal axes, then the off diagonal terms in Eq. (1 6) are zero, and the equation of the ellipsoid becomes:
c,, x 2 + c,, y 2 + c,, 22 = 1
(17)
where the lengths of the semiaxes are given by [Cii]p”2.The value of this property in any direction (1) defined by direction cosines a,,, sly, a l z will be:
c = c,, a; + c,!
2 a[,2 + c,, alz
=(x2+y2+z2)’
(18)
so the length of any radius of the property ellipsoid (Fig. 4) is equal to the reciprocal of the square root of the magnitude of the property in that direction.
X
t
X:
Ax = XI1  x_L (15)
91
Figure 4. Property ellipsoid
92
1
Tensor Properties of Anisotropic Materials
xgd
1.1 Macroscopic and Microscopic Properties
tity can be used as an order parameter. Alternatively a dimensionless order parameter tensor can be defined as
Liquid crystals as anisotropic fluids exhibit a wide range of complex physical phenomena that can only be understood if the appropriate macroscopic tensor properties are fully characterized. This involves a determination of the number of independent components of the property tensor, and their measurement. Thus a knowledge of refractive indices, electric permittivity, electrical conductivity, magnetic susceptibilities, elastic and viscosity tensors are necessary to describe the switching of liquid crystal films by electric and magnetic fields. Development of new and improved materials relies on the design of liquid crystals having particular macroscopic tensor properties, and the optimum performance of liquid crystal devices is often only possible for materials with carefully specified optical and electrical properties. The anisotropy of liquid crystals stems from the orientational order of the constituent molecules, but the macroscopic anisotropy can only be determined through measurement of tensor properties, and macroscopic tensor order parameters can be defined in terms of various physical properties. The anisotropic part of a second rank tensor property can be obtained by subtracting the mean value of its principal components:
xtj = xap  x Sap
(19)
where the Kronecker delta is equivalent to aunit second rank tensor or unit matrix, such that for a=P, i5xx=Syv=Szz= 1, otherwise all other components are zero. Note that S, = 3, because of the repeated suffix convention. The advantage of using " P is that it is traceless, and the sum of the diagonal elements is zero. For an isotropic material zap=xSap, and so x $ = O ; thus the quan
x'"'
and without loss of generality the maximum value of a principal component (say Q,,) of Qap can be set equal to one, so that:
QZ,
=1
2 [Axmax] = constant x 3
(21)
This provides the definition of the constant, and the macroscopic second rank tensor parameter becomes:
The quantity [Ax,,,] refers to the anisotropy of the tensor for a fully aligned state for which the order parameter is one. For a biaxial phase (i.e. a phase which has different properties along each of the three principal axes), the macroscopic order parameter in principal axes can be written as:
L defining Q = [ ~ x m a x ]  l (
xZz 51 (xxx+ xyJ)) xyy)
and P = [Axmax]' 3 (xxx. Other de2 finitions of QaP are possible, but the chosen one maintains the correspondence between the macroscopic order parameter and the microscopic one to be introduced next. One problem with the macroscopic order parameter as defined through Eq. (23) is that it has
I . 1 Macroscopic and Microscopic Properties
been assumed that the principal axes of the property xap and the order parameter tensor coincide. While this is necessarily true for uniaxial materials, it is not true for biaxial materials, the principal axes for which will be different for different properties. The relationship between macroscopic properties and molecular properties is a major area of interest, since it is through manipulation of the molecular structure of mesogens, that the macroscopic liquid crystal properties can be adjusted towards particular values which optimize performance in applications. The theoretical connection between the tensor properties of molecules and the macroscopic tensor properties of liquid crystal phases provides a considerable challenge to statistical mechanics. A key factor is of course the molecular orientational order, but interactions between molecules are also important especially for elastic and viscoelastic properties. It is possible to divide properties into two categories, those for which molecular contributions are approximately additive (i.e. they are proportional to the number density), and those properties such as elasticity, viscosity, thermal conductivity etc. for which intermolecular forces are responsible, and so have a much more complex dependence on number density. For the former it is possible to develop a fairly simple theory using single particle orientational order parameters. In the context of liquid crystals, single particle angular distribution functions are of major interest. They give the probability of a single molecule having a particular orientation with respect to some defined axis system, but they contain no information on pair correlations between molecules. A familiar example of single particle angular distribution functions is the hydrogenic s, p, dorbitals, which are used via the square of the wave function to determine the probability distribution for a single electronic charge in
93
an atom. For a manyelectron atom the wave function for the electrons is often written as the sum of component orbital contributions. In an analogous fashion, the distribution of molecular orientations in a liquid crystal can be represented as a sum of contributions of particular symmetries. Restricting attention to axially symmetric molecules having an axially symmetric distribution of orientations with respect to the director (zaxis), it is convenient to use Legendre functions P , (cos 8 ) to describe the angular distribution functionf(8):
(24) The expansion in Legendre polynomials or more generally spherical harmonics is chosen because they are orthogonal functions. The coefficients uL in the expansion can be obtained by multiplying both sides of Eq. (24) by PL(cos 8 ) and integrating over 8, with the result: rl
j UL
(cOS8)f(8) s i n e d o
=(2L+l)O
(25) jf(8)sin 8 d 8 n
The ratio of integrals in Eq. (25) is the definition of the average value of P,(cos8) over the single particle angular distribution function, so the single particle distribution function can now be written as:
1 f (6)= ; L
The amplitudes of the coefficients in this expansion now have a special significance:
94
1 Tensor Properties of Anisotropic Materials
they are the order parameters for the distribution function. A knowledge of all order parameters will provide a complete description of the single particle angular distribution function, and the magnitude of each order parameter gives the contribution of a particular symmetry to the distribution function for the disordered structure. If we wish to consider the distribution function for a molecule requiring three angles to specify its orientation, f @, y ) must be expanded in terms of a set of orthogonal functions which span the orientation space of the Euler angles. A convenient set of such functions are the Wigner rotation matrices, denoted Di,,,,(6, @, y),so the single particle angular distribution function becomes (see [ 3 ] for further details):
(
[email protected] L
where as before the coefficients uL,m,rr can be obtained from the orthogonality condition to give:
(6,@, y))are generand the quantities (Di,, alized orientational order parameters, the indices L, m, n relating to the angular variables 6, @, y. The symmetry of the constituent molecules and the symmetry of the liquid crystal phase provide some constraints on the terms which contribute to the distribution function. For example if a molecule has inversion symmetry, then only terms even in L will contribute; similarly for molecules with a C2 rotation axis along the zdirection, only terms even in n will survive. A full set of symmetry operations and nonvanishing order parameters is given by Zannoni [4]. The number of independent order parame
ters necessary to specify the angular distribution function will also be reduced by the symmetry of the liquid crystal phase, see for example [ 5 ] . Returning to the simple case of uniaxial molecules having inversion symmetry in a uniaxial phase, the distribution function can be written as:
and the two leading order parameters are ( P z (cos 6)) and (P4 (cos 6)): the former is often referred to as S. One point to notice is that order parameters are multivalued in the sense that different distributions may give the same value for an order parameter, hence the value of information on more than one order parameter. For example, a distribution in which the molecular axes were at an average angle of about 55" to the zaxis would give ( P 2(cos 19))close to zero with a negative (P4(cos 6)).An isotropic distribution of molecules is indicated by all order parameters being zero. Alternative but equivalent definitions of order parameters as tensor quantities are sometimes more convenient, particularly in relation to physical properties. These definitions are only usefully compact for systems in which either the molecules or the phase are uniaxial. For a uniaxial liquid crystaI phase of biaxial molecules, the single particle angular distribution function can be written as [ 3 ] : 1 + 3 Su 1,
+ 9S,py6
+ 5 Sap 1, 1, l p I,
16
lp
+ .. .
where l,=lx, I,, I, are direction cosines of the director with respect to the molecular axes, and the quantities S, Sup, Supyand are ordering tensors of ranks 1, 2, 3 , and 4, respectively, and the summation convention has been adopted. For phases with inversion
1.1
Macroscopic and Microscopic Properties
,h.
95
96
1
Tensor Properties of Anisotropic Materials
symmetry all ordering tensors of odd rank are zero, and the first nonvanishing tensor order parameter Sap is sometimes known as the Saupe ordering matrix. Definitions of the ordering tensors as averages over direction cosines are:
eters of the different molecular axes with respect to a uniaxial director. If the distributions of the two shorter molecular axes (say x and y) are not identical, then S ~ x # S y y , which represents a local biaxial ordering of molecular axes. This may be expressed in terms of anew orderparameterD=S,,S,,, and the Saupe ordering matrix can be written as:
  (1S  D ) 2 0 0
These tensors are defined to be zero for an isotropic phase. For uniaxial molecules there is only one independent component for each of the tensors:
0
  (1S + D ) 2 0
0 S
(33)
If the Saupe ordering matrix is written in terms of the laboratory axis frame, but assuming now that the molecules are uniaxial, then phase biaxiality can be described in terms of the order parameter P , which is nonzero for tilted smectic phases and other intrinsically biaxial phases. For example the diagonal ordering matrix for the molecular long axis z can be written as:
  (1S  P ) 2 0
0
One advantage of this representation of order parameters is that it readily describes nonuniaxial molecular order in a macroscopically uniaxial liquid crystal phase. If the reference axis frame has been chosen to diagonalize the ordering tensor, then its principal components are the order param
0
0
  1( S + P ) 2 0
0
(34)
S
and the magnitude of P is a measure of the different probabilities of finding the zmolecular axis along the X and Y directions of the laboratory or phase reference frame. The Cartesian tensor representation can be extended to describe the orientational ordering of biaxial molecules in biaxial phases by introducing [6] a fourth rank ordering tensor: (35)
1.1
where is the cosine of the angle between the molecular axis a and the laboratory or phase axis i. The tensor Sap,ij still describes second rank orientational ordering, and should not be confused with the ordering tensor SalpyGwhich refers to fourth rank orientational order. For a suitable choice of both sets of axes, the 81 components of Sap,jj can be reduced to nine such that i=j and a=P. This is equivalent to defining three diagonal Saupe ordering matrices, one for each of the three axes, i=X, I: 2:
Taking the diagonal components of these three matrices allows the construction of a 3 x 3 matrix:
(37) and the generalized biaxial order parameters can be defined as follows. The long axis ordering is described by S=S,Z,, while the phase biaxiality for a uniaxial molecule is given by P=S&SiYz. For biaxial molecules in a uniaxial phase the biaxial order paramter is D=S$xSfy, but it would be equally possible to define a biaxial order parameter with respect to the Xaxis, such that D’=S:xSfy, and this would equal D“= SJxSJv for uniaxial phases. However, if the phase is biaxial, then the biaxiality defined with respect to phase axes X and Y will be different, and this new form of biaxiality is described in terms of a new biaxial order parameter:
(
= ( S Z  s;,)  SZx  SYyI.) ..
(37 a>
In terms of averages over Euler angles, these may be defined as:
97
Macroscopic and Microscopic Properties
\
 2 cose sin 24 sin 2w]
/
Slightly different definitions have been adopted by some other authors with different numerical factors. The advantage of the definitions in Eq. (38) is that these order parameters are simply related to the components of the Saupe ordering matrices Eq. (34), as indicated in Table 1. The order parameters introduced in the preceding paragraphs are sufficient to describe the orientational order/disorder of rigid molecules in liquid crystal phases. They will be used to relate molecular properties to macroscopic physical properties, but there are additional sources of order/disorder which may affect physical properties. For flexible molecules certain physical properties or responses may be sensitive to a particular group or bond within the molecule, and under these circumstances it is the order parameter of that moiety which determines the measured anisotropy. As an example, the degree of order of flexible alkyl chains attached to a rigid molecular core is reduced by internal rotation of the chain segments. Using selectively deuteriated mesogens, deuterium magnetic resonance is able to measure the order parameters of different segments of a flexible chain, and it has been shown that as expected the orientational order decreases along the chain away from the rigid core of the molecule [ 7 ] . Local biaxial ordering of molecules in uniaxial liquid crystal phases can be detected by spectroscopic techniques such as lin
98
1 Tensor Properties of Anisotropic Materials
ear dichroism and NMR. It is often more convenient to probe the biaxial order of solutes in liquid crystal hosts, for example a detailed analysis of the *D NMR of fully deuteriated anthracene d l o in various liquid crystal solvents yields both S and D order parameters [8]. These are illustrated in Fig.5, where they are compared to mean field calculations with the ratio (A) of uniaxial and biaxial energies as an adjustable parameter. It is reasonable to assume that the orientational order parameters introduced will also be appropriate for smectic and columnar phases. However, there are additional contributions to the order/disorder, which can contribute to the measured anisotropy in physical properties. The characteristic structural feature of smectic and columnar phases is the presence of some translational order, and so the radial distribution function will have long range periodicity in certain directions, the amplitude of which will be determined by a suitable order parameter. Furthermore, there is the likelihood of coupled orientational and translational order: for example in a smectic A phase molecules will be more likely to be aligned parallel to the layer normal (the director) when their centres of mass coincide with the average layer position. For disordered smectics there is one dimensional positional order, and assuming uniaxial molecules in a uniaxial smectic phase, the corresponding single particle distribution function can be written as [9]:
(39)
where translational (z) and translationalrotational (0)order parameters can be defined as :
Columnar phases have two degrees of translational order, and the corresponding order parameters now require averages over periodic functions in two spatial dimensions; for completeness we include the distribution function for a uniaxial columnar phase consisting of uniaxial disclike molecules:
l+2(cos(
F)cos[7))
. cos( ~  ) c o s [ ~ ~ )
+ 20 . P
(
P2 (cose)cos (*;)cos( ~
7))
*(cos*~cos(~)cos(~)+..
The contribution of translational order parameters to the anisotropy of physical properties of liquid crystals has not been studied in detail. Evidence suggests that there is a very small influence of translational ordering on the optical properties, but effects of translational order can be detected in the measurement of dielectric properties. There are strong effects in both elastic properties and viscosity, but the statistical theories of these properties have not been extended to include explicitly the effects of translational order.
1.1
Macroscopic and Microscopic Properties
99
the molecules:
xap = N (‘cap ) = N (aay
) K$)
(43)
The average over the products of direction cosine matrices contains the orientational order parameters, and in terms of the principal components of the anisotropic part of the macroscopic tensor property becomes:
4;)
0.0
00
0.4
0.2
0.6
0.8
S Figure 5. Uniaxial and biaxial order parameters for anthracene d,(, in different liquid crystal solvents: (0)  ZLI1167 (best fit L=O.6); (0)  E9 (L=0.4); (0) Phase 5 (L=0.3), reproduced from [8].
Having defined orientational order parameters, it is now possible to develop a general statistical theory which relates the physical properties of molecules to the macroscopic properties of liquid crystal phases. There are however many simplifying approximations which have to be introduced to give usable results. An important factor is that the nature of the property will determine the order parameters that will be included: in particular a property of tensor rank n will in general require order parameters up to tensor rank n to specify it. If K~~ is a molecular second rank tensor property, the principal components of which are ~!,m),~y’,) and K;:) defined in a molecular axis system, then using the transformation rule for second rank tensors, the property in a laboratory frame is: (m)
Kap = aa, ap6 k^rs
(42)
Ignoring the effect of molecular interactions, which is a gross assumption, the macroscopic response “ P measured in a laboratory axis frame will be the molecular property multiplied by the number density, averaged over all possible orientations of
x
Those terms in Eq. (44) which have nonzero averages depend on the symmetry of which by Neumann’s principle must contain the symmetry of the phase to which it relates. If the phase is uniaxial, the principal components of xk? become:
x$),
where the order parameters S and D are defined by Eq. (38). Comparison of Eq. (45) with the definition of the macroscopic order parameter Eq. (22) shows that:
100
1
Tensor Properties of Anisotropic Materials
axial phases:
Reduced Temperature
xf’
xf’)
Figure 6. Reduced values and as a function of reduced temperature plotted according to Eq. (45) using order parameters calculated using mean field theory. Open squares (0)assume no molecular biaxiality, so D =O; full circles ( 0 )are for an assumed molecular biaxiality of 0.3 and a A value of 0.3.
For perfect alignment Q r i = S = 1, and the macroscopic anisotropy (Ax),,, = N [ k i y ’ 1 / 2 k ~ ~ ) + k which ~ ’ ] , is simply N times the molecular anisotropy. Both order parameters S and D contribute to the anisotropy of second rank tensor properties, but they cannot be separated from a single measurement of the macroscopic anisotropy. The behavior of the macroscopic property components as a function of temperature is illustrated in Fig. 6 for a material of positive molecular anisotropy, for various values of the order parameters S and D calculated from mean field theory; for a negative anisotropy material the signs of the parallel and antiparallel components are interchanged. If the liquid crystal phase is biaxial, then any second rank tensor property has three independent principal components. These are the diagonal elements of the anisotropic tensor and can be expressed in terms of the order parameters introduced for bi
xgb,
It has been assumed that molecular properties contribute additively to the macroscopic tensor components, which are consequently proportional to the number density. If intermolecular interactions contribute to the physical property, then deviations from a linear dependence of the property on density are expected. Also the contribution of orientational order will be more complex, since the properties will depend on the degree of order of interacting molecules. Effects of molecular interactions contribute to the dielectric properties of polar mesogens, and are particularly important for elastic and viscoelastic properties. Molecular mean field theories of elastic properties predict that elastic constants should be proportional to the square of the order parameter; this result highlights the significance of pairwise interactions.
1.2 References I ] J. F. Nye, Physical Properties of Crystals, Oxford University Press, Oxford, 1985. [2J S. Altmann, Rotations, Quaternions and Double Groups, Oxford University Press, Oxford, 1986, p. 65.
1.2 References [3] C. Zannoni in Nuclear Magnetic Resonance of Liquid Crystals (Ed.: J. W. Emsley), D. Reidel, Dordrecht, Netherlands, 1983, p. 1. [4] C. Zannoni in Molecular Physics ofLiquid Crystals (Eds.: G. W. Gray, G. R. Luckhurst), Academic Press, London, 1979, p. 51. [S] Z. Luz, D. Goldfarb, H. Zimmermann in Nuclear Magnetic Resonance of Liquid Crystals (Ed.: J. W. Emsley), D. Reidel, Dordrecht, Netherlands, 1983, p. 351.
101
[6] D. W. Allender, M. A. Lee, N. Hafiz, Mol. Cryst. Liq. Cryst. 1985, 124,4552. [7] J . W. Emsley, G. R. Luckhurst, C. P. Stockley, Proc. R. Soc. Lond. 1982, A381, 117. [8] J. W. Emsley in Nuclear Magnetic Resonance of Liquid Crystals (Ed.: J. W. Emsley), D. Reidel, Dordrecht, Netherlands, 1983, p. 379. [9] C. Zannoni in The Molecular Dynamics ofLiquid Crystals (Eds.: G. R. Luckhurst, C. A . Veracini), Kluwer, Dordrecht, Netherlands, 1994, p. 34.
2 Magnetic Properties of Liquid Crystals David Dunmur and Kazuhisa Toriyama
In Sec. 1 of this chapter it is shown that macroscopic anisotropy in liquid crystals can be related to molecular properties through appropriate microscopic orientational order parameters, as in Eq. (47) of that section. This relationship assumes that the macroscopic response of a liquid crystal is simply the sum of the individual molecular responses averaged over an orientational distribution function (i.e. interactions between molecules are ignored, except to the extent that they determine the orientational order). For most physical properties such an approximation is very crude; however, magnetic properties are only very weakly influenced by intermolecular interactions, and so it can be assumed that the magnetic response of liquid crystals is simply the aggregated molecular response. The weak interaction between molecules and magnetic fields is shown by the magnetic permeability relative to that of free space for nonferromagnetic materials, which is close to unity. The magnetic response of materials depends on their electronic structure, and the susceptibility may be negative, characteristic of diamagnetic compounds, positive denoting a paramagnetic response, or ferromagnetic which indicates a permanent magnetization resulting from coupling between electrons
on constituent atoms, ions or molecules; ferromagnetism is largely restricted to the solid state. Both diamagnetic and paramagnetic liquid crystals are known, and ferromagnetic liquid crystals have been prepared from colloidal suspensions of ferromagnetic materials in a liquid crystal host.
2.1 Magnetic Anisotropy Like other tensor properties of liquid crystals, the magnetic susceptibility is anisotropic, and so magnetic fields can be used to control the alignment of liquid crystal samples. This is perhaps the single most useful application of the magnetic properties of liquid crystals, and the combination of magnetic field alignment with some other measurement forms the basis of many experimental investigations. Macroscopically the magnetic susceptibility relates the induced magnetization M to the strength of the magnetic field, but assuming that local field effects are ignored, the susceptibility is usually defined in terms of magnetic induction B . For this chapter the magnetic induction will be referred to as the magnatic field, and the magnetization is
2.1
given by: I
magB
M a = h xap
p
(1)
where po is the permeability of free space. The magnetic contribution to the free energy density becomes: gmag = j ~ a d ~ a = djBaXapdBp
1 I = g o  p XapBaBp
(2)
xapis a volume susceptibility, but a molar susceptibility xggl may be defined as (3) where Vmol is the molar volume. The susceptibility has the symmetry of the material, so expressing this in terms of the principal axes of gives for the free energy density:
x
gmag = go 
1
1
Po
. (xIIcos2 e + xI.sin2 e
[email protected] + xIsin2 e cos2 @)
(4)
where 8 and @ are polar angles defining the orientation of B with respect to the principal axes of the susceptibility. For a uniaxial material and:
xL,=xL
where Ax=x,,xI, and n is the director, which also defines the principal axis of the
Magnetic Anistropy
103
susceptibility for uniaxial materials. From Eq. ( 5 ) it is clear that the sign of the anisotropy A x will determine the orientation of the director with respect to a magnetic field. In order to minimize the free energy, the director will align parallel to the magnetic field for a material having positive A x , while for negative A x the director will be perpendicular to B ; both situations can occur in practice. As explained earlier, any anisotropic property can be used to define a macroscopic order parameter, and because it is largely unaffected by molecular interactions, the magnetic susceptibility is a particularly useful measure: definitions are given as Eqs. (21) and (22) of Sec. 1 of this chapter. The value of Axmax corresponding to perfect alignment can in principal be obtained from measurements on single crystals or from molecular susceptibilities. Eqs. (45) and (47) of Sec. 1 of this chapter relate a macroscopic susceptibility to a microscopic molecular property reap, and introduce appropriate order parameters. The molecular susceptibilities K ~ . K~,,,, ~ , K~~ are defined for the principal axes of the molecular susceptibility, which may not coincide with the axes that define the local orientational order; however, it is usually assumed that any differences can be neglected. Measurements of the magnetic susceptibility can provide a useful route to the order parameters of liquid crystals [ I , 21, but require a knowledge of the molecular susceptibilities. These are not usually available for mesogens, but they can be obtained from single crystal measurements, provided full details are available for the crystal structure; the method for deriving molecular susceptibilities from crystal susceptibilities is explained in detail in [ 3 ] .
104
2
Magnetic Properties of Liquid Crystals
2.2 Types of Magnetic Polarization
n
2.2.1 Diamagnetism A diamagnetic response is the induction of a magnetic moment i n opposition to an applied magnetic field, which thereby raises the free energy. Thus a diamagnetic material will be expelled from a magnetic field, or will adjust itself to minimize the diamagnetic interaction. Most liquid crystals are diamagnetic and this diamagnetism originates from the dispersed electron distribution associated with the molecular electronic structure. The diamagnetic susceptibility is a second rank tensor, and its principal components can be expressed as:
where e is the electronic charge, me is the mass of an electron, I , m, n are the molecular axes, and the quantities (m2+ n 2 )are averages over the electron distribution for a plane perpendicular to the component axis (I in this case see Fig. 1). The induced diamagnetic moment depends on the extent of the electron distribution in a plane perpendicular to an applied magnetic field. In a molecule, delocalized charge makes a major contribution to K ~ and in particular the ring currents associated with aromatic units give a large negative component of diamagnetic susceptibility for directions perpendicular to the plane of the aromatic unit. It is for this reason that the diamagnetic anisotropy of most calamitic
m
Figure 1. Diagram of molecular axes with representation of the perpendicular plane.
mesogens is positive since both components are negative, but > xII .
I xl I I I
2.2.2
Paramagnetism
Molecular paramagnetism is mostly connected with unpaired electron spins, which have associated magnetic moments. For paramagnetic mesogens the electron spin is introduced by metal centres, and one of the motivations for research into metalcontaining mesogens is the desire to prepare paramagnetic liquid crystals. Orientation by an external magnetic field of the magnetic moment derived from an electron spin will induce a magnetization along the field direction, and so provides a positive contribution to the magnetic susceptibility:
(7) where ge is the electronic gvalue, s is the total electron spin quantum number and pus is the Bohr magneton. lCPara is the isotropic molecular paramagnetic susceptibility, and ~ the~ coefficient , of 1/3 arises from the isotropic average of (cos26 ) over the spin orientation in a magnetic field. The temperature dependence of K~~~~ follows a simple Curie Law, and as written there is no anisotropy in K ~ since ~ in~ most ~ molecules , the unpaired electron spin is decoupled from the
2.2
molecular structure and will align with an external magnetic field independently of the orientation of the molecule. Anisotropy in K~~~~ can be introduced if the gvalue becomes anisotropic. The gvalue is in fact a tensor quantity which describes the modification to the magnetic field experienced by the electron spin arising from the electron distribution in the molecule. It is analogous to the nuclear shielding in nuclear magnetic resonance, and it contributes to the magnetic internal energy as: Umag
= g&
Y e sa Ba
Types of Magnetic Polarization
105
Thus for a uniaxial g, tensor, the paramagnetic susceptibility anisotropy and mean susceptibility can be written as:
[(R$
(gig2]
(8)
where ye is the electronic magnetogyric ratio and s, is the vector component of the electronic spin. Interaction between an electron spin and its local electronic environment changes g, from its freeelectron value of 2.0023. These interactions are termed spinorbit interactions, since they arise from a coupling between the electron spin and the angular momentum of the molecular orbitals. The principal components of the molecular paramagnetic susceptibility can be written as:
(9) Hence using Eq. (45) of Sec. 1 of this chapter for a uniaxial liquid crystal, and neglecting any biaxial local order gives for the anisotropic part of the paramagnetic susceptibility:
Care is necessary in defining the principal axes of the g, tensor, since they are determined by the local symmetry of the freeelectron spin, and therefore usually differ from the molecular axes that define the orientational order of the mesogen. A consequence of Eq. (1 1) is that there can be competition between paramagnetic and diamagnetic contributions to the macroscopic anisotropy, so the alignment of a paramagnetic mesogen in a magnetic field will be determined by the larger of Axdia and
Axpara. There is a further contribution to the molecular paramagnetic susceptibility from magnetic field induced distortion of the orbital angular momentum: this is known as temperature independent paramagnetism (TIP), and is the precise magnetic analogue of the electronic polarizability that determines the response of a molecule to a high frequency electric field. The importance of icTCTIp 9 for mesogens is yet to be established: it is only likely to be significant for molecules with lowlying excited electronic states that are connected to the ground state by magnetically allowed dipole transitions; such states are also important in the circular dichroism spectra of molecules. Taking account of all contributions to the molecular susceptibility, the components of the
106
2
Magnetic Properties of Liquid Crystals
macroscopic susceptibility for a uniaxial liquid crystal composed of uniaxial molecules can be written as:
x
~ N A K ~ ' " S~ N A K ~ I ' S 3 +
XI1 = +
L=X
N A K ~ s"  N
s
A K ~ I ~
3
2.2.3 Ferromagnetism At sufficiently low reduced temperatures, and/or strong spinspin interactions, spin magnetic moments can become ordered in a parallel array to give ferromagnetic materials, or ordered in an antiparallel fashion to give an antiferromagnetic structure. This behavior is rare in organic materials, for which ferromagnetic organization only occurs at low temperatures. There is a requirement for unpaired electron spins, and so in the context of liquid crystals, possible ferromagnetic materials will almost certainly require metalcontaining mesogens. The contribution of ferromagnetic or antiferromagnetic coupling to the susceptibility can be described in terms of a modified Curie Law, known as the CurieWeiss Law, and the isotropic susceptibility can be written as: N p o s z p ; S(S1) 3kg(T0)
xpara =
(14)
where the characteristic temperature 0, the Curie temperature, is a measure of the ferromagnetic coupling, and marks the onset of permanent magnetization. If 0 is negative, then the local magnetic interactions are antiferromagnetic and 0 is called the NCel
temperature. Although no ferromagnetic liquid crystals have been discovered so far, ferromagnetic liquid crystals can be prepared by the dispersion of ferromagnetic particles in a liquid crystal host. In preparing such systems it is desirable to make the ferromagnetic particles very small, so that each particle has a permanent magnetic moment. Normally in the absence of an external magnetic field or special conditioning, the permanent magnetization characteristic of ferromagnetic materials forms in domains of opposing magnetic moments, so that the total magnetisation is cancelled. However for sufficiently small particle sizes, the domain wall energies become relatively too high to sustain, and single domain particles are preferred. This effect is known as superparamagnetism or collective paramagnetism, and dispersed particles satisfying the requirements for single magnetic domains act in fluids as micromagnets: such systems are known as ferrofluids. The dispersion of single domain ferromagnetic particles in a liquid crystal host can form anisotropic ferrofluids or ferromagnetic liquid crystals.
2.3 Diamagnetic Liquid Crystals Most liquid crystals are diamagnetic and their magnetic anisotropy arises from the electronic structure of the mesogens. Delocalisation of electronic charge will enhance the diamagnetic susceptibility and aromatic groups in particular make a large contribution to the diamagnetic susceptibility. In Table 1 are listed molecular susceptibility components for a number of molecules to indicate the likely contributions of various groups to mesogenic structures. These values have been obtained from susceptibility measurements on single crystals.
2.3
107
Diamagnetic Liquid Crystals
Table 1. Molecular susceptibility components from single crystal measurements. Compound and molecular axes
Molecular susceptibility components
Ref.
1.19
0.44
0.44
[31
 I .46
0.99
0.82
131
1.38
0.59
0.69
[31
2.3 1
0.78
0.85
131
3.13
0.96
0.97
[31
t
m
1.13
. I
.33
[231
Table 2. Diamagnetic susceptibilities for liquid crystals. Compound and acronym
Diamagnetic susceptibilities
Ax/IO’ m’ kg’
x/l 0’ m3 kg’
1.51
8.43
[21
1.31
8.66
PI
0.46 0.42
C7H15
Ref.
141 9.32
kCN 0.38
Most thermotropic mesogens contain aromatic groups, and since the component of the diamagnetic susceptibility perpendicular to a benzene ring is greater than the inplane component, liquid crystals composed
8.87
[41
PI
of calamitic mesogens will have a positive diamagnetic anisotropy, while liquid crystals of disclike molecules will have a negative diamagnetic anisotropy. Thus calamitic nematics and smectics will tend to align
108
2
Magnetic Properties of Liquid Crystals
with their directors along the direction of an external magnetic field, while discotic liquid crystals will align with the director perpendicular to the field. Replacement of aromatic rings by saturated groups such as cyclohexyl, bicyclooctyl or alkyl chains will reduce the anisotropy of the molecular core, so that liquid crystals based on the transtranscyclohexylcyclohexyl core have a negative anisotropy due to the attached terminal groups. Some results for the magnetic susceptibilities of liquid crystals are given in Table 2.
2.4 Paramagnetic Liquid Crystals Known paramagnetic liquid crystals are based on metalcontaining mesogens, which have a variety of metal centres and coordination geometries [ 5 , 6 ] .A requirement for paramagnetism is an unpaired spin, but to have an influence on the magnetic anisotropy, there must also be a significant gtensor anisotropy. The effect of competi
tion between diamagnetic and paramagnetic contributions to the susceptibility is illustrated by the behavior of salicylaldimine complexes of copper [7, 81. These are formed from copper(I1) having a d9 electron configuration, which results in a square planar geometry around the metal centre. The gtensor anisotropy is such that (g:.)’
> f ( . n , O )
wavelength deformations parallel to the xaxis for splay, parallel to the yaxis for twist and parallel to the zaxis for bend. Under these circumstances, the angle between the director at the origin and that at position R becomes:
(89) The way in which 8(R) varies with position depends on the form of the torsional deformation applied to the liquid crystal, and in order to calculate the principal elastic constants, it makes sense to calculate the free energy density for 'normal mode' deformations, i. e. those which correspond to splay, twist and bend. These can be achieved easily by confining the director to a plane, and assuming the undisturbed director at the origin to be along the zaxis. q is the wavevector of the deformation, and for q constrained to the x, z plane, the components of the director as a function of position become:
qz bend Gelbart and Ben Shaul have shown that a more consistent director distribution giving rise to normal mode elastic deformations is:
I
qx(l+ qz1l splay tanO(R)= qy twist qz(1 qx)' bend
1
qxu  42) splay or B(R)= qy twist qz (1 + qx) bend
(90)
Substituting these results into Eq. (88) gives:
n, = sinq . R; ny = 0; n, = cosq . R Director configurations corresponding to pure splay, twist and bend are illustrated in Fig. 16 and to the lowest order of approximation can be described in terms of long
f The macroscopic expression for the elastic free energy density (Eq. 25) is: 1 2v
g  go =  J k ,
' ( V . n)2 + k2
+ k3 3 ((n V>nI2dR '
Figure 16. Deformations of director for splay, twist, bend.
2
(n. v x n)2 (92)
Using the expressions for 8(R) corresponding to pure splay, twist and bend deformations gives the result:
5.5
1;
L
g go =
1
~
k2 q2 twist
(93)
k3 q2 bend
Combining Eqs. (91) and (87) and equating the result for the free energy density to the macroscopic expression Eq. (93) gives:
Molecular Aspects of Torsional Elasticity
175
theory, are a single particle angular distribution function, an attractive intermolecular potential and a hard particle pair distribution function. An immediate result of the above theory is that since the elastic constants depend on the product of single particle orientational distribution functions, they will depend on the product of order parameters.
5.5.2 Results from Lattice Models For the simplest distribution function, only the term involving the second derivative in Eq. (94) is nonzero, and the torsional elastic constants are given by an average over the square of the intermolecular distances x, y and z. Since macroscopic uniaxiality is assumed, the averages over x and y , perpendicular to the undisturbed director, will be equal, with the result [43]:
,
k , = k22 =constant p 2 S 2 b ( x 2 ) and
k , , =constant p2S2b(z2) The two terms in the square brackets of Eq. (94) can be identified as a temperature independent internal energy term, and a temperature dependent entropy term resulting from the hard particle pair distribution function. From this equation it can be seen that the calculation of the principal elastic constants of a nematic liquid crystal depends on the first and second derivatives with respect to the angle 8 of the single particle orientational distribution function. Any appropriate angular function may be used forf(Ql, 8(R)), but the usual approach is to use an expansion in terms of spherical harmonics. The necessary mathematical manipulations are complicated, but give relatively compact results. Thus the ingredients of a molecular calculation of torsional elastic constants within the van der Waals
(95)
where b is an energy parameter. If a lattice model is assumed, then the averages over x and z will relate to the unit cell dimensions, or the dimensions of an 'interaction volume'. The result, Eq. (95), fails to account for the observed difference between splay and twist elastic constants, and it fails to provide a useful basis for investigating the effects of molecular structure on elastic properties.
5.5.3 Mean Field and Hard Particle Theories The first attempt at a molecular theory of elastic constants due to Saupe and Nehring [44] assumed an attractive pair potential of the form u I 2 =  b r  6 P2(c0s812), and set
176
5
Elastic Properties
gl:;, equal to that for hard spheres of diameter 0,with the result that:
This suggests that the elastic constants for splay and bend should be equal. The difference between k , and k , , has been identified as due to a term in (P2(cos8)) (P4(cos6)), and while this usually leads to k , , > k , particular choices of intermolecular potential can result in k , , < k , or indeed
,,
a change in sign of the quantity
,
[lk: ~

I] as a function of temperature [45]. Various authors [46, 471 have reported calculations of torsional elastic constants for hard spherocylinders. These neglect any attractive interactions, and so only give entropic contributions to the elastic free energy; their results can be summarized as:
where k =  1( k , , + k , , + k , , ) , and A and A’ 3 depend on the details of the potential. For hard spherocylinders, the parameters A and A’ are:
9 (3R2  8) A = 2 R 2  2 and A’= (98) 7 R2 + 20 16(7R2+20)
where R + 1 =(Zlw); 1 is the length and w is the width of the spherocylinder. Calculations of the principal elastic constants for various molecular models, with both attractive and repulsive interactions have been reported by various authors [48  521.
5.5.4 Computer Simulations Some progress has been made in computer simulation of torsional elastic properties [53, 541. A variety of methods is available for modelling elastic distortions, but the most used technique is based on the direct calculation of the amplitude of director fluctuations. In Sec. 5.2.2 of this Chapter the background to long range director fluctuations was outlined, and it was found that the mean square amplitude of the director component along z could be expressed in terms of the splay and bend elastic constants and the wave vector for a particular deformation mode (it is assumed that for the undistorted liquid crystal, the director lies along the z axis). In order to allow for the influence of local molecular disorder, the fluctuations in the director order parameter are calculated, assuming that for long wavelength fluctuations, the molecular order parameter simply scales the director order parameter. Thus the Fourier components of the order parameter are written as:
Qap ( 4 ) = (p2 (cos8)) ( 3 3 n f f (4)np ( 4 ) Solp 1) (99)
Using the results Eqs. (38) and (39) give expressions for the fluctuation in the order parameter as [53]:
Experimental Aspects of Elastic Constants and Comparison
5.6
0.0
I
375
'
380
I
I
I
I
385 390 395 400 Temperature (K)
I
405
I 410
Figure 17. Comparison of calculated and theoretical elastic constants for pazoxyanisole [ 5 3 ] (units are lo" N).
where ql,and q1 are the components of the distortion mode wave vector parallel and perpendicular to the undisturbed director. Comparisons between theory and experiment are encouraging (see Fig. 17), although sometimes at the expense of assuming rather high values for the local molecular order parameters; this is attributed to a weakness in the theory which neglects longrange correlations [ 5 3 ] .
5.6 Experimental Aspects of Elastic Constants and Comparison with Theoretical Predictions The statistical theories of elasticity have shown that the principal elastic constants depend on the single particle distribution functions and the intermolecular forces. The former can be accounted for in terms of order parameters, but intermolecular parameters are more difficult to interpret in terms of molecular properties. Results for hard particle potentials relate the elastic constants to particle dimensions, but the depen
177
dence of elastic properties on details of molecular structure is more obscure. Measured values for the torsional elastic constants of nematics are of the order of lo', N, corresponding to k T ( 4 x lo*' J)/l(lOy m), where T = 300 K and 1is a molecular dimension. The effect of elastic distortions on molecular interactions is very small, so that the assumption of strainindependent distribution functions is justified. For example the elastic energy in a 1 pm liquid crystal 2 nematic cell is only film in a ~ 1 twisted =l OP2' Jlmolecule, which compares with an intermolecular energy of about lop2' JI molecule. The angular displacement per molecule in such a cell is lo' rad, and the small energies associated with such torsional strain mean that direct mechanical measurement of elastic constants in liquid crystals is difficult. Indirect experimental measurements of torsional elastic constants indicate that for many materials k , , > k , I > k 2 2 . It is usual to consider ratios of elastic constants, and most measured values lie in the ranges 0.5 < k , , / k , < 3.0 and 0.5 < k 2 , / k l < 0.8. Simple mean field theory predicted that k 3 , = k l I < k , , , which is clearly in error. For rigid molecules increasing the molecular length increases k3,Ikl while increasing the width decreases k 3 , / k I I , in qualitative agreement with the results of hard particle theories. However within a homologous series, increasing the length of an alkyl chain causes the ratio k,,lk, to decrease, which is likely to be a result of increased flexibility rather than any change in effective shape. For SmA phases the torsional elastic constants for twist and bend are expected to be very large, and it is observed that k , , and sometimes k,, measured for a nematic phase increase dramatically with decreasing temperature as an underlying smectic phase is approached. Shortrange smecticlike ordering will influence the measured elastic
178
5
Elastic Properties
constants; long alkyl chains promote smectic phase formation, and as a result k33/klI may increase in a homologous series with increasing chain length. The main temperature dependence of elastic constants is due to the order parameter. Following the predictions of mean field theory Eq. (96), reduced elastic constants ci have been introduced, which should be independent of temperature, defined by:
Experimentally the cis do change with temperature, and this can be attributed to the influence of repulsive interactions on the elastic properties.
5.7
References
[I] C. W. Oseen, Trans. Faraday Soc. 1933,29,883. [2] F. C. Frank, Discuss. Faraduy Soc. 1958,25, 19. [3] P. G . de Gennes, J . Prost, The Physics ofLiquid Crystals, Oxford University Press, Oxford, 1993, p. 98. [4] G. Vertogen, W. H. de Jeu, Thermotropic Liquid Crystals, Fundamentals 1988, p. 74. [5] Ref. [3], p. 341. [6] Ref. [3], p. 349. 171 R. D. Polak, G. P. Crawford, B. C. Kostival, J. W. Doane, S. Zumer, Phys. Rev. E 1994, 49, R978. [8] J. Charvolin, J. F. Sadoc, J . Phys. Chem. 1988, 92, 5187. [9] J. Nehring, A. Saupe, J. Chem. Phys. 1971, 54, 337. [lo] F. M. Leslie, I. W. Stewart, M. Nakagawa, Mol. Cryst. Liq. Cryst. 1991, 198, 443. [ I I ] Ref. [ 3 ] ,p. 351. [I21 Ref. [3], p. 74. [I31 S. Chandrasekhar, G. S. Ranganath, Adv. Phys. 1986, 35, 507. [ 141 M. Kleman, Liq. Cryst. 1989, 5, 399. [I51 T. E. Faber, Liq. Cryst. 1991, 9, 95. 1161 B. J. Berne, R. Pecora, Dynamic Light Scuttering, John Wiley, New York, 1976, p. 27. [ 171 S. Chandrasekhar, Liquid Crystals, Cambridge University Press, Cambridge, 1992, p. 167. [ 181 J. P. van der Meulen, R. J . J. Zijlstra, J . de Phys. 1984,45, 1627. 1191 J. H. Seddon, R. H. Templer, Phil. Trans. R. Soc. Lond. A 1993,334,377.
[20] V. FrCedericksz, V. Zolina, Trans. Faraduy Soc. 1933, 29, 919. [21] J. Nehring, A. Saupe, J. Chem. Phys. 1971, 54, 337. (221 A. J. Derzhanski, A. G. Petrov, M. D. Mitov, J . de Phys. 1978,39, 272. [23] T. Motooka, A. Fukuhara, K. Suzuki,Appl. Phys. Lett. 1979,34, 305. [24] T. Motooka, A. Fukuhara, J. Appl. Phys. 1979, 50, 6907. [25] Ref. [4], p. 94. [26] H. J. Deuling, Sol. State Phys. Suppl. 14 (Liquid Crystals), Ed.: L. Liebert, Academic Press, London 1978, p. 77. [27] F. M. Leslie, Mol. Cryst. Liq. Cryst. 1970, 12, 57. [28] H. J. Deuling, Mol. Cryst. Liq. Cryst. 1974, 26, 281. [29] C. Maze, Mol. Cryst. Liq. Cryst. 1978,48, 273. [30] M. J. Bradshaw, E. P. Raynes, Mol. Cryst. Liq. Cryst. 1983, 91, 145. [31] H. J. Deuling, Sol. Stat. Commun. 1974, 14, 1073. [32] M. G. Clark, E. P. Raynes, R. A. Smith, R. J. A. Tough, J. Phys. D. 1980, 13, 2151. [33] T. Uchida, Y. Takahashi, Mol. Crysr. Liq. Cryst. 1981, 72, 133. [34] G. Barbero, Z. Naturforsch. 1984, 39a, 575. 1351 L. M. Blinov, Electrooptical und Magnetooptical Properties of Liquid Crystuls, J. Wiley, Chichester, 1983, p. 240. [36] V. G. Chigrinov, Kristallogrufiya 1988,33,260. [37] Ref. 131, p. 364. [38] Ref. [ 3 ] ,pp. 347, 376. [39] S. P. A. Gill, F. M. Leslie, Liq. Crysr. 1993, 14, 1901. 1401 W. M. Gelbart, A. BenShaul, J . Chem. Phys. 1982, 77, 916. [41] W. M. Gelbart, J. Chem. Phys. 1979, 71, 3053. 1421 M. A. Cotter, J. Chem. Phys. 1977, 66, 4710. [43] H. Gruler, 2 Nuturforsch. 1975, 3012,230. [44] J. Nehring, A. Saupe, J. Chem. Phys. 1972, 56, 5527. [45] W. M. Gelbart, J . Stecki, Mol. Phys. 1981, 41, 145 1. [46] R. Priest, Phys. Rev. 1973, A7, 720. [47] J. P. Straley, Phys. Rev. 1973, A8, 2181. [48] A . Ponerwierski, J. Stecki, Mol. Phys. 1979,38, 1931. [49] H. Kimura, M. Hoshino, H. Nakano, Mol. Cryst. Liq. Cryst. 1981, 74, 55. [50] B. W. van der Meer, F. Postma, A. J. Dekker, W. H. de Jeu, Mol. Phys. 1982,45, 1227. [51] Y. Singh, S. Singh, K. Rajesh, Phys. Rev. 1992, A44, 974. 1521 M. A. Osipov, S. Hess, Mol. Phys. 1993, 78, 1191. [53] B. TjiptoMargo, G. T. Evans, M. P. Allen, D. Frenkel, J . Phys. Chem. 1992, 96, 3942. 1541 M. A. Osipov, S. Hess, Liq. Cryst. 1994,16,845.
6 Phase Transitions 6.1 Phase Transition Theories Philippe Barois
6.1.1 Introduction The understanding of continuous phase transitions and critical phenomena has been one of the important breakthrough in condensed matter physics in the early seventies. The concepts of scaling behavior and universality introduced by Kadanoff and Widom and the calculation of nongaussian exponents by Wilson and Fisher are undeniably brilliant successes of statistical physics in the study of low temperature phase transitions (normal to superconductor, normal to superfluid helium) and liquidgas critical points. But no other field in condensed matter physics has shown such a rich variety of continuous or weakly firstorder phase transitions than liquid crystals: order parameters of various symrnetrics, anisotropic sealing behaviors, coupled order parameters, multicritical points, wide critical domains, defect mediated transitions, spaces of low dimensionality, multiply reentrant topologies are currently found in liquid crystals, at easily accessible temperatures. Beside their famous technical applications in optics
and electronic displays, liquid crystals can certainly be regarded as a paradise of the physics of phase transitions. The main features of the most general phase transitions encountered in liquid crystals are presented in this section.
6.1.2 The IsotropicNematic Transition 6.1.2.1 Mean Field Approach (Landaude Gennes) The nematic phase being the liquid crystal of highest symmetry, its condensation from the isotropic liquid should be the simplest to describe. Indeed, molecular theories convincingly explain the natural onset of nematic ordering in a population of anisotropic molecules with excluded volume interaction (Onsager) or in mean field theory (MaierSaupe). Regarding the effect of symmetry on the isotropic to nematic (IN) phase transition, the phenomenological approach is useful too. It was explained in Chapter I11 of this volume that the order parameter of the nemat
180
6.1
Phase Transition Theories
ic phase is a symmetric traceless tensor Q , that can be constructed from any macroscopic tensor property such as the magnetic susceptibility xii. For a uniaxial nematic for instance, the order parameter can be defined as [I]: QIj
$XI, 1 +2xI)s,)
(1)
x
in which xll and are susceptibilities parallel and perpendicular to the director respectively and 6,] is the Kronecker unity tensor. The normalization constant G is generally chosen to ensure Q,,= 1 for a perfectly ordered nematic. Such normalization suggests that Q,, is similar to the scalar order parameter S defined in microscopic theories from the statistical distribution of molecular axes (see Chap. 111, Sec. 1 of this volume). This is not exactly true, however, since macroscopic quantities may not be a simple sum of uncorrelated microscopic susceptibilities (think of dielectric polarizability). Consequently, macroscopic nematic order parameters Q,, defined from different macroscopic tensor properties (such as magnetic susceptibilities and refractive indices) may not show the same temperature behaviour. Experimental differences are, however, very weak [ 2 ] . In the eigenframe, the Q, matrix reads [I]:
xrJ
The phenomenological scalar order parameter q = Q,, is nonzero in nematic phases and vanishes in the isotropic phase. 77 is nonzero in biaxial nematics only and referred to as the biaxial order parameter. The symmetric invariants of Q, may be written as [ I , 31:
0 3 = 4Qij Qjk Qki = 9(q2  V 2
(3)
The second and third order invariants can be regarded as independent in the biaxial phase with the constraint < 0;. Equality 0: = is reached in the uniaxial nematic. A Landaude Gennes free energy may now be expanded in powers of the two invariants 0, and 0, [ l , 351:
032
02
AF = FN  &,
(4)
= a 0 2 + b o g +  C1C T ; 2
+do203 +eo3 1 2 2
Uniaxial Nematic The most common case of uniaxial nematics can be treated first: the free energy expansion reduces then to [ 11: 1
~ ~ i n i a x i= a l2A ( T ) q 2
+ T1 B q 3
+qcqJ 1 +0(q5)
(5)
As usual with Landau theories, the phase transition is governed by the coefficient of the quadratic term A ( T )=a(TT*). Other coefficients B and C are supposed to have weak temperature dependance. The presence of a third order term, imposed by the symmetry, drives the transition first order [ 1, 61 at a Landau temperature TNI determined by 2B2=9aC(TNIT*).It must be emphasized that such third order term reflects the physical relevance of the sign of q: think about a nematic arrangement of long rods with director n parallel to reference axis 2, q > 0 corresponds to long axes lining up along 2 whereas q < O corresponds to rods parallel to the (x,y) plane with no angular order in this plane. If the first case is, of course, physical for rods, the second is more appropriate for discs. Corresponding uni
6.1.2 The IsotropicNematic Transition
axial nematic phases are often called cylindric and discotic respectively [4, 51. Below 7'Nr,the order parameter varies as:
in which T** is the absolute limit of superheating of the nematic phase. The order parameter at the transition is:
3a (TNI 7'") qc =  (7) B Experiments do confirm the first order character of the IN transition: discontinuities are observed but are weak enough to justify the relevance of the Landau expansion. Biaxial Nematic The stability of biaxial nematics is calculated by minimizing the free energy (Eq. 4). The stability of the model requires c>O, e > 0 and ce > d2 (higher order terms have to be considered in the expansion otherwise). The absolute minimum of AF is straightforwardly obtained at [ l , 3, 51: I
0 2 =
~
bdae ce  d 2
 = adbc and o3 ce  d 2 ~

Finally, the transition lines from uniaxial nematic to biaxial are determined Eq. (8) with the constraint Oil2= 6iJ3. At lowest order in b, the slope of the two lines at their meeting point a = b = 0 is given by:
The complete phase diagram is obtained with the selection rule 62 2 6.32 and reproduced in Fig. 1 [ 11. Note that a direct transition INb occurs at a single point a = b = 0 on the line (Eq. 10) [7]. The biaxial nematic region separates two uniaxial nematics N, and N_ of opposite sign. N+N, transitions are second order since the condition 4 / 2 = ( j y 3 can be approached continuously from the biaxial phase. Experiments on lyotropic systems [4, 51 do confirm the existence of a biaxial nematic phase separating two uniaxial nematics of opposite birefringence. Experimental features are in good agreement with the Landaude Gennes mean field approach. If the condition c e >d2 is not satisfied, the minimum energy is clearly obtained with 0, as large as possible within the limit
(8)
The phase diagram is calculated in the (a, b ) plane, as usual with Landau theories. The various possible transition lines are obtained as follows: 
I
The first order isotropicuniaxial nematic corresponds to the set of constraints A F = O and ~ i / ~ = o : / At ~ =first q . order in b, its equation is:
(9) 
181
The isotropicbiaxial nematic line is determined by AF=O and independent 0, and 0,which leads to the trivial equation: aIN,,=+b
C

le
(10)
1 Figure 1. Phase diagram in the a, b plane resulting from minimization of Eq. (4) with biaxiality in the case c e < d 2 .N, andNare uniaxial nematics with positive and negative order parameter respectively. N, is a biaxial nematic. Solid lines are firstorder transformations, dashed lines are secondorder transformations.
182
’ 6. I
Phase Transition Theories
$ > (y2.(y  (y3 is then the physical limit in this case and the biaxial domain is replaced by a direct first order transition from a positive to negative nematic [ 11.
6.1.2.2 Fluctuations Like for any weakly first order phase transition, the mean field approach is expected to fail close to the temperature of transition TNI when fluctuations of the order parameter reach correlation lengths much larger than molecular sizes. Spatial variations of the order parameter are classically accounted for by adding a gradient term % L (Vq)2 to the expansion (Eq. 5 ) and taking the new expression as a local Hamiltonian ( L is a positive Landau coefficient). Up to second order in q, the model is exactly soluble (Gaussian model) but has no condensed phase (it becomes unstable for A(T)Tp.I>T*. The first step beyond mean field and Gaussian approximations is to expand the partition function in powers of the interaction (i.e. terms of order higher than 2 in q ) and integrate over Gaussian fluctuations. It is a standard result that such perturbation expansion presents infrared divergences (i.e. for wavenumber k + O ) in three dimensions [8]. It can be used, however, to estimate the critical domain TGinzT * , TGinzbeing the Ginzburg temperature at which the lowest order contribution of the interaction is of order the mean field value [ 1, 9, 101:
tG
(
L 7B2kBT TGinr T* = a 4n2L3
213
)
Experimental estimates of B lead to a noticeable critical domain (TGinzT*of order 1 to 10 K [l]). Significant deviations from mean field predictions are indeed commonly observed [ 111. For instance, the differ
ence (T**T,,) is smaller than its mean field value B2/36aC which shows that fluctuations decrease the effective value of B. Note that this leads to underestimate the critical domain by setting the experimental value of B in Eq. (12). The divergences of the perturbation expansion can be overcome by length scale transformations of the renormalization group method [ 121.Each step of the process consists in integrating out fluctuations of large wavenumber k close to the upper cutoff A, say Al b
x, and zL are two dimensional vectors in the plane (x, y) and (qx, qy) respectively. The mean field free energy density reads:
AFNs~As~c

For C, 0, Z(q)has peaks at qI1= f Qll corresponding to fluctuations into the SmA
with CII, Dll, D,, and u > 0 and a =
In Fourier space, AFNSmASmCreads: N
AFNs~As~c
x
w2+ u w 4
/
(43)
where Qi= ClI/2Dll. The free energy (Eq. 43) is minimized the usual way : 
I
For C,>O, the minimum is reached for q L = O and q r O f q , , . A second order NSmA transition occurs at the mean field temperature T= TNSmA.
Figure 2. NSmASmC phase diagram from Chen and Lubensky [46]. All transitions are second order in mean field but fluctuations lead to a first order NSmC transition [47]. The line C,=O separates two regions in the nematic phase with diffuse Xray scattering centered about yL=O (CLzO) and ql+O (C, p = p o ( r ) + p 6 ( r ) cos 4 ( 8 + higher harmonics
$1 (44)
r is a 2d vector of Cartesian coordinates x = r cos 8 and y = Y sin 8. The correlation function of the radial distribution p o ( r )falls
192
6.1 Phase Transition Theories
off exponentially in the SmB and SmA phases. The amplitude P6(r) describing the sixfold order vanishes in the SmA phase only. A possible order parameter of the SmASmB transition is therefore:
Frank energy, is n . curl n (=  2 nlP in the example of a simple cholesteric helix). A natural extension of the Frank energy density to chiral nematics is [ l , 591:
(47) The phase @accountsfor spatial fluctuations of the orientation of the local sixfold axes. The order parameter v6 has two components and the SmASmB transition is expected to belong to the X Y universality class. Experiments do confirm the second order nature of the transition but high resolution a.c. calorimetry gives values of the specific heat exponent a about 0.6 [57] inconsistent wih theXYclass (a = 0.06). High sensitivity heat capacity measurements on freely suspended thin films (down to four layer) show a crossover from bulk (a=0.59) to a two dimensional cusplike behavior with a = 0.26 [58].
6.1.6 Phase Transitions in Chiral Liquid Crystals 6.1.6.1 Chirality in Nematic and Smectic Liquid Crystals Experiments show that the introduction of chirality (chiral mesogen or chiral dopant) in a nematic phase generates a spontaneous twist of the director, n=(cos2n:zlP, sin 2 nz / P , 0 ) for instance for a helical twist of pitch P along the direction z. The higher the chirality (i.e. fraction of chiral dopant for instance), the higher the twist (i.e. the shorter the pitch). It is thus clear that twist is a structural response coupled to the microscopic constraint chirality. How can these two physical quantities be linked in a quantitative way? The covariant expression of the local twist, commonly used in the
+(nxcurl K3 2
n)2 hn.curl n (48)
in which the field h coupled with the twist is a measure of the chirality. In the superconductor analogy, h is analogous to the magnetic field H imposed by external currents (or more exactly, to the component of H along A; other components are coupled to bend). In cholesterics, no other energy depends on twist and Eq. (48) is minimum (=h2/2K,) for the helical solution of pitch P =2 nK,lh = 2 nlko: n = (sin 2 n z l P , cos 2 n z l P , 0) which satisfies V . n = 0, n x curl n = 0 and nscurl n = hIK,. Note that the pitch then gives a measure of the chirality. The sign of h reflects the handedness of the helix. In defectfree smectic phases of constant layer thickness d, twisted arrangement of the layers are forbidden as can be shown easily: let A and B be two points in a smectic phase and N (r) the (oriented) layer normal at position r. The (algebraic) number of layers crossed along a path going from A to B
B is Id'.
[f)independent of the path A B.
A
This property implies that there exists a potential $such as Nld= V@whichin turn leads to curl ( N l d ) = 0. In a SmA phase, the layer normal N identifies with the director field n so that curl n = 0: twist and bend cannot develop on a macroscopic scale. The penetration of twist requires either nonuniform layer thickness d(r) (which can be achieved on a limited scale: the twist penetration
6.1.6 Phase Transitions in Chiral Liquid Crystals
depth &, Eq. (23))or defects such as dislocations which make pathdependent the inB
. In mean field, n * curl n = 0 A
everywhere in the SmA phase with no defect and Eq. (48)implies that the free energy density of the cholesteric phase is decreased by the twist term  h2/2K, with respect to the untwisted SmA. The cholesteric to SmA transition becomes first order at a temperature TN*A = TNA I h Ila lower than TNA (u, and a are defined from Eq. (17)). In a SmC phase, the layer normal N no longer coincides with the director field n. Nonzero twist and bend (i.e. curl n#0) are permitted. The well known structure of the director helix is n (r) = (sin 8 cos 2 n z l P , sin 8 sin 2 nzIP, cos 8) for a layer normal along z and a SmC tilt 8 (Nn=cos8).The twist and bend terms of the Frank energy are:
(49)
Note that the gain in twist energy associated with the SmC* helix is coupled to a loss in bend energy. Phase transitions between chiral phases will be described below in the frame of the mean field approximation.
6.1.6.2 Mean Field Chiral NSmASmC model The chiral version of the NSmASmC model of Chen and Lubensky was investigated by Lubensky and Renn [59]. The mean field free energy density is: (50) AFNSmASmC*
= mNSmASrnC
smectic order parameter, AFNSmASmCreduces to Eq. (42).It is more convenient to define the z axis along the layer normal in the smectic phases:
(51) y(r>= yoeik.' = v, eikz with k = (0, 0, k)
and the director n as:
n = (sin8 cos@,sin8 sin@,cos8)
(52)
yo,k, 8,and @ are then treated as variational parameters. The important parameter is cos 8= n klk independent of the choice of the coordinate system. The three phases of interest are thus characterized by: 1//0=0,
8 = E , V,@=ko 2
for the N* phase ~0 $0, 8 = 0 , k = q 0 for the SmA phase
vO+o,e+o,?2
k+qO
(53) where k, = h/K2= 2 ZIP and qo is the wavenumber of the SmA phase. Using Eqs. (51) and (52)in the free energy density, Renn and Lubensky obtain: for the SmC* phase
In. curl n/= 2n sin . 28 P In x curl nl = 2nsin 8cos 8 P
193
Chiral
IAFFrank
in which AFNSmAsmC is the smectic part of the NSmASmC model and AFgYi;' is given by Eq. (48).In the simplified version of the mean field model (Eq. 41) of the
(54)
AFN*SmASmC*
+ CI, (kcos0  q 0 l 2 lv012
+ (C,k2 sin2 8 + DLk4sin4 8)lvo12 1 + K(8)sin28(Vz@)2 +hsin28(Vz@) 2 where a = a'(T
TNsmA)
and
K(8)= K, cos28+ K2 sin28
(55)
Equation (54)forms the basis for the derivation of the N*SmASmC* phase diagram. Rather than using k and 8as independent parameters, it is convenient to use kll= k cos 8 and k,= k sin 8. Straightforward minimization with respect to k and V, @ yields:
194
6.1
Phase Transition Theories
and the free energy density is finally a function of only two variational parameters tan 0 and yo: AFN*SmASmC*
= a i y 0 i2
+12 4 ~ 0 i 4
+ (c, 902 tan2 e + D~ 904 tan4 e)Iy012 1 h2 tan2 8 2 K3 1+(K21K3)tan28
SmACmC* line is second order: the director tilt 0 grows continuously at finite twist V, $ = 2 d P =  h / K , across the SmASmC* transition (Eq. 56 with 19=0). It is interesting to calculate the value of the Ginzburg parameter K = 4 1 5 that controls the transition from type I to type I1 behavior. With the coherence length { and the twist penetration depth given by Eqs. (22) and (23), one gets:
(57)
(59)
The final minimization is somewhat tedious but presents no difficulties [59]. The equations for the phase boundaries are
diverges in the vicinity of the NSmASmC point where C , vanishes. The type I1 condition is thus expected to be fulfilled close to the NSmASmC point. In presence of chirality, this is precisely the place where a liquid crystal analog of the Abrikosov flux phase should show up. The structure of this new liquid crystalline state will be described in subsequent section.
/
\I12
K
6.1.6.3 Twist Grain Boundary Phases Structural Properties
The N*SmASmC* phase diagram is shown in Fig. 3 . The N*SmA and N*SmC* lines are first order whereas the
U
N*
I
Figure 3. Chiral N*SmASmC* phase diagram from Lubensky and Renn [ 5 9 ] .Solid lines are first order and dashed lines second order.
The most spectacular outcome of the analogy with superconductors is undoubtedly the identification of twist grain boundary smectic phases (TGB for short) as liquid crystal analogs of the Abrikosov flux phase in type I1 superconductors. The existence and structural properties of the TGB phases were first predicted theoretically by Renn and Lubensky [60] (RL) in 1988 and discovered and characterized experimentally by Goodby and coworkers shortly after [26, 611. The highly dislocated structure of a TGB phase is shown in Fig. 4. Slabs of SmA materials of thickness lb are regularly stacked in a helical fashion along an axis fi parallel to the smectic layers. Adjacent slabs are continuously connected via a grain boundary constituted of a grid of parallel equi
6.1.6 Phase Transitions in Chiral Liquid Crystals Screw Dislocations
Grain Boundaries
Smectic Layers
Figure 4. Structure of the TGB phase (from [60,62]).
spaced screw dislocation lines analogous to magnetic vortices. The finite twist angle of each grain boundary is A 8 = 2 sin' (dl2 Id) where d is the smectic period and Id the distance between parallel screw dislocations within a grain boundary. Twist penetrates the smectic structure just as magnetic induction penetrates the type I1 superconducting phase via the Abrikosov lattice of magnetic vortices. The difference lies in the lattice structure: two dimensional hexagonal packing of parallel lines for superconductors, twisted array of rows in TGBs. RL pointed out that the crystallographic nature of a TGB stack depends on the ratio of the slab thickness to the helical pitch 1 h l P (or equivalently A812 n).If the ratio 1 h l P is rational (=plq with p , q mutually prime integers) the structure is periodic of period p P = q l,, with qfold symmetry about the 2 axis. Such TGB stack is referred to as commensurate. Reciprocal space is formed of q equispaced Bragg spots distributed on rings of radius 2 n l d in planes qy,qL.If q differs from crystallographic values 2 , 3 , 4 or 6, the commensurate TGB structure is quasicrystalline rather than crystalline. If on the other hand &/P is irrational, the TGB stack is nonperiodic (or incommensurate). The scattering is dense on a ring of radius 2 nld and axis q x .Reciprocal spaces of the commensurate and incommensurate TGB phases are consequently qualitatively different.
195
On the experimental point of view, a TGB structure is characterized by five parameters (d, P, lh, Id and A8) linked by two structural relations: (60) A 8 = 2sin'(d12ld) and 1!L = A812n P Full experimental characterization requires measurement of three independent parameters. The layer spacing d (of the order of 3 to 4 nm) and the helical pitch P (a few pm) are easily deduced from Xray and optical measurements. The third parameter can be the twist boundary angle A 8 which can be measured in the case of commensurate TGB only. For incommensurate TGB [61], other parameters are inferred from the RL theoretical estimate & = Id which yields 1, and 1, of the order of a few tens of nm and A8about 15". Critical Fields hCl and hcZ The thermodynamic critical field h, above with the SmA phase becomes globally unstable to the N* phase at some temperature TN*SmAlower than To follows from Eq.
(5th):
The critical fields h,, and hc2 of the SmATGB and TGBN* transitions were calculated by RL from the superconductor model. The lower critical field h,, is reached when the SmA phase becomes unstable to the formation of TGB, that is when the gain in twist energy compensates the cost in the formation of grain boundaries. On the other hand, the upper critical field hc2 corresponds to the stable growth of a nonzero smectic order parameter in the N* phase,
196
6.1
Phase Transition Theories
that is the inverse susceptibility of the smectic order parameter changes sign. The result is [60]:
hc2 = \ 2 K h c ( l + O ( k o / q o ) )
(62)
For large enough ic(i.e. type I1 condition ic > 1/.\/2), hCl 0.
SAMPLE
6.2.1.3 Experimental Methods Differential Scanning Calorimetry Differential scanning calorimetry (DSC) is by far the most commonly used thermal technique for studying liquid crystals. It is a very useful and sensitive survey technique for discovering new phase transitions and for determining the qualitative magnitude of thermal features. However, DSC is not well suited for making detailed quantitative measurements near liquid crystal phase transitions. The reason for this can be understood by considering Fig. 2. In Fig. 2(a) representative enthalpy curves for a firstorder and secondorder transition are given. In part (b) the corresponding DSC responses (for heating runs) are compared. In a DSC measurement, a constant heating (or cooling) rate is imposed on a reference sample, which results in a constant and rapid temperature ramp (see Fig. 2). A servosystem forces the sample temperature to follow that of the reference by varying the power input to the sample. What is recorded then is the differential power dHldt (between reference and sample), and the integral j(dHldt)dt for a DSC peak approximates the enthalpy change associated with the corresponding
Ttr
Tm
T (t)
Figure 2. (a) Schematic representation of the temperature dependence of the enthalpy Hof aliquid crystal sample near a firstorder (solid curve) or secondorder (dashed curve) phase transition at Ttr. The dasheddotted line gives the enthalpy of a (DSC) reference material with a nearly constant heat capacity and without a phase transition. (b) Corresponding DSC responses (from heating runs) for the firstorder (solid curve) and secondorder (dashed curve) cases of part (a).
transition. However, as can be seen in Fig. 2(b) the DSC response is very similar for a firstorder transition with latent heat AHL and a secondorder transition with a comparable integrated enthalpy change 6 H . The broadening of the DSC signal for the firstorder case is due to the fact that the latent heat cannot be delivered to the sample instantaneously. The DSC response will be at a maximum for a temperature T, well above T,, for a heating run and well below T,, for a cooling run. The difference between T , and T,, depends on the scan rate that is chosen. The DSC response for a secondor
6.2.1 Thermal Methods
der transition, given by the dashed curve in Fig. 2(b) is qualitatively the same. It is thus very difficult to distinguish between firstand secondorder transitions and almost impossible to detect the difference between the latter ones and a weak firstorder transition with significant pretransitional specific heat capacity variation. Furthermore, there is additionally a problem of thermodynamic equilibrium with DSC instruments. Although slow rates of the order of 0.1 K min' are possible, the best operational conditions of DSC machines are realized for fairly rapid scan rate (above 1 K minI). However, many liquid crystal phase transitions require scan rates which are typically two to three orders of magnitude slower than slow DSC scans.
Traditional Adiabatic Calorimetry The classical method for measuring the specific heat capacity of a sample as a function of temperature is called adiabatic calorimetry and carried out by the stepwise addition of accurately measured small increments of electrically supplied heat [ 14, 151. The heat capacity (at constant pressure p ) , C,, of a sample can be obtained from the measured total heat capacity
AQ c, = C p + C h==AT
AH
(7) AT provided the heat capacity of the sample holder, Ch, has been independently determined in a calibration experiment. In the experiment a known amount of heat AQ is thus applied and the corresponding temperature rise ATmeasured. This AT step has of course to be sufficiently small compared to the curvature of the H ( T ) curve at a given (average) temperature T, especially near a transition, which makes the method somewhat tedious and slow. Anisimov and coworkers [2,16] have mainly used this method for the investigations of liquid crystals.
213
Adiabatic Scanning Calorimetry Much of the intrinsic difficulties with DSC measurements and the tedious data collecting process of traditional adiabatic calorimetry can be avoided by adiabatic scanning calorimetry. In this technique a measured heating power is continuously applied to (or extracted from) the sample and sample holder. It was used in the 1970s for the study of liquidgas [ 171 and liquidliquid critical points [ 181 and first applied to liquid crystals by us [19] and later also by Anisimov et al. [20]. In the dynamic modes the total heat capacity C , is now given by:
In Eq. (8) the total heating power P I has been divided in two parts: Pf the power applied electrically to a heater, heating the sample and sample holder, and P: representing leaks with an (adiabatic) shield surrounding the sample holder. For cooling runs P: has to be given a controlled negative value. By keeping P I or f, constant, combined with increasing or decreasing the sample temperature, four practical modes of operation are obtained [3,21]. These modes require different settings for the servosystems controlling the temperature and maintaining adiabatic conditions, or a controlled heat transfer between sample holder and shielding. The most interesting operating conditions are the ones with constant heating or cooling power ( P I constant). As will be pointed out, this has distinct advantages at firstorder transitions. On the other hand, in modes in which f,is kept constant, one runs basically into the same kind of problems as in case of the DSC technique, even if one uses substantially lower scanning rates. It is sufficient to consider here only the constant heating mode (the constant cooling mode is analogous). In this case P I =
214
6.2
Experimental Methods and Typical Results
Pe and P: is kept negligibly small. In order to obtain the heat capacity of the sample one has to measure P;, f, and C,. Pt is easily obtainable from a measurement of the d.c. current through and the voltage drop across the heating resistor on the sample holder. The rate f,has to be obtained by numerical differentiation of the carefully measured time dependence of T with the sensor in close thermal contact with the sample. Values of C,(T) can be derived from calibration runs without the sample or with calibration fluids in the sample holder. In fact, the numerical differentiation is not necessary because the time dependence of temperature can be easily converted into a more basic result, namely, the enthalpy versus temperature. Indeed, after subtracting the contribution due to the sample holder, one gets H ( T )  H ( T , ) = P ( t  t , ) , the index s refers to the starting conditions of the run. P = P ,  P,, with P, the power needed to heat the sample holder. Here, Tis the sample temperature at time t. In this manner, the latent heat can also be obtained. If a firstorder transition occurs at a certain temperature Ttr, a step change will occur in H(T) in the interval AT= tfti until the necessary (latent) heat AH, has been supplied to cross the transition. One then can write: H ( T )  H ( i r ; ) = P(t1  t s ) + P ( t f  t i ) T
From the above considerations, it should be clear that running an adiabatic scanning calorimeter in the constant heating (or cooling) modes makes it possible to determine latent heats when present and distinguish between firstorder and secondorder phase transitions. On the basis of Cp= P / f , it is also possible to obtain information on the pretransitional heat capacity behavior, provided one is able to collect sufficiently detailed and ac
curate information on the temperature evolution T ( t )during a scan [ 19,211. Details of the mechanical construction and alternative operating modes of previously used adiabatic scanning calorimeters, can be found elsewhere [ 3 , 211. Figure 3 gives a schematic representation of a recently constructed wide temperature range version. A. C. Calorimetry The a.c. calorimetric technique is very well suited to measure pretransitional specific heat capacities. Indeed it measures C, directly and not the enthalpy H . This method has been extensively used for the investigation of liquid crystals by Johnson [22], Huang [23251, Garland [4,26,27] and their coworkers. For a.c. calorimetry an oscillating heating power Pa, = P,, ( I +cos ot)is supplied to a sample (in a sample holder), usually loosely coupled to a heat bath at a given temperature To, and from the amplitude ATac of the resulting temperature oscillation (see Fig. 4) the specific heat capacity of the sample can be derived. From Fig. 4, it should also be clear that for a firstorder transition one can not determine the latent heat AHL in this way. In a basic onedimensional heat flow model [28,25] for a planar sample with thermal conductivity IC,, the sample is assumed to be thermally coupled to the bath at Towith a finite thermal conductance Kb, but the coupling medium (gas) is assumed to have zero heat capacity. The following results are obtained: ATac
6.2.1 Thermal Methods
215
Figure 3. Schematic diagram of an adiabatic scanning calorimeter. Electric heaters and thermistors are denoted by H and R. PTR is a platinum resistance thermometer. The whole calorimeter is placed in a hot air temperature controlled oven. Details on a sample holder with stirring capabilities have been given elsewhere [21].
Ht
Figure 4. Enthalpy H curve for a firstorder transition at T,, and schematic representation of the a s . calorimetric and standard adiabatic methods for determining the heat capacity C,. AHacand ATac are, respectively the amplitude of the enthalpy variation and the corresponding temperature change. T, is given by Eq. (1 1). In the standard adiabatic method, C,=(AH/AT), is obtained from the temperature increase AT resulting from the heat input AH.
In Eq. (1 1) Ta is the average sample temperature (see Fig. 4) and ATdc is the offset between bath and sample temperature. In Eq. (10) K, is the thermal conductance for heat flow perpendicular to the surface of the planar sample. zl is the sample bath relaxation time and z, is a combined (internal) relaxation time for the sample and addenda (heater, temperature sensor, and sample holder when present). z1and z, result, respectively, in a low and high frequency cutoff. In the normal a.c. calorimetric mode one chooses a frequency w so that wz, t l . Now the initial temperature is T ( m )and the final one To.For the heating run the time dependence of the temperature of the cell over the time regime O l t s t , is given by [6, 341: (17) T(t)= To+ K ; l P ( t  z,) + z1K;' Pexp( tlq) For a cooling run ( P negative) a similar expression is obtained: (18) T(t)= T(m)+ K;'P(t zl)+ z,K;' Pexp( tlz,) The thermal conductance can be derived from:
Kh = Po(T,

To)]
(19)
and the heat capacity in both cases is given by:
Equation (20) is identical to Eq. (8) if one identifies P: with Kh(To T ) .In normal adiabatic scanning calorimetry one imposes P: = 0 (or T= To)for heating runs or P: constant for a cooling run [3, 211. Here, however, ( T  To)and P are time dependent, because P(t') is the power at time t' corresponding to the cell temperature T(t') lying in the interval To to T ( m ) .dT/dt is obtained by fitting T ( t )data over a short time interval centered at t'. In comparison with the conventional transient method, this method has the advantage of avoiding large transient disturbances (by step increases or decreases of P ) and also an optimal nearly linear behavior of dTldt, except for regions with very rapid H variation with T. This new method also allows a determination of the latent heat of a firstorder transition with a twophase region [35]. In the twophase region Eq. (20) represents an effective heat capacity C,. Outside the twophase region C, is identical to C(T). One identifies a firstorder transition by observ
218
6.2 Experimental Methods and Typical Results
ing anomalous behavior of C, and the occurrence of hysteresis. The latent heat can be derived from the following expression
AHL= j [ P  K b ( T  T o ) ] d t  j [ C h +C,)dt T
fl
where twophase coexistence exists between T , ( t , ) and T 2 ( t 2 ) , c h is the heat capacity of the sample holder, and C, = X , C, +Xb Cb (with X the mole fraction) the heat capacity of the two coexisting phases that would be observed in the absence of phase conversion. By integrating Eq. (20) between T I( t l ) and T ( t ) , and assuming P, Kb and To constant one also arrives at the following expression for the temperature dependence of the enthalpy:
H ( t )  H ( t , ) = P(f 2 t:) 2
(22)
t
T (t ) dt + Kb To(t  ti )
Kb 11
The calorimeter developed at MIT [6, 351 and shown in Fig. 5 , can also be operated in the new relaxation mode.
The Photoacoustic Method Photoacoustics is well established [36] for the investigation of optical and thermal properties of condensed matter, but it has only rather recently been applied to liquid crystals [374 11. The photoacoustic technique is based on the periodic heating of a sample, induced by the absorption of modulated or chopped (electromagnetic) radiation. In the gas microphone detection configuration the sample is contained in a gastight cell (Fig. 6). The thermal wave produced in the sample by the absorbed radiation couples back to the gas above the sample and periodically changes the tempera
;
b
c
d i e )
Figure 6. Schematic representation of a photoacoustic measuring cell with microphone detection: (a) copper cell body, (b) thermistor, (c) gold plated sample holder with sample, (d) quartz window, (e) condenser microphone, (f) Teflon microphone holder, solid dots are Orings; heating elements for temperature control are not shown.
ture of a thin gas layer (with a thickness determined by the thermal diffusion length p g ) above the sample surface. This will result in a periodic pressure change in the gas cell which can be detected by a microphone. A general onedimensional theoretical model has been developed by Rosencwaig and Gersho [42]. Assuming a sinusoidal variation, part I = Zo/2 exp (i w t ) of the radiation intensity will give rise to a timedependent harmonic surface temperature variation 8= Ooexp (i wt). Starting with this temperature variation one arrives at the following result for the corresponding pressure variation in the gas [42]: tjp = [ y gpi p g / ( 2 Tol g ) ] ~ e  1 n ’ 4 Qel(wtw/4)
(23) where ‘/s is the ratio of the specific heat capacities at constant pressure and constant volume of the gas, Po and To the static pressure and temperature, p g the thermal diffusion length of the gas and 1, the gas length between the sample and the light window in the planar geometric configuration. Rosencwaig and Gersho [42] derived the follow~
6.2.1
ing explicit relation for Oo (0) for a homogeneous sample on top of a backing material:
. ( r  l)(b +.Ilea'  ( r + ~ ) (b1)e@ + 2(b  r ) e B (g + I)(b+ 1)eO'  (g  l ) ( b i ) c  u / p ]
[ ~
In this equation p is the optical absorption coefficient of the sample, 1 is the sample thickness and CT=(1 + i ) a with a= l/p the thermal diffusion coefficient and p the thermal diffusion length of the sample. One further has: b = Kb fq,p K', g = K, agp c', r = (1i)pp/2. Here, and also in Eq. (23), quantities without subscript refer to the sample and the subscripts g and b refer to the cell gas and the sample backing material. For measurements in liquid crystals, one usually works in the optically and thermally thick regime (eff'%eeff',eP'), resulting in substantially simplified expressions. This means that p' and p of the sample have to be much smaller than the sample thickness, 1. The contribution of the backing material then disappears from the expressions. One then obtains for the photoacoustic microphone signal Q = 4 eCV, with amplitude 4 and phase ty (with respect to the radiation modulation) [38]:
ys Po Z0t(2t2 + 2t + 1 ) p 2 4 = 2:2ToZg(l+s)lcgug2
(25)
tanty=l+l/t
(26)
with t=pClp/2 and s = a K ( K ~ u , )  ' . The Eqs. (25) and (26) allow the simultaneous determination of the heat capacity per unit volume (pC,) and the thermal conductivity of the sample by solving for t and s. This gives
pc, = pKgogst'O'
Thermal Methods
219
However, one should arrange the measuring conditions in such a way that l/t=2/(pp) is not too small compared to 1 in Eq. (26). This can to some extent be done by choosing the proper modulation frequency (changing p) and/or changing p by choosing an appropriate wavelength A for the modulated light source. In any case one also has to measure (in a separate experiment) p (A). Moreover, Eqs. (25) and (26) for 4 and tycontain several other quantities related to the cell characteristics, the cell gas and the light source, which have to be known in order to arrive at quantitative results for pC, and K. This problem is usually solved by simultaneous or separate calibration runs with a sample of known optical and thermal parameters [39, 401. In photoacoustics, as in a.c. calorimetry, relatively small periodic temperature variations (in the mK range) are used, and only small amounts of samples are needed. The small temperature variations allow measurements very close to phase transitions but latent heats of firstorder phase transitions can also not be obtained in this way. One of the important advantages of photoacoustical techniques is the possibility of simultaneously measuring the heat capacity and the thermal conductivity in small samples. These methods also offer the possibility of investigating anisotropic thermal transport properties and to carry out depth profiling in thermally inhomogeneous samples [40]. Studying the thermal conductivity anisotropy requires homogeneous samples with known director orientation. This can be achieved by placing the photoacoustic cell and/or sample in an external magnetic field. It should also be pointed out that with the extension of the standard a.c. calorimetric technique by Huang et al. [24], one can also measure simultaneously the heat capacity and the thermal conductivity. In this case
220
6.2
Experimental Methods and Typical Results
a.c. calorimetric measurements have to be extended to high frequencies into the regime where the thermal diffusion length ,u=[2 d(pC, w)]' I 2 of the sample becomes comparable to the sample thickness in which case the second term in Eq. (10)can no longer be neglected. The Photopyroelectric Method
If we consider a pyroelectric transducer, with thickness I, and surface area A, in a onedimensional configuration, a change of the temperature distribution e ( x , t ) relative to an initial reference situation O(x, to) will cause a change of polarization. This in turn induces an electric charge given by: (29) q ( t )= j[e(x,t)e(x,t,)]dx PA lp =e(t) PA LP 0 lP with p the pyroelectric coefficient of the transducer. Consequently also a current is produced:
.
1
P
=p A dO(t)
lp dt
Usually the electric signal from the pyroelectric transducer is detected by a lockin amplifier. Thus only the a.c. component of the temperature variation gives rise to the detected signal. The signal depends, of course, on the impedance of the transducer and of the detecting electronics. The pyroelectric element can be represented by an ideal current source with a parallel leakage resistance and capacitance, while the detection electronics can be described by an input capacitance and a parallel load resistance [43]. Circuit analysis results then in a general expression for the signal V ( w )[44,45]. Under properly chosen experimental conditions [44], however, it is possible to arrive at a simultaneous determination of the specific heat capacity and the thermal conductivity of a sample in thermal contact with the
pyroelectric detector. A suitable setup for liquid crystal samples is given in Fig. 7. The wavelength of the modulated light, the modulation frequency, sample and detector thicknesses I , and 1, are chosen in such a way that the sample and transducer are optically opaque, the detector thermally very thick (&4I,) and the sample quasithermally thick (,us51,).One then obtains for the signal amplitude and phase [46]:
$ ( w ) = tan'(wr)(w/2a,)''21,
(32)
where subscripts s, p and m, respectively, refer to the sample, the pyroelectric transducer and to the medium in contact with the sample front surface. I , is the nonreflected light source intensity, 17, is the nonradiative conversion efficiency, p is the density and e = ( p C K)'/* is the thermal effusivity. R and rare a circuit equivalent resistance and time constant. From Eq. (32) it is possible to determine the sample thermal diffusivity a,. Inserting a, in Eq. (3 1) yields the sample effusivity. The thermal conductivity and specific heat capacity are then given by: C, = e, pi'
a['12 and
K, = e, a;112(33)
i n c i d e n t light quartz cell absorbing layer sample,
I
pyroelectric transducer
signal out
Figure 7. Schematic diagram of a photopyroelectric cell for liquid crystal samples [46].
22 I
6.2.1 Thermal Methods
6.2.1.4 Calorimetric Results High resolution calorimetry has been extensively used to study the many important and often puzzling phase transitions in thermotropic liquid crystals of rodlike molecules. Discotic liquid crystals seem to be, from the calorimetric point of view, less exciting because most phase transitions are first order with little pretransitional fluctuation effects [47]. Although lyotropic liquid crystal systems show complex phase behavior, they have not been studied calorimetrically in great detail, because calorimetric signatures of phase transitions tend to turn out quite small [48]. No attempt will be made to give an exhaustive treatment of any of the transitions discussed further. Thermal results will be presented to show what can be accomplished for typical cases with highresolution calorimetric experiments, careful analysis and theoretical interpretation. More extensive overviews can be found elsewhere [l61. A detailed account of calorimetric studies of free standing liquid crystal films can be found in a review article by Huang [49].
The IN Transition The only difference between the nematic phase and the isotropic phase is the orientational order. A proper description of this orientational order requires the introduction of a tensor of the second rank [7, 81. This tensor can be diagonalized and for anisotropic liquids with uniaxial symmetry, the nematic phase can be described by only one scalar order parameter. The thermodynamic behavior in the vicinity of the NI transition is usually described in terms of the meanfield Landaude Gennes theory [7]. For the uniaxial nematic phase one can obtain the expansion of the free energy G in terms of the modulus of an order parameter Q.
GGo 1 = AQ2 2
(34) 
~
1 BQ3 +CQ4 1 3 4
+ 61 DQ6 +... 
In the isotropic phase Q=O and in the nematic phase Q # O . In Eq. (34) one has A =a ( T  T*)/TN_,and B > 0. The presence of the cubic term, which does not disappear at TNI,leads to a firstorder transition with a finite discontinuity in the order parameter (QNr= 2 B/3 C). T* is the stability limit of the isotropic phase. For B = 0, a normal secondorder transition at TN, is expected. The excess heat capacity in the nematic phase is given by [ 161: C, = aQ(
(35) P
with T** the stability limit of the nematic phase. One, thus, has an anomalous contribution with an exponent a= 1/2 in the nematic phase, resulting in a jump in Cpat TN, equal to A C , = ~ L Z ~ / C T In~the _ ~case . of a mean field secondorder (B=O and C>O) transition the singular contribution (see Fig. lc) follows from the meanfield behavior (with the critical exponent p= 1/2) of the order parameter [ 161. For the enthalpy discontinuity at TN1 one obtains H,HN=2aB2/9 C2. When B=O, there is no enthalpy jump or latent heat and one has a critical point (Landau point) on an otherwise firstorder line. Because of the presence of this (small) cubic term in Eq. (34), the NI transition should (normally) be weakly first order. This is in agreement with experimental observations. In Fig. 8, part of the enthalpy curve near TNI is shown for hexylcyanobiphenyl (6CB), a compound of the alkylcyanobiphenyl (nCB) homologous series [5]. The nearly vertical part of the enthalpy curve corresponds to the
222
6.2 Experimental Methods and Typical Results
t" r 
100

1
$ 300 I
200 
100 28 5
0
29 2
29 3
29 4
29 5
T 1°C
)
Figure 8. Temperature dependence of the enthalpy near the nematic to isotropic transition for hexylcyanobiphenyl (6CB) [ 5 ] .
latent heat of the NI transition. It is not perfectly vertical because of the small (=20 mK wide) impurityinduced twophase region. AHLfor the transitions in 6CB is (293 +3) J/mol. This latent heat is indeed quite small, about two orders of magnitude smaller than the latent heat at the melting transitions in these cyanobiphenyl compounds [19, 501. Because the latent heat at the NI transition is very small and since the orientationa1 interactions between liquid crystal molecules are short range, one might expect many physical properties to display criticallike behavior, described by power laws with the appropriate critical exponents. These fluctuation effects are, indeed, observed in many properties including the specific heat capacity. Figure 9 gives the temperature dependence of C, near the NI transition for the same substance as in Fig. 8. No data points are displayed in the coexistence region, whose width is indicated by the narrow box around the arrow marking TNI.
290
,T, 295
300
30 5 T 1°C I
Figure 9. Temperature dependence of the reduced heat capacity per mole (R is the gas constant) near the nematic to isotropic (NI) transition for hexylcyanobiphenyl (6CB). The width of the arrow on the temperature axis represents the twophase region [ 5 ] .
Since the Landaude Gennes theory is a meanfield theory, one can only expect a qualitative description of the specific heat capacity anomaly [2, 161. Attempts to determine a critical exponent a have been largely unsuccessful due to the firstorder character of the NI transition. Fits with Eq. (6) must be made separately for data above and below TN,with different effective critical temperatures (T* and T**), which both are different from the firstorder transition temperature. For T < TN1, typical a,,, values lie in the range 0.30.4 but depend strongly on the fitting range. For T > TN1, an even wider range of aeff values between 0.1 and 0.5 is observed. Furthermore (2'"  TNJ and (T**  TNJ values obtained from C, fits are consistently about onetenth the magnitude of those from several other properties [2,16]. The experimental behavior of the NI transition is quite well characterized, but theoretical understanding is still rather poor.
6.2.I
Blue Phase Transitions
600I
In the case of optically active molecules one arrives at a special situation for the nematic phase. In addition to the long range orientational order there is a spatial variation of the director leading to a helical structure. The local preferred direction of alignment of the molecules is slightly rotated in adjacent planes perpendicular to the pitch axis. This phase is usually called chiral nematic (N*) or cholesteric phase. The helical pitch in the N* phase is substantially larger than molecular dimensions and varies with the type of molecules. For a long pitch one has a direct firstorder transition between the isotropic phase and the chiral nematic phase with characteristics very similar to the normal NI transition in nonchiral compounds. For chiral nematics with short pitch (typically less than 0.5 pm), a set of intermediate blue phases (BP) are observed between the isotropic and the N* phase [51531. In order of increasing temperature these phases are denoted BPI, BPI, and BPI,,. The first two blue phases have threedimensional cubic defect structures, whereas BPI,,, which is also called the fog phase appears to be amorphous [51531. Different phase transitions involving blue phases are expected theoretically to be firstorder [54] except the BPI,, to isotropic transition which could become second order [54] in an isolated critical point at the termination of a firstorder line [6, 551. Figure 10 shows C , results of cholesteryl nonnanoate (CN) with adiabatic scanning calorimetry [56]. From Fig. 10 it is clear that there are substantial pretransitional heat capacity effects associated with the BPII11 transition, which means that a large amount of energy is going into changing the local nematic order. The other transitions appear as small, narrow features on the BP1,II transition peak. From the inspection of the en
500
21
I
100 09 5
I
223
Thermal Methods I
I
I
CN
I
90 0
I
90 5
I
91 0
I
91 5 T 1°C)
Figure 10. General overview for the reduced heat capacity per mole C,/R for a temperature range covering all phase transitions involving the blue phases in cholesteryl nonanoate (CN) [ 5 6 ] .
thalpy behavior, it was found that these small features correspond to firstorder transitions with very small latent heats [56]. In CN the BPI,,I transition was also observed to be first order. This can be seen in Fig. 11 where the enthalpy versus temperature is given for a Trange of 0.2 K below and 0.2 K above the transition. Further calorimetric studies by Voets and Van Dael [57, 581 have shown that the latent heat for BPI,,I decreases as the chiralty of the molecule increases and that its magnitude varies considerably as a function of composition in binary mixtures of R and Senantiomers. Recently an a c . and nonadiabatic scanning calorimetry investigation of the chiral compound S,S(+)4”(2methyl
butylphenyl)4’(2methylbutyl)4biphenyl4carboxylate (S,SMBBPC), which has very short pitch, yielded the results given in Fig. 12 [55]. By combining these two calorimetric techniques one can show that there are sharp firstorder transitions with small latent heats at the N*BPI and the BPIBP,,, transitions (the BPI, phase is absent in this compound). However, no thermodynamic
224
6.2 Experimental Methods and Typical Results
3.5 EZ
s3.0
V
BPI11

I
2.5
I


2.0 I
T
("0
Figure 11. Detailed plot of the enthalpy near the phase transition from the blue phase 111to the isotropic phase in cholesteryl nonanoate (CN). Note that for clarity a large linear background 140 R (TT,) with T, =90.73"C, has been subtracted from the direct data. The two vertical dashed lines indicate the width of the twophase region [56].
BPI,,I transition occurs in this S,Senantiomer of MBBPC. One only observes a supercritical evolution. As pointed out by Kutnyak et al. [55] an investigation of S,Sand R,Renantiomers of MBBPC should allow one to find the BPI,,I critical point and determine its critical exponent. The observed continuous supercritical evolution implies that the BPI11 and I phases must have the same macroscopic symmetry allowing, as in the case of the liquidgas transition of simple fluids, the firstorder line to terminate in an isolated critical point. The NSmA Transition
This transition has been the most extensively studied of all liquid crystal phase transi
I
. ._. The sharp peaks from nonadiabatic scanning through the N*BPI and BPlBPl,, regions are due to latent heat effects at the firstorder transitions. No such effects are seen for the BP,,,I transition, because this is only a continuous supercritical evolution not a true phase transition in this material [55].
I
1
I
1
I
I I I
/
I 1 101 Ill I I
00
02
I' I I I I II I
OL
I
I 1
u 6
08
0
XlO
Figure 13. Phase diagram of 8CB + IOCB mixtures. Heavy solid and dashed lines are, respectively, secondorder and firstorder transitions. TCP is the NA tricritical point. Vertical dashed lines indicate the measured mixtures [64].
tions. In spite of vigorous experimental and theoretical efforts, many aspects of the critical behavior of this simple kind of onedimensional freezing, are not yet understood,
6.2.1
making this transition an intriging and challenging problem in the statistical mechanics of condensed matter. The SmA liquid crystalline phase results from the development of a onedimensiona1 density wave in the orientationally ordered nematic phase. The smectic wave vector q is parallel to the nematic director (along the zaxis) and the SmA order parameter U,I = 1 W I ei@ is introduced by p ( r )= po [ 1 + Re ye'^']. Thus the order parameter has a magnitude and a phase. This led de Gennes to point out the analogy with superfluid helium and the normalsuperconductor transition in metals [7, 591. This would than place the NSmA transition in the threedimensional XY universality class. However, there are two important sources of deviations from isotropic 3DXY behavior. The first one is crossover from secondorder to firstorder behavior via a tricritical point due to coupling between the smectic order parameter U,I and the nematic order parameter Q. The second source of deviation from isotropic 3DXY behavior arises from the coupling between director fluctuations and the smectic order parameter, which is intrinsically anisotropic [60621. The firstorder to secondorder crossover can be qualitatively understood on the basis of a meanfield approximation for the excess smectic free energy (above the nematic one) as formulated by de Gennes [7]:
A G = a I WI
+ 6, I K,II + (SQ)2/2xC I WI 2SQ
(36) where a = a. ( T  TNA) /TNA = a. E ; bo, C> 0; and SQ the change in the nematic order induced by the formation of the smectic layers, and the temperature dependent nematic susceptibility [7] whose value at TN* depends on the width of the nematic range. Minimization of AG with respect to SQ yields:
x
AG = a1 W I
+ bl wl4 + C I
WI6
(37)
Thermal Methods
225
with b = bo C2x/2. For narrow nematic ranges x ( T N  A ) is large and bO for stability reasons). For wide nematic ranges x(2’NA) is small and b>O, the transition is then secondorder. In this meanfield approach the Cp behavior would then be given in Fig. 1(c). A tricritical point occurs for b = 0. The specific heat capacity in the low temperature side then diverges with a critical exponent a= 1/2. In Fig. l(c) one then has max cp
00.
The crossover from first to secondorder behavior and the disappearance of measurable latent heats with increased widths of the nematic ranges has been shown on the basis of adiabatic scanning calorimetry of the 4’nalkyl4cyanobiphenyl(nCB) binary mixtures 9B+lOCB [63] and 8CB + lOCB [64]. The investigation of 8CB + lOCB mixtures with nematic ranges from 7 K to zero (see the phase diagram in Fig. 13) resulted in a partly first and partly secondorder SmA line with a tricritical point at XlOcB= 0.3 14. In Fig. 14 the enthalpy curves near TNA are given for several mixtures of 8CB + lOCB with firstorder transitions. Along the secondorder part of the transition line one would expect 3DXY critical behavior at least in the limit of the critical point. In real experiments, one observes crossover between XY critical and tricritical behavior, resulting in aeffvalues where axy< a,,< %c because the temperature range for most experimental data is limited to lo’ l / f lit, is Type I1 (flux lines penetrate but the penetration is not complete). The analogue of studying superconductors in a magnetic field (curlA#O) is to turn on spontaneous twist deformations (ncurln, chirality, a property of cholesteric liquid crystals) in the liquid crystal case [23]. The transition is analogous to a Type I superconductor and the N*SmA transition, in a high enough chirality limit, is analogous to Type I1 superconductors ex
282
6.3 Fluctuation and Liquid Crystal Phase Transitions
hibiting the analogue of a vortex lattice in what are now known as twist grain boundary phases (TGB) [42]. Renn and Lubensky proposed a model for the analogue of the vortex lattice [43] for the N*SmA transition [42]. Simultaneously and independently such a phase was discovered by direct observation, supported by Xray analysis as well as freezefracture, by Goodby et al. [44] between the isotropic liquid and a SmC* phase. The first TGBA phase found to exist between N* and SmA was studied in a dynamic experiment [45]. In the RennLubensky model, uniform separated by sheets of SmA of extent parallel planes of screw dislocations, twist relative to each other [46]. When Dasgupta and Halperin included fluctuations in the HLM effect [47], they found that the second order nature was restored in the high IC limit of superconductors. Recently in a dynamic experiment [45], there was no interface between cholesteric and TGBA in a material for which lcwas esIn timated to be =3 times larger than ll. addition, the N phase region did not propagate (i.e. either advance or retreat): TGBA grew as SmA melted and was squeezed out by an advancing SmA phase. These observations [45] support a second order TGBAN* phase transition [4]. High resolution specific heat measurements raise the possibility of another interesting scenario [48]. These measurements show a large broad feature well above the TGBN* transition and only a tiny (if any) latent heat at the N*TGB transition. A similar behavior was observed at the first TGBAN* transition [45] in a different compound making it a possible generic feature of TGBN* transitions. In this case [45], the size of the heat signature at the TGBAN* transition was time dependent. Chan et al. [48] suggest that the broad pretransitional heat feature was consistent with
tL,
the formation of a liquid of screw dislocations condensing into either a glassy or an ordered TGB phase [49]. They point out [48] the resemblance between their phase diagram and a theoretical one for a Type I1 superconductor with strong thermal fluctuations where, with decreasing temperature, a vortex liquid state condenses into either a glassy or an ordered state [50].Whether the second order nature of the N*TGBA transition [45] is a result of fluctuations obliterating the small HLM singularity or a proposed [50] (but not yet experimentally verified) [5 13 liquidglass transition calls for more work. Materials with TGB phases with a large temperature range [52] may help clarify this question relevant not only to liquid crystal and high T, superconducting materials, but also other complex materials such as polymers, electrorheological fluids and ferrofluids [42].
6.3.6 Transitions between Tilted and Orthogonal Smectic Phases In the SmC phase, the director tilts relative to the layer normal at an angle, 6+.# 0, breaking the continuous rotational symmetry in the plane of SmA layers. The order parameter for this transition is &, the angle between the layer normal and the director. Guillon and Skoulios [ 5 3 ] suggested that a direct measure of S, is given by cos 4=d,/dA where dc is the layer spacing measured in the C phase and d A is its (maximum) value at TSmASmC. According to theory [54], this transition is in the 3DXY universality class. Although measurements by the MIT group found mean field exponents and unobservably small critical regimes (&,,=700 nm) [55], a compound studied by Delaye [56] in light scattering, as well as optical measurements in other compounds by Ostrovskii et al. [57] and Galerne [58], and
6.3.7 BSmBSmA
Xray layer spacing measurements of Keller et al. [59], observable critical regimes were found with 3DXY exponents as expected by theory [54]. Recently Ema et al. [60] found that, with ‘significant correctionstoscaling’, their high resolution specific heat measurements agreed with theoretical expectations [54] at the SmCgSmA transition. The SmCg phase is composed of alternating layers of equal and opposite tilt [61]. Ema et al. [60] give a nice summary of these transitions in the context of critical phenomena as well as a sense of the detailed scrutiny high quality data are subjected to in such studies. The controversy over the nature of the SmASmC transition was essentially resolved by Benguigui and Martinoty [62]. These authors addressed the question of why fluctuation effects can be observed on long lengths scales with ultrasound propagation but not by specific heat or Xray measurements. In particular in sS5, where specific heat, Xray and dilatometric measurements found meanfield behavior, ultrasound damping measurements showed significant fluctuation effects [63]. Most recently [64], they further elucidated the question of how certain compounds do show meanfield behavior while others show critical behavior at long wavelengths. Their explanation rests on the AndereckSwift theory of the SmASmC transition [65] that couples the SmC order parameter to gradients in the density and gradients in the layer spacing.
6.3.7 BSmBSmA Transitions The SmB phase is another example of a phase where entropic effects are important. SmA is a two dimensional isotropic liquid in the plane of its layers. B is a three dimensional hexagonal crystal. SmB inplane or
283
dering is between these two with long range hexagonal bond orientational order and short range translational order that is not correlated from layer to layer [66]. A simple picture is that in the SmB phase, molecules are delocalized on a hexagonal grid [59]. Xray diffraction patterns of B are resolution limited while those of SmB are not [67]. Although a first order SmBSmC* transition has been observed [59], most of the work has concentrated on the expected fluctuation dominated SmBSmA transition [68]. So far, none of the exponents observed at this transition fit a recognizable universality class. Nounesis et al. measured the divergence in the thermal conductivity and found dynamic critical exponents consistent with tricritical values [69]. As they had already established that a= 0.6, very different from expectations of static critical phenomena (i.e. 3DXY) they suggested that the SmBSmA transition, at least in the compound they were studying (650BC) [70), was driven towards a tricritical point because of a coupling between hexatic order and a short range ordering field such as a ‘herringbone’ structure from a nearby, lower temperature crystal E phase [ 11. However, later extensive work on different compounds along a SmBSmA transition line, with SmB temperature ranges between 0.8 K and 22 K, found ~ 0 . along 6 the entire line [71]. These authors point out that only a tricritical point (not a line) is compatible with a coupling between bondorientational order and short range positional order. Gorecka et al. [72] studied a compound in thick freely suspended films exhibiting a BSmBSmA phase sequence. They found no significant difference in hexatic properties in this system and those with SmBE transitions [71]. The exponent for the hexatic order parameter was found to be p = O . 15
284
6.3 Fluctuation and Liquid Crystal Phase Transitions
k0.03 which the authors point out is consistent with the three state Potts model in three dimensions [68]. They could not exclude the possibility that the SmBA transition in their material was first order. The suggestion was that the hexatic order parameter did not fully crossover from mean field to 3DXY. It was also found that while there is a sharp discontinuity in the inplane positional correlation length at the SmBB transition, suggesting a strongly firstorder transition, there was no measurable enthalpy change. Fluctuation effects at the more fluid of liquid crystal phase transitions have been sensitively probed using techniques exploiting long length scales. Indeed, ultrasonic wavelengths are highly sensitive to hexatic fluctuations in SmA. Gallani et al. [73] found evidence of hexatic fluctuations at the SmASmB transition resulting in a strong damping and velocity anomaly in the A phase of an ultrasonic wave. Their data suggests that the inplane hexatic ordering couples to SmA layer undulations which in turn have a nonlinear coupling to the sound velocity field.
6.3.8 Fluctuations at Critical Points A line of first order phase transitions between two phases with the same symmetry may end at a critical point where fluctuations are expected to dominate. The classic example of this is the liquidgas critical point.
6.3.8.1
BP,,,Isotropic
The analogue of the pressuretemperature plane in a liquidgas system is the temperaturechirality plane for blue phase transitions. Along the lines of the classic liq
uidgas example, Keyes [74) suggested that as the BPI11 and isotropic phases have the same symmetry, the line of first order phase transitions could end at a critical point. Voigts and van Dael found, [75] later verified by others, that, with increasing fraction of a chiral component, the latent heat at the BPII11 transition decreased. More recently, Kutjnak et al. [76] located a BP1,II critical point and characterized its behavior with high resolution calorimetry and measurements of optical activity. They report that both measurements are consistent with mean field behavior instead of the theoretically expected [77] king fluctuation behavior. They suggest that mean field behavior is observed because 5, is large. However, measured values [74] of {,,=1.5 nm (i.e. a molecular length scale).
6.3.8.2 SmA, and SmA, These two smectic phases have the same symmetry but their layer spacings are different and incommensurate. In SmA,, the layer spacing is about the molecular length while in SmA, it is 1.21.3 times the molecular length. As the critical point is approached, fluctuations become so large the critical point explodes into a bubble of a disordered statecholesteric if the compounds are chiral and nematic if they are notembedded in SmA. [78] On the other hand, a line of first order phase transitions between SmA, and SmA,, for which the layer spacing is about twice the molecular length, ends at a critical point [79]. Prost and Toner [SO] developed a dislocation melting theory for a line of firstorder SmASmA phase transitions ending at a NSmA,SmA, triple point. The firstorder nature of this triple point for a nematic bubble has been verified by Wu et al. [81]. Furthermore, it was predicted that this line could continue linearly into the nematic region to end at a NN crit
6.3.10
ical point [SO]. At the triple point on a nematic bubble [78], such a line would have to bend nearly 90". But, at a nematic 'estuary' connected to a nematic 'ocean' (i.e. not surrounded by SmA), evidence has been found for a critical point terminating a firstorder line of NN transitions. [82]
6.3.8.3 NAC Multicritical Point A point where three fluctuation dominated phase transition lines meet in a 2dimensional parameter space is also expected to exhibit universal features. An extensively studied liquid crystal candidate was the NSmASmC point in mixtures [83], in a pure compound under pressure [84] and at the reentrant NSmASmC multicritical point [ 8 5 ] . The situation may be summarized as follows. The systems studied showed qualitative and quantitative similarities. However, the exponents exhibited were not in the expected universality class for three second order phase transition lines meeting at a point. This is likely because, in the NSmASmC case, the NSmC transition line is first order [86] as is the NSmA transition line, [26] leaving only the SmASmC secondorder phase transition line.
6.3.9 Conclusion Given the rich variety to their broken symmetries, enormous strides in perfecting low molecular weight organic liquid crystal materials for applications in industry, as well as important advances in measurement technologies of material properties under wellcontrolled conditions, liquid crystals emerge as useful materials to explore the intricate and beautiful interplay in nature between symmetry and spatial dimensionality at phase transitions.
References and Notes
285
6.3.10 References and Notes [I] P. G. de Gennes, J. Prost, The Physics of Liauid Crystals, Clarendon Press, Oxfoid 1993, C h p ters I and 11. P. Pfeuty, G. Toulouse, Introduction to the Renormalization Group and to Critical Phenomena, John Wiley and Sons, New York 1977. J. Thoen, in Phase Transitions in Liquid Crystals, (Eds.: S. Martellucci, A. N. Chester) Plenum, New York 1992, pp. 155174; C. W. Garland, ibid, pp. 175187; J. Thoen, Int. J. Mod. Phys. B, 1995,9, 2157; in Liquid Crystals in the Nineties and Beyond, (Ed.: S. Kumar) World Scientific Publ. Co, 1995, pp. 1980. P. E. Cladis, W. van Saarloos, D. A. Huse, J. S . Patel, J. W. Goodby, P. L. Finn, Phy. Rev. Lett. 1989,62, 1764; G. Dee, J. S . Langer, Phys. Rev. Lett. 1983, 50, 383. M. A. Anisimov, P. E. Cladis, E. E. Gorodetskii, D. A. Huse, V. E. Podneks, V. G. Taratuta, W. van Saarloos, V. P. Voronov, Phys. Rev. 1990, A41, 6749, See also: P. E. Cladis, J. Stat. Phys. 1991, 62, 899. G. Grinstein, private communication, 1980, Pfeuty and Toulouse [2]. A recent review is: J. R. Dorfman, T. R. Kirkpatrick, J. V. Sengers,Annu. Phys. Chem. 1994,45, 213. A. Schenzle, H. R. Brand, Phys. Rev. 1979,A20, 1628. H. R. Brand, S. Kai, S . Wakabayashi, Phys. Rev. Lett. 1985, 54, 555. A recent overview of this aspect of critical phenomena is: B. Schmittmann, R. K. P. Zia, Statistical Mechanics of Driven Difusive Systems,Academic Press, New York 1995. I See for example: L. Benguigui, D. Collin, P. Martinoty, J . Phys. I (Paris) 1996, 6, 1469. In this paper, the authors show that the dynamic exponent, y , associated with high frequency damping at a second order phase transition is frequency dependent so that simple scaling laws obtained from mode coupling calculations should not apply. However, in some smectics, where the regular part of the specific heat behavior is large compared to the fluctuation amplitude, deviations from these laws may be too small to measure. For a recent perspective on fluctuation effects in nematic liquid crystals see: Z. H. Wang, P. H. Keyes, Phys. Rev. E, 1996,54,5249. H. R. Brand, H. Finkelmann, Liquid Crystal Elastomers, Vol. 111 and references therein. M. Olbrich, H. R. Brand, H. Finkelmann, K. Kawasaki, Europhys. Lett. 1995, 31, 281. P. G. de Gennes, Mol. Cryst. Liq. Cryst. 1971, 12, 193. See also ref [ l ] F. Hessel, H. Finkelmann, Polym. Bull. 1985, 14, 375; H. Leube, H. Finkelmann, Makro
286
6.3 Fluctuation and Liquid Crystal Phase Transitions
mol. Chem. 1990, 191, 2707, ibid 1991, 192, 1317. [ 171 See for example: W. Wedler, P. Hartmann, U. Bakowsky, S . Diele, D. Demus, J . Muter: Chem. 1993,2, 1195. [I81 L. J. Yu, A. Saupe, Phys. Rev. Lett. 1980, 45, 1000. The system is mixtures of potassium laurate, Idecanol and DzO. This system also exhibits a reentrant nematic transition (cf. the Chapter in this Handbook on Reentrant Phase Transitions). The higher temperature nematic is rodlike while the lower temperature nematic is disclike. In addition, the isotropic liquid is also reentrant in this system. [19] H. Brand, J. Swift, J. Phys. Lett. 1983, 44, L333. C. Cajas, J. B. Swift, H. R. Brand, Phys. Rev. 1983, A28, 505 (statics); ibid 1984, A30, 1579 (dynamics). [20] A. Saupe, P. Boonbrahm, L. J. Yu, J. Chem. Phys. 1984,81,2016. [21] M. Roy, J. P. McClymer, P. H. Keyes, Mol. Cryst. Liq. Cryst. Lett. 1985, I , 25. [22] W. McMillan, Phys. Rev. 1971, A4, 1238; ibid. 1972, A6, 936; ibid 1974, A9, 1720.; K. K. KObayashi, Phys. Lett. 1970, A31, 12.5. [23] P. G. de Gennes, Solidstate Commun. 1972,10, 753; P. G. de Gennes, J. Prost, The Physics of Liquid Crystals, Clarendon, Oxford 1993, Chapter X. [24] C. W. Garland, G . Nounesis, Phys. Rev. E. 1994, 49, 2964 and references therein. [25] cyanooctylbiphenyl and cyanononylbiphenyl respectively. The small discontinuities in 8CB and 9CB escaped the fine net of adiabatic calorimetry (J. Thoen, H. Marynissen, W. van Dael, Phys. Rev. Lett. 1984,52, 204; Phys. Rev. 1982, A26, 2888; H. Marynissen, J. Thoen, W. van Dael,Mol. Cryst. Liq. Cryst. 1985,124, 195) and high resolution Xray diffraction (B. M. Ocko, R. J. Birgeneau, J. D. Litster, Z. Phys. 1986, B62,487) but were caught by the front propagation test [5]. [26] B. I. Halperin, T. C. Lubensky, S. K. Ma, Phys. Rev. Lett. 1974,32,292 for superconductors and B. I. Halperin, T. C. Lubensky, Solid State. Comm. 1974, 14, 997 for the NSmA transition. [27] P. Sonntag, PhD Thesis, University of Louis Pasteur de Strasbourg I (1996) and to be published (1997). [28] T. C. Lubensky, J. Chim. Phys. 1983, 80, 31. [29] T. C. Lubensky, G. Grinstein, R. Pelcovits, Phys. Rev. 1982, B25, 6022. [30] D. R. Nelson, J. Toner, Phys. Rev. 1981, B24, 363 and J. Toner, Phys. Rev. 1982, B26, 462. A. J. McKane, T. C. Lubensky, J . Phys. (Paris) Lett. 1982, 43, L217. [31] A. R. Day, A. J. McKane, T. C. Lubensky, Phys. Rev. 1983, A27, 1461.
[32] B. R. Patton, B. S. Andereck, Phys. Rev. Lett, 1992, 69, 1556; B. S. Andereck, B. R. Patton, Phys. Rev. 1994, E49, 1393. [33] See for example [27]. [34] P. E. Cladis, Phys Lett. 1974, 48A, 179 and unpublished. This is a qualitative result. While it may not be possible to make elastic constant measurements for K2 and K , deep enough into the NSmA critical regime to establish quantitative certainty about critical exponents, there should be no problem for K , which does not diverge at this transition. [35] Unlike paraMBBA, the orthoMBBA isomer is not liquid crystalline. It was synthesized by Gary Taylor at Bell Labs (ca. 1970) to ‘fine tune’ liquid crystal electrooptic response for devive applications. While the shape of pMBBA is rodlike, that of oMBBA resembles a bent rod. [36] F. Brochard, J. Phys. (Paris) 1973, 34, 41 1. F. Jahnig and F. Brochard, J. Phys. (Paris, 1974, 35, 301. See also: K. A. Hossain, J. Swift, J.H. Chen and T. C. Lubensky, Phys. Rev. 1979, B19, 432. [37] K. Kawasaki, Phys. Rev. 1966, 150, 291; Ann Phys. 1970, 61, 1. See also review article [7]. [38] Ch. Gahwiller, Phys. Rev. Lett. 1972, 28, 15.54; Mol. Cryst. Liq. Cryst. 1973, 20, 301. P. Pieranski, E. Guyon, Phys. Rev. Lett. 1974, 32, 924. [39] See for example: P. E. Cladis in Nematics: Mathematical and Physical Aspects, (Eds.: J.M. Coron, J.M. Ghidaglia, F. Helein) Kluwer Academic Publishers, Boston 1990; and H. R. Brand, C. Fradin, P. L. Finn, P. E. Cladis, Phys. Lett. A 1997. [40] P. Martinoty et al. (Phys. Rev. E 1997) at the firstorder SmCSmF transition where nevertheless, fluctuations are observed by anomalies in ultrasonic measurements and H. Yao, T. Chan, C. W. Garland, Phys. Rev. 1995, E S l , 4584 at the firstorder SmCSmI critical point. See also Ill]. [41] Type I1 superconductors in a magnetic field (and in the appropriate geometry) are characterized by the following properties. P. G. de Gennes, Superconductivity of Metals and Alloys, W. A. Benjamin, Inc. (pub.), New York, 1966. The Meissner effect is not observed except in weak fields, HH,,, magnetic field lines penetrate but the penetration is not complete. de Gennes points out that this region was first experimentally discovered by Schubnikov in 1937 but is known as the vortex state from the microscopic theory derived by A. Abrikosov, Zh. Eksp. Teor: Fiz. 1957,32, 1442 [SovietPhysics JETP 1957, 5, 1 1741. For H>Hc2, no expulsion of flux is observed however superconductivity is not completely destroyed. Experimentally the transition at Hc2 is second order. In the interval Hc2~H 10 mm) [48, 491. This situation is appropriate for studying the core structure of dislocations and disclinations. Let us start from a perfect cholesteric liquid (assumed to be lefthanded) and isolate a virtual cylinder, the axis of which coincides with the twist axis (Fig. 22 a). The arrangement of the directors at the lateral surface of this cylinder is represented in Fig. 22 a’, a rectangle obtained by unfolding the limiting cylindrical surface, after cutting along a generator AA’ (or BB’). The positions of the directors lying within the drawing plane form a series of oblique stripes, corresponding to a double helix at the cylinder periphery, and this is also the case for positions of directors normal to this plane. Directors at +45” form a quadruple helix and are represented by a series of nails. A crosssection of this cholesteric cylinder, at the level of line nm is shown in Fig. 21 a” to recall the constant director orientation within a thin ‘cholesteric layer’, and it can be verified that the nail orientations along line nm in Fig. 22 a’ correspond well to the expected obliquities of the directors relative to the interface in the successive sectors of the cylinder in Fig. 22 a”. If we now apply the Volterra process, there are two possible ways to obtain a screw dislocation, as indicated in Fig. 22 b and c, when the length of the Burgers vector isp/2, the halfhelicoidal pitch. In a simple model it is assumed that the directors
32 1
have a planar distribution, normal to the screw axis. The arrangement of directors remains that of parallel stripes in rectangles AA’BB’ transformed into parallelograms in Fig. 22 b‘ and c’. However, due to the Volterra process, the double helices in Fig. 22 a and a‘ are replaced by triple helices in Figures 22b and 22b’ and simple helices in Fig. 22c and c’, which also are lefthanded. The lateral distribution of directors along the circumference nn’ can be prolonged towards the core, the director orientation being constant along any radius. One then refinds the two classical patterns of disclinations in nematics (Fig. 22 b” and c”), considered above in Fig. 10. The patterns of various screw dislocations are represented in Fig. 23, either in meridian or crosssectional views. The directors are coplanar and lie normal to the screw axis, as in Fig. 22, but have various Burgers vector lengths (multiples of p/2). The orientations of vectors b andp (Burgers vector and helical pitch vector) are identical if the spontaneous twist and the screw dislocation follow the same handedness. By convention, we say that the Burgers vector length b and the helical pitch p are positive when the corresponding distortions (and the spontaneous twist) are righthanded. These two lengths are negative if they both correspond to lefthanded orientations. Each screw dislocation is characterized by an integer Z, which can be positive or negative, such that b = Z p / 2 ; the cholesteric liquid is perfect when Z=O. The locus of the horizontal directors lying at a constant angle to the cylinder forms helices at the surface of the limiting cylinder, or a set of equidistant circles for Z=2. A 180” arc of these helices for radial directors is represented in each of the drawings in Fig. 23, except for the case when Z=2. All meridian sections of these screw dislocations are equal and superimpose through
322
7
Defects and Textures
.B
 ' ' _ ' ......... . ...... .......... . . .7 .............. ........ ...................
A'"'.. C'

5..........

.......... 11 r n . . . i .... ?....7 . . . . .r. . . . . . . . . ........ .... ....... ........... ......... .................

+
I
............B'
A' ./
the corresponding helicoidal displacement. It can be verified that the pitch of this helix is h=(Z+2)p/2). The hatched part of the meridian section allows one to generate the whole screw dislocation by means of the corresponding helical motion. This hatched region is absent from the top figure, since the helix is replaced by a series of coaxial circles and a pure rotation suffices to generate the whole structure, with different patterns according to the section level (concentric circles, spirals, diverging radii). The crosssections of the various screw dislocations in cholesterics show disclination patterns similar to those encountered in nematic liquid crystals and correspond to
nrn
ABA'B' are transformed into parallelograms (b' or c') and the distributions of the directors are changed along a transverse circle nm. This leads to two different patterns in the core (b" or c") when the molecules are assumed to remain horizontal. (Drawn in collaboration with F. Livolant.)
solutions of V2@=0 in the plane [54, 591. The core patterns corresponding to odd values of Z cannot be made continuous, since the ribbon of directors centred on a simple circuit closed about this defect line is a Mobius strip. Conversely, the disclination structures obtained for even values of Z (2, 2, 4, 6) can be made continuous, as indicated in Fig. 24af, the expected meridian structure corresponding to Fig. 24 g [59611. The director that was normal to L in Fig. 23 is now made oblique by the presence of a component n, which grows continuously from 0 to 1 , from the periphery of the core ( p ) to its axis (0) in Fig. 24g. The two dotted areas correspond to zones of in
7.3
N.2
Srl
z = 2
...............
.............. /
...............
..............
..................................... N.0
S=O
Z=O
323
Topological Structure of Defects
_
............ ._
................................ "4
5.1
'
z=.4
1 ................. 
:&
;; ) ; ................ ................ . . ,  ;1,:; .............. i.?..........c. .;.....yq .... ..: c .............. :1[;.. .............. ............. d..j .. 1; . v..... . . ............. .......... ........... . I I 1: ......=..
i ..............
.:
:1 : ............ ..............   )Tk( i
...=....;.(I 4
Figure 23. Meridian views of a righthanded cholesteric liquid, after the application of the Volterra process creating screw dislocations, and the corresponding patterns in crosssection. The parameters indicated below each pattern are N , s = N / 2 and Z= 2 blp, the ratio of the Burgers vector to the halfhelical pitch, both of which have positive length if the twist and the screw distortion are righthanded. The helical arcs indicate how one passes by helical displacement from the pattern on the left (hatched rectangle) to the corresponding one on the right (also hatched). The pitch of these helices is h = p + b. The crosssection patterns verify that @ = @ o + N q 1 2 , and one has N =  Z .

"
.w.. f
j ..............)

L
L&Z 7
Figure 24. Transverse and meridian patterns of continuous cores in evenindexed (or nonMobian) screw dislocations in cholesterics. (af) Transformations of transverse patterns for Z=2 (ac), 2 (d), 4 (e) and 6 (0,by 'escape in the third dimension'. (g) Meridian section expected from (ad), L representing the axis of the screw line. (h) Another type of meridian section, also compatible with the production of screw dislocations along the axis L. (i, j) Two patterns deduced from (h), where the locus of the vertical directors consists of L and a set of equidistant rings with Z =  2 (i) or a helix with Z=O (j),the observation axis being either parallel to L or close to it.
324
7
Defects and Textures
verted twist. The meridian section in Fig. 24e is quite different: this screw dislocation was observed in cholesteric spherulites, the cholesteric layers of which are nested concentrically and, therefore, lie parallel to the external interface [62]. This defect, often called a 'radius of disclination', presents a continuous structure and has been modelled in both crosssections and in meridian sections [63]. A planar twist zone is differentiated along the screw axis, with an orientation opposite to that of the spontaneous twist, with a pitch slightly larger than the spontaneous one. Alternative meridian structures are possible, and avoid twist inversion by the introduction of point singularities at regular intervals along the screw axis [59] (as has been supposed to occur along the disclination diameter of some cholesteric spherulites [63]). The continuous meridian structure shown in Fig. 24 h also avoids twist inversions but these have been shown to occur in the two structures shown in Fig. 24i and j [49, 601. The core structure of cholesteric disclinations was interpreted by KlCman and Friedel [2,3]. The rotation vector considered in the Volterra process is normal to the cholesteric axis and is either parallel to the molecules or normal to them, this resulting in a core structure that is either continuous, with a longitudinal nematic alignment of directors in the core (A disclinations), or discontinuous (z disclinations), with a singular line of the type encountered in nontwisted nematic liquids. Now, consider around any of these disclination lines a closed circuit C and the ribbon generated by the set of directors centred along C [44, 531. Figure 26 shows a short straight segment of such a circuit, at a place where the director n is nearly constant, and the corresponding ribbon. One can replace a segment C , of this circuit by a curved segment C ; , which adds one helical turn and
.:fjA;,.>..L.2..2..z ,/ L,..r..t...r..T..r.
:
c...z..................
=..,\Iv>..ll;..x...lI;.. :... r c rh
t
'%............................. c c k
Figure 25. Local addition of a helical turn to a ribbon of directors (see text).
joins C tangentially at the two extremities of C ,. The addition of a helical turn modifies by one unit the 'linking number' of the two closed lines formed by the ribbon edges, but does not change the status of the ribbon, which is either the separation of the two faces, or their communication in the case of a Mobius strip. Note that the edges of a closed strip form either two closed curves, in a nonMobius strip, or a single closed curve, in the case of a Mobius strip. In the study of such strips, there is also the problem of points the director of which is locally tangential to C, but in this case a slight modification of the circuit suffices to avoid such points [44]. The main result in this study is that simple circuits closed about A disclinations give nonMobius strips with a vector n, whereas those closed around z disclinations are of the Mobius type. The core needs, to be continuous in order to be surrounded by nonMobius strips. Similar ribbons built with the twist vector C centred along such circuits are of the Mobius type for the four disclinations shown in Fig. 25.
7.3 Topological Structure of Defects
a 
325
........................... +c  cc 4 4
I + 
b ni
d... ”c ............... . _. .
.=...*.
y[= .... .;i:
.. .=.
..
.................. ..................... ; ................... c c c t

.......................
Figure 28. Progressive disjunction of edge dislocations in cholesterics (lefthanded twist). The open circles show the locus of vertical directors. (a) Planar model of a ‘very thin thread’. (b) First step of the disjunction into a k and a z+ dislocation. (c) Crosssection of a ‘thin thread’, with complete disjunction of the two disclinations k and z+, corresponding to a Burgers vector of length b = p / 2 . (d) Edgedislocation ofthe type kk+,with b = p . (e) A kk+pair withb= 3p.
When a large pitch cholesteric liquid is introduced within a wedge of two rubbed glasses, the ‘GrandjeanCano wedge’ [64], edge dislocations form and arrange in parallel, those with large Burgers vectors lying in the thickest regions of the wedge. Planar models such as the one shown in Fig. 27 apply in the thinnest zones, whereas in thicker areas the directors present vertical components in the vicinity of the defect and this transforms the dislocation lines into pairs of disclinations (Fig. 28 ac), with a z on the left and a A+ on the right [48,65]. Edge dislocations having larger Burgers vectors transform into dislocation pairs of the type A’A, with a fully continuous distribution of directors (Fig. 28 d and e).
326
7
Defects and Textures
These structures are well evidenced when cholesteric layers extend normally to the preparation plane, with weak anchoring conditions, resulting in socalled ‘fingerprint textures’. Disclinations are well observed in these conditions between crossed polarizers, if the pitch is large enough, and the presence of a central black zone is demonstrative of a A core; this is not the case with a zdisclination. The A+A associations are the most frequent. It can be verified that the set of directors centred on a circuit forming a simple loop around such disclination pairs is not a Mobius strip when the core is continuous, but is of the Mobius type when one of the two disclinations of the pair is a z disclination. Conversely, the ribbon obtained with the cholesteric axis C along such circuits is not of the Mobius type, whatever the nature of the two disclinations forming the dislocation. Disjunctions into disclination pairs are general in liquid crystals when the Burgers vector is large enough, and this holds for both edge and screw dislocations. This was first considered for edge dislocations in cholesterics [2, 31, but also applies to screw dislocations (see Fig. 24 i and j).
7.3.6 Optical Contrast All the translation defects shown in Fig. 28 are easily prepared in a wedge obtained, for instance, when a coverslip lies tangentially along a generator of a cylindrical lens, both the lens and the coverslip having been treated to obtain a planar anchorage with a preferential direction. A drop of nematic liquid added together with a small amount of a twisting agent allows one to obtain a pitch of 2030 ym. After this cholesteric mixture has been introduced between the two glasses, edge dislocations stabilize on both sides of the contact generator and form a se
ries of parallel lines that is easily observed under natural light. The use of a single polarizer or analyser is sufficient to vary the defect contrast considerably. As the local ellipsoid of indices is positively uniaxial and the twist is weak, the electric vector of any penetrating wave rotates as the director orientation (Mauguin’s condition: the wavelength being very small compared to the cholesteric pitch) [66, 671. If the electric vector of the incident beam is normal to the anchoring direction, the wave propagates as an ordinary ray, whereas if it is parallel the resulting extraordinary ray deviates and the image of the threads is much more shadowy and fuzzy [ 1 1,681. The use of a polarizer the main axis of which is perpendicular to the common anchoring direction of the two glasses gives clearcut ordinary images of threads, much thinner than the half cholesteric pitch p/2, and by analysis of the whole system several types of thread can be distinguished. Very thin threads in the vicinity of the contact generator between the cylindrical lens and the coverslip are poorly contrasted, and correspond to the planar structure shown in Fig. 28 a. The thin threads lie in slightly thicker regions of the preparation and correspond to the model shown in Fig. 28c. Horizontal streams decrease the contrast of these threads, which then resemble ‘very thin threads’, this probably being due to a horizontal alignment of directors [48, 651. The thick threads observed at the periphery correspond to the model shown in Fig. 28 d, but often form groups of parallel lines, separated by a distance that is the halfhelical pitch, as shown in Fig. 28e. The positions of thin and thick threads are indicated in Fig. 28 by open circles; many observations have led to the conclusion that these correspond to the locus of directors
7.3
parallel to the optical axis of the microscope, i.e. normal to the preparation plane, which is usually called the vertical [48]. Most papers dealing with thick and thin threads in nematics and large pitch cholesterics generally consider that these threads represent disclination cores. This is true for thin threads, but generally not so for thick ones. The confusion arises mainly from the fact that the core of a defect line corresponds to a strong maximum of curvature and it is highly likely that vertical directors will be found in its vicinity. A good approximation is to say that thick threads represent the locus of points where n,=n,.=O, and n,= 1, but the optics are complex, and this simply remains a first approximation.
7.3.7
Classification of Defects
As shown in every part of this section, liquid crystals are states of matter some of which are most appropriate for illustrating remarkable situations in combinatorial topology. The fluidity of mesophases is compatible with different types of curvature resulting in large series of defects, particularly disclinations, and the best tools for their definition and classification are the ‘homotopy groups’, the applications of which to liquid crystals are numerous [69781, but their use is somewhat arduous; they can be understood as a mathematical generalization of the Volterra process [72]. All the ‘topologically plausible’ points, lines and walls and their rehandlings are predicted without exception by this theory. The Volterra process has been used to define singular lines, but not defects as points, walls and certain structures with a continuous core. The theory also considers the rehandlings of defects [48, 531. However, it is worth remembering that among the defects that are ‘topologically plausible’, many of them do
Topological Structure of Defects
327
not exist, since they involve considerable energies; the simplest example is that of disclinations which are topologically plausible in threedimensional crystals  these have drawn [79] but are excluded in true crystals for energy reasons. This is also true for most liquid crystals. Geometrical and mechanical constraints are forgotten in purely topological considerations, and these are presented in the next section. Translation and rotation vectors are still the best tools in crystallography and for defining and classifying defects in liquid crystals. We have distinguished above between edge and screw dislocations, which are translation defects characterized by a Burgers vector, either normal or parallel to the line, but these defects often lie oblique to this vector as in threedimensional crystals, and the structure ofjogs and kinks has mainly been studied in cholesterics [48]. Disclinations (or rotation dislocations) introduce a rotation vector v that is either normal to L, a twist disclination, encountered mainly in planar models (see Figs. 9, 18 and 27), or parallel to L, a wedge disclination, more frequent in smectics and cholesterics. In the latter, we deal with four vectors: the directorn, the cholesteric axis C , the rotation axis v and the line axis L . Let us recall that, in A disclinations, v is parallel to n , but normal to C . In zdisclinations, v is normal to n and C (see Fig. 25); in disclinations, v is normal ton, but parallel to C (see Fig. 23). Note also that these disclinations, when they run parallel to the twist axis, reproduce the structure of screw dislocations in cholesterics. The symbols A, z and are often followed by an exponent +n,n,+2n,  2 q etc. corresponding to the rotation angle of the director after one 2 n turn along a small circle surrounding the core line of the defect. These exponents are often reduced to +, , 2+, 2. Figure 25 shows a a a T+= and a z=(often abbreviated as A+,A, z+,
x
x
rK,rK,
328
7
Defects and Textures
x
z),whereas Fig. 23 shows a series of disclinations from to The purely orientational order of nematics leads to discontinuities that are discrete structures in the form of points and thin threads. Continuous defects also exist, but some of these cannot be deformed continuously into the monocrystal and therefore should be classified as genuine defects. The presence of a spontaneous twist in a nematic liquid facilitates such situations, the main example being that of thick threads forming interlocked rings [48, 49, 53,731.
x + * ~x  ~ ~ .
7.4 Geometrical Constraints and Textures 7.4.1 Parallel Surfaces and Caustics in Liquid Crystals Many liquid crystals show a lamellar aspect, due to layers of uniform thickness arranged along parallel surfaces, and this is well observed in polarizing microscopy for some cholesterics, when the layer outlines are apparent (see Fig. 6). In these two micrographs, the layers change direction abruptly along straight or curvilinear segments belonging to the hyperbola branches, since they correspond to successive intersections of nearly circular profiles centred on two different points lying in the same optical section. The layers in fact form spirals, owing to the helical structure of cholesterics, rather than circular rings, and their thickness varies due either to real changes in helical pitch, or to apparent variations when layers are oblique. When the cholesteric pitch is less than 0.5 pm, the parallel profiles of the cholesteric layers cannot be resolved in light microscopy, but the straight or bent segments due to
abrupt changes in orientation remain well contrasted. These segments belong to hyperbola branches or ellipses, or parabolae, and form wellstructured arrangements that are found not only in short pitch cholesteric but also in smectic phases [ l 11. Parallel contours are also evident in smectic phases viewed under a polarizing microscope. In the case of smectic C* phases, for example, these contours are due to the helical periodicity, while in smectic E and lyotropic lamellar phases they occur when defects accumulate along certain lamellae or groups of lamellae. Normals to parallel layers form straight lines, as do the light rays with respect to waves in an isotropic medium, and they envelop two surfaces, calledfocul surfaces or caustics [ 19, 801. However, their presence in the mesophase produces a discontinuity wall, which generally disjoins into alternate +n and n disclinations [20, 811. Caustics are often absent from liquid crystals, since layers can be poorly curved, with ‘virtual caustics’ located outside the liquid crystal. For instance, layers are nearly horizontal in stepped drops of smectics, when the conditions are homeotropic along the glass and at the air interface. They appear to interrupt along oblique ‘cliffs’, arranged as more or less concentric level lines, and distortions are observed in their vicinity [82]. There are also examples of parallel spherical layers, with caustics reduced to a single point. The most extreme case of degeneracy of caustics occurs when each of the two surfaces reduces to a unique singular line and not to a series of lines as indicated above.
7.4.2 Dupin’s Cyclides and Focal Conics Surfaces C that are envelopes of spheres centred along a curve L have their normals
7.4 Geometrical Constraints and Textures
passing through L; conversely, all surfaces with normals converging along a curve L are envelopes of such families of spheres (Fig. 29 a). The contact curves between the spheres S and the envelope C are circles y. The normals along y converge towards A, the centre of the sphere S, and form a revolution cone, the axis of which is tangent to L in A. Cylindrical bilayers, which are straight, bent, or helical in myelin figures, are an example of such surfaces, which are envelopes of spheres of equal radius centred on a straight, bent or helical line L. Each caustic surface can reduce to lines L and L’ and a simple example is presented in Fig. 29b; the parallel surfaces are the nested and parallel tori, forming a +2n disclination L, the whole system presenting a revolution symmetry about a vertical axis, which is itself a second defect line L’. These tori are surfaces generated by (at least) two families of circles, their meridians and parallels, which also are their lines of curvature. The general problem of surfaces the normals of which pass through two curves L and L’ was solved by Dupin [83] and the first applications were considered by Maxwell; the general theory was developed in the 19th century [83] and in more recent articles [84]. Such surfaces Z are envelopes of spheres in two different ways  either a family of spheres S centred on L, or a family of spheres S‘ centred on L’  and there are two spheres S and S’ tangent at any point M of Z.The revolution cone associated with a contact circle y of S contains L’, and vice versa. If one knows one sphere S and three spheres S’ tangent to S, the family S can be defined (and the S’ family also). The three spheres S’ cut each other at two points, 0 and R, either real or imaginary. Let 0 be an inversion centre with a coefficient k=OM . Om=0Q2, where M and m are two homologous points aligned with 0. The three
329
L
Figure 29. Cyclides are surfaces the lines of curvature of which are circles. (a) An envelope X of a family of spheres S, centred in A describing L, and contact circles y. (b) Nested tori, the normals of which pass through the circle L and the axis L’, one sheet being suppressed to avoid intersection of the surfaces. (c) General aspect of Dupin’s cyclides, the normals of which pass through an ellipse E and a hyperbola H. (d) A focal domain built on the arc FM of a hpyerbola and on the arc PAA’N of the ellipse E. AA’ is the major axis with the two foci FF’. H’ is the virtual hyperbola branch. D and D’ are circular intersections of Dupin’s cyclides, the revolution cones being represented by their generators or director lines.
spheres S’ transform into three planes p’ and the spheres S transform into spheres s tangent to the planes p‘, their envelope being a revolution cone c, and thus the inverse of the surface X. The tangent planes to this cone are the inverse of spheres S’, which also pass through 0 and R, and the line L’ lies in the mediator plane of O n . L’ is planar
330
7
Defects and Textures
and belongs to all revolution cones of the normals converging on L, and is therefore a conic, an ellipse or a hyperbola or a parabola; this also holds for L. These two lines are conics, one being the locus of the vertices of the revolution cones passing through the other one. This situation is that of,focal conics, which lie in two normal planes intersecting along their major axes, the vertices of one conic coinciding with the foci of the other one. In general, an ellipse is associated with a hyperbola of inverse eccentricity, and this leads to a set of nested toroidal surfaces, the Dupin cyclides (Fig. 29 c), a system that is less symmetrical than the one shown in Fig. 29 b. In this case, instead of a
revolution symmetry and a mirror plane (Fig. 29b), there are two mirror planes at right angles to one another, which are the planes of the two focal curves. Smectic A phases often contain pairs of focal conics (see Fig. 7 a and b) that are well contrasted in the liquid, even in the absence of polarizers. A more common situation is the presence of arcs of conics associated in pairs (Fig. 29d). The parallel Dupin cyclides and the associated revolution cones form three mutually orthogonal systems of surfaces [7], and therefore the lines of curvature of any surface in one system are its intersections with the surfaces of the other two systems. The toroidal shape of Dupin’s
/”
‘
I
’D
Figure 30. Dupin’s cyclides and their deformations. (a) A toroidal Dupin cyclide and its circular lines of curvature y and y‘, the planes of which intersect along the axes A (joining 0 and a)and A’, respectively. Two tangential planes along two symmetrical circles T intersect along A. (b) A parabolic Dupin’s cyclide, with its two focal parabolae P and P’, its circular curvature lines y and y‘, and its axes A and A‘. (c) Three parallel, but separated, parabolic Dupin’s cyclides. The lines represent sections by planes x = O , y=O and z = 0; at the top of the figure, two conical points are present, as in (b), but the spindleshaped sheet has been removed (Rosenblatt et al. [SS]). (d, e) Edge and screw dislocations ‘compensate’ the bend and the twist of directors in a set of equidistant surfaces normal to the director lines.
7.4 Geometrical Constraints and Textures
cyclide is indicated in Fig. 30a. Conical points of Dupin’s cyclides are present all along the two conics, but one of the two sheets is absent, since interpenetration of layers is impossible. The forbidden conical sheets are shown explicitly in Fig. 29 d. The case of confocal parabolae is particularly frequent in the lamellar phase of lyotropic systems [85] and the corresponding Dupin’s cyclides (Fig. 30 b and c). Micrographs of focal conics were presented in the pioneer work by Lehmann [lo], and, some years later, in that by Friedel [ 1 11 who, together with Grandjean, observed the alignment of the positively uniaxial ellipsoids of indices along the straight segments joining points on the two associated conics [ 111. The transition to the solid crystal obtained after cooling often shows the formation of thin crystalline lamellae lying normal to these molecular alignments between the two conics (ethylazoxycinnamate or its mixture with, for example, ethylazoxybenzoate). The paired conics remain generally recognizable in this solid texture, which is called a pseudomorphosis [11] or paramorphosis [13, 141. By reheating the preparations one can revert to the initial liquid crystalline texture, with the focal conics located in the same places. This suggested the presence in these liquids of fluid layers forming sets of parallel Dupin’s cyclides, with molecules lying normal to them [86]. Very similar textures and defects were found in soaps and other lyotropic systems, which justifies the term ‘smectic’ chosen by Friedel for these lamellar liquid crystals [ l 11, the structures of which were rapidly confirmed by the first Xray diffraction studies [87]. The persistence of various textural aspects and domains through many phase transitions is common, and several examples have been described [13, 141.
33 1
7.4.3 Slight Deformations of Dupin’s Cyclides In a perfect system of parallel Dupin cyclides, the unit vectors normal to surfaces align along straight segments joining two focal conics. A deformation resulting in a local bend modifies the layer thickness or involves edge dislocations (Fig. 30d). Similarly, screw dislocations compensate a twist, when for instance focal conics are replaced by different curves. This is indicated in Fig. 30e, in which the layers are assumed to extend normally to straight segments, the extremities of which belong to two rectilinear segments AC and BD instead of to two arcs of focal conics. Suppose, for example, that AB, AC and BD are parallel to the axes of a trirectangle trihedron. The intersections of layers with the four faces of the tetrahedron ABCD form concentric circular arcs, the concavities of which alternate, showing that layers are saddleshaped. Moreover, successive arcs joined at their extremities do not form a closed loop, but a helical path. The geometry of this tetrahedral domain requires the presence of righthanded screw dislocations, whereas the mirror image of ABCD would lead to lefthanded defects. The local density of these defects within a lamellar structure (total Burgers vector in the unit volume) is Inxcurlnl for pure edge dislocations and In . curl n I for pure screw dislocations [88]. Polygonal textures such as those shown in Fig. 6 associate not only horizontal segments (curvi or rectilinear), but also vertical ones, joining centres to the vertices of polygons at the upper and lower faces of the mesomorphic slab, between the slide and the coverslip. The positions of these segments are shown schematically in Fig. 3 1 a for the cholesteric phase occupying the vertical prism AA’CC’BB’DD’. The cholesteric axes, normal to layers, join points belong
332
7
Defects and Textures
Figure 31. (a) Prismatic subunit of a polygonal field, in cholesteric and smectic A phases. Double lines represent focal segments. (b) The prismatic unit shown in (a) decomposes into five tetrahedral domains. (c) General aspect of the layers in a square polygonal field; double lines represent the array of focal segments. (d) Very acute conical points along focal segments are not only rounded, but are also rehandled by a n disclination. This actually introduces two conical walls, but the layers also are slightly rounded and more focal curves are involved.
ing to the two contours A’ABB’ and CC’D’D indicated by a doube line. Therefore, the prism decomposes into five tetrahedra (Fig. 3 1 b) filled with saddleshaped cholesteric layers. In each tetrahedron two opposite edges, called focal curves or focal segments, play the role of focal conics. These segments often are conics, but not in a focal position.
The whole texture is made of such prisms, juxtaposed in continuity. These divergences from the Dupin cyclides model can result in the presence of either translation dislocations or layer thickness variations, or in layers that are slightly oblique to segments joining the conjugated contours. The cholesteric layers extend continuously across the triangular faces joining the tetrahedra, except for the focal segments A’ABB’ and CC’D’D. There are no other discontinuities across the vertical faces joining all the prisms into a texture such as the one shown in Fig. 10a and b. Note, however, that the two radii of curvature show a discontinuity along the oblique edges of the tetrahedral domains, which is probably attenuated by slight deformations. Polygonal textures often form square lattices in cholesteric and in smectic A phases. The global arrangement of nested parallel layers, between the horizontal slide and coverslip is shown in Fig. 31 c. The layers lie vertically at the upper and lower faces of the mesophase and are oblique in between, but they are not perfectly perpendicular to straight lines joining the conjugated segments, and thus show important thickness variations, particularly in the vicinity of focal segments. This is often corrected by a rehandling such as the one illustrated in Fig. 31 d.
7.4.4 Textures Produced by Parallel Fluid Layers The main patterns present in these textures are shown in Fig. 5 for lyotropic lamellar phases and in Fig. 32 for thermotropic liquid crystals.
7.4.4.1
Planar Textures
Layers lie parallel to the slide and the coverslip, a more or less frequent situation in
7.4
ft
333
smectic A and cholesteric phases, when the glasses have not been treated for molecular anchoring. These textures are produced regularly in smectic A phases, where strong homeotropic conditions prevail, while a planar anchoring with an easy horizontal direction is required for cholesterics. In general, edge and screw dislocations are present within these planar textures (Fig. 32 a) and are often seen by light microscopy of cholesteric phases of sufficiently large pitch [20], whereas these defects are detected only by electron microscopy in cryofractured, mainly lyotropic, smectic phases [89]. In some cases, edge dislocations intercalating a unique smectic layer can be visualized by means of light microscopy; an example of this has been described in smectic C phases, together with all the technical details of the optics [90]. Some edgedislocations, however, present large Burgers vectors and disjoin into +n and n disclinations; layers intercalated between these disclinations lie vertically and form brilliant stripes in polarizing microscopy or oily streaks (see Fig. 5 d), a common textural pattern in smectic A and cholesteric phases [ 1 1 ].
i Df
Geometrical Constraints and Textures
is s
Figure 32. The main types of texture in layered liquid crystals. (a) Planar texture with edge (E) and screw (S) dislocations. (b) Two tangent focal domains, and their tangent ellipses and the converging arcs of hyperbola. (c) Nested ‘hats’ along a focal line. (d) Screw superimposed on a focal line. (e) Focal lines attached to the upper and lower interfaces. (f) Focal domains tangent along a series of coplanar generators; contacts between domains are parallel or antiparallel. (8) Section of (d) along the symmetry plane, showing the discontinuities in the curvature at the antiparallel contacts. (h) General patterns in fans, associating +nand n disclinations and edge dislocations (and also focal curves, not shown). (i) Schematic distribution of textures in the vicinity of the isotropic phase in lamellar thermotropic liquids: ft, fan texture: is, isotropic phase of the mesogen; p, planar texture: pf, polygonal fields; s, spherulites.
7.4.4.2 Focal Conics and Polygonal Textures We have already considered the polygonal networks of cholesteric liquids, which assemble saddleshaped layers close to Dupin’s cyclides, and the focal segments of which differ from those of focal conics (see Sec. 7.4.3). Friedel and Grandjean [21] described in smectic A phases a texture much closer to Dupin’s cyclides, with genuine focal conics. As for cholesterics, this texture is obtained when a thin film of the isotropic phase of the mesogenic compound separates the mesophase from the two glasses. The mesophase itself is divided into focal domains, each one being defined by its
334
7
Defects and Textures
two conjugated arcs of conics (see Fig. 29 d), which determines uniquely the corresponding family of parallel Dupin cyclides. Each domain is limited by fragments of revolution cones joining along edges, which are either generators or arcs of these conics. The fragments of Dupin cyclides filling these domains are essentially saddleshaped (see Fig. 32 b), but are hatshaped along the focal curves, with a strong maximum of curvature and layer thickness (see Fig. 32c). This can be viewed in cholesterics by using light microscopy (see Fig. 6) and in lyotropic smectic phases by using electron microscopy [89]. Screw dislocations sometimes superimpose on focal curves, as shown in Fig. 32 d [54]. When focal lines run horizontally, attached to the upper and lower interfaces limiting the mesophase, the layers form halfcones, which also present a rounded apex (Fig. 32e). Focal domains in smectic A phases are tangent along generators of their limiting cones, the contact being either parallel or antiparallel‘in Fig. 32f, where the major axes of ellipses are aligned, and this allows one to obtain a view of layers in the mediator plane (Fig. 32g). The dashed lines in Fig. 32 g represent the contact generators between the tangent focal domains, either parallel and without discontinuity of the radii of curvature, or antiparallel and with a discontinuity. It is worth remembering that, as for cholesterics, these discontinuities of curvature present in the model are attenuated or smoothed out by a rapid but continuous change in the sign of the curvature. Such tangent domains are illustrated in Fig. 33, which shows a lattice of ellipses, just below the coverglass. The ellipses are separated into different sectors, which end in a polygonal field at the top lefthand side of the micrograph. The sectors are separated by lines that are particular polygon edges, and in fact each sector belongs to a polygon.
The ellipses are tangent to other ellipses and to the polygon edges. Their focal hyperbolae converge to a point on the opposite interface, which is a vertex of the conjugated polygonal lattice. This means that, withi n the polygon plane, the major axes of the ellipses converge to a point that is the vertical projection of a vertex common to several polygons of the conjugated lattice. When three ellipses are tangent, the free space left between them is often occupied by another ellipse at the base of a narrower focal domain, tangential to the surrounding domains, and the interstices can in turn be filled by narrower cones. It has been proposed that this iterative process persists down to a few molecular lengths [91], and therefore below the resolving power of the light microscope. This view is justified in models that keep all layers normal to the horizontal interfaces, thus limiting the polygonal field. It is also justified by energy estimates and by cryofracture images, which often show very local conical deformation involving a few bilayers only [89]. However, in thermotropic smectic phases forming polygonal networks, very small ellipses seem to be absent, their size rarely being less than the 1/20 of the polygon diameter. On the contrary, the interstices are assumed to form spherical domains, the layers being spherical and centred on the polygon vertex, where the hyperbolae of the surrounding focal domains converge [92].
7.4.4.3 Fan Textures Layers that are mainly vertical and the presence of disclinations (see Fig. 32 h) are the two very common characteristics of fan textures in smectic and cholesteric phases. The name ‘fan texture’ comes from the circular contours that are often visible around disclinations in, for example, cholesterics, and from the frequent radial decorations (see
7.4 Geometrical Constraints and Textures
335
Figure 33. Polygonal field (top left) and elongated polygons, with their long edges converging at a +rr disclination. 4Cyano4’noctylbiphenyl plus Canada balsam; crossed polarizer. Scale bar: 50 pm.
Fig. 33) seen in smectic A phases. Focal curves and translation dislocations are not excluded from fan textures. The fan patterns themselves can be absent from certain arrangements of disclinations, which however belong to the family of fan textures. This is illustrated by the rhombus in Fig. 34a and b, where two +ITand two IT disclinations are associated with several focal curves at the top and bottom levels of the mesophase.
7.4.4.4 Texture Distribution in Lamellar Mesophases When smectic A or cholesteric phases are in equilibrium with their isotropic phase, the mesophase is present in the preparation in the form of bltonnets or droplets, and extends here and there over larger domains, with a definite distribution of textures. Fans lie in the vicinity of the isotropic interface, whereas planar textures are rarely in contact with it, and polygons are observed along zones separating fans from planes.
336
7
Defects and Textures
Figure 34. Cholesteric textures: (ac) MBBA plus Canada balsam: (d) MBBA plus cholesterol benzoate. (a, b) Two views at the coverslip and slide levels of a fan texture, with lozenges associating two + K and two n disclinations, linked by pairs of focal lines. (c) Planar domains separated by walls of nearly vertical layers. (d) One of the walls is associated with horizontal and vertical focal lines, appearing as intercalated black spots. (a, b) Crossed polarizers: (c, d) natural light. Scale bars: (a, b) 20 pm: (c, d) 50 pm.
As indicated above and illustrated in Fig. 32 i, layers lie horizontally in planes and show some translation dislocations. They are oblique in polygonal fields and generally cross the focal lines at points where they are strongly hatshaped, whereas elsewhere they are saddleshaped and dislocations are present, often superimposed on the focal lines. In fans, the layers are vertical and all types of defect (disclinations, focal curves, dislocations) are present.
This texture distribution is common, but corresponds to a rather schematic model, indicating that highenergy defects, such as disclinations, are found mainly in the vicinity of the isotropic transition. Other situations are observed in thick preparations of cholesterics, for example, where planar domains can be interrupted by walls of vertical layers (Fig. 34c and d), due to edge dislocations disjoining into disclination pairs (see Fig. 5 d). Despite these par
7.4
ticular examples, the presence of disclinations remains a general character of fan textures. The textures described above belong to the same phase and are not separated by sharp interfaces. The frontiers are fuzzy and are often the sites of hybrid, but interesting, textures. Among these, at the limit between polygons and fans, one finds occasional chevrons, the organization of which is shown in Fig. 35 [93]. Chevrons and related textures are common in smectic phases but, at the horizontal interfaces, the directors must be adjusted to the anchoring conditions [88, 931. They are regularly produced when opposite sides of polygons are extremely elongated in a given direction [20]. This leads to arrangements as those represented in Fig. 35. When vertical anchoring of layers is preferred, ellipses or parabolae can form at the interfaces, with the corresponding focal domains, but the layer anchoring remains oblique in the interstices between domains [93]. This situation is also realized in Fig. 33 with a radiating series of extremely elongated polygons, centered around a +n disclination.
Geometrical Constraints and Textures
7.4.4.5
337
Illusory Conics
The analyis of focal conic systems in liquid crystals is made difficult by the presence in pictures of lines, which often resemble focal conics or focal curves but actually are not. It was indicated above that conics such as polygon edges are not in a focal position, and that many lines differ from conics but play a focal role. Figure 36 shows an example of a cholesteric texture simulating the presence of a series of parabolae, but this aspect is due to complex behavior of the polarized light, associated with a frequent moirC pattern. This texture is simply interpreted in Fig. 37 on the basis of an examination of the orientations of the layer and the focal lines, which are straight or slightly curved in this texture, but not parabolic.
7.4.4.6 Walls, Pseudowalls and Broken Aspects True walls are defined by a director discontinuity extending over a surface within a liquid crystal, but these defects are excluded from nematic, cholesteric and smectic A phases (see Sec. 7.2.3). Grain boundaries comparable to those of true crystals are associated with translation dislocations, which lie parallel within the wall or form
Figure 35. A model of chevron textures (the chevrons are viewed from the top) showing alternating angular and rounded contours, at both the slide and the coverslip level. Prismatic domains d and d’ are filled with antiparallel conical sheets, in continuity along the generators r, s, t and u. Parabolic contours M, N and P join and form angles along the lines L at the coverslip level C, and similarly arcs M’, N’and P’ join and form angles along the lines L’ at the slide level S .
338
7
Defects and Textures
Figure 36. A cholesteric texture simulating the presence of focal parabolae. (a, b) Optical sections at the coverslip and slide levels. MBBA plus cholesterol benzoate, crossed polarizers. Scale bar: 20 pm.
diverse networks [9]. The presence of such defects is probable in smectic phases having twodimensional order within layers, and in certain columnar phases. This also holds for smectic systems, when the hexagonal or rectangular arrangements are coherent over several lamellae (smectics B, E, G, H, etc.) the order being threedimensional. When smectic layers are mainly horizontal, the existence of walls often leads to mosaic textures, each domain extending over the entire thickness of the preparation. A platelet texture is observed when the do
mains of the horizontal layers are much thinner than the mesomorphic slab, and superimpose here and there, with their distinct orientations [13, 141. When vertical layers bend concentrically about +n disclinations, circular bands of different colour or shade appear, indicating changes in the crystallographic orientations along grain boundaries. These banded textures are common in orthorhombic smectic E phases. A planar wall has been described in smectic C* phases, giving rise to a particular chevron texture. This has been shown
7.4 Geometrical Constraints and Textures
S /
Figure 37. Model of the arrangement of layers and focal lines in the texture shown in Fig. 36. (a) Distribution of layers. (b) Vertical and horizontal focal lines at the top (coverslip C) and bottom (slide S ) levels of the mesophase.
by highresolution Xray scattering in surface stabilized ferroelectric samples obtained by cooling from the smectic A phase [94]. At the smectic C transition, the layers progressively tilt symmetrically in two opposite directions, by an angle of about lo", whereas molecules are tilted horizontally within layers at about 20" from the normal to the layers. The long axis of molecules show a quasi uniform orientation within this wall and the two domains, but the ferroelectric polarization changes abruptly across the wall and breaks its apparent symmetry. This type of chevrons leads to complex textures [95]. In smectic A phases, such a change in the orientation of layers along a wall involves a discontinuity of molecular alignment. If the wall is replaced by a narrow zone of strong
339
ly curved layers, this involves an equal splay of molecules, and the structure is generally handled by dividing it into a set of focal curves or even disclinations. The case for smectic C phases is different, as such walls often are compatible with a uniform alignment of molecules, facilitated by a dilatation modulus of the layer thickness that is much smaller than that for smectic A phases. This leads to noticeable undulation instabilities [96]. Molecules rotate within layers and, conversely, layers show different possible orientations with respect to a molecular alignment. In chevrons such as those shown in Fig. 35, the layers are at a constant angle to the lines L and L', an angle which can be chosen to be that of the tilt [57].The discontinuity i n the layer orientation in the ferroelectric display can be smoothed by focal curves and other defects, which are weakly contrasted because the molecular orientation is not really altered by their presence. Singular lines often attach to interfaces. Among the numerous examples given here is the case that occurs in nematic phases at the slide or coverslip level (see Fig. 9) and that of largepitch cholesteric phases at various interfaces (see Figs. 19 and 20). Such lines are due to the presence of horizontal directors that are forbidden at a horizontal interface. The locus of horizontal directors i n the bulk form a surface, which shows a higher mean refractive index and appears contrasted under natural light or in phasecontrast microscopy. The clearcut interface line seems to extend into a wall within the bulk, but actually this is a mere optical illusion, which is the origin of the socalled Grandjean planes in cholesteric phases [44]. Broken aspects are classical in focal conics or fan textures of tilted smectics, and also originate from singular lines attached to an interface. This is observed in smectic C phases when disclinations like those shown
340
7
Defects and Textures
in Fig. 21 ad adhere at an interface and separate two different molecular orientations. The smectic layers lie almost vertically (i.e. perpendicular to the interface), whereas the molecules are horizontal within the layers at the interface contact. However, the molecular orientation remains continuous in the bulk. The lines limiting these interfacial domains are either parallel or normal to layers and this creates a contour composed of straight segments alternating with arcs at right angles and with some interspersed irregularities [97]. These interface textures superimpose broken patterns onto smectic focal domains and fans, not only in smectic C phases but also in more ordered types of tilted smectic phases such as SmF, SmG and SmH [13, 141.
7.4.5 Origin of Spirals in Chiral Liquid Crystals Cholesteric layers show spiral contours (Fig. 6 a and b) around polygon centres and vertices (see Fig. 6 a and b). Analogous patterns decorate cholesteric droplets (see Fig. 2). Such spirals have also been found in thin sections of stabilized analogues of cholesterics, i.e. in biological materials assembling long biopolymers such as chitin, in various arthropod carapaces (crabs, insects) [27331. To explain these patterns, let us start from cholesteric layers arranged as nested toroidal surfaces (see Fig. 29 b). This situation is shown schematically along a meridian plane in Fig. 38 a; the lefthanded twist and three section planes (13) are illustrated in Fig. 38 bd. The hatched zone in Fig. 38 a indicates the part of the drawing to be suppressed in order to obtain a situation similar to that of layers in contact with an isotropic phase of the mesogen at level 1 (Fig. 38b). Going up Fig. 3 8 a one passes continuously from a uniform alignment of
directors (d) to a doublespiral pattern (c) and a pair of A+n disclinations (b). These three steps are assembled into a unique pattern in Fig. 38 e, which indicates how a continuous deformation resembling a whorl produces a disclination pair and a spiral the orientation of which is linked to that of the twist. Figure 31 d shows how the presence of a z disclination eliminates very acute conical shapes of nested layers. This arrangement of layers creates a rhombic and conical domain in the midpart of most of the polygon edges in Fig. 6 a. Careful examination of the layers under natural light at a level close to the coverslip generally shows a structure like the one shown in Fig. 38 f. The I" disclination forms a helical halfloop [20] due to the cholesteric twist, a situation very similar to that described in other helical cholesteric patterns (see Sec. 7.3.4). Spirals and concentric circles are common in the focal domains of smectic C* phases [97]. They are produced by lines such as those shown in Fig. 21c and d. These disclination lines have often been observed in preparations of vertical or slightly tilted layers. The molecules lie almost parallel to the glass plates at their contact, with uniform alignment, whereas the helical arrangement is present in the bulk. Equidistant and parallel disclinations of the type indicated shown in Fig. 21c and d separate the chiral and nonchiral domains; these have been called 'unwinding lines' [%I. They are present at two levels: in the neighbourhood of the upper and lower plates; and adjoining the thinner regions of the preparation, where they form loops or simple helical lines [97]. When focal domains are differentiated in smectic C* phases, with ellipses attached to a glass, the molecules also lie parallel to the glass, and this prevents the formation of a helical structure, which does, however, occur at a distance in the bulk. Unwinding
7.4
Geometrical Constraints and Textures
34 1
a
d .3........
f
lines therefore appear, and produce patterns the principle of which is closely related to that described above for cholesterics. The main differences are that in smectic C* phases, the distance between two successive lines i s p , the helical pitch, whereas in cholesterics the periodicity is pI2, and the double spiral in cholesterics is reduced to a single one in smectic C phases. One can also observe concentric circular lines, the successive radii of which differ by p , and this is explained by the presence of a screw line superimposed on the vertical focal line, as in cholesterics (see Fig. 32 d).
f
Figure 38. Continuous passage from a focal line to disclination pairs in a cholesteric liquid. (a) Meridian section of the texture corresponding to a threedimensional representation of the structure shown in Fig. 29b; the nail convention indicates the presence of a lefthanded twist. (bd) Distribution of directors at levels 13 in (a), presented with the nail convention. (e) An imagined pattern to show in one picture the continuous passage from a uniform alignment at the periphery to a whorllike texture, with two disclinations in the core. In (b) and (e), the separated segments corresponding to horizontal directors are represented by continuous lines. (f) Helical shape of the il" disclination in Fig. 3 1 d and the lozenges of polygonal edges shown in Fig. 6.
7.4.6 Defects and Mesophase Growth Defects, particularly screw dislocations, play an important role in the growth of true crystals [9]. Liquid crystal germs present the defects that were described in detail by Friedel and Grandjean [21] for smectic A phases. The germs elongate perpendicular to the mean direction of the layers, the surface tension being anisotropic, and the focal domains present in the batonnet are arranged such that the layers lie normal to the isotropic interface. A focal line is often present
342
7
Defects and Textures
along the axis of the biitonnet, and screw dislocations can be superimposed [54], which could accelerate the transition and facilitate the elongation. Cholesteric rodlets and spherulites having parallel layers can be devoid of inner defects, but this does not prevent their growth. However, surface points or surface lines are present. Some n disclinations, resulting from germ coalescence, are frequent, but disappear by confluence with the isotropic interface, as for nematic droplets. Spherulites showing concentric layers present a disclination radius or diameter, but this structure is due to a topological constraint and does not seem to be linked to liquid crystal growth. Very rapid growth of cholesteric phases often generates screw dislocations of the two types shown in Fig. 24i and j , and this has been filmed by Rault in pazoxyanisol added to cholesterol benzoate [98,99]. Slow growth does not result in the production of these defects. Experiments have also been done at phase transitions from nematic to smectic A phases, starting from a twisted situation between two glasses with a strong planar anchoring, the two easy directions being at right angles (see Fig. 9). Thin threads are present at the junction of twisted zones (lefthanded and righthanded). These transform at the smectic transition into a broken helical line, composed of a series of triplets comprising (1) a focal curve, (2) a segment of a +n disclination and (3) a focal curve, the two focal segments (1 and 3) being conjugated [ 1001.Considerations such as those developed for Fig. 30e show that numerous screw dislocations attach to the +n line and form a radiating pattern that is visible under the light microscope, which suggests the presence of important Burgers vectors. Lyotropic lamellar systems often show undulated or helical arrangements of focal domains [ 1011, possibly similar to those of thermotropic phases [ 1001.
7.4.7 Defect Energies and Texture Transformations Translation dislocations do not strongly modify the orientation of the directors or layers at long distances, as disclinations in liquid crystals do, and focal conics occupy an intermediate position (see Fig. 32 i). This indicates a gradation of energies, which will be considered below using some examples.
7.4.7.1 Disclination Points Let us begin with simple defects, such as those that occur in capillary tubes (see Fig. 8). In the lefthand part of Fig. 8 a there is a radial point in the vicinity of which the directors are supposed to be aligned radially: n (M) = r / r , with r =OM and r being the positive distance separating M from 0, the core of the defect. Then divn =2/r; the twist and bend, whether spontaneous or not, are absent, and the density of the elastic energy is given by 
dv
2ki’ or d F = 8 n k l l d r r
Integrating the elastic energy over a sphere centred on 0, of radius R, yields
F= 8~kIlR Such a purely radial arrangement of directors is more plausible when twist and bend are forbidden, particularly in smectic drops immersed in an isotropic fluid creating homeotropic conditions. This is realized for some spherical 4cyano4’noctylbiphenyl (8CB) droplets immersed in water or glycerol (Fig. 39a), but for most droplets in this domain the spherical symmetry is reduced to revolution symmetry by a focal domain attached at the centre, with smectic layers normal to the interface (Fig. 39 b). This means that interfacial tension depends on the angle of directors at the interface, with
7.4
Geometrical Constraints and Textures
343
nent of OM (0 being an arbitrary point of the line), then dF d i v n = 1 and =r dv or d F = n L Figure 39. Spherical smectic droplets of 8CB in water or glycerol. (a) Presence of a radial singularity. (b) A focal domain associating a focal radius and a circle. The distribution of the layers is drawn in a meridian plane.
a strong minimum for molecules lying normally and a less marked one for those parallel to this interface with water or glycerol. In nematics, director lines form diverse patterns around singular points, associating splay, twist and bend in different proportions [ 1021. In a spherical nematic droplet floating in an isotropic medium, with the directors parallel to the interface, two singularities appear at two diametrically opposite poles, with radial arrangements similar to the one shown in Fig. 12 a. For a spherulite of radius R, with k , =k,, =k, and assuming that the twist is absent, F = S n k R . This means that the volume energy due to a radial point at the centre of the spherulite is appreciably higher than that of two surface points. This confirms that defects ‘prefer’ to join an outer interface in order to minimize their energy, and this is reinforced by the fact that nematic molecules generally align with the isotropic interface, rather than lying normally.
41 2r2
h!.d r
( r )
where L is a given length of the singular line. The energy cannot be integrated from 0 to R, as for the radial point, and a cutoff is required. A radius core R, that is close to molecular dimensions is introduced; E, is the core energy per unit length. Hence the line energy density E in the capillary or in a myelin form is
E = E,
+ n kll In(
a)
The disclination patterns usually considered in energy calculations in nematics are the solutions of a Laplace equation v2@=0of the type
,
(see Sec. 7.2.4; in energy calculations, the topological parameter s =N/2 is now generally used rather than N ) . In this case k , =k,, =k,, =k, and
,
divn = cos(@  q)d@ rd9 (nxcurln)2 =
do2 d r 2 + r2d q 2
7.4.7.2 Disclination Lines
from which we deduce
As shown in Fig. 8 b, lateral homeotropy in a capillary tube filled with a smectic A phase results in pure splay that is distributed homogeneously about a disclination line, together with cylindrical symmetry. Note, however, that core rehandlings are observed [42]. If r represents the transverse compo
dF 2=dv
ks2 k z Ls2 d r or d F = r2 r
E = E,
+ kns2In( $)
For s= 1, we now refind the energy of the radial disclination of a smectic liquid in a
344
7
Defects and Textures
capillary tube. At the nematic transition, this disclination relaxes, with an ‘escape in the third dimension’ (see Fig. 8 a), the splay lying mainly along the axis and the bend at the periphery. In the absence of twist, one has: rIR=tan 8I2 (where R is the inner radius of the capillary, r is the distance from point M to the axis, and 8 is the angle separating the director at point M from the axis). This means that the director lines have a meridian profile of constant shape and, to a first approximation, the textures in two different tubes of radii R 1 and R, differ only by a pure dilation of ratio R,IRl. The total deformation remains constant and the energy does not depend on the inner radius R. The energy per unit length is E = 3 k z , in disclinations s = + 1, with a continuous core [39411. For s=1, E = k z The passage from a planar structure of a disclination to a continuous core suppresses the factor In (RIR,), and represents a nonnegligible energy saving. Vertical disclination lines normal to horizontal layers in smectic C phases also form nuclei. Polarizing microscopy shows that these nuclei have four branches, and when examined in projection onto the layer plane the observed patterns correspond to @ = O0+ s cp, with s = +1. It has been demonstrated that the tilt angle of molecules with respect to the normal to layers is variable, but decreases to zero in the vicinity of the disclination core [ 1031. This also resembles an ‘escape in the third dimension’, and is mainly due to the low value of the dilatation modulus B . Interactions of disclinations have been studied in nematic and smectic C schlieren textures, which associate nuclei interpreted as vertical disclinations. Assuming a purely horizontal distribution of directors and an ‘elastic isotropy’, within any horizontal plane and in the vicinity of disclination Di, centred on Oi, we have 0= Oi + si( p i . At any
point M in the texture, the director is defined as @ = Q0 + C si ‘ p i , but this superposition principle requires that R, Q r,2 4r [ 1041.The energy of a disclination pair is given by
The first term disappears when s1=s2, a common situation in schlieren textures of nematic and smectic C phases. In general, CsiIm 0, m being the total number of nuclei in the texture [ 11,451. The second term in the energy represents the interaction: disclinations of opposite sign (sl s,cO) attract because variations in E and rl2 occur in parallel [45], whereas they repel when they are of like signs (sl s,>O).

7.4.7.3
Focal Curves
The energy of a focal domain defined by the ellipse E and the corresponding hyperbola branch, extending from one focus of E to infinity, is: E = kl,zL(l
 e2) ln(aIR,)
L being the ellipse perimeter, e its eccentricity and a its half major axis. The energy of focal domains was also calculated for pairs of parabolae [ 1051. It was indicated in Fig. 32c that layers along the conics are not exactly conical but present a rounded apex, with a local thickness maximum. Assuming curvature radii very large relative to the layer thickness, 8 being the angle between the normal to layer and the focal curve, whose maximum 8, remains small, the energy associatings play and layer dilatation, is per unit length: E = zk11(6J2 In(1.46RIr)
7.4 Geometrical Constraints and Textures
with r2A/&, A being the penetration length (kl,/B)”2 11061.
7.4.7.4 Translation Dislocations All the expressions given above for disclination and focal curve energies are similar to those for screw and edge dislocations in true crystals [9, 151, but the situation is different for translation dislocations in smectics. The presence of a screw dislocation of weak Burgers vector does not introduce any splay and does not really modify the layer thickness even at small distances [16]. The energy is reduced to a core term and therefore interaction terms are absent in the frame of the linear theory. This is not the case for edge dislocations in this approximation [ 1061, and one has the expression: E = Ec+kllb2/2ARc with A2=kll/B, b being the Burgers vector length. Actually, edge dislocations in smectics generally split into parallel disclinations +z and z, distant of b/2 [16] and this introduces a pure splay in domains of nested cylindrical layers, whose energy is: K kl ln(6/2 Rc)/2. A third term zc is to be added and corresponds to the core energy of the K, what leads to a more complex expression: E = k , , b 2 / 2 A R c + ~ k ln(b/2Rc)/2+zc ll When parallel edge dislocations lie in the same plane, their interaction is negligible; but if they lie at different levels, dislocations attract or repel according to their relative positions and orientations [ 1071.
7.4.7.5 Simulations of Defects and Textures Computer models have been used to simulate the distribution of directors in nematic disclinations and textures, the partial dif
345
ferential equations being replaced by finite difference equations [108, 1091. For instance, in a square lattice, the cell i, the director of which is specified by an angle @;, has four neighbouring cells i’. If the elasticity is isotropic V2@=0, the interaction energy is Ei = C sin2(aitQi). Differentiating with respect to gives the best orientation in cell i (generally a minimum of E;, not only differ by a few a maximum) if the degrees:
The total energy over the model is then:
Note that a knowledge of @ along the cells at the periphery is generally sufficient to deduce the entire pattern, since it leads to a linear system with an equal number of equations and unknowns, plus a determinant different from zero, as indicated in early work on Dirichlet’s problem [ 1 101. It is also possible to start from a given distribution of 0, with various boundary conditions such as those known to produce disclinations, and to recalculate the different @; averaged over the four neighbouring cells. This leads first to a decrease in E , the process being repeated iteratively towards a complete relaxation. One can verify that a planar + 2 dis~ clination disjoins into a pair of +K disclinations, due to the presence of the s2 term in the energy: The total energy of two disclinations s = 1/2 represents the halfenergy of a single disclination s = 1. Obviously, there are textures where integer indices are preferred, for many reasons: escape in the third dimension, point singularities, certain anchoring conditions, and topological constraints (such as in smectic C phases) all forbid halfinteger values of the s indices.
346
7
Defects and Textures
These methods have been refined to give a constant splay/bend ratio in purely planar systems, and they allow one to reproduce the wellknown aspects of disclinations in pure bend or pure splay situations. These models have also been extended to three dimensions by taking the twist into account, and one can refind the geometries of director lines in capillary tubes or other cases of 'escapes in the third dimension'.
7.4.7.6 Defect Nucleation Many defects originate from a nonparallel coalescence of germs (Fig. 40). In addition, mechanical constraints generate edge and screw dislocations, or another pattern called 'elementary pinch' (Fig. 41), which is also found in cholesterics and probably at the origin of focal domains in smectics. This pattern seems, therefore, to be essential in texture transformations.
Figure 40. Schematic representation of defects created by the coalescence of nematic germs.

+= a 
h
Elementary pinches differentiate from local fluctuations that are able to diverge and produce large defects, if certain constraints are present. In cholesterics, the formation of elementary pinches is continuous, since it involves the nucleation of a A A+ pair [48]. These pinches are produced in the same way in nematics submitted to electric fields (see Fig. 5 a in Stieb et al. [ 1111). In largepitch cholesterics, the transition from a constrained aligned state to the relaxed twisted state also involves the nucleation of these elementary pinches. The constrained state is due, for example, to strong homeotropic conditions, and is relaxed by a progressive increase in the distance separating the two horizontal plates [ 1 121, or by a transverse electric field, if the dielectric anisotropy is negatively uniaxial [I 13, 1141. Many textures arise from a field or a dynamics created in a previously aligned liquid crystal [ 115, 1161. Such evolutions are also observed in cholesteric mixtures in equilibrium with the isotropic phase, with fans along the interface, and with polygons and planar textures generally at a greater distance from the isotropic transition. Gentle heating modified the positions of the textures by means of local transformations, but hydrodynamic streams are absent, or almost so. Cholesteric layers, which are initially planar, arrange progressively into domes and basins, and the transformation is continuous, the explanation being derived from Fig. 38 ae. This also arises from local fluctuations forming directly elementary pinches, which easily transform into spiral patterns.
7.4.7.7 Textures and Defect Associations Figure 41. Creation of defects in a lamellar liquid crystal. (a) Edge dislocation due to a layer rupture. (b) Deformation of an edge dislocation into the helical structure of a screw dislocation. (c) Differentiation of an elementary pinch. (d) A pair of elementary pinches transforming into a pair of edge dislocations.
Defects form complex networks, but between these singular structures the liquid crystal is regularly curved. The geometry is often well defined, and one may think that a knowledge of the network would be suf
7.4
ficient to rebuild the complete director distribution. Actually, this is a difficult problem, the solution of which depends on its accurate formulation. For instance, two parallel disclinations d+and d can be associated to give either an edge dislocation (as in Fig. 28 d and e) or an elementary pinch (see Fig. 41 b), or very different textures. On the contrary, the presence of two conjugated focal curves defines unambiguously the director distribution within the corresponding domain, with the exception of the exact layer position. Three types of defect association have been encountered in this discussion: superposition of defects, concurrence of lines at singular points and conjugation between two lines or two points. Among superpositions, the first case is simply that of lines of identical nature, for instance translation dislocations that join or disjoin, with additive laws for the Burgers vectors. As indicated above, the energy of these dislocations increases as the square of the Burgers vector b2, and in principle they split into series of elementary dislocations. However, in practice, they are seen to assemble or separate in, for example, cholesterics. This fact underlines the importance of boundary conditions and the presence of other defects in their vicinity. Another common association is that of two +n disclinations, which add to form a 27r disclination. The reverse transformation occurs during the course of water evaporation in a myelin form which is squashed between a slide and a coverslip. The dissociation of one line into several lines often occurs at definite points, or in restricted volumes, and these singular points have their own topologies and energies that are rarely considered in theories. Focal curves can branch into pairs and ramify (see Fig. 27 in Friedel and Grandjean [21]). Trees of focal conics have even been photographed in the bulk, near an airsmec
Geometrical Constraints and Textures
347
tic A interface, with several ramification steps, as in fractals [ I 171, Lines of different nature can also be superimposed. Screw dislocations often run along focal lines (see Fig. 32d), and disclination lines can play the role of focal curves (see Fig. 33 and other examples in Bouligand [ZO]). The main systems of concurrent lines are those of converging hyperbolae at the vertices of polygons in smectic phases and tangent conics (ellipses and hyperbolic edges of polygons), which are often replaced by systems of branching focal curves. Focal curves can attach at definite intervals along disclinations. All the points considered where such sets of lines converge, also have their own topologies and energies, depending on the textural environment. The vertices of two focal conics are singular, since they correspond to a reverse in the orientation of the materialized conic sheets of Dupin’s cyclides. These points often disjoin into pairs of lower energy (see Fig. 31 d and Fig. 11 in Bouligand [53]). At a transition from a smectic A to a smectic C phase disclination lines appear in focal domains, linking the two conics, and are of the type shown in Fig. 21 a and b [118]. Their origin is easily understood from Figs. 14 and 25 in Bouligand and KlCman [57]. Much more work has been concerned with systems of conjugated lines, mainly pairs of focal conics and pairs of disclination lines of opposite indices, forming typical patterns of dislocations or elementary pinches. Such associations also exist between singular points showing complementary topological properties, as occur in the capillary tube (see Figs. 8a, 13a and b). Note that certain associations are strictly obligatory. For example, a singular point in the bulk of a nematic liquid, or in a largepitch cholesteric, always lies along a thick thread, since these threads correspond to the locus of vertical directors (i.e. parallel to the
348
7
Defects and Textures
microscope axis), and all possible directions (vertical in particular) are represented in the immediate vicinity of such points. This thick thread is itself vertical in the case in Fig. 8 a for an observer looking from above the capillary tube, and the pattern seen under apolarizing microscope is that of nuclei (see Fig. 4.16 in Meyer 1471).
7.4.7.8
Crystals of Defects
The distribution of defects in mesophases is often regular, owing to their fluidity, and this introduces pattern repeats. For instance, square polygonal fields are frequent in smectics and cholesteric liquids. Such repeats occur on different scales  at the level of structural units or even at the molecular level. Several types of amphiphilic mesophase can be considered as ‘made of defects’. In many examples the defect enters the architecture of a unit cell in a threedimensional array and the mesophase forms a ‘crystal of defects’ [119]. Such a situation is found in certain cubic phases in waterlipid systems [ 1201and in blue phases [ 1211. Several blue phases have been modeled as being cubic centred lattices of disclinations in a ‘cholesteric matrix’. Mobius disclinalions are assumed to join in groups of 4 x 4 or 8x8, but in nematics or in largepitch cholesterics such junctions between thin threads are unstable and correspond to brief steps in recombinations. An isotropic droplet or a Ginsburg decrease to zero of the order parameter probably stabilizes these junctions in blue phases. Similarly, the recently discovered smectic A* phases [ 122, 1231 are layered like ordinary smectic A phases, but show a regular twist and the director follows the distribution that is classical in cholesteric liquids, whereas bend and twist are forbidden in principle (curln =O). Layers are disrupted by nearly equidistant twist grain boundar
ies, each of which is composed of quasiequidistant and parallel screw dislocations, normal to the helical axis, and well evidenced by freezefracture studies [ 1241. In columnar liquid crystals also, twist and splay are excluded in principle, but twist boundaries are plausible when these systems are strongly chiral [ 1251.The existence of such cholesteric columnar phases awaits confirmation.
7.5
References
[ I ] M. J. Press, A. S. Arrott, J. Phys. Paris 1975,36, C I  177. [2] M. KICman, J. Friedel. J. Phys. Paris 1969, 30, c443. [3] J. Friedel, M. KlCman in Fundamental Aspects of Dislocation Theory (Eds.: J. A. Simmons, R. de Wit, R. Bullough), National Bureau of Standards, Washington, DC, Special Publication 3 17, NO. I, 1970, pp. 607636. [4] Y. Ouchi, K. Ishikawa, H. Takezoe, A. Fukuda, K. Kondo, S. Era, A. Mukoh,Jpn. J . Appl. Phys. 1985,24 (Supp. 2), 899. [ 5 ] N. A. Clark, T. P. Rieker, Phys. Rev. A 1988,37, 1053. [6] D. Hilbert, S . CohnVossen, Anschaufiche Geometrie (Geometry and the Imagination), Chelsea, New York 1990. [7] H. S. M. Coxeter, Introduction to Geometry,2nd ed., Wiley, New York 1989. [8] N. H. Hartshorne, A. Stuart, Crystals and the Polarizing Microscope, 4th edn, Arnold, London 1970. [9] S. Amelinckx, Solid State Phys. 1964, Suppl. 6 , I. [lo] 0. Lehmann, Fliissige Kristalle, Verlag W. Engelmann, Leipzig 1904. [ I I ] G. Friedel, Ann. Phys. 1922, 18, 273. [ 121 G. Friedel, Colloid Chemistry, Vol. I , Chemical Catalog Co., 1926, pp. 102136. 1131 D. Demus, L. Richter, Textures qfLiquid Crystals, 2nd edn, VEB Deutscher Verlag, Leipzig 1980. [I41 G. W. Gray, J. W. G. Goodby, h e c t i c Liquid Crystals, Textures and Structures, Leonard Hill, Philadelphia 1984. [I51 S. Chandrasekhar, G. S . Ranganath, Adv. Phys. 1986, 35, 507. S. Chandrasekhar, Liquid Crystals, Cambridge University Press, London 1977.
7.5 [I61 M. KICman, Points, Lines and Walls in Liquid Crystals, Magnetic Systems and Various Ordered Media, Wiley, Chichester, NY 1983. M. Kltman, Rep. Prog. Phys. 1989, 52, 555; Liq. Cryst. 1989, 5, 399. [17] D. Chapman (Ed.), The Structure of Lipids, Methuen, London 1965. [18] J. Nageotte, Morphologie des Gels Lipozdes, Mye'line, Cristaux Liquides, Vacuoles,Actualite's (Sci. Ind., 431/434), Hermann, Paris 1936. F. 0. Schmitt, K. J. Palmer, Cold Spring Harbor Symp. Quant. Biol. 1940,94. D. M. Small, M. C. Bourgks, D. G. Dervichian, Biophys. Biochim. Acta 1966, 125,563. F. B. Rosevear, J. Am. Oil Chem. Soc. 1954,31,628. [ 191 Y. Bouligand in Geometry in Condensed Matter Physics, World Scientific, Singapore 1990, Chap. 4; J. Phys. Paris 1990, 51, C735. I201 Y. Bouligand, J. Phys. 1972, 33, 715. Y. Bouligand in Dislocations in Solids (Ed.: F. R. N. Nabarro), North Holland, Amsterdam 1979, Chap. 23. [21] G. Friedel, F. Grandjean, Bull. SOC. Mineral. 1910, 33,409. 1221 Y. Bouligand, P. E. Cladis, L. LiCbert, L. Strzelecki, Mol. Cryst. Liq. Cryst. 1974,25,233. [23] W. A. Jensen, R. B. Park, Cell Ultrastructure, Wadworth, Belmont, CA 1967. D. W. Fawcett, The Cell, 2nd edn, W. B. Saunders, Philadelphia 1981. [24] H. Moor, K. Miihlenthaler, J. Cell. Biol. 1963, 17, 609. [25] R. R. Balmbra, J. S. Clunie, J. F. Goodman, Proc. R. Soc. London, Ser. A 1965,285,534.J. F. Goodman, J. S. Clunie in Liquid Crystals & Plastic Crystals, Vol. 2 (Eds.: G. Gray, P. A. Winsor), Ellis Horwood, New York 1974, pp. 123. 1261 F.Livolant, Physica 1991, A176, 117; J. Mol. Biol. 1991, 218, 165. 1271 Y. Bouligand, Solid State Phys. 1978, Supp. 14, 259. [28] Y. Bouligand in Liquid Crystalline Order in Polymers (Ed.: A. Blumstein), Academic Press, New York 1978, Chap. 8. [29] Y. Bouligand, J. Phys. Paris 1969,30, C490. [30] S. Caveney, Proc. R. Soc. London, Sex B 1971, 178, 205. [31] M.M. GiraudGuille, H. Chanzy, R. Vuong, J. Struct. Biol. 1990, 103, 232. 1321 M.M. GiraudGuille, Int. Rev. Cytol. 1996,166, 59. 1331 Y. Bouligand, Tissue Cell 1972,4, 189. [34] Y.Bouligand, 7th lnt. Congr: Electron Microscopy, Grenoble 1970, 3, 105. 1351 M.M. GiraudGuille, Calcg Tissue Int. 1988, 42, 167. 1361 M.M. GiraudGuille, J. Mol. Biol. 1992, 224, 861. L. Besseau, M.M. GiraudGuille, J. Mol. Biol. 1995, 251, 197.
References
349
[37] Y. Bouligand in Physics ofDefects (Eds.: R. Ballian, M. KlCman, J.P. Pokier), North Holland, Amsterdam 1980, pp. 7808 1 1. 1381 J. E. Proust, L. Ter Minassian, E. Guyon, Solid State Commun. 1972, 11, 1227. [39] C. Williams, P. Pieranski, P. E. Cladis, Phys. Rev. Lett. 1972, 29, 90. 1401 R. B. Meyer, Phil Mag. 1973, 27,405. [41] A. Saupe, Mol. Cryst. Liq. Cryst. 1973, 21, 211. [42] P. E. Cladis, Phil. Mag. 1974,29,641.P. E. Cladis, A. E. White, w. F. Brinkman, J. Phys. Paris 1979, 40, 325. [43] A. M. J. Spruijt, Solid. State Commun. 1973, 13, 1919. 1441 Y. Bouligand, J. Phys. Paris 1974, 35, 215. [45] J . Nehring, A. Saupe, J. Chem. Soc., Faraday Trans. I1 1972, 68, 1. 1461 M. KlCman in Dislocations in Solids (Ed.: F. R. N. Nabarro), North Holland, Amsterdam 1980, pp. 5,245297,35 1 4 0 2 . G. Ryschenkov, M. KICman, J. Chem. Phys. 1976,64,413. [47] R. B. Meyer, Mol. Cryst. Liq. Cryst. 1972, 16, 335. [48] Y. Bouligand, J. Phys. 1974, 35, 959. [49] Y. Bouligand in Dislocations in Solids, Vol. 5 (Ed.: F. R. N. Nabarro), North Holland, Amsterdam 1980, pp. 301347. [SO] V. Volterra, Ann. Ecole Normale Sup. 1907, 24, 401. [ S 11 A. E. H. Love, A Treatise on the Mathematical Theory of Elasticity, Dover, New York 1944. [52] J. Friedel, Dislocations, International Series Monographs on Solid State Physics, No. 3, Pergamon, Oxford 1964. [ S 3 ] Y. Bouligand inPhysicsofDefects(Eds.: R. Ballian, M. KICman, J.P. Pokier), North Holland, Amsterdam 1980, pp. 66871 1. [54] F. C. Frank, Discuss. Faraday Soc. 1958,25, 19. [SS] P. G. de Gennes, 3. Friedel, C. R. Heb. Acad. Sci., Paris B 1965, 268, 257. 1561 P. E. Cladis, M. KICman, Mol. Cryst. Liq. Cryst. 1972, 16, 1. [57] Y. Bouligand, M. KICman, J . Phys. Paris 1979, 40, 79. [58] M. Brunet, C. Williams, Ann. Phys. Paris 1978, 3, 237. [59] Y. Bouligand, M. Kltman, J. Phys. Paris 1970, 31, 1041. [60] J. Rault, Phil. Mag. A 1973, 28, 11. [61] M. KlCman in Dislocations in Solids, Vol. 5 (Ed.: F. R. N. Nabarro), North Holland, Amsterdam 1980, pp. 245297. [62] C. Robinson, J. C. Ward, R. B. Beevers, Faraday Soc. Discuss. 1958,25, 29. [63] Y. Bouligand, F. Livolant, J. Phys. Paris 1984, 45, 1899. 1641 R. Cano, Bull. Soc. Fr. Mine'r. Cristallogr. 1967, 90, 333; 1968, 91, 20.
350
7
Defects and Textures
[65] G. Malet, J. Marignan, 0. Parodi, J. Phys. 1978, 9, 863. G. Malet, J. C. Martin, J. Phys. Paris 1979,40, 355. [66] C. Mauguin, Bull. Soc. Mine'ral. 1911,34,6,71. [67] P. G. de Gennes, The Physics of Liquid Clystals, Oxford University Press, Oxford 1974. [68] F. Grandjean, Bull. Soc. Fr. Mine'ral. 1919, 42, 42. [69] G. Toulouse, M. KICman, J. Phys. Paris 1976, 37, L149. [70] V. Poenaru, G. Toulouse, J. Phys. Paris 1977, 38, 887. [71] M. KICman, L. Michel, G. Toulouse, J. Phys. Paris 1977, 38, L195. [72] M. KlCman, J. Phys. Paris 1977,38, L199. [73] Y.Bouligand, B. Derrida, V. Poenaru, Y. Pomeau, G. Toulouse, J. Phys. Paris 1978,39,863. [74] M. KICman, L. Michel, J. Phys. Paris 1978,39, L29; Phys. Rev. Lett. 1978,40, 1387. [75] V. Poenaru in IllCondensed Matter (Eds.: R. Ballian et al.), Les Houches X X l Summer School Proc., 1978, p. 265. [76] M. D. Mermin, Rev. Mod. Phys. 1979, 51, 581. [77] H. R. Trebin, Adv. Phys. 1982,31, 195. [78] M. V. Kurik, 0. D. Lavrentovich, Sov. Phys. Usp. 1988,31, 196. [79] W. F. Harris, Sci. Am. 1977, 237 (6), 130. [80] M. Born, E. Wolf, Principles q f f p t i c s ,6th edn, Pergamon, Oxford 1980. [81] Y.Bouligand, J. Phys. Paris 1973, 35, 603. [82] F. Grandjean, Bull. Soc. FK Mine'ral. 1916, 39, 164. [83] C. Dupin, Applications de Ge'ome'trie et de Me'canique, Bachelier, Paris 1822. J. C. Maxwell, Q. J. Pure Appl. Maths. 1867, 34; On the Cyclide, Scientific Papers, Cambridge University Press, Cambridge 1890, 2, 144159. C. M. Jessop, Quartic Surfaces, Cambridge University Press, Cambridge 1916. G. Darboux, Ge'ome'trie Analytique, GauthierVillars, Paris 1917. H. Bouasse, Optique Cristalline, Polarisation Rotatoire, Erats Me'somorphes, Delagrave, Paris 1925. [84] W. Bragg, Trans. Faraday Soc. 1933, 29, 1056. J. P. Meunier, J. Billard, M o l . Cryst. Liq. Cryst. 1969, 7, 421. M. Kltman, J. Phys. Paris 1977, 38, 1511. [85] C. S . Rosenblatt, R. Pindak, N. A. Clark, R. Meyer, J. Phys. Paris 1977, 38, 1105. [86] G. Friedel, G. Grandjean, C. R. Acad. Sci., Paris 1911, 152, 322. [87] M. de Broglie, E. Friedel, C. R. Acad. Sci., Paris 1923, 176, 738. E. Friedel, C. R. Acad. Sci.,Paris 1925, 180, 269. [88] Y. Bouligand, J. Phys. Paris 1972, 33, 525. [89] M. KICman, C. Williams, C. E. Costello, T. GulikKrzywicki, Phil. Mag. 1977, 35, 33. [90] S. T. Lagerwall, S. Stebler, Les Houches Summer School Proc. 1981, X X X V ,757.
[91] R. Bidaux, N. Boccara, G. Sarma, P. G. de Gennes, 0. Parodi, J. Phys. Paris 1973, 34, 661. [92] J. P. Sethna, M. KICman, Phys. Rev. A 1982.26, 3037. [93] Y. Bouligand, J. Microsc. France 1973, 17, 145. [94] T. P. Rieker, N. A. Clark, G. S. Smith, D. S. Parmar, E. B. Sirota, C. R. Safinya, Phys. Rev. Lett. 1987,59, 2658. [95] N. A. Clark, T. P. Rieker, Phys. Rev. A 1988, 37, 1053. [96] D. Johnson, A. Saupe, Phys. Rev. A 1977, 15, 2079. [97] L. Bourdon, J. Sommeria, M. KICman, J. Phys. Paris 1982, 43, 77. [98] J. Rault, Solid State Com. 1971, 9, 1965. [99] J. Rault, Phil. Mag. 1973,28, 11. [loo] C. E. Williams, Phil.Mag. 1975, 32, 313. [loll M. B. Schneider, W. W. Webb, J. Phys. Paris 1984,45, 273. [ 1021 F. R. N. Nabarro, J. Phys. Paris 1972,33,1089. [lo31 S. T. Lagerwall, S. Stebler, Ordering in Strongly Fluctuating Condensed Matter (Ed.: T. Riste), Plenum, New York 1972, p. 383. [lo41 C. M. Dafermos, Q. J. Mech. Appl. Math. 1970,23, 49. [I051 M. Kltman, J. Phys. Paris 1977, 38, 1511. [ 1061 P. G. de Gennes, C. R. Hebd. Se'anc. Acad. Sci., Paris l972,275B, 549. [I071 M. KICman, C. Williams, J. Phys. Paris, Lettres 1974, 35, L49. [lo81 S. E. Bedford, T. M. Nicholson, A. H. Windle, Liq. Cryst. 1991, 10, 63. S. E. Bedford, A. H. Windle, Liq. Cryst. 1993, 15, 31. I1091 T. Kimura, D. G. Gray, Liq. Cryst. 1993, 13, 2330; Macromolecules 1993, 26, 3455. [ 1101 H. B. Philips, N. Wiener, J. Math. Phys. MIT 2nd Ser., March 1923. [ I I I] A. Stieb, G. Baur, G. Meier, J. Phys. Paris 1975, 36C1, 185. A. E. Stieb, J. Phys. Paris 1980, 41, 961. [I121 F. Lequeux, P. Oswald, J. Bechhoefer, Phys. Rev. A 1989,40,3974. [ I 131 P. Ribikre, S. Pierkl, P. Oswald, Phys. Rev. A 1991,44,8198. [I141 F. Lequeux, M. KlCman, C. R. Hebd. Acad. Sci.,Paris 1986,303,765;J. Phys. Paris 1988, 49, 845. [ 1151 F. Rondelez, J. P. H u h , Solid State Commun. 1972, 10, 1009. F. Rondelez, H. Arnould, C. R. Hebd. Acad. Sci., Paris B 1971, 273, 549. [116] P. Oswald, J. Behar, M. Kltman, Phil. Mag. A 1982, 46, 899. [I171 J. B. Fournier, G. Durand, J. Phys. I! France 1991, I , 845. [118] A. Perez, M. Brunet, 0. Parodi, J. Phys. Paris 1978, 39, L353.
7.5 References [119] W. Helfrich in Physics of Defects (Eds.: R. Ballian, M. KlCman, J.P. Poirier), North Holland, Amsterdam 1980, Course 12, pp. 716755. [120] H. Delacroix, A. Gulik, T. GulikKrzywicki, V. Luzzati, P. Mariani, R. Vargas, J. Mol. B i d . 1988,204, 165; 1993,229,526. [I211 S. Meiboom, S . Sammon, D. W . Berreman, Phys. Rev. A 1983, 28, 3553.
35 1
[122] J. W. Goodby, M. A. Waugh, S. M. Stein, E. Chin, R. Pindak, J. S. Patel, Nature 1989,337, 449. [123] G. Strajer, R. Pindak, M. A. Waugh, J. W . Goodby, Phys. Rev. Lett. 1990, 64, 1545. [124] K. J. Ihn, J. A. N. Zasadzinski, R. Pindak, Science 1992,258,275. [125] R. D. Kamien, D. R. Nelson, Phys. Rev. e, Statistical Physics 1996, 53, 650.
8 Flow Phenomena and Viscosity E Schneider and H. Kneppe A complete assessment of the literature on the hydrodynamics of liquid crystals is beyond the scope of this handbook. Therefore, only the most important fundamentals for the description of flow phenomena will be discussed. Further details can be found in the references cited at the end of each section and in the review articles and books of Porter and Johnson [l], de Gennes [2], Stephen and Straley [3], Jenkins [4], de Jeu [ 5 ] ,Vertogen and de Jeu [6], and de Gennes and Prost [7]. Two review articles of Leslie [8, 91 are exclusively devoted to this subject. Experimental results for uniaxial nematic liquid crystals are described in Vol. 2 A of the recently published Handbook of Liquid Crystals. The hydrodynamic theory for uniaxial nematic liquid crystals was developed around 1968 by Leslie [lo, 113 and Ericksen [12, 131 (LeslieEricksen theory, LE theory). An introduction into this theory is presented by F. M. Leslie (see Chap. 111, Sec. 1 of this Volume). In 1970 Parodi [14] showed that there are only five independent coefficients among the six coefficients of the original LE theory. This LEP theory has been tested in numerous experiments and has been proved to be valid between the same limits as the NavierStokes theory. An alternative derivation of the stress tensor was given by Vertogen [ 151.
In 197 1 the Harvard group [ 161 presented a different form of the constitutive equations which gives very compact expressions for systems with nearly uniform director orientation. The results of both theories agree. Nevertheless, the LEP presentation is preferred in most of the experimental and theoretical studies in this field. The constitutive hydrodynamic equations for uniaxial nematic calamitic and nematic discotic liquid crystals are identical. In comparison to nematic phases the hydrodynamic theory of smectic phases and its experimental verification is by far less elaborated. Martin et al. [ 171 have developed a hydrodynamic theory (MPP theory) covering all smectic phases but only for small deformations of the director and the smectic layers, respectively. The theories of Schiller [ 181 and Leslie et al. [ 19, 201 for SmCphases are direct continuations of the theory of Leslie and Ericksen for nematic phases. The Leslie theory is still valid in the case of deformations of the smectic layers and the director alignment whereas the theory of Schiller assumes undeformed layers. The discussion of smectic phases will be restricted to some flow phenomena observed in SmA, SmC, and SmC* phases. Although the constitutive hydrodynamic equations for nematic and polymeric liquid
8.1
crystals are identical the following discussion is only devoted to monomeric systems. Polymeric liquid crystals exhibit a great variety of special effects which restrict the application of standard hydrodynamic theory. Reviews on this topic are given by Wissbrun [21] and Marrucci and Greco [22].
Most of the hydrodynamic effects observed in nematic liquid crystals can be explained by the LEP theory. Its generality is sufficient for the following discussion. According to this theory the viscous part of the stress tensor oiifor an incompressible uniaxial nematic liquid crystal is
oij= alninj$pnknp+ @njNi + a,niNj + a , ~ ,+ a5njKknk+ a6niYknk (1) using the notation of Clark and Leslie [23] and usual summation convention. V is the symmetric part of the velocity gradient tensor (2) and N is the rotation of the director n relative to the fluid
(3)
A superposed dot denotes the material time derivative. The Leslie coefficients a, are assumed to be independent on velocity gradient and time. They depend on temperature and pressure. Four of the coefficients are related one with another via the Parodi equation [ 14, 241 @
+ a, = a,  a5
353
which is a consequence of the Onsager relations. Thus, the viscous properties of an incompressible nematic liquid crystal can be described by five independent coefficients. In the following, we assume a steady and laminar flow of the liquid crystal.
8.1.1 Shear Viscosity Coefficients ql, q2,q3,and q12
8.1 Nematic Liquid Crystals
N . = 4 (v. 1 .  v . .)n. 2 1.J J.1 J 1 or N = ri  (curlv) x n 2
Nematic Liquid Crystals
(4)
Figure 1 shows the system of coordinates which is used in the following discussion. The liquid crystal flows parallel to the xaxis, and the velocity gradient is parallel to the yaxis. The orientation of the director n is described by the angles @ and 0
n = (sinOcos@, s i n 0 sin@, cos0)
(5)
Assuming that the velocity is only a function of y, the only nonvanishing components of the velocity gradient tensor are 1 (6) V, = V, = zv,,y If the orientation of the director is fixed, for example by application of an external magnetic or electric field, Eq. (3) reduces to 1 N =( sin 0 sin @, sin 0 cos @, 0) v , , ~ (7) 2 If a liquid crystal is sheared between two infinite plates parallel to the xzplane, a constant velocity gradient parallel to the yaxis results. Assuming stationary flow the stress component oxycan be calculated from
z
T Figure 1. Director orientation with respect to the flow velocity and the velocity gradient.
354
8
Flow Phenomena and Viscosity
Several notations for the shear viscosity coefficients are used. The notation used here oxY = ( a ,sin4 @sin2@cos2 stems from Helfrich [25]. A different notaa tion was proposed by Miesowicz [26]. ~sin20sin2~+~sin20cos2c#j The shear viscosity coefficients q l , q2, 2 2 a a and q3can separately be determined in shear +A+ L s i n 2 @sin2c#j flow experiments with adequate director or2 2 ientations [27].
Eqs. (1) and (57).
ql: nllgradv
Collecting terms with the same dependence on the director orientation and calculation of the viscosity q= oxylux,ygives
a cos20 +4 2 +alsin4 OCOS* @sin2c#j
(9)
Therefore, it makes sense to introduce a new set of viscosity coefficients (see Fig. 2)
1 2 1 772 =  ( a 4 2 1 771
773
=  ( a 4 +a5 a21
=p
+a6
772:
nllv
q3:n l u ,n l g r a d v For the determination of q12at least three experiments are necessary. Two for the determination of q1and q2and one experiment with a director orientation where the influence of q l 2on the shear viscosity is maximal (0=90°, @=45"). Then, q12can be calculated according to 7712
= 477(90", 45")  2(771 +
772)
(13)
Methods for the determination of the shear viscosity coefficients are described in Vol. 2A of the recently published Handbook of Liquid Crystals.
+a31
8.1.2 Rotational Viscosity
4
v 1 2 =a1
Rewriting Eq. (9) gives
q(~,@ = )ql sin2@sin2@+ q2sin20cos2@
+ q3c0s20 + qI2sin4@cos2@sin2@
(1 1)
Viscous torques are exerted on the director of a liquid crystal during a rotation of the director and by a shear flow with a fixed director orientation. The density I, of the viscous torque is obtained by application of the LeviCivita tensor 1
eijk= 1
lo
i , j , k cyclic i , j , k anticyclic otherwise
(14)
on the stress tensor. Only the skew symmetric part 771
772
773
Figure 2. Definition of the shear viscosity coefficients q,, q2, and q3. The outer pair of arrows symbolizes the shear flow.
8.1
of the stress tensor (Eq. 1) gives a contribution
r.= &"y k ass= kJ &.' 1Jk ((a,  a3)njNk 1
+ (a5  a d n j v k , n p l
(16)
or
r= n x (Y,N + y 2 v 4
(17)
355
V contains components depending on z , the only nonvanishing stress tensor components are ox. and oyxand in these components only terms with the coefficients a,and a, are nonvanishing. We obtain from Eqs. ( 3 ) and (1)
N = ( sin@, cos@, O)@
(21)
and
with y1=a,a,;
y2==a5
(18)
is called rotational viscosity or rotational viscosity coefficient. At first the viscous torque on a rotating director is calculated. If the liquid crystal is at rest the last term in Eq. (17) vanishes. A director rotation in the xyplane gives
r, =  yl d
(19)
Multiplying with the volume of the liquid crystal we obtain the viscous torque
M,=
Nematic Liquid Crystals
y,dv
(20)
The torque which has to be applied on the director for this rotation amounts to M,. If a liquid crystal at rest is surrounded by a vessel the torque exerted by a rotating magnetic or electric field on the director must be transferred to the vessel. This torque will be calculated for a completely filled vessel with quadratic cross section. The liquid crystal and the vessel are assumed to be at rest and the director is rotating in the xyplane (see Fig. 3 ) . As in this case neither the director and its rotation N nor the velocity gradient tensor
Y
Figure 3. Surface forces on a vessel due to a rotating director.
ox,= ( a,sin2@+ a, cos2@)d
o,,= (a,cos2@ a, sin2@)&
(22)
Multiplying by the areas ay and a, of the vessel gives the forces f, and f,
f, =  oxyay= (a2 sin2@ a, cos2@)daY f,,=  oy,a, = ( a,cos2@+ a, sin2@)da, (23) There are no forces on the base and the top plate. The total torque is, therefore,
M , = (q a,)dV
(24)
which is in agreement with the torque exerted on the director (Eq. 20). In principle, Eq. (23) allows determination of the Leslie coefficients a, and a, separately. a, corresponds to the force on the surface if the director is perpendicular to it, a, corresponds to the force for the parallel case. The magnitude of the torque does not depend on the shape of the container. It is only a function of the volume of the liquid crystal, that is the number of rotating molecules. The torque on a body with volume V suspended in a liquid crystal has the same magnitude but different sign. The rotation of the director can be achieved by application of rotating magnetic or electric fields [ 5 , 281. For larger samples magnetic fields can be applied with less experimental problems. In the following we will therefore consider a liquid crystal in a rotating magnetic field with constant field strength and angular velocity. The results are identical for a rotating sample in a fixed
356
8 Flow Phenomena and Viscosity
field if the calculation is carried out with respect to the rotating sample. The torque exerted by the magnetic field on the director amounts to
M
= 1 P ~ X ~ H ~ V S ~ ~~(Y/  0)
2 where
x u = XI1 
(25)
(26)
XL
is the anisotropy of the magnetic susceptibility which is assumed to be positive and H is the magnetic field strength. Under stationary conditions and small angular velocities of the field rotation the director follows the magnetic field direction with a constant phase lag Y @, see Fig. 4. The viscous and the magnetic torque become equal y l & = 1 P ~ X ~ H ~ @I S ~ ~ ~ ( Y (27) 2 Increasing the angular velocity of the rotating field increases the phase lag between field and director until the maximum magnetic torque is exerted at a phase lag of d 4 . The corresponding angular velocity is the critical angular velocity @=
bances by the surrounding surfaces the predicted oscillations are usually not observable and an inhomogeneous director rotation results [30]. Measuring the torque on a sample of a nematic liquid crystal in a magnetic field rotating with an angular velocity smaller than the critical one represents a relatively simple method for the determination of the rotational viscosity coefficient. Below the critical angular velocity Eq. (24) is valid nor with d j = Y! Neither the phase lag !I@ the anisotropy of the magnetic susceptibility have to be known.
8.1.3 Flow Alignment If a nematic liquid crystal with a fixed director orientation is sheared a torque according to Eq. (17) is exerted on the director
If the direction of flow and shear gradient are the same as in Fig. 1 , the torque on the director becomes
A further increase of the angular velocity leads to a nonstationary behaviour. The solutions of the corresponding differential equation
r=
d = dcsin 2(Yt  0)
The following discussion is simpler in a coordinate system which refers to the director (see Fig. 5). The @axis is parallel to z x n and the @axis is parallel to the n x @ vector.
(29)
are known [29]. Their characteristic feature is a periodicity in time. Because of distur
z?r,y
coso coso, (a,  ol, sin@cos@sin@, sin2@(@sin2@a, cos2dj)) (31)
r
'I
li Yj/
1
,/ ,I
*!,/>
+X
rj
Figure 4. Director alignment in a rotating magnetic field.
Figure 5. System of coordinates for the director orientation.
8.1
The torques with respect to this system of coordinates are
I, =  vx,y(a,+ a3)s i n 0 c o s 0 sin@ cos@ (32)
I, = ux,ys i n 0 (a,sin2@ a, cos2@)
(33)
If the director is free to rotate there will be either a rotation to a stable orientation (flow alignment, see Fig. 6) or a continuous rotation (tumbling) under the influence of the shear gradient. Which case is observed depends on the signs of a,and a,. Because of thermodynamical arguments (see Sect. 8.1.9) the rotational viscosity coefficient must be positive.
'/l=a,a,>O (34) That is, a,> 0 and a, < 0 is not allowed. All nematic liquid crystals investigated up to now exhibit negative a, values. Therefore we will discuss in the following only different signs for a,. Some nematic liquid crystals show positive a, values in the neighbourhood of a nematiclsmectic transition. For positive a, the sign of the torque component r, does not depend on @. This leads to a continuous rotation if the director is orientated in the shear plane (@= 90'). The sign of the torque component r, depends on @, that is, the director is stabilized in the shear plane for two quarters of a revolution and destabilized for the other two quarters. Because of the additional influence of surface alignment and elastic torques the real movement of the director is difficult to predict [31].
Y
Figure 6. Flow alignment.
Nematic Liquid Crystals
357
Negative a,and a, values are the most frequent combination for nematic liquid crystals. Under these circumstances no torque is exerted on the director in three orientations (a) 0=0' (b) 0=90', @=ao (c) @=90', @=@o where tan@,,
=+,a3/~2
(35)
Equations (32) and (33) show that only the orientation (b) is stable against deviations from this orientation. Experiments have shown that a, % a, is usually valid. Microscopic theories [32, 331 in which the molecules are assumed to be ellipsoids of revolution predict
I I I I
%+)
2
a2
where a and b are the length of the ellipsoid parallel and perpendicular to the symmetry axis and a perfect parallel alignment of the molecules (S= 1) is assumed. Thus, the flow alignment angle is usually small. For a flow aligned liquid crystal the viscosity is given by
qo = q1sin2@, + q2 cos2a0 = 772 + (771  772) sin2@, = q2  (a, a,) sin2O0
+
(37)
neglecting a small term with the coefficient a,. Inserting Eq. (35) yields 770
= 772  cc,
(38)
As a, is negative and usually small as compared with q2, the viscosity under flow alignment is somewhat larger than q2. Mostly the difference can be neglected. Equation (38) is only valid for a uniform director orientation. In a capillary with circular cross section there are regions along the surface and the capillary axis where the orientation of the director disagrees with the
358
8
Flow Phenomena and Viscosity
In hydrostatic equilibrium without electric and magnetic fields the molecular field is parallel to the director and the elastic torque re=nxh capillary
lary.
flow alignment angle (see Fig. 7 and Sec. 8.1.4). By choosing proper values for radius and flow velocity and by a surface treatment the influence of these regions can be minimized. Theoretical studies on the flow alignment can be found in the papers of Manneville [34], Carlsson [35], and Zuniga and Leslie [311.
8.1.4 Viscous Flow under the Influence of Elastic Torques Except for the short discussion at the end of the last section, a uniform director alignment has been assumed up to now. Surface alignment and inhomogeneous fields can lead to an inhomogeneous alignment and the occurrence of elastic torques. For a complete description of hydrodynamics of nematic liquid crystals these elastic torques have to be included. The equilibrium condition for the elastic torques corresponds to the minimum of the elastic energy under the constraint of constant director length. It is convenient to introduce a molecular field h [36] h = h,
+ hT + hB
(39)
where the three terms describe splay, twist and bend distortion of the liquid crystal. hs = kl ,grad divn; hT = k2,{(ncurln)curln+curl[(ncurln)n]} hB = k33{(n X CUrln)X CUrh + curl[n x (n x curln)]) (40)
(41)
vanishes. As the values of the three elastic constants are comparable and the expression for the molecular field is rather complicated, the one constant approximation k11
= k22 = k33 = k
(42)
is often preferred and the molecular field becomes h = kV2n
(43)
Elastic terms have to be taken into account in the equations for the balance of linear and angular momentum. If the body forces are assumed to be conservative their scalar potential can be added to the pressure in the equation for the linear momentum. Nevertheless, as director rotation and shear stress are coupled both equations have to be combined for a solution of a given problem. At low shear rates viscous torques on the director can be neglected. Then the equations for linear and angular momentum are uncoupled and the orientation of the director in the bulk can be calculated for any given surface orientation by solving the equation for angular momentum. Using the obtained director profile the equation for linear momentum can then be integrated. The apparent viscosity will be a function of the choosen surface orientation and the elastic constants. At high shear rates the director orientation in the bulk is dominated by flow alignment. The influence of elastic torques is restricted to small boundary layers at the surfaces and regions where the velocity gradient changes sign. Therefore the apparent viscosity is close to the value for flow align
8.1
ment and does not depend on the surface orientation or elastic constants. At medium shear rates director orientation and velocity profile can only be obtained by numerical calculations. In the following the flow between parallel plates with a surface alignment parallel to the pressure gradient is calculated [37]. The orientation of the capillary is the same as in Fig. 10. The equation for linear momentum is: (44) where g (a)is the viscosity g(@) = q, sin2@+q2cos2@
kQf’ + ux,,(g(@o)

g(@)>= 0
ues of the nondimensional parameter D= T3P,x k
where 2 T is the distance of the plates. The different slopes of the curves for y = O and T are due to the different velocity gradients in these areas. Integration of the velocity with the aid of Eqs. (44) and (46) gives the apparent viscosity =
(46)
or with the aid of Eq. (44) (47) where Q0 is the flow alignment angle. This equation is solved numerically. The alignment at the surface is assumed to be @=O. Figure 8 shows @ as a function of y / T for (q,q2)/q2=8,@,=O.l, and different val
(49)
@’(T) (that is, 0’ at the plates) is taken from the numerical solution. Figure 9 shows the viscosity ratio q2/qas afunction of 1/D= klT3pp, for (ql  q2)/q2=8 and different flow alignment angles. llq gives an asymptotically linear dependence on 1/D for large Dvalues. Some general predictions can be made with the aid of the scaling properties [ 191 of the LeslieEricksen equations. Neglecting the molecular inertia, the substitution
r* = h r; t* = h2 t ; p* = p l h 2 ; 05 = o,/h 2
I 0.0
Figure 8. Alignment angle @as a function of y / T for different values of the nondimensional parameter D.
1
g(@o) 3k@’( T )
T2PJ
(45)
The small a,term has been neglected. The equation for angular momentum is:
359
Nematic Liquid Crystals
(50)
1
0.5
1/D
1.0
Figure 9. Viscosity ratio q2/q as a function of 1/D=k/T3p,,for different flow alignment angles.
360
8
Flow Phenomena and Viscosity
Stationary flow and i=z gives
+Y
Figure 10. Transverse pressure in a capillary with rectangular cross section.
leaves the form of the differential equations unchanged. The scaling parameter h can be the gap width. Currie [37] has shown that the apparent viscosity is mainly a universal function of a nondimensional parameter depending on the specific geometry of the flow and a parameter which depends on the surface orientation and the flow alignment angle. Flow phenomena in the presence of elastic torques have been studied in the Couette [38, 391 and the Poiseuille geometry [40].
The second term vanishes because of the translational symmetry in flow direction and the last term vanishes for an infinite width of the capillary. The remaining stress tensor element amounts to
and therefore
The xcomponent of Eq. ( 5 1) becomes
For the case studied this leads to
leading to the final result
8.1.5 Transverse Pressure Due to the tensor properties of the viscosity a nematic liquid crystal will generally not flow along the pressure gradient. If flow direction and director are neither parallel nor perpendicular a pressure gradient is observed transverse to the flow direction. The skew director orientation can be accomplished by application of a magnetic field to the liquid crystal flowing in a capillary. As an example the flow in a long capillary with rectangular cross section will be discussed (see Fig. 10). The width 2 Wof the capillary is assumed to be considerably larger than its thickness 2 T. Therefore the velocity gradient across the capillary width can be neglected. The largest transverse pressure difference is observed for a director orientation in the xzplane ( @ = O ) . The transverse pressure can be derived from the equation for the conservation of linear momentum
The transverse pressure gradient passes through a maximum at approximately @=45". A transverse pressure for this case and an angle dependence according to Eq. (57) has been experimentally confirmed [41]. In principle this experiment can be used for the determination of viscosity coefficient ratios. Because of experimental difficulties it should only be used to demonstrate the tensor property of the viscosity of nematic liquid crystals. If the director is orientated in the shear plane (@=90") a pressure gradient is also generated along the velocity gradient. The conservation of linear momentum gives for i=y  P , y + CJYX,X +
o y v w+
%*z = 0
(58)
The second term vanishes for symmetry reasons. The last term is the symmetric counterpart to the third term in Eq. ( 5 2 ) , but vanishes under our assumptions (infinite
8.1 Nematic Liquid Crystals
width). Neglecting a small term with the coefficient a, gives
P , =~ a, sin@ cos@ vx,yv
(59)
and with Eq. ( 5 5 )
p , x= (ql sin2@+ q2cos2@) vx,yu
(60)
36 1
nent gives
The first and third term in this equation vanish due to the translational symmetry. Neglecting a term with the usually small coefficient a, gives
the final result becomes ~
p,y a6sin@cos@ P , ~ q1sin2 + q 2 cos2 0
As the thickness of the capillary is smaller than its width the pressure difference across the thickness is considerably smaller than the difference across the width.
8.1.6 Backflow An externally applied torque on the director can only be transmitted to the surfaces of a vessel without shear, if the director rotation is homogeneous throughout the sample as assumed in Sect. 8.1.2 for the rotational viscosity. Otherwise this transmission occurs partially by shear stresses. The resulting shear flow is called backflow. As there is usually a fixed director orientation at the surfaces of the sample container, a director rotation in the bulk of the sample by application of a roating magnetic field leads to an inhomogeneous rotation of the director and to a backflow [42]. We study a nematic layer (Fig. 1 1 ) confined between two parallel plates of infinite dimension. The director is assumed to lie in the x,y plane and the pressure is constant. The inertial terms in Eq. (5 1) can be neglected under usual conditions and the x compo
Figure 11. Director orien

tation under the influence of a magnetic field.
+ vx,,(q sin2@ +
cos20))= o
(63)
and integration with respect to y leads to d(a,cos2@ %sin2@) + vx,,(ql sin2@+ q2c0s2@)= const.
(64)
The integration constant may still depend on time and can be determined from the boundary condition at the solid surface or in the middle of the cell. Equation (63) shows that every inhomogeneous director rotation is coupled with a velocity gradient. We assume a homeotropic orientation of the director at the solid surfaces and apply a magnetic field in the x,y plane with an orientation nearly parallel to the y axis. The magnetic anisotropy is assumed to be positive and the strength of the magnetic field to be small. Then the deformation will be small and one gets from Eq. (64) 
a,@+ 77, vx,y =  a,@max
(65)
For a common liquid crystal with negative a,and positive q , a positive angular velocity d of the director will be coupled with positive shear gradients at the solid surfaces as the angular velocity vanishes there. This leads to a positive rotation of the bulk and an increase of the angular velocity of the director with respect to a fixed system of coordinates. This effect is usually described by introduction of an effective rotational viscosity coefficient yT which is smaller than ‘/I. The exact solution for this and other cases [42,43] shows that the effective rotation
362
8
Flow Phenomena and Viscosity
a1 viscosity coefficient can be as small as 25% of y,. Backflow effects are not observed for a planar orientation of the director and a rotation of the magnetic field in the surface plane (twist geometry).
8.1.7 Discotic Liquid Crystals Nematic discotic liquid crystals consist of disclike molecules with a preferred parallel orientation of their short molecular (symmetry) axes. There is no translational order. The symmetry of the liquid crystal agrees with that of usual calamitic nematic liquid crystals consisting of rodlike molecules. Accordingly, the stress tensor for calamitic and discotic nematic liquid crystals are identical. Nevertheless, there are some differences in the flow phenomena due to differences in flow alignment. The flow alignment angle depends on the ratio of the axes of the molecules according to Eq. (36)
The flow alignment angle for discotics should therefore be approximately 90". A stability analysis shows that the angle above 90" is the stable one [44]. Thus for both types of nematic liquid crystals the configuration with the large dimension nearly parallel to the flow direction is the stable alignment. Figure 12 demonstrates this phenomenon.
grad v
8.1.8 Influence of Temperature and Order Parameter on the Viscosity Coefficients The theory of Leslie and Ericksen is a macroscopic theory. Predictions for the temperature dependence of the viscosity coefficients can only be derived from microscopic theories. Because of several simplifications whose validity is not obvious the results of these microscopic theories are in some cases contradictory and at best qualitatively correct. A general feature is an exponential temperature dependence as known for isotropic liquids with comparable activation energies for all viscosity coefficients far away from the clearing point. This temperature dependence is superposed by an individual dependence on the order parameter whose influence dominates in the neighbourhood of the clearing point. Up to first order all authors predict a linear dependence of the Leslie coefficients a,,, a,, a, as well as a, and a quadratic dependence of a, [12,33,45,46]. The viscosity coefficient a, should be independent of the degree of order. The dependences of the shear viscosities on the order parameter are more complicated. Different results were obtained for the rotational viscosity. However, there are strong arguments that the rotational viscosity vanishes at the clearing point with S2. According to most theories the dependence on the order parameter and the gen
grad v
T
fi
Figure 12. Flow alignment of nematic discotic and a nematic calamitic liquid crystals. The director alignment is shown schematically by the alignment of one molecule.
8.1 Nematic Liquid Crystals
363
era1 temperature dependence can be separ
traut and Hess [33] suggest the ansatz
where g i ( T ) is related to a relaxation process in the nematic liquid crystal. If the activation energies for the various relaxation processes are equal the ratio between two Leslie or shear viscosity coefficient should be constant far away from the clearing point which has been observed experimentally. Kuzuu and Doi [45] obtained the following expressions for the Leslie coefficients
This and other mesoscopic theories assume that the molecules consist of rigid rods or ellipsoids, that a special form of the interaction potential is valid and that there are no pretransitional phenomena due to a smectic phase. As real liquid crystal molecules do not show such properties these theories only allow a very rough description of the experimental observations. A comparison between some theories has been presented by Kroger and Sellers [47].
2
al =  2 f  I ~ ~ p2 + 1
8.1.9 0!4
= f 27 p(27 1 5 &
2s4)
(69) (70)
3 5 p +1
(7 1) where the common factor f is
Concluding Remarks
The six Leslie coefficients can not be measured directly. They can only be determined with the aid of several experimental methods which ususally lead to combinations of these coefficients. Taking into account the Parodi equation, the six coefficients can be obtained from five linear independent viscosity coefficients. Thus, the four viscosity coefficients ql, q2, q3, and qI2and the rotational viscosity coefficient '/1 give
ckT P2 1
f=20,p2+i L
c is the number density of molecules,p=alb
the aspect ratio and D,is the effective rotational diffusion coefficient. The parameter A is connected to the flow alignment angle 1 COS2@0 = (73)
a
and can be calculated from the theory. The expression for A contains the order parameter S2. S2 and S4 are the averages over the Legendre polynomials of second and forth order of the equilibrium distribution function. S2 corresponds to the usual order parameter. As S4 is usually not known Ehren
a3 =
1 T(%  7h + Yl)
a 4 = 2173
1 + Ih  4773  Yi) 2 1 (171 + 3%  4%  y1) 2
a5 = (37h a6
(75)
Furthermore, Eqs (lo), (1 8) and (35) lead to (171

772) cos 2@0 = Yl
(76)
which can be used to introduce the flow alignment angle a0into Eq. (75) instead of q1,q2 or x. Owing to thermodynamical ar
364
8
Flow Phenomena and Viscosity
guments [8] the values of the Leslie coefficients are subject to the conditions
+ 3a4 + 2a5 + 2a6 > 0; 2a4 + a5 + a, > 0; (77)
a, > 0; 2 a , “/1 > 0; 4y1(2a4 + a5
+ a(j)> (q+ a3 + a6  as)*
or 173 > 0; 1712 + 2(171 + 172) > 173 + Yl ‘/1 > 0; Yl{2(171 + 172)  Yl I > (172  17d2
gradient there are three main cases (see Fig. 13) which are labelled according to the indices of the shear viscosity coefficients of nematic liquid crystals. The helical axis h is assumed to be parallel to the zaxis for the following discussion. @describes the angle between local director n andxaxis (see Fig. 14).
(78)
The fourth condition in Eq. (77) has been omitted in Eq. (78) as it follows from the third and the fifth. Whereas ql, q2, q3,and yl must be positive q,2can have either sign.
8.2 Cholesteric Liquid Crystals Under isothermal conditions the constitutive equations for the description of flow phenomena in nematic and cholesteric liquid crystals are identical [48]. Nevertheless, a series of novel effects are caused by the helical structure of cholesteric phases. They arise firstly because of the inhomogeneous director orientation in the undistorted helix and secondly because of the winding or unwinding of the helix due to viscous torques. Regarding the orientation of the helical axis with respect to velocity and velocity
I
I1
8.2.1 Helical Axis Parallel to the Shear Gradient (Case I) The cholesteric liquid crystal is sheared between two parallel walls at z = kT. Leslie [49] and Kini [50] have studied this case with different boundary conditions. Leslie assumes that the pitch of the helix remains constant at the walls whereas Kini assumes a fixed orientation of the director at the wall with an orientation which corresponds to that of the undistorted helix. Both boundary conditions are difficult to realize in an experiment. In spite of the different orientations at the walls the results of the calculations are qualitatively the same. In the bulk the director orientation is determined by elastic and viscous torques. Transverse flow in zdirection is excluded. The differential equations can analytically be solved for small helix distortions. If the pitch Po is comparable to the cell thickness 2 T the volume velocity and the appar
I11
Figure 13. Orientation of the helix with respect to the shear gradient. The pair of arrows symbolizes the shear flow.
x
Figure 14. Orientation of the helical axis and the director with respect to the coordinate system.
8.2 Cholesteric Liquid Crystals
ent viscosity respectively are oscillating functions of the pitch for constant cell thickness. The reason for this effect is the oscillating mean value of the director orientation. With decreasing pitch these oscillations die out and the apparent viscosity approaches the limiting value
V ( P , = 0) = 21721734172 + 173)
(79)
For larger shear rates the helix will be distorted. The corresponding differential equation can only numerically be solved. The calculations of Leslie and Kini show, that for a given pitch and cell thickness the apparent viscosity starts with a plateau for small shear rates and decreases with increasing shear rates to the viscosity which is observed for flow alignment. The necessary shear rates for this transition depend on the pitch. The smaller the pitch the larger are the necessary shear rates as the resistance against a distortion increases with decreasing pitch. The influence of static shear deformations has been studied in several papers [5 1, 521.
8.2.2 Helical Axis Parallel to the Flow Direction (Case 11) The flow of a cholesteric liquid crystal through a narrow capillary with circular cross section according to Fig. 15 is the
gm helical axis
Figure 15. Flow of a cholesteric liquid crystal parallel to the helical axis.
365
most simple example for this case. The orientation at the capillary wall should be consistent with the helical structure and the pressure gradient along the capillary axis should be small. Helfrich [53] assumes that the helical structure remains undistorted and a permanent rotation of the director in the flowing liquid crystal results. The director rotation is coupled with a specific energy dissipation of
E = y1Q2 = y,(y) 2nv V

2
For small pitches and large velocities this term exceeds the energy dissipation by Poiseuille flow and the resulting flow velocity is nearly constant across the cross section (plug flow). The dissipated energy is taken from the pressure gradient along the capillary. This leads to
In contrast to Poiseuille flow the volume flow depends only on the square of the capillary radius. For P 4 R the apparent viscosity exceeds yl by far. According to Helfrich this type of flow is called permeation. Kini et al. [54]have studied the same problem using the equations of continuum theory. They could show that the velocity profile is almost flat except a small layer near the capillary wall. Neglecting the boundary layer the equations presented above were obtained.
8.2.3 Helical Axis Normal to v and grad v (Case 111) The cholesteric liquid crystal is sheared between two parallel walls. It is assumed that the walls d o not influence the director orientation (weak anchoring) and that the flow velocity is parallel to the movement of
366
8
Flow Phenomena and Viscosity
the walls. Under these assumptions the continuum theory gives the differential equation
where
are a nondimensional time z,position {, and a nondimensional parameter k of the system. k,, is the twist elastic constant and Po is the pitch of the undistorted helix. For small k values the helical structure remains undistorted and its pitch constant. Then Eq. (82) allows a simple calculation of the director rotation:
(84)
flow through a round capillary. According to the section on the rotational viscosity this director rotation is coupled with a torque on the liquid crystal. The torque generation must be compensated by elastic deformations or additional circular flow. For a flow of a cholesteric liquid crystal through the gap between two coaxial cylinders the torque is partly transferred to the walls of the cylinders. Fischer et al. [55] used a fixed outer cylinder and determined the torque on the inner cylinder. Equation (20) gives for the torque on the walls M = y p v = +y1 2n VV (87) P for a sample with volume V. The experiments could only demonstrate the existence of the effect, as the flow in the experiment was dominated by shear flow and only a minor part (some %) resulted from permeation.
which gives @ ,f

VX,Y
2
(85)
Thus a permanent director rotation results. The apparent viscosity amounts to
1
%pp = p 1 + ? 7 2 )
(86)
which agrees with the value for a fixed helix, as there is no rotation of the director with respect to the fluid in both cases. For larger k values the helix becomes distorted and its pitch increases with k. Finally, the helix unwinds and a flow aligned structure appears.
8.2.4 Torque Generation Under Flow In the case of geometry I1 the director of the cholesteric liquid crystal rotates during the
8.3 Biaxial Nematic Liquid Crystals Shortly after the first observation of a biaxial nematic phase by Yu and Saupe [56] the hydrodynamic theory of the uniaxial nematic phase was extended to the biaxial case in several papers [57601. The following description is similar to that given by Saupe [59] as well as Govers and Vertogen [60], but the notation is different. A biaxial nematic phase is characterized by two orthogonal directors a and b of length 1. Introduction of a third orthogonal vector c of length 1 simplifies the notation of the following equations. According to Saupe, Govers and Vertogen the viscous part of the stress tensor of an incompressible biaxial nematic phase is the sum of the sym
8.3 Biaxial Nematic Liquid Crystals
metric part 0s. 1J
8.3.1 Shear Viscosity Coefficients
= ,ul(a.a.Vbb+ b.b.V"") I J
Z J
+ p2(bibbjV"'+ cjcjVbb) + p&;cjvua + a;ujVC"') + ,u4(a,bj + ajbj)Vab + pu,(bicj+ bjci)Vb" + p6(cjaj+ cjai)Vca + p7(aibj+ ajbi)Ah + p8(bicj+ bjci)B" + &(cj aj + cjai)Ca
For a fixed director orientation and a flow according to Fig. 16 the velocity gradients and the director rotations relative to the fluid are vx): = vvx = wx): =wYt =  2 2/1 x,y (94)
(88)
and the skew symmetric part 0; =
p7(aibj ajbi)VUh + p8(bic, bjcj)vb" + illg(ciaj  cj ai)V"'" + ,ulo(ajbj ajb,)Ab + p, l(bici  bjcj)B" + p&a;  CjUi)C"
CI . =  W V. cJ. (95) and the viscosity q= oxylvx,,becomes
A . =  W 1J. a J. ;
1
2
17 = 2
2
by
(P4 + 2P7 + PIO) + 2/43 + f i l l )
+c:a;@6 + 2rllg + PI21 + a;b:(P4  2P7 + PIO)
(89)
+b;C3Ps2P8+Pd +c;a:(P62rllg+P12) + 2axaybxby(2Pl+ P4  PI01 +2bxbycxcy(2P2+ P5  P11) +2c.x5axay(2P3 + APul2)1
are the symmetric and the skew symmetric part of the velocity gradient tensor and
(96)
In principle, the director components can be (91)
are the director rotations relative to the fluid. Furthermore, the following notation is used
xu = x p u p ;
BI . =  W .'J b .J ;
+&;(PS
where V . = 1( V ,. + v . . ) ; W . . =1 ( ~ j , j  ~ j ,(90) ;) V 2 l,J J.1 lJ 2
A . = a .  W.a.; B,=b, W.6.; I I I J J lJ J c.I = c.1  WU. CJ .
367
Y;= Yp4uq; Y U V =l&4qvp (92)
The viscous torque is obtained according to the procedure in Sect. 8.1.2 on the rotational viscosity.
expressed in terms of Eulerian angles. However, the resulting expression is rather lengthy and the cyclic structure of Eq. (96) is lost. Director orientations with all directors parallel to the coordinate axes are described by the first six terms, for example, the orientation a IIx and b IIy corresponds to the
4 = &ijkUsJ= 2&ijk(P,Ukb;vub+ /&bkC;VbC+ &Ckajv'" + /LloakbjAb + , l . L l ~bkC;B' + /112Cka;ca) (93) Equations (88) and (89) include the case of the stress tensor for the uniaxial nematic phase [ 5 9 ] .
z
f
grad
Figure 16. Director orientation in a biaxial nematic phase with respect to the flow velocity and the velocity gradient. The case cllz is shown where as the equations in the text correspond to the general case.
368
8
Flow Phenomena and Viscosity
viscosity coefficient 2 ,u7+ pI0).The last three terms give a maximum contribution if two directors lie under 45" in the xy plane, i.e. they correspond to the a, term of uniaxial nematics. Thus, nine coefficient combinations can be determined with the aid of flow experiments.
8.3.2 Rotational Viscosity Coefficients The last three terms in the torque Eq. (93) describe the torques due to director rotations. The three main cases are rotations around a, around b, and around c . The latter corresponds to &,#O in Fig. 16. The viscous torques for these cases are
r, =  2PI I @a; r b =  2P12@b; r, =  2 p 1 0 ~ c
(97)
describes the rotation around the where i axis. The three rotational and the nine shear viscosity coefficients according to Eq. (96) represent a complete set of coefficients.
8.3.3 Flow Alignment It is assumed that the c director is parallel to the z axis, e.g. by application of a magnetic field. A shear flow z ~ exhibits ~ , ~ a torque on the directors around the z axis. Calculation with Eq. (93) gives
r, =  2PN&  ?&7 r, = 0 and &, = 0 give
Correspondingly, the flow alignment angles around all axes are cos2oa = ;Pl 1 P8
COS2@6 = ;P12 &
P10 cos2CPc = ~
(101)
PI
The conditions for the first two viscosity coefficient ratios correspond to Eq. (100). A discussion of the stability of the various solutions is presented in the paper of Saupe [59]. Brand and Pleiner [61] as well as Leslie [62] discuss the flow alignment without the restriction that one director is perpendicular to the shear plane.
8.4 SmC Phase The hydrodynamic theory for SmC phases was developed by Schiller [ 181 and Leslie et al. [19]. Schiller as well as Leslie et al. assume a constant layer thickness, a constant tilt angle and do not include the permeation, that is, the dissipation of energy by the penetration of molecules through the layers. Furthermore, Schiller neglects the distorsion of the layers in contrast to Leslie et al. The Leslie theory is, therefore, somewhat more general. The orientation of the SmC phase is described by two directors. The director a is normal to the layers and c is parallel to the layers in the direction of the tilt. The a director, the preferred direc
cos2@c + P,0) (98)
PI 0 COS2@, = ~ P7
Z
(99)
This equation only has solutions for
e /
/
Figure 17. Definition of the directors a and c for an SmC phase.
8.4 SmC Phase
tion of the long molecular axes, n,and c lie, therefore, in a plane (Fig. 17). According to the theory of Leslie et al. [19] the viscous part of the stress tensor is the sum of the symmetric part 0;
=
and the skew symmetric part 0;=
grad v

hvj+ plVaauiaj + p2(Kaaj+ y"ui)
+ p3vVccci cj + p4(v," c; + I$"C;) + p5Vac(aicj + uj ci)+ Al(Aiuj + Aj ui) + &(Cicj + Cj ci)+ &A"(u, cj + uj ci) + K1(v,"Cj + p i + FCUj + p i ) + ~ c , ( V " " ( a+~ cuj~ci)+ 2V""uiaj) + K3(V'"(Uicj + uj Ci) + 2V""CiC j ) + z , ( C i a j + Cjui)+ z 2 ( A i c j + A j c i ) + 2z3ACaiu,+ 2z4ACcicj (102)
a,(yaui yauj) + q y c c i  v,cc.)I + &Vac(uicj  uj ci) + d4(Ajai  Aiuj) + &(c. C .  ci C j ) + &A"(ai C j  U j Ci) + z,(Y ci  yacj)+ z2(q"ui F C U j ) + z,V""(Uicj uj Ci) + z4Vcc(uicj  aj ci) + ~ 5 ( A~ij  Ai cj + Cj ~i  Ci ~ j )( 1 03) / , l

The notation is the same as described in Sect. 8.3. The stress tensor contains 20 independent coefficients. It fulfills the Onsager relations. The viscous torque is obtained according to the procedure used for nematic liquid crystals
d
X
Figure 18. Definition of angles for a flow experiment in the SmC phase.
layers. The a director and the z axis are, therefore, parallel to one another. As a flow perpendicular to the layers is largely supressed due to the permeation effect, the flow has to be parallel to the xy plane. Furthermore, it can be assumed without loss of generality for this calculation that the flow is parallel to the x axis. The c director lies in the xy plane and its direction is described by the angle @. The velocity gradient lies in the yz plane and is described by the angle Y. Under these conditions the effective viscosity calculated from the stress tensor Eqs. (102) and (103) becomes
i'
q= pO+p42a2+A5)sin2@ 1 +(po +p4 + 2 a 2 +as)cos2@ 2 + p 3 sin2@cos2@}sin2Y
+
vz + & ck v"" + &Ak + &CkA" + z2vk + 23 CkVaa+ z4ckvcc + 5 ck) + C j ( a & + d5Ck + 2,v;
{i
(pug+ p 2  2 4 + A4)sin2 1
= & i j k o z j =  2&ijk{ aj ( 1 1
+ 2gAk))
+(po + p 2 +p4+ p 5  2 a l + 2 a 2 2
+ a4+ a5+ a6lcOs2 Y  T~  7 2 + 25 + 2(23  Z ~ ) C O S ~
2a, +(K,
(104)
.sin @ sin Y cos Y
8.4.1 Shear Flow with a Fixed Director Orientation The xy plane of the system of coordinates (Fig. 18) used for the following calculation is assumed to be parallel to the smectic
369
(105)
We define, therefore, a new set of viscosity coefficients 771
= 21( p 0 + p 4  2 a 2 + d S )
772
= ?(PO
1
773 = P3
p4
2&? + j15
370
Flow Phenomena and Viscosity
8
The viscous dissipation requires
774 = T1( P O + P 2  2 a I + A 4 )
775
a,
1
= Z(p0 + P2 + p4
pS
 2 4 +2a22a3+a4+as+a6)
q6
=K17172+r5
777
= 2(23  7 4 )
(106)
and get finally
q = (ql sin2@+ q2cos2@ + q3 sin2@cos2@)sin2Y (107) + (q4sin2@+ q5cos2@)C O S ~ Y + (q6+ q7 cos2@)sin@ sinYcosY The flow properties of a SmC phase with fixed director orientation and a flow parallel to the layers can, therefore, be described by seven independent viscosity coefficients. The experimental determination of these coefficients should be connected with a series of problems. If the coefficients q4 or q5 are determined in a capillary with a rectangular cross section with T+ Wand the layer parallel to one of the plates as in Fig. 20 I. The thickness has to be constant over the whole sample with an accuracy that is not easy achieved [63,64]. There are similar problems in the measurement of the other coefficients. Minor difficulties should occur in a shear experiment with a small lateral movement of one of the plates.
8.4.2 Rotational Viscosity Equation (104) allows to calculate the viscous torque which is exerted on the c director during a rotation around the a director with a constant tilt angle 0. It is assumed that the liquid crystal is at rest. The only nonvanishing term in Eq. ( 1 04) is that with the coefficient A5.
r, =  2 & & i k = 2 A 4
cj c
k
 2&(c,cy  c y c x )
(1 08)
>o
(109)
It is often interesting to compare the rotational viscosity coefficient “/1 in the nematic phase and
yT = 21,
(110)
in the SmC phase. Then it has to be taken into account that ri and k are different and that the torque on c is only the projection of the torque on n. A rotational viscosity coefficient suitable for a comparison with the coefficient yl in the nematic phase is, therefore
A magnetic field rotating in the xy plane leads to a rotation of the c director. The calculation is similar to that in the nematic phase. However, it has to be taken into account that the interaction with the magnetic field is different for the two phases. Principally, the magnetic susceptibility of an SmC phase is biaxial with the main susceptibilities parallel to n (xl),perpendicular to n in the layer plane (x2)and perpendicular to these two directions (;c3).In a good approximation x2=x3can be assumed and the magnetic torque on the c director becomes = &xaii2 1 sin20sin2(y (1 12) 2 where y is the angle between field direction and x axis and
Z=xI

x2
x1
0x2
In the biaxial case sin2 O+x3cos2 has to be used instead of ;la sin2 0.As in the nematic phase there is a critical velocity
’ 2 ,u0xaH2 sin 0 (1 14) 4 4 up to which the director follows the field rotation with a phase lag. A, can be determined
.
=
8.4 SmC Phase
from the torque on the sample
leads to
4 ux,ysin2Qo < 0 8.4.3 Flow Alignment The SmC phase is sheared between two parallel plates of infinite dimension. The distance between the plates is so large that the influence of the surface alignment at the plates can be neglected in the bulk. The orientation of the directors, the velocity and the velocity gradient is the same as already discussed for the shear flow experiment (Fig. 18). Furthermore, a rotation of the director c is now allowed. Calculation of the torque according to Eq. (104) and rz=O gives 2a4+
{(a,+ & c o s 2 0 ) s i n ~ + (7,
(1 16)  zl)sin@cos!P) u , = ~0
where u , is~ the velocity gradient. For ty=O this equation gives 2&@+ (z, zI)sin@ux,,= 0
(1 17)
Time independent solutions of this equation are
a = = ;a=n
(1 19)
1, is always positive (see Eq. 109). For As> 1 % I there is no flow alignment. For
A, < I & I
a time independent solution is
COS2@()= AS
(121)
Assuming ux,y>Oand&> Ogives astable flow alignment for sin 2 O00, a stable flow alignment is obtained at @=O for z,> z1 and at @= n for z,< z1. For ty= 90" Eq. ( I 16) gives 2 a s a + (a5+ 4 c 0 s 2 ~ux,y ) =o
37 1
(120)
22
which gives four solutions for O0.The stable solutions are found by an expansion of Eq. (1 19) around the flow alignment angle (@= a0+ A@) for small deviations. This
8.4.4 SmC* Phase The viscous part of the stress tensor for the SmC and the ferroelectric chiral smectic (SmC") phase agree with one another. The flow phenomena with a fixed director orientation discussed in the foregoing section can not be observed due to the inhomogeneous director orientation in the SmC* phase. However, there is a large interest in rotational movements of the director in ferroelectric displays. In surface stabilized ferroelectric liquid crystal cells the liquid crystal is sandwiched
372
8
Flow Phenomena and Viscosity
A rearrangement gives oij= p l a i a j ~ p a k a+p(Al Figure 19. Director alignment in a ferroelectric liquid crystal cell.
between two glass plates which are treated to give the book shelf alignment shown in Fig. 19 with two stable director orientations at the glass plates. Due to the alignment of the director at the glass plates and due to the short distance of the glass plates the helical structure of the SmC* phase is surpressed and the orientation of the c director is nearly homogeneous within the cell. The Leslie theory assumes a rotational movement on the cone during the switching from n to n'. Other trajectories have also been discussed. Carlsson and ZekS [67] found out that the viscosities for a movement of the n director on the cone and perpendicular to it are identical. Experiments [68] have shown that the movement occurs on the cone apart from a small deviation due to the electroclinic effect.
+(
SmA Phase
+ plvp""aiaj+ pz(&aaj + 5 " U J
+ Iq(Aiaj + Ajai + yaui  Y a a j )
+ A4(Aj ai  A , ~
j )
(123)
and the viscous torque =  2~ijkaj(AiV;+A4Ak)
+(
(125)
~ +2 4)aivkak
r= 2a x (A4A + A,Va)
(126)
As the symmetry of the SmA and the nematic phase agree, the structure of the stress tensors is identical and the connection between the coefficients is
a,
%pal  a4 u3eail, + a4
a4 epfJ
y, 9 2A4
a5ep2 a, y 2 ~ 2 a 1 a6eP2+ al (127)
Up to now the influence of the permeation effect has been neglected and the Eqs. (123126) give only meaningful results if the flow velocity component perpendicular to the layers can be neglected. In the other case the permeation effect, that is, an energy dissipation for a flow perpendicular to the layers, has to be taken into account, For this purpose the layer normal is assumed to be parallel to the z axis (Fig. 20) and the stress tensor becomes = Plyz4r4z+
+ (a, + ~
(4  a 4 ) A i 4 z +
~ ) h~ y j~ + (Pz  A,) v z ijz + (P2 +
The stress tensor for the SmA phase can be obtained from the two director theory for the SmC phase by elimination of all terms containing the c director. The sum of the symmetric and the skew symmetric part becomes oij =
~ 2 al)ajKkak
and
oij
8.5
 &)ujAi
+ ( A , + A4)aiAj+ hvj
( 124)
f
i (128) ~ ~
4)yz 4,
According to Helfrich [53], de Gennes [69], and Martin et al. [ 171 the permeation can be described with the additional term 1 (129) P,z= (i %>
r
in the equation of motion, ( v z  i ) is the flow velocity with respect to the layer structure. In the following the flow of a SmA phase between two infinite plates will be considered. In contrast to the discussion of nematic phases these plates will be assumed to be at rest as moving plates are not always compatible with the layered structure. The three main cases are outlined in Fig. 20.
8.6 References
373
Z 1
 "2 (PSZ
I 0 T
Figure 20. Flow of an SmA phase between two parallel plates (hatched). The layer normal is parallel to the zaxis.
For the cases I and I11 parabolic velocity profiles as known for isotropic liquids result. The viscosity coefficients are caseI:
Y
T
Figure 21. Velocity profile for a flow with permeation (case I1 of Fig. 20).
I1
I11
O
flow is neither parallel nor perpendicular to the layer normal. The elastic behaviour of the smectic layers, the permeation effect and the viscous flow lead to a great variety of phenomena in SmA phases: effects due to the compression of the layers [70,71], flow behind obstacles [69, 721, and instabilities [73, 741.
q1= T1( p o + ~ 2  2 A l + A 4 )
1 case 111: q3 = po 2
8.6 References
For case I1 the permeation has to be taken into account. 1 P,z + 772 v,,yy   vz = 0 (131)
5
with
Integration gives the velocity profile (133)
where (134)
is the thickness of the shear dominated part and 2 T is the distance of the plates. Thus T l b 1 gives a plug flow and TIAa 1 gives a shear dominated velocity profile (Fig. 21). The viscosity coefficient p, can only be determined in a flow experiment where the
[ l ] R. S. Porter, J. F. Johnson in Rheology, Theory and Applications (Ed.: F. R. Eirich), Academic Press, New York 1967. [2] P. G. de Gennes, The Physics ofLiquid Crystals, Clarendon Press, Oxford 1975. [3] M. J. Stephen, J. P. Straley, Rev. Mod. Phys. 1974,46,617704. [4] J. G. Jenkins, Ann. Rev. Fluid. Mech. 1978, 10, 197219. [5] W. H. de Jeu, Physical Properties of Liquid Crystalline Materials, Gordon and Breach, New York 1980. [6] G. Vertogen, W. H. de Jeu, Thermotropic Liquid Crystals, Fundamentals, Springer Series in Chemical Physics 45, Springer, Berlin 1988. [7] P. G. de Gennes, J. Prost, The Physics ofLiquid Crystals, 2ndedn, Clarendon Press, Oxford 1995. [8] F. M. Leslie in Advances in Liquid Crystals (Ed.: G. H. Brown), Academic Press, New York 1979. [9] F. M. Leslie, Mol. Cryst. Liq. Cryst. 1981, 63, 1 1 1128. [ 101 F. M. Leslie, Quart. J. Mech. Appl. Math. 1966, 19,357370. [ l l ] F. M. Leslie, Arch. Ratl. Mech. Anal. 1968, 28, 265283. [12] J . L. Ericksen,Arch. Ratl. Mech. Anal. 1966,23, 266275.
374
8 Flow Phenomena and Viscosity
[ I 3 1 J. L. Ericksen, Mol. Cryst. Liq. Cryst. 1969, 7,
153164. [14] 0. Parodi, J. Physique 1970, 31, 581584. [15] G. Vertogen, Z. Naturforsch. 1983, 38a, 12731275. [16] D. Forster, T. C. Lubensky, P. C. Martin, J. Swift, P, S. Pershan, Phys. Rev. Lett 1971, 26, 101610 19. [I71 P. C. Martin, 0. Parodi, P. S . Pershan, Phys. Rev. A 1972,6,24012420. [ l a ] P. Schiller, Wiss.Z. Univ. Halle 1985,34,6178. [I91 F. M. Leslie, I. W. Stewart, M. Nakagawa, Mol. Cryst. Liq. Cryst. 1991, 198, 443454. [20] S . P. A. Gill, F. M. Leslie, Liq. Cryst. 1993, 14, 19051 923. [21] K. F. Wissbrun, J. Rheol. 1981, 25, 619662. [22] G. Marrucci, F. Greco, Adv. Chem. Phys. 1993, 86, 331404. [23] M. G. Clark, F. M. Leslie, Proc. R. Soc. Lond. A 1978,361,463485. [24] P. K. Currie, Mol. Cryst. Liq. Cryst. 1974, 28, 3353 3 8. [25] W. Helfrich, J. Chem. Phys. 1969, 51, 40924105. [26] M. Miesowicz, Bull. Acad. Polon. Sci. Lett., Ser. A, Sci. Math. 1936, 228247. [27] Ch. Gahwiller, Phys. Lett. 1971, 36A, 3 113 12. [28] V. Zwetkoff, Acta Physicochimica CJRSS 1939, 10,555578. 1291 F. M. Leslie, G. R. Luckhurst, H. J. Smith, Chem. Phys. Lett. 1972,13,368371. [30] K. B. Migler, R. B. Meyer, Physica D 1994, 71, 4 12420. [31] I. Zuniga, F. M. Leslie, Europhys. Lett. 1989, 9, 689693. [32] W. Helfrich, J. Chem. Phys. 1969,50, 100106. 1331 H. Ehrentraut, S. Hess, Phys. Rev. E 1995, 51, 220322 12. [34] P. Manneville, Mol. Cryst. Liq. Cryst. 1981, 70, 223250. [ 3 S ] T. Carlsson, Mol. Cryst. Liq. Cryst. 1984, 104, 307334. [36] P. G. de Gennes, The Physics of Liquid Crystuls, Clarendon Press, Oxford 1975, p. 68. [37] P. K. Currie, J . Physique 1979,40, 501505. [38] R. J. Atkin, F. M. Leslie, Quart. J . Mech. Appl. Math. 1970, 23, S3S24. [39] P. K. Currie, Arch. Ratl. Mech. Anal. 1970, 37, 222242. [40] R. J. Atkin, Arch. Ratl. Mech. Anal. 1970, 38, 224240. [41] P. Pieranski, E. Guyon, Phys. Lett. 1974,49A, 3, 237238. [42] P. Pieranski, F. Brochard, E. Guyon,J. Physique 1973,34,3548. 1431 F. Brochard, Mol. Cryst. Liq. Cryst. 1973, 23, 5 158, [44] T. Carlsson, J. Physique 1983, 44, 90991 1. [45] N. Kuzuu, M. Doi, J. Phys. Soc. Jpn. 1983, 52, 34863494.
[46] M. A. Osipov, E. M. Terentjev, Z. Nuturfursch. 1989,44a, 785792. [47] M. Kroger, H. S. Sellers, J. Chem. Phys. 1995, 103,807817. [48] F. M. Leslie, Proc. R. Soc. A 1968, 307, 359372. [49] F. M. Leslie, Mul. Cryst. Liq. Cryst. 1969, 7, 407420. [50] U. D. Kini, J. Physique Coll. C3 1979, 40, 6266. [51] N. Scaramuzza, R. Barberi, F. Simoni, F. Xu, G. Barbero, R. Bartolino, Phys. Rev. A 1985, 32, 11341 143. [52] V. G. Kamenskii, E. I. Kats, Sov. Phys. JETP 1988,66, 10071012. [53] W. Helfrich, Phys. Rev. Lett. 1969,23,372374. [54] U. D. Kini, G. S . Ranganath, S . Chandrsekhar, Pramuna 1975,5, 101106. [55] F. Fischer, J. Grupp, J . Physique Lett 1984,45, L 109 1L 1095. [56] L. J. Yu, A. Saupe, Phys. Rev. Lett. 1980, 45, 1000 1003. [57] H. Brand, H. Pleiner, Phys. Rev. A 1981, 24, 27772787. [58] M. Liu, Phys. Rev. A 1981,24, 27202726. [59] A. Saupe, J. Chem. Phys. 1981, 75,51185124. [60] E. Govers, G. Vertogen, Physica 1985, 133A, 337344. [61] H. Brand, H. Pleiner, J . Physique 1982,43,853858. [62] F. M. Leslie, J. NonNewtonian Fluid Mech. 1994,54,241250. [63] L. Leger, A. Martinet, J. Physique 1976,37, C38997. [64] P. G. de Gennes, J. Prost, The Physics of Liquid Crystals, 2nd edn, Clarendon Press, Oxford 1995, p. 432. [65] T. Carlsson, F. M. Leslie, N. A. Clark, Phys. Rev. E 1995,51,45094525. [66] M. Osipov, E. M. Terentjev, Mol. Cryst. Liq. C r y ~ t1991, . 19{, 429435. [67] T. Carlsson, B. ZekS, Liq. Cryst. 1989, 5, 359365. [68] I. Dierking, F. Giesselmann, P. Zugenmaier, G. Pelzl, P. Schiller, Cryst. Res. Technol. 1992, 27, 727739. [69] P. G. de Gennes, Phys. Fluids 1974, 17, 16451654. [70] R. Bartolino, G. Durand, J. Physique 1981, 42, 144514s 1. [71] R. Bartolino, G. Durand, J. Physique Left.1983, 44, L79L83. [72] P. Oswald, J. Physique Lett. 1983, 44, L303
L309. [73] P. Oswald, S. I. BenAbraham, J. Physique 1982,43, 11931 197. [74] J. Marignan, 0. Parodi, J. Physique 1983, 44, 26327 1.
Behavior of Liquid Crystals in Electric and Magnetic Fields Lev M. Blinov
9.1 Introduction As is well known, liquid crystals are very sensitive to electric and magnetic fields [ 11 and it is this property which allows their application in display and other optical devices technology. The field effects may be divided into three groups. The first includes the electric or magneticfieldinduced changes in the microscopic structure of a liquid crystal phase. This implies that the field is directed in such a way with respect to the director that, under the action of the field, the orientational state of the mesophase is unchanged (the field stabilizes the director distribution). The second group includes changes in the macroscopic structure, due to a destabilization and reorientation of the director under direct action of the electric or magnetic field. The backflow effects accompanying the distortion in the transient regime are driven by the director reorientation (primary process) and are of secondary importance. The fluid is considered to be nonconducting. The effects caused by the electric field and related to the conductivity of a liquid crystal are included in the third group (electrohydrodynamic instabilities). All these effects
are dissipative in nature and have no magnetic analogs. Due to the strong anisotropy of liquid crystals, field effects are accompanied by dramatic changes in optical properties. The electrooptical properties of liquid crystals have been studied very actively since the beginning of the century, and many important phenomena have been discovered. The earlier theoretical and experimental results on the physical properties of liquid crystals, including certain electric field effects, have been reviewed in a variety of books [ 151, as have the details of electrooptical effects [691, and many results relating to theproperties of liquid crystalline materials and their application in devices have been reported [lo121. The present section is devoted to a discussion of electric field effects i n various liquid crystal phases, with an emphasis on the physical aspects of the phenomena. The discussion is based on classical results, although the most important recent achievements in the field are also mentioned. As ferroelectric liquid crystals are covered in detail in other chapters in this book, they are discussed only briefly here for the sake of completeness. Electrooptical properties of
376
9
Behavior of Liquid Crystals in Electric and Magnetic Fields
polymer liquid crystals have recently been discussed in detail [ 131; here, only specific features of polymer mesophases relevant to their field behavior are mentioned.
9.2 Direct Influence of an Electric or Magnetic Field on Liquid Crystal Structure 9.2.1 Shift of Phase Transition Temperatures In general, when an external field is applied to a nonpolar or polar liquid crystal, a quadratic or linearinfield term, respectively, must be added to the expression for the free energy density of the medium. The quadraticinfield energy terms describe the interaction of the electric or magnetic field with the dielectric X, or diamagnetic ya anisotropy of susceptibility:
g H = T1 Y a H 2
electric liquid crystals. More generally, the
P E term is also used to describe other polarized systems; for example, in the discussion of the flexoelectric effects in nonpolar phases as nematics or cholesterics where the polarization P is induced by a mechanical distortion. The field terms may stabilize or destabilize the intrinsic thermodynamic order of a mesophase, and hence increase or decrease the temperature of its transition to a less ordered phase. The shift in the transition temperature is calculated by comparing the electric (magnetic) energy with the transition enthalpy or some other competing thermodynamic quantity (e.g. elastic energy). Below we consider examles.
9.2.1.1 SecondOrder Transitions Smectic ASmectic C Transition In this case we must compare a gain in the electric (or magnetic) energy with a loss of the softmode elastic energy characterized by a change in tilt angle 8. Thus, for the electric field case, the shift in the AC transition temperature is [7]:
(3)
(1 b)
The linear terms describe the interaction of the fields with media, polarized or magnetized either spontaneously or by external factors other than electric field itself. In ferroelectrics and ferromagnetics the magnitude of the spontaneous polarization Ps or magnetization M s is finite and the energy term is
As ferromagnetic mesophases are still to be discovered the linear term (Eq. (2 a) or (2 b)) is important only when considering ferro
where n is the director, E,= 1 + 4 n ~is, the dielectric anisotropy and a is a parameter of the Landau expansion for the AC transition: g=
~
1 a ( T  Tc.A) 8 '
2
+ 41 be4 
(4)
and g, is taken in the form of Eq. (1a). The sign of the shift depends on the field direction. If E is parallel to the normal h to the smectic layers and 0, the field stabilizes the smectic A phase and TcA decreases. An oblique field (&,>O) induces a tilt, and thus stabilizes the smectic C phase and Tc.A increases.
9.2 Direct Influence of an Electric or Magnetic Field on Liquid Crystal Structure
Smectic ASmectic C* Transition For the chiral smectic C* phase, which is ferroelectric, in addition to the quadratic term (Eq. (1 a) or (1 b)) the linear term proportional to polarization P must be taken into consideration. As a rule, the linear term exceeds the quadratic one and the free energy may be taken in form:
1 a 0 9’ g =
p2 + 1 b g4+ __ CP9
PE ( 5 ) 2 X.l where ao=a ( T  TC.*) describes the elasticity for 69 changes, P is the polarization,
2

4
C is the tiltpolarization coupling constant (or piezocoefficient), and is the background dielectric susceptibility, which may be taken from the isotropic phase. In Eq. ( 5 ) the smectic C* is assumed to be unwound and all chiral terms important for a helical ferroelectric are omitted. Strictly speaking, even for an infinitely small electric field the secondorder AC* transition disappears. However, the softmode dielectric susceptibility maximum characteristic of that transition is still observed at the “apparent” transition temper
xL
377
ature T,. With increasing field T,,, increases according to expression [ 141:
Such a shift governed by the second term in the Landau expansion and strongly dependent on piezocoefficient C has been observed experimentally [ 14, 151. The experimental points for a multicomponent ferroelectric mixture [14] and the fit using Eq. (6) is shown in Fig. 1.
9.2.1.2 Strong FirstOrder Transitions Isotropic Liquid Nematic Transition In the case of positive dielectric anisotropy of a nematic, even a weak field makes the isotropic phase uniaxial and the NI phase transition disappears (see Pikin [7], Chap. 4). However, the apparent NI phase transition temperature may change with the electric or magnetic field. For &,>O and E lilt, the quadraticinfield energy terms (Eq. (la) and (lb)) reduce the free energy and stabilize the anisotropic phase. In the
Figure 1. The voltage dependence of the shift in the softmode susceptibility maximum temperature [14]: (a) mixture 1; (b) mixture 2. Dotted lines correspond to Eq. (6). Cell thickness 10 pm.
378
9
Behavior of Liquid Crystals in Electric and Magnetic Fields
case of an electric field, the transition temperature increases by the value [ 161 (7)
where AHt is the enthalpy of the NI phase transition, is the dielectric permittivity of the nematic phase parallel to the director, and is the dielectric permittivity of the isotropic phase. Experimentally, for rather high positive dielectric anisotropy of the nematic phase when E,,  qso= 10, and a typical value of AH, = 5 x I O4 erg cmP3,a shift of the order of 0.8 K is anticipated for a field strength of lo5 V cm' (about 300 CGS units). The shift of the firstorder NI transition is described theoretically with a Landau type expansion over two variables, orientational order parameter S , and polarization P [ 171. In the case of the electric field directed along the nematic optical axis the expansion is as follows: g= 1 a(TT:)S2
2
~
1 b S 3+ 1 cS4 3 4
+2px2o + O P 2 S + L2K P 2 S 2  P E
(8)
xo
where is the susceptibility of the isotropic phase, while parameters 0 and K represent the anisotropy of the susceptibility of the nematic phase. With this form of the free energy, as expected the shift of the transition is proportional to the square of the field, the coefficient a playing the role of the transition heat in Eq. (7):
The experimental investigation of the fieldinduced shift of the NI transition was carried out using a pulse technique [ 171, which allowed rather strong electric fields to be applied to samples. The data [ 171 are shown in Fig. 2 for two nematic cyanobiphenyls, 5CB and 6CB, that differ in
I
I
I
I
0.5
1
2
3
AT ("C} Figure 2. Change in the NI transition temperature with the electric field in ( I ) 5CB and (2) 6CB [ 171. A double logarithmic scale is used.
their latent heats of the NI transition ( I .5 x I O4 erg cm3 and 2.5 x 1O4 erg cm3 for 5CB and 6CB, respectively). The results are consistent with both the phenomenological approach (Eq. (8)) and microscopic theory [17], operating with the number density, and the magnitude, and direction of the molecular dipoles. At extremely high fields the isotropic phase should be indistinguishable from the nematic one, even well above the zero field transition temperature, since the uniaxial order induced by a magnetic or ac electric field in the isotropic phase will be comparable with the nematic orientational order. However, such fields are hardly accessible, even with the pulse technique. Much stronger changes in order parameter may be achieved with ferroelectric transitions (see below). For negative dielectric anisotropy of the nematic phase, E,< 0, the external field may induce a biaxial nematic phase. With increasing field one may reach the tricritical point 1181 where the firstorder NI transition becomes a secondorder one. AC", AG", C*G", and NC* Ferroelectric Transitions
For these transitions the electricfieldinduced shifts of transition temperatures are
9.2 Direct Influence of an Electric or Magnetic Field on Liquid Crystal Structure
379
linear functions of the field. The AC* transition may be either second or first order, while the AG* and C*G* transitions are first order [19, 201. Thus, to calculate the transition shift, we should compare the transition enthalpy with the linearinfield free energy term (Eq. (2)). The ClausiusClapeyron equation for solid ferroelectrics is well known: E / kV
(9) Here, APs is the difference in spontaneous polarization between the two phases under consideration. For the firstorder transition the coefficient b in the Landau expansion must be negative and a term of the sixth order in the tilt angle has to be included: g = 1 a. e2 ~
2
+p 2
+ 41 b e 4 + 61 ce6 

CPBPE
2x1
The coefficient c enters the expression for the shift in the transition temperature [19, 201 :
Experimentally, a field strength of the order of lo5 V cm' induces a AT value of the order of 1 K for a AHr of about 3 x lo5 erg ern?' KI and APs = 300 nC cm2. An example of the A T ( E )experimental dependence is shown in Fig. 3. Field dependence was also observed for the firstorder NC* transition temperature. For a field strength of about 2 x 1 O5 V cm' the phase transition point increased by 0.6 K [21]. For a compound with a much higher spontaneous polarization in the C* phase, approximately the same shift is induced by a field one order of magnitude lower [=I.
cm1
Figure 3. Electric field strength dependence for the C*G* phase transition (compound A7, [19]).
9.2.1.3 Weak FirstOrder Transitions N  A Transition The latent heat of this transition is usually small and may even vanish if the width of the nematic temperature range is sufficiently large [23]. Thus, the transition can be either of first or second order. For the secondorder transition the discontinuity in the orientational order parameter S and, hence, the dielectric (or diamagnetic) susceptibility, disappears and the field influence on both phases is the same. Thus we do not anticipate any fieldinduced shift in the NA transition temperature. For the weak firstorder transition there is a small discontinuity in both S and n, dielectric (and magnetic) susceptibilities, and the shift depends on the competition between two small quantities: the difference in susceptibilities for the nematic and smectic A phases on the one hand and transition enthalpy on the other. In particular, the field may induce a change in the phase transition order, from first to the second order, as shown in Fig. 4 [24].
Smectic A  C* Ferroelectric Transition This case has been analyzed in detail both theoretically and experimentally [25]. The
380
9
Behavior of Liquid Crystals in Electric and Magnetic Fields

N
200 L
c
d
Q
0.7
Q ,R 0.5

0.3
01
0.1
0.9
T"
I .o
Figure 4. Fieldinduced changes in order parameters for a smectic A liquid crystal. Q, orientational order parameter; curves a,, b,, and cQ show the temperature dependence of Q at various fields. R, order parameter describing the coupling of translational and orientational order, curves u R , b,, and C , show the temperature dependence of R. The field increases from curves a to curves c and results in a change in the NC transition from first to second order [24].
temperature dependence of the electric displacement D at various bias fields for the chiral compound C7 (I) is shown in Fig. 5. C2H50 (CH3)C" HC" H(C1) 
I The change in the AC* transition from first to second order can be clearly seen in Fig. 5 . The tricritical point corresponds to the following sets of parameters: Tc = 55.8"C (i.e. 0.8 K above the zerofield point), E, = 5 x lo4 V cm' and D, = 100 nC crnp2. A theoretical description of the experiment can be obtained using the same approach; that is, using the Landau expansion (Eq. (10)). Equation (10) has been solved numerically and the results of the calcula
0'
55.0 55.5 temperature
56.0
5
5
('0
Figure 5. Temperature dependence of the electric displacement of C7 (0 at various field strengths. E (in kV cm'): (a) 10, (b) 20, (c) 30, (d) 40, and (e) 50. (+) Increasing and (0) decreasing temperature runs
V.51.
tions are shown in Fig. 6, where the molecular tilt angle, which is the order parameter of the AC* transition, is given as a function of the external electric field for various temperatures. The parameters used to fit the experimental (Fig. 5 ) and theoretical (Fig. 6) curves were (in CGS units): a= 8 . 9 ~ 105ergcm3 K',b=1.3x107ergcm',c =6.6x107 erg cm', TO=51.4"C, x1=0.33, C = 2.9 x lo3 CGS (in [25] these parameters are given in SI units).
9.2.2 Influence of the Field on Order Parameters As the fieldinduced reorientation of the director occurs at rather weak fields, the geometries worth discussing here for nonpolar mesophases are: (i) the field parallel to the director and E,>O; and (ii) the field perpendicular to the director and &, *
I
I I 1
0.1.
;
I
,
,
,
*
I
,,, ,
,
0. When an electric field is applied to the BPI11 (foggy) phase with E,> 0, the broad selective reflection peak typical of this less ordered phase decreases in intensity and, at some threshold voltage, is replaced by a sharp peak at longer wavelength [43]. Thus, the transition to a new phase occurs. The symmetry of the new phase has not yet been established. For a system with E,
2(a2 )*
(a4
+ a5  a21 (a3 a 2 1
(35 a) (35 b)
for the splay and bend distortion, respectively. The effective viscosity for the splay dis
tortion changes by less than 1% and the bend distortion viscosity is smaller than K by 1020%; thus the corresponding transient process including the backflow effect is faster. Weak boundary anchoring increases both z, and 7., This is easily understood, if we remember that a finite anchoring energy W s results in an increase in the apparent thickness of the cell according (Eq. (28)). The classical results just discussed have been applied successfully to the determination of the elastic moduli K,, and Leslie's viscosity coefficients a, of conventional nematics. The experimental data may be found in books [3,8 lo]. The measurement of the director profile throughout the cell, including the surface layers, allows the anchoring energy to be calculated. The profile of the director distortion above the threshold of the Frederiks transition is shown in Fig. 1 1. The difference between curves I (Ws=m) and 2 (0 < W s< ) is a measure of the anchoring energy. The simplest estimate comes from the comparison of the magnetic field coherence length at the threshold field H, [66  681:
with the sum d + 2 b (Eq. (28)). When the applied field is much higher than the threshold of the Frederiks transition, the field coherence length becomes comparable with the surface extrapolation length itself b. This condition corresponds to the second threshold of the complete reorientation of a liquid crystal, including the surface layers (curve 3, Fig. 11). Thus, the second threshold field also allows b (and W s )to be calculated. The direction of the fieldinduced rotation of the director is, in principle, degenerate. The clockwise and anticlockwise directions are equally probable. Thus, domain
tH
9.3
Distortions due to Direct Interaction of a Field with the Director
389
1. 
walls appear, separating the two areas (domains) with different director orientations [69]. The wall movement influences the dynamics of the transition; the corresponding theory is presented in [70]. The Frederiks transition induced by an electric field has certain specific features not observed in the magnetic field equivalent. First, as the dielectric anisotropy is usually much higher than the magnetic one, the distortion leads to a spatial dependence of the dielectric susceptibility and a certain inhomogeneity in the electric field. Secondly, the character of the distortion may be affected by the electric conductivity and the influence of the flexoelectric effect. A discussion of these effects may be found in literature (e.g. [8, 91). More interesting features of the Frederiks transition are observed in the case of the simultaneous action of an electric and magnetic field. If a magnetic field is applied parallel to the nematic director n 11 H and ya> 0, it increases the apparent elastic coefficient by an additional quantity of y a H 2 d 2 / n 2 , which results in higher values of the corresponding threshold voltages. However, this is not the only result of applying a magnetic field [71]. If a stabilizing magnetic field is applied along the homogeneously or homeotropically oriented director and a destabilizing electric field is applied perpendicular or parallel to the substrate plane,
’
Figure 11. The geometry of the bend Frederiks transition (a) and the profile of the director deviation, induced by an external field (b). ( 1 ) H > H , , Ws=m; (2) H * > H > H , , o I w ~ I ~ ; (3) H > H * , o< wS Uth the period of domains w varies as w U’ (Fig. 16).

Flexoelectric Domains The flexoelectric term 6F i n nematic free energy
SFf =  [elE n divn  e3 E ( n x curln)] d z
”
(45)
may result in a twodimensional spatially periodic structure in the bulk. The application of an external dc electric field to a homogeneously oriented nonconductive nematic layer gives rise to a pattern of the domains parallel to the initial director orientation [ 1001. The period of the stripes w t h and the threshold voltage Uth of their appearance has been found [ 101 1031 by minimizing the free energy of the nematic in an electric field, taking into account the term given by Eq. (45). A detailed experimental study of the dependence of the threshold and period of the longitudinal domains on the dielectric anisotropy and other parameters of nematic liquid crystals [ 1041 has shown very good agreement between theory and experiment. The flexoelectric modulated structure
Figure 16. Flexoelectric domains in the nematic liquid crystal 4butyl4’methoxyazoxybenzene [ 1041: (a) U = 16 V, (b) U=25 V, (c) U = 5 0 V (&,=0.25, d = 11.7 pm). (d) Variation in the domain period for different ~ ~ v a l u e( s1 ): &,=0.25; (2) 0; (3) +0.15.
395
9.3 Distortions due to Direct Interaction of a Field with the Director
9.3.2 Twisted Nematics and Cholesterics 9.3.2.1 Twist and Supertwist Structures
Twist Effect If the directions x and y of the planar orientation of nematic liquid crystal molecules on opposite electrodes are perpendicular to each other and the material has a positive dielectric anisotropy, then when an electric field is applied along the z axis (Fig. 17) a director reorientation occurs which is a combination of the splay, bend, and pure torsional distortions [109]. In the absence of the field (Fig. 17a), the light polarization vector follows the director and, consequently, the structure rotates the light polarization vector through an angle n/2 [ 1 101. This specific waveguide regime (Mauguin's regime) occurs when the phase delay satisfies the condition An d / A% 1 .
I
t
Lo II
Ut,,,=z E ( 4 K l l + Cta
K332K22)
1'
(46)
When the applied voltage exceeds this threshold, the director deviates from the initial orientation so that the linear z dependence of the azimuthal angle disappears and the tilt angle becomes nonzero (Fig. 17b). The qualitative character of the functions @(z)and O(z)for different voltages is shown
Light
Light p (polarizer)
x
A 1 P (analyzer)
Bright
As in the case of the Frederiks transition (discussed in Section 9.3.1.1 of this Chapter), the theoretical interpretation of the twist effect is based on the minimization of the free energy of the system. In this case, however, the problem is two dimensional, since both the azimuthal angle @ ( z )and the tilt angle O(z) are considered to be dependent on the z coordinate. In the case of the infinitely strong anchoring, the threshold for the distortion includes all three elastic moduli of a nematic liquid crystal [ 11 11:
Electrode
Figure 17. Twisteffect. Left: below threshold; Right above threshold
396
9
Behavior of Liquid Crystals in Electric and Magnetic Fields
n/l
ni2
% Q
ni4
9^ 0
i
d
dl2
0
d
z
(4
(b)
Figure 18. Dependence of director angles $ ( z ) and 0 ( z ) in the twist effect for different voltages: (a) U z, where zd is the relaxation time of the director (Eq. (34)); the deviation angle decreases and the threshold voltage diverges [146]. The other flexoelectric structure can arise in a very thin planar cholesteric layer with a certain set of material parameters. The in
403
1
where u ( r )is the displacement of the smectic layers from their equilibrium position, and the z direction coincides with the normal to the layers. Thus, it makes sense to investigate the Frederiks transition in the geometry corresponding to the splay distortion only. Let us assume a socalled ‘bookshelf geometry’, in which the smectic layers
404
9 Behavior of Liquid Crystals in Electric and Magnetic Fields
are perpendicular to the substrates, forming a sandwichtype cell of thickness d, and the director is oriented in the plane of the cell (e.g. along the x axis). If the magnetic anisotropy is positive (y,>O) and a magnetic field is applied, the Frederiks transition should take place. The threshold for the transition coincides formally with that for a nematic (Eq. 27)); however, the amplitude of the distortion 6 , for fields exceeding the threshold is very small, being of the order of As/d [ 1491, where a smectic characteristic length
is of the order of few layer thicknesses. Thus, even in this, favorable case of the allowed splay distortion, the Frederiks transition is, in fact, unobservable (ghost transition). Instead, one observes a texture transition accompanied by the appearance of a number of defects.
Dielectrically Induced Texture Transitions Texture transitions are particularly pronounced when an electric field is applied to materials having a large dielectric anisotropy. A planar texture undergoes transition to a quasihomeotropic optically transparent texture via intermediate structural defects [ 150,1511. The threshold voltage observed experimentally for a transition from a planar to a homeotropic texture depends on the layer thickness according to U K d’ (for the Frederiks transition the threshold voltage is independent of thickness). A model that accounts for the experimental data (at least partly) has been developed by Parodi [ 1521 who assumed the formation of transition layers between the surface and the bulk of a sample. A discrepancy between the calculated and observed periods of the texture instability may be due to a nonuniform
‘chevron’ structure of the original ‘bookshelf’ geometry. Chevron structures with smectic layers broken by a certain angle are often observed in both smectic C and smectic A layers [1531. The kinetics of the relaxation of the homeotropic fieldinduced texture to a focal conic one depends on the surface treatment [ 154 1561. A rough surface which provides a strong anchorage facilitates relaxation [ 1561.
Frederiks Transition in a Smectic C Phase Depending on the arrangement of the smectic layers and the director of the liquid crystal relative to the limiting surfaces, four different configurations can be identified. For each of them there are at least three alternatives for the direction of the field. Thus, 12 variations in all can be obtained and these have been studied theoretically by Rapini [149]. In most of the configurations the Frederiks transition is a ghost one, since it requires the collapse of the smectic layers. However, in three instances [ 1571 the field only induces rotation of the director around the normal to the layers, leaving the layer structure unchanged. Let us identify the three principal values of the dielectric permittivity as E~ ( i = 1, 2, 3 ) , where E~ corresponds to the direction along the director, corresponds to the direction perpendicular to the plane of the tilt, and eZ corresponds to the direction perpendicular to the preceding two [8, 91. When the field is oriented along the director, a Frederiks transition is possible when E~ > E ~ The director should rotate around the normal to smectic layers, not changing its angle The corresponding threshold field is proportional to ( E ~ E&+. A field perpendicular to the director and lying in the plane of the tilt induces the same distortion when E~ > E ~ Now . the threshold for reorientation
a.
.
9.3 Distortions due to Direct Interaction of a Field with the Director
of the director is proportional to ( E ~  E , )  ~ . Finally, when the field is perpendicular to the tilt plane the same rotation takes place at threshold proportional to ( E , cos2B + E~ sin2sz  ~ ~ 1  i . Measurements have been made of the Frederiks transition in various smectic C liquid crystals [ 158 1611, using the conventional sandwich cells and optically transparent electrodes. The director was oriented uniaxially by rubbing the electrodes, and the smectic layers were tilted with respect to the cell plane (a ‘bookshelf’ geometry). Due to positive dielectric anisotropy, an electric field applied along the cell normal ( z direction) (Fig. 22) induces director rotation around the normal to the smectic layers. The threshold field for the director deviation can be calculated neglecting the distortion of the smectic layers [158] and assuming &* = E ~The . threshold depends on the angle p between the normal and xy plane. For p=O, when the xy plane cuts half of the director cone (with an angle B at the apex) the threshold field is
where K* is an effective elastic constant. When the cone just touches the xz plane
405
(p=B)(Fig. 22), the threshold field increases proportionally to cos 0.Both such cases have been studied using various substances [ 1591611. For a certain set of parameters, the theory predicts a bistable behavior of the smectic C phase in a strong field. Such bistability has been observed in the form of the fieldinduced motion of domain walls, accompanied by a hysteresis in the process of the director reorientation. The walls appear due to the equally probable fieldinduced rotation of the director clockwise and anticlockwise, and separate the two areas of different director orientation. In the absence of walls the dynamic behavior may be described, as in nematics, by adding a viscous torque to the elastic and electric ones. For the fieldoff state, the distortion decays with the ‘nematic’ time constant (see Eq. (34), where K* should be substituted for K22).The time of the response to an electric field can only be calculated for the simplest case when p=0, T,= yl/ &,sin2R(E2Ez), where E , is defined by Eq. (69). Thus, the response of the smectic C phase is sin2R times slower than that of the nematic phase. However, in experiments the same substance often responds faster in the smectic C phase than in the nematic one [1591611. This may be due to the smaller value of y, when the motion of the director is confined by the cone surface. The same phenomenon has been observed for the ferroelectric smectic C phase [ 1621. The domainwall motion makes the dynamics of switching more complicated; the fieldinduced wall velocity has been calculated by Schiller et al. [70]. Frederiks Transition in the Hexagonal Smectic I Phase
Figure 22. Geometry of the Frederiks transition for a planaroriented smectic C liquid crystal.
Frederiks transition in the hexagonal smectic I phase (and also in the smectic C phase with a weak hexagonal order [1631) has
406
9 Behavior of Liquid Crystals in Electric and Magnetic Fields
some specific features. In the smectic I phase the director n forms a fixed angle 8 with respect to the smectic layer normal. The lines between the centers of gravity of neighbouring molecules within a smectic layer form a hexagonal structure and the director is oriented toward one of the six vertices of the hexagon. Thus a fieldinduced reorientation of the director is accompanied by a reorientation of the bond direction. The latter requires some additional energy, which must be added to the elastic term in the free energy expansion. The calculations of the threshold electric voltage for the Frederiks transition from a ‘bookshelf’ geometry 11641 show that it may be presented in the form
Cr;=U;[l+f(K,L,G,h,d)]
(70)
where Uc is the ‘smectic C threshold voltage’ from Eq. (69); K , L, and G are elastic moduli related to the director, bond reorientation, and the coupling between the two; h is a constant related to the constraint on the director to be along one of the six preferred directions due to the hexagonal order; and d is the cell thickness. Thus, the threshold voltage for a smectic I phase, is in contrast to nematic and smectic C phases, thickness dependent.
The other group of polar materials comprises mirrorsymmetric (achiral) phases of point symmetry groups from C2,, to C,,,. Examples of these are many classical solid crystalline ferroelectrics, such as BaTiO, triglycinsulfate, and thiourea. Recently polar properties (probably antiferroelectric) have also been observed in a noncrystalline (mesomorphic) achiral molecular material [165,166]. The basic idea was to use the polyphilic effect to form ‘building elements’ of a polar phase. According to this concept, chemically different moieties of a molecule tend to segregate to form polar aggregates or lamellas which result in the formation of polar phases. The direction of the spontaneous polarization is allowed to be in the plane of the lamellas or layers (transverse ferro or antiferroelectric) or perpendicular to the layers (longitudinal ferro or antiferroelectric [ 1671). In the particular case by Tournilhac et al. 1165,1661, field reversible piezoelectric and pyroelectric effects were observed in a tilted, highly disordered metastable phase [168] of a polyphilic compound.
9.3.3.2 Chiral Ferroelectrics and Antiferroelectrics In 1975, the first ferroelectric liquid crystal (FLC), called DOBAMBC (111),
Polar Achiral Polyphilics Polar crystalline and mesomorphic phases are divided into two groups according to their symmetry. One group is composed of chiral molecules having point group symmetries ranging from C , to C,. Examples of this type are liquid crystalline chiral phases (smectic C*, discussed in Section 9.3.3.2 of this Chapter, F*, I*, etc.) differing in the character of the inplane packing of their molecules within a smectic layer. These ferroelectric phases manifest reversible switching of their spontaneous polarization.
was synthesized 11691. Since then FLCs have been the object of intensive investigation. A contemporary version of the general phenomenological theory, including the dynamic behavior, can be found in various books [7, 1701. Many experimental results and the discussion of FLC parameters may be found in other publications [8, 9, 171, 1721 and in the other chapters of this book.
9.3
Distortions due to Direct Interaction of a Field with the Director
407
A comprehensive review devoted to antiferroelectric liquid crystals has also been published [ 1731.Thus, for the sake of completeness, only the field effects of fundamental importance are discussed here. Smectic C* Phase Ferroelectrics The symmetry of the ferroelectric smectic C* phase corresponds to the polar point group C2. When proceeding along the z coordinate perpendicular to the smectic layers, the director n and the polarization vector P directed along the C, axis rotate; that is, a helix of pitch h is formed. In the presence of an external field the total free energy includes the elastic energy of director deformations F d , the surface energy F,, and energy FE of the interaction of a ferroelectric phase with the field E :
F = Fd + F ,
+ FE = j g d dT+JW, d o V
s
+ Vj [  P E  E ) d T In general, the elastic term includes the elasticity related to the reorientation of the director (nematic moduli K J , and to a change in the tilt angle (coefficients a , b, c, etc., of the Landau expansion; see e.g. Eq. (10)). The corresponding expression for gd is very complex and may be found in Pikin [7]. The surface energy includes both the dispersion and the polar terms of the anchoring energy Ws.Below we consider a few rather simple cases. The ClarkLagerwall Effect. This effect is observed in thin surfacestabilized FLC (SSFLC) cells where the smectic layers are perpendicular to the substrates, the thickness is less than the helical pitch ( d l h ) ,and the helix is unwound by the walls [ 174 1761 (Fig. 23). The electric field of opposite polarity switches the direction of the spontaneous polarization between the UP and
Figure 23. The ClarkLagerwall effect. In a thin SSFLC cell the electric field of opposite polarity switches the spontaneous polarization between the UP and DOWN positions, which correspond to the LEFT and RIGHT positions of the director.
DOWN positions which correspond to the LEFT and RIGHT positions for the director that moves along the surface of a cone, the axis of which is normal to the layers and parallel to the cell substrates. In the LEFT and RIGHT positions the director remains parallel to the substrates and the SSFLC cell behaves as a uniaxial phase plate. The total angle of switching equals the double tilt angle 13. The variation in the azimuthal director angle @ in the ClarkLagerwall effect is described by the equation for the torque equilibrium, which follows from the minimization of the free energy (Eq. 71):
a@
y,,, = K at
a2@+ P, E sin@ ax &
+L E 2 sin@cos@
4n
where the FLC is assumed to be uniaxial and y,,, is the viscosity related to the motion of the director along the cone surface mentioned. When the helix is unwound by the cell walls, the first term on the lefthand side vanishes.
408
9
Behavior of Liquid Crystals in Electric and Magnetic Fields
The polar Wp and dispersion Wd surface terms are included in the boundary conditions:
For polarizations P greater than 10 nC/ cm2, driving fields E less than 10 V pm', and dielectric anisotropies I &,I less than 1 we have
1 &I,
E/4z Q P
(74)
and, consequently, the third term on the righthand side of Eq. (72) may be omitted. For I I = 0 and infinitely strong anchoring there is a threshold for the switching of a SSFLC cell [ 1771
(75) Here the elastic modulus Kis defined in such a way that it includes O2 (see e.g. [7]). In the absence of backflow and at not very high voltages, the response times in the ClarkLagerwall effect are determined by
The backflow effect may decrease the response time severalfold [177]. If the inequality given by Eq. (74) is invalid, as occurs for sufficiently high fields, the response times of the ClarkLagerwall effect increase sharply for positive E, values. Conversely, for negative values of E,, the corresponding switching times become shorter [ 178, 1791. For I E, I E/4 Z SP the FLC switching times are approximately governed by the field squared, as in the Frederiks effect in nematic phases. For weak anchoring conditions, two regimes of switching exist in SSFLC cells, separated by threshold field E,, [ 1801:
(77)
For E <E,, one observes the motion of domain walls, separating the regions of differently oriented polarization P and P. The switching time is defined by the domainwall motion. If E >E,, (the ClarkLagerwall regime), the switching time is determined by Eq. (76). At certain pretilt angles at the boundaries and high applied voltages, the switching may have the character of solitons or kinks in the function @ ( z )spreading from one electrode to the other [ 1811. Deformed Helix Ferroelectric Effect. The deformed helix ferroelectric (DHF) effect observed in shortpitch FLCs [139, 182, 1831 is a particular case of a more general phenomenon of the fieldinduced helix distortion observed in the very first investigations of FLCs [169, 1841. A theoretical explanation of the effect is given by Ostrovskii and coworkers [ 185 1871. The geometry of a FLC cell with the DHF effect is presented in Fig. 24. The polarizer at the first substrate makes an angle p with the helix axis and the analyzer is crossed with the polarizer. The FLC layers are perpendicular to the substrates and the layer thickness d is much larger than the helix pitch h,. A light beam passes through an aperture a s h , , parallel to the FLC layers, through the FLC cell. In an electric field M the FLC helical structure becomes deformed, so that the corresponding dependence of the director distribution cos@as a function of coordinate 2 m l h , oscillates between the two plots shown. These oscillations result in a variation in the effective refractive index (i.e. an electrically controlled birefringence appears). The effect takes place up to strengths sufficient to unwind the FLC helix
E, =
r2 K q i 16 P,
Here the elastic modulus K is defined as for Eq. (75).
9.3 Distortions due to Direct Interaction of a Field with the Director
This means that for E = E , it is possible to establish the memory state. If the helix is weakly distorted, fast and reversible switching could be obtained in the DHF mode [188]. Electroclinic Effect Near the Smectic ASmectic C* Phase Transition. The electric field may induce a tilt of the director in the orthogonal smectic A phase near the smectic Asmectic C* phase transition (electroclinic effect [ 189, 1911). The electroclinic effect may be understood within framework of the Landau phase transition theory [7]. If the dielectric anisotropy is negligible, the free energy density of the smectic A phase may be expanded over the fieldinduced tilt angle 8:
Light beam
I
+
I
I
409
'
"?+/)..
. .. . . . . . . . . . . .
.
. :. . . . . . . . . . . . . . .. . Analyzer
I
t
R = Iu %
2
+ Ib e 4
+p 2
p L p P %  P E (80)
2x1
xI
9
where a=a(TT,), b>O, is the background (far from the transition) contribution to the dielectric susceptibility, and & is the tiltpolarization coupling constant (piezocoefficient). Under the assumption that b = 0, the minimization of g with respect to 8 and the polarization P results in the fielddependent tilt angle:
'
VI
&
Figure 24. The deformed helix ferroelectric effect.
The characteristic response times of the effect at low fields E/E,G 1 are independent of FLC polarization Ps and field E and are defined only by the rotational viscosity ye and the helix pitch h,: (79) For E close to the unwinding field E,, the pitch h increases sharply to h s h , . Consequently, the helix relaxation times Z, to the initial state also increase: Z,/Z,X h 2/ h2o .
The coefficient e, is known as the electroclinic coefficient. According to Eq. (8 l ) , the electroclinic coefficient becomes infinite at T=T, (in fact, it is limited by the term b 84 ~141). The dynamics of the electroclinic effect are, in fact, the same as the dynamics of the ferroelectric soft mode. The switching time may be derived from the equation for the balance of the viscous, elastic, and electric torques:
ye
ae
1a (T  T,) 8
at
+ /+, xi E
(82)
410
9 Behavior of Liquid Crystals in Electric and Magnetic Fields
It follows from Eq. (82) that the switching time of the electroclinic effect is independent of the electric field, and is defined only by the tilt rotational viscosity ye and the elastic modulus a:
The experimental data confirm the linear increase in the tilt angle with increasing E for the electroclinic effect and independence z, of E [ 1901 (Fig. 25). The switching time re may be calculated more precisely if the fourthorder term in b e 4 is taken into account. In this case, a decrease in z, for larger electric fields is observed [192]. At present, the electroclinic effect is the fastest of the known electrooptical effects in liquid crystals. Domain Mode. A remarkable domain structure has recently been observed in FLCs possessing high spontaneous polarization (>lo0 nC cmI) [1931951. A very stable spatially periodic optical pattern arises in layers of FLCs with their molecules oriented parallel to the substrates after a dc field treatment of the cell. The stripes are oriented perpendicular to the director orientation and their period is inversely proportional to the polarization magnitude squared, and independent of cell thickness.
The optical pattern may be observed for several months after switching off the dc field. The theoretical model is based on the consideration of a stabilizing role of the structural defects (dislocations) interacting with free charges in a FLC layer. The tilted layer structure responsible for such defects has been observed by direct Xray investigation. The fieldoff domain structure has also been observed after the application of the electric field to the smectic A phase of a ferroelectric substance with very high spontaneous polarization [ 1961. The phenomenon is assumed to arise due to a break in the smectic layers (very similar to that just mentioned) induced by a strong electroclinic effect. Ferroelectric Liquid Crystal Polymers. The symmetry requirements necessary for ferroelectricity in lowmolecularmass compounds are also valid for polymer mesophases. If a tilted chiral smectic phase is stable after a polymerization process, it must be ferroelectric. Following this idea the first polymeric liquid crystalline ferroelectric was synthesized by Shibayev et al. [ 1971. The substance is a comblike homopolymer (ZV) y
3
CCCH2f
CH3
COO (CH2)ro
. ,0 . o o o 0g
ACzH~
IV
9 ' 21 I 60
10.2
d 40
20
0
20
I
40
60
E (Vlw)
Figure 25. Dependence of the tilt angle 8 and the response time z, on the electroclinic effect in a FLC cell (T=25"C) [190].
with a polymethacrylate chain as a backbone and flexible spacers, COO(CH2),,C00, separating the phenylbenzoate mesogenic units from the backbone. Transverse (with respect to mesogenic units) dipole moments provided by several COO groups are weakly coupled to the chiral terminal fragment, and thus the spontaneous polarization of the substance is small. Later, a variety of comblike and main chain polymers manifesting
41 1
9.3 Distortions due to Direct Interaction of a Field with the Director
chiral smectic C*, F*, and other phases were synthesized (for reviews see [ 13, 1981). The field behavior of polymer ferroelectric liquid crystals is very similar to that typical of lowmolecularmass compounds. In general, all processes are very slow due to the high viscosity of polymer materials. An interesting feature of the polymers is their ability to form, on cooling, a glassy state with a frozen spontaneous polarization. Such solid materials have pyroelectric and piezoelectric properties.
Antiferroelectrics A possibility of the antiferroelectric behavior of low temperature, highly ordered, chiral phases and the herringbone packing of smectic layers with an alternating tilt of the director was first discussed in connection with their very strong fieldinduced pyroelectric response [199]. In such a structure the direction of the inplane polarization also alternates and the whole structure is antiferroelectric. The characteristic switching time in such phases is very long (seconds). The slowly switchable smectic X phase [200] appears to belong to the same family of antiferroelectrics. A rather fast tristable switching typical of solid antiferroelectrics has recently been reported [2012041 for chiral liquid crystalline phases of MHPOBC
In fact, MHPOBC shows a very rich polymorphism [208]: S m I i  64°C  S m C i  118.4"C SmCi  119.2"C  SmC * 120.9"C SmCi  122°C  SmA  148°C  I where S m C i and SmCg are antiferroelectric phases, SmC* is a typical ferroelectric phase (discussed in the previous section), and SmC; is a ferrielectric phase. On a macroscopic scale the phases are twisted, with a characteristic pitch depending on temperature. Antiferroelectric phases have been observed in many other compounds, including polymers [209], and have been investigated in detail (for a review see e.g. t 1731). The application of an electric field has a considerable effect on the phase transition points in MHPOBC [210]; the phase diagram (electric field versus temperature) is shown in Fig. 26. A very narrow lowtemperature ferrielectric phase is seen (FIL) between the S m C i and SmC; phases mentioned earlier. In addition, even a weak field strongly influences the boundary between the SmC; and SmC* phases. Further inves
(V).
co~~H(cH~)c,H,,
V A third, fieldoff, state, in addition to the two stable states known for the ClarkLagerwall effect, has also been shown to be stable, and a layered structure with alternating tilt has been established by optical [205, 2061 and scanning tunneling microscopy [207] techniques.
117
118
119
120
121
122
123
124
T(" c) Figure 26. Electric field versus temperature phase diagram of MHPOBC [210].
412
9 Behavior of Liquid Crystals in Electric and Magnetic Fields
tigations have shown [211] that the fieldinduced transition between the two phases in MHPBOC involves the formation of a variety of ferrielectric configurations. An even richer fieldinduced polymorphism has been observed in binary mixtures of MHPOBC and MHPOCBC [210]. A typical double hysteresis loop for electrooptical switching of the antiferroelectric SmCz phase is shown in Fig. 27. There are two fieldinduced uniform states and a zerofield third state which may be either uniformor twisted [212]. The transition from the antiferroelectric to the ferroelectric state proceeds through intermediate ferrielectric states. With increasing frequency in the range 10100 Hz, the double hysteresis loop gradually transforms into the conventional ferroelectric loop [213]. The characteristic time corresponds to the time of the formation of domains of the antiferroelectric phase. The lowfrequency switching (0.2 Hz) of the SmC; phase reveals a triple hysteresis loop with two intermediate (+ and ) ferrielectric states and two final ferroelectric states. At higher frequency, conventional ferroelectric switching is observed.
Applied Voltage / V
Figure 27. A double hysteresis loop typical of the electrooptical switching of the antiferroelectric phase [212].
Chiral Lyotropics and Discotics Lyotropic Systems. Water solutions of certain amiphiphilic molecules (e.g. lipids) form lamellar lyotropic phases with a tilt of molecules to the layer normal. When the same molecules are chiral or other chiral molecules (guests) are introduced into the lamellas (host), the lamellar phase satisfies all the symmetry requirements of a ferroelectic phase (in formal analogy to SmC"). One of the best chiral additives to be introduced in lyotropic phases is cholesterol, which induces rather high spontaneous polarization in thermotropic SmC matrices [214]. In the L' phase, where matrix molecules are tilted, the chiral mixture (ethylene glycol doped with cholesterol) manifests a one order of magnitude higher piezo response than the undoped mixture. An even more striking difference between the undoped and doped samples (two orders of magnitude) is observed when a dc poling field is applied [215]. With increasing concentration of the dopant the piezo response grows. A dramatic difference between the piezo response of the undoped and the cholesterol doped samples has also been observed for water solutions [216]. Certainly the electric behavior of chiral analogs of the lyotropic phases is much more pronounced than that of their achiral counterparts and, therefore, cholesterol induces ferroelectricity in both systems studied (based on ethylene glycol and water). Discotic Ferroelectrics. Columnar mesophases with chiral diskshaped molecules whose normals are tilted with respect to the column axis also manifest ferroelectric switching [217]. In such phases the direction of the spontaneous polarization is perpendicular to both the column axis and to the normal to the molecular disks. The tilt of the disk forms a helix with its axis oriented along the columns. In an amphiphilic
9.4
pyrene derivative, the positive and negative voltages rotate the direction of the minimum refractive index (which is perpendicular to the column axis) through a certain angle (about +20") clockwise or anticlockwise, respectively. The other homolog from the same series shows a fieldinduced change in the structure of the phase with an increase in the spontaneous polarization from 60 to 180 nC cmP2 [218]. The two phases are thought to have different sublattices of elliptic and polar columns. The switching times vary over a very broad range (from 1 ms to 100 s), being strongly dependent on the field (as z x K 4 ) and temperature. The lowfield phase is switched five times faster than its highfield counterpart. The columnar phases have some advantages over ferroelectric smectics (e.g. they are shock resistant) [218].
9.4 Electrohydrodynamic Instabilities In this section we discuss electrohydrodynamic (EHD) instabilities, that is electricfieldinduced phenomena that are caused by the flow of a liquid crystal (see also [8,219]. The reason for the flow is electrical conductivity, which has been disregarded in previous sections. The flow may arise either independently of the anisotropic properties of substance, as in isotropic liquids (isotropic modes of the electrohydrodynamic instability), or may be driven by the conductivity anisotropy, as in liquid crystals (anisotropic modes). The threshold for EHD instabilities depends on many parameters, such as the electrical and viscoelastic properties of substance, the temperature, and the applied field frequency. Due to flow distortion of the director alignment, the instability is usually accompanied by a characteristic optical
Electrohydrodynamic Instabilities
413
pattern that depends on optical anisotropy of substance. This pattern formation is a special branch of physics dealing with the nonlinear response of dissipative media to external fields, and liquid crystals are well accepted model objects for the investigation of such phenomena [220]. To date, the most important results on EHD instabilities have been obtained for nematic liquid crystals (for a review see e.g. [221]).
9.4.1 Nematics 9.4.1.1
Classification of Instabilities
Electrohydrodynamic instabilities in nematics may be classified according to their threshold voltage (or field) dependence on .the physical parameters of the liquid crystal (cell geometry, field frequency, etc.). The most important case for which all the typical instabilities may be observed is a planar cell with homogeneously oriented director. Instabilities in cells with homeotropic or tilted molecular orientations have some specific features, but the general mechanisms are the same. A qualitative phase diagram (the threshold voltage versus the frequency of the applied ac field) for different electrohydrodynamic instabilities in homogeneously oriented liquid crystals is shown in Fig. 28. Among the instabilities shown there are two isotropic modes. One of these is well known from experiments on isotropic liquids and occurs at very low frequencies due to some injection processes at electrodes (injection mode). The other is also observable in ordinary liquids (such as silicon oil), but is seen particularly clearly in nematics, due to their optical anisotropy. The latter mode occurs over a wide frequency range due to ion drift to the electrodes as in electrolysis (electrolytic mode). Both isotropic
414
9
Behavior of Liquid Crystals in Electric and Magnetic Fields
J
+
rl
P 0 rl
.0 c 0
A c
Low f r e 
isotropic q u e w
mde ( i n j e c t i o n mode)
c
Frequency
EHD instabilities are driven by the electriccurrentinduced flow, even at zero conductivity anisotropy. The other two instabilities shown in Fig. 28 may be observed only in liquid crystals (nematic, cholesteric, and smectic C). The first is the CarrHelfrich instability, which is caused by a lowfrequency electric field and occurs in the form of elongated vortices with their axis perpendicular to the original director alignment. The vortices cause a distortion of the director orientation, which is observed optically as a onedimensional periodic pattern (KapustinWilliams domains). The other anisotropic mode is observed only in highly conductive liquid crystals. For its interpretation the inertial term avlat for the fluid velocity must be taken into account, which is why this mode may be called inertial mode. The different modes may interfere with each other, even near their thresholds, and a variety of patterns may be observed. For example, ‘chevrons’ occur due to interference between the electrolytic and inertial modes, and a transient periodic pattern due to backflow effects accompanies the Frederiks transition. Well above the threshold, when the induced distortion is nonlinear with the applied field, many other patterns
Figure 28. Threshold voltage as a function of frequency for different electrohydrodynamic instabilities in homogeneously oriented nematics.
are observed, including travelling waves or periodically pulsing modes [221]. The most important EHD instabilities are discussed below.
9.4.1.2
Isotropic Modes
Nematic liquid crystals are weak electrolytes containing a certain amount of ions. The ions may be intrinsic or created by an external electric field, which favors the dissociation of neutral molecules (chemical degradation). They may also appear as a result of electrochemical reactions at electrodes due to the injection of additional charge carriers. In some cases, the appearance of EHD instabilities in the nematic phase does not correlate with such inherent liquid crystalline properties as dielectric E, or conductivity 0,anisotropy. The only physical reason for these instabilities might be a nonuniform ion distribution along the direction z parallel to electric field. Standard Equations
To describe the fieldinduced motion of a liquid, a set of fundamental equations should be written which may be solved under certain assumptions. The first is the equation of motion in the Euler form:
9.4
+ (UV)u = f
@!

P where p is the density of the liquid, u is its velocity, t is time, and f is the force per unit volume, which includes the pressure gradient (gradp), the gravity force pg, the electric forcef,, and forces due to viscous friction fvisc that depend on the fluid velocity v: at
f =gradp+pg+fE
+fvisc
(85)
The second equation to be taken into consideration is the equation for the conservation of mass (or the continuity of liquid):
aP + divpv = 0

Electrohydrodynamic Instabilities
415
length of an experiment). Then, the second term on the lefthand side of the Eq. (90) vanishes and we get a new form:
Even now there remain serious problems to be solved. In fact the charge density Q (r,t ) in Eqs (87) and (91) depends not only on the external field but also on the velocity of charged fluid. Thus, Eqs (89) and (91) have to be complemented by an equation for the conservation of charge (continuity of the electric current): "Q+div J = O
at
at
The force exerted on the liquid by an external field is due, in the simplest case, to the space charge of density Q:
fE=QE
(87)
In the case of a space and time dependent force f, Eqs (84)(87) have no general solution and the problem must be simplified. For example, we may ignore the gravity force and the pressure gradient and, in addition, consider the fluid to be incompressible (i.e. p=constant). Then the friction force is written simply as [222]:
where q is the viscosity coefficient, and Eqs (84), (86), and (87) take the form of the flow continuity equation divv = 0
(89)
and the NavierStokes equation
+ (UV)v = q v2v+ f E
av at
~

P
P As before, Eq. (90) is nonlinear and has a simple solution only for low fluid velocities when the Reynolds number is small (Re = p vllq Q 1, where 1 is a characteristic
where J is the current density, which includes the ohmic term, the convective term due to the charge transfer by the moving liquid, and the diffusion term due to the gradient of the charge carrier density:
J
= 0 E + Jc,,,
+ Jdiff
(93)
Finally, there is a coupling between the charge and the electric field strength given by Maxwell's equation: 47~ Q divE = ___ &
(94)
Equations (89)(94) govern the behavior of an isotropic liquid in an electric field. For very weak fields the liquid is conducting but immobile. With increasing field a nonuniform spatial distribution of Q and E arises due to an ion drift to electrodes orland charge injection, and the liquid starts moving in order to satisfy the minimum of entropy production. The corresponding critical field Ecritis considered to be the threshold field for the appearance of an EHD instability. Below we discuss the two particular cases mentioned earlier, namely the injection mode and the electrolytic mode.
416
9
Behavior of Liquid Crystals in Electric and Magnetic Fields
Injection Mode
where
Let us consider a plane sandwich cell into which the cathode injects electrons that negatively charge neutral molecules. Due to an excess negative charge density Q(z> near the cathode, a force Q E is directed to the anode and tries to shift the charged layer of a liquid to the right (Fig. 29a). Since the cell is sealed and the liquid is incompressible, a circular convective flow occurs in order to reduce the internal pressure (Fig. 29b, c). This case resembles the wellknown Benard problem in the thermoconvection of liquids. The threshold of the instability may be estimated from Eqs (89)(94). For simplicity, consider the onedimensional case when the z component of the velocity is harmonically dependent on the transverse x coordinate:
z,=P d 2
(97) 77 r2 is a characteristic time for the relaxation of a vortex with diameter d. In the continuity equation (Eq. (92)) we leave only the ohmic and convective terms:
uz(x)= u, cos7T x
is the Maxwell time for the space charge relaxation. The convective term in the current obeys the equation:
d
(95)
The halfperiod of the cosine wave is assumed to be equal to the vortex diameter, that is to the cell thickness d. Differentiating Eq. (95) twice and substituting the result into Eq. (91) we get
Vortex
J=uE+Qu
(98)
When calculating div J it should be borne in mind that electrical conductivity results mainly in the relaxation of the space charge inhomogeneities along the x coordinate and E, may be considered to be uniform. Thus,
where ZQ =
&
4x0
where v, is assumed to be constant and a is the gradient of the injected charge density. Therefore, the current continuity equation
Figure 29. EHD instability caused by the injection rnechanism. (a) Distribution of the injected charge at voltages below the threshold for convection. (b) Change in the charge distribution due to convection. (c) Cylindrical convective vortices.
9.4
(Eq. (92)) becomes
aQ +  + a aQv , = O at
ZQ
and we have a pair of equations (Eqs (96) and (102)) completely analogous to the set describing the thermoconvective instability [223 2251. To calculate the critical field for the injection instability it is assumed that,precisely at the threshold, the time dependences v7 (t) and Q (t) are described by an exponential growth function exp(st) with s=O, which means that at the threshold the velocity and charge density neither increase nor decay. This is a general principle and is called the “exchange of stability” (see e.g. [226]). Calculating the determinant for the set of linear equations (Eqs (96) and ( 102)) we obtain the critical field for any given injection strength a:
E crit. =  P
a Z , ZQ
= ~ 4n3ro a&d2
(1 03)
Finally, assuming a linear space charge distribution along the normal to the cell, a= c?Q/dz =: Qo/d, and introducing the ion mobility p = o/Q,,,we arrive at the threshold voltage independent of the cell thickness in the form
This differs from the more rigorous theoretical expressions only by the use of a numerical coefficient [202, 2031. For typical parameters of a dielectric liquid ( q =: 1 P, p = lop5cmP2V’ sfl and E =: lo), Ucrit= 1 V. However, in some cases (e.g. for conductive liquids) T may be as high as 100, or even more [227, 2281. Experimentally, in thin nematic liquid crystal cells, the critical voltage is of the order of few volts. The instability appears at a dc field or at very low frequencies (Fig. 28). The optical pattern
417
Electrohydrodynamic Instabilities
depends on the geometry of the experiment; in the isotropic phase the fluid motion may be observed using a strioscopic technique [229], or by following the motion of foreign particles. In nematics the areas of strong velocity gradients are easily visualized under a polarizing microscope due to the director distortion by shear. For example, in planarly oriented nematics an optical pattern in the form of beans is observed [230, 2311. Electrolytic Mode The other important ‘isotropic’ instability is the socalled electrolytic mode [232, 2331. It appears in any fluid phase (isotropic, nematic, cholesteric, smectic A) within a wide frequency range in the form of small vortices near cell electrodes. The reason for the instability is a nonuniform space charge distribution (Fig. 30) due to an electrolytic process in the bulk of the substance (positive and negative ionic charges are separated during the period of the applied external ac field and move to opposite electrodes). The vortices are seen under a microscope in the form of small linear prechevron domains (in homogeneously oriented nematics), Maltese crosses (homeotropic orientation) and more complicated structures (cholesterics and nematics with a shortrange smectic order). However, when there is no coupling between the flow and the diz
1.1
vortex
E
Ibl
Figure 30. Electrolytic EHD mode. (a) Distribution of the density of positive ( Q + ) and negative ( Q  ) charges during one period of the applied ac field. (b) Vortex motion of the fluid near the electrodes.
418
Behavior of' Liquid Crystals in Electric and Magnetic Fields
9
rector (the isotropic and smectic A phases) the vortices may be observed only by using foreign floating particles. The instability has a welldefined field (not voltage) threshold that is dependent on the frequency of the applied field according to E 0~ w*. To calculate the threshold it is assumed [7] that the charge density gradient along the layer thickness obeys the law:
x
where is the electrokinetic coefficient, which may be evaluated using the Maxwell equation:
x=
r,.P
2
9x

(109)
77 ( 9 + 4 2 ) 2 Now the vortex has dimensions wx=n/ql and w,= L , = nlq, along the x and z axes, respectively. The latter depends explicitly on the field frequency (see Eq. (108)). The threshold field Ecrit may be found using Eqs (96) and (102) and the same procedure described as earlier. For a square wave excitation with frequency f and amplitude E the different expressions are obtained in two frequency ranges: At low frequencies, w 9 4 n (TIE,
&
4 n Lh
and at high frequencies, ~ $ n4(TIE,
Here L , is a characteristic (Debye) length where the space charge is concentrated: LD
The only difference is in the characteristic relaxation time for a hydrodynamic vortex:
=(g) I 2
where D is an ion diffusion coefficient. When the frequency w of the applied field is increased, the ions do not have time to overcome the gap between the electrodes and concentrate in more extended regions of thickness r

7
I
Thus, the electrohydrodynamic instability appears in regions near the electrodes and vortices have a characteristic dimension L,, which is smaller than the gap between electrodes. Using the same current continuity equation (Eq. (98)) we arrive at the same set of equations (Eqs (96) and (102)) for small amplitudes of velocity v and space charge Q.
1
Ecrit= B
(y)'
where A and B are numerical constants (given in [233, 2341). The characteristic size of the vortices at the threshold wcrithas also been found. The thresholds for the formation of vortices in silicone oil, carbon tetrachloride, acetone, and in the isotropic phase of MBBA have been measured [232,233] and it was shown that Ucrit=wi and that the threshold decreases with decreasing viscosity. More detailed measurements of the dependences Ucrit(w) in pure and doped MBBA at various temperatures (for sandwich cells) have also been made. The threshold for the vortex motion was taken as the onset of the circulation of the solid particles in the electrode plane. The shape of the Ucrit(0) curves depends on the electrical conductivity. For high electrical conductivity the curves have a plateau proportional to (T in the lowfrequency region and a char
9.4
acteristic dependence Ucrit0~ wf independent of O, and, in turn, in an accumulation of the space charge around extremum points
(8,=0) of the director distribution (Fig. 32a). The x component of the current is J,
Ex +oaE 8
(1 13)
where the new component of the electric field E, is related to the space charge distribution Q ( x ) and the director angle O(x) by Maxwell’s relationships (divD=O, divJ=O):
Substituting 8 from Eq. (1 12) into Eqs (1 14) and ( I 15) we have for the space charge distribution:
9.4
At a certain critical voltage the destabilizing viscous torque M,, which comes from the interaction of the space charge with an external field, becomes sufficiently large and is not compensated for by the stabilizing elastic M , torque. The nematic liquid begins to move with a velocity v under the action of a pushing force proportional to  Q (x) E in accordance with the NavierStokes equation (Eq. (91)) (written for the steady state regime):
where q = ( i ) (a,+a,%)isacombination of Leslie’s viscosity coefficients a,. The velocity v, in turn, supports the director fluctuation e ( ~ )in , accordance with the torque balance equation:
Combining Eqs (1 16)( 1 18) we derive the following formula for the threshold voltage: Ucrit
= Ecrit d
above which a periodic pattern of vortices forms with a period w, = d along the x axis. The whole process is governed by the anisotropy of conductivity. The threshold is diverged when 0,vanishes (e.g. in the case of nematics with shortrange smectic order). The threshold is proportional to the ratio q / a , of the two viscosities which, roughly speaking, are proportional to each other. Thus the threshold seems to be independent of viscosity and the instability may be easily observed in very viscous materials (e.g. polymer liquid crystals). The reason for this
Electrohydrodynamic Instabilities
42 1
is the compensation for two effects: (a) in very viscous media the velocity of vortex motion is lower ( q coefficient); and (b) the coupling between the flow and the director (a,coefficient) is much stronger. A more precise expression for the threshold voltage, derived by Helfrich [236], includes also a nonvanishing value of the dielectric anisotropy. All the dependences predicted by the simplest theory have been confirmed qualitatively by experiment [8, 91. In order to interpret the experimental data more precisely, some additional approaches have been developed. Generalization of the Simplest Model. In the onedimensional case, the diameter of the vortex is assumed to be equal to the cell thickness. In a more precise twodimensional approach [2402421 this assumption is not used and the stability of the systems is studied using the variation of the wavevector qx= z / w xalong thex axis. The threshold voltage found is in excellent agreement with experiment [243]. Later, a threedimensional version of the theory [244], which allows for the arbitrary anchoring energy, explained more complex domain patterns, such as oblique rolls [245 2471. Such rolls are seen for materials having a small negative dielectric anisotropy and large 0,.If the flexoelectric term is included in the field interaction energy [2482501 the symmetry of the problem is changed; this may also account for twodimensional vortex patterns (e.g. oblique rolls). A recent review [25 11 contains many interesting details concerning this problem. In order to discuss the behavior of the instability threshold as a function of the applied field frequency, the time dependent terms fi (af3/at) and @/at must be added to the equations for the director and charge continuity. Estimates show that the inertial term for the velocity avlat in the NavierStokes equation may be disregarded even in
422
9
Behavior of Liquid Crystals in Electric and Magnetic Fields
the transient regime (except when discussing the inertial mode in strongly conducting nematics; see below). Thus we have a set of two coupled linear equations for the space charge Q ( x ) and the curvature y=aO/ax [225, 2521:
and
This pair of equations has the same form as the set (Eqs (96) and (102)) for the injection instability. However, the fluid velocity is not included in the new set explicitly, and the destabilization is due to the coupling terms QEIq and oeff y e , where a,,, is an effective constant including the anisotropy of conductivity that is responsible for the instability. The fielddependent time constant for the reaction of the director to the field was discussed earlier (Eqs (33) and (62)). Near the threshold zr%zQ. The solution of set (Eqs (120) and (1 2 1)) represents a threshold voltage that is independent of frequency in the range co+ l/zQ (conductance regime) and increases critically when o+co,,,=l/zQ. Such a dependence is shown qualitatively in Fig. 28. For frequencies above w, another regime is predicted by the same theory where the director driven by flow is oscillating clockwise and anticlockwise in the ac field. The threshold for this ‘dielectric regime’ should also diverge with o,+O. In experiments, however, the modes observed at w > w, survive even at zero conductive anisotropy. Evidently, these instabilities (electrolytic and inertia modes) have a lower threshold than that predicted for the dielectric regime of the CarrHelfrich mode. If a substance has a small positive E,, the homeotropically oriented samples are stable
against pure dielectric perturbation; however, the convection may be observed due to EHD destabilization. The vortices have a short period and result in an optical pattern in the form of a short pitch grid. The period of the pattern is (a2/@+times less than d (10 times in typical nematics) [ I , 8 , 9 , 2 5 I]. For higher E, the direct transition to the chaotic state may be observed [253]. Behavior Above the Threshold. At voltages higher than the threshold of the CarrHelfrich instability, the normal rolls transform in more complex hydrodynamic patterns. One can distinguish zigzag and fluctuating domain patterns which, in turn, are substituted by the turbulent motion of a liquid crystal accompanied by a strong (dynamic) light scattering. The corresponding ‘stability diagram’ [226] is shown in Fig. 33 (see the discussion of the dielectric regime above). To calculate the wavevectors and amplitude of the distortions, a set of nonlinear equations must be solved. More generally, the problem of describing the transition from a regular electrohydrodynamic vortex motion to turbulence is a part of the classical problem, concerning the transition from laminar to turbulent flow of a liquid. Some progress has been achieved
frequency f
Figure 33. Voltage versus frequency phase diagram for electrohydrodynamic (convection) instabilities in the low frequency regime [226].
9.4
recently in understanding the nonlinear behavior of nematics in terms of bifurcation, phase transition, and dynamic chaos theories (for reviews see [226, 25 1 , 2541. In the splay Frederiks transition geometry (homogeneous orientation, large dielectric anisotropy E,%O) an interesting transient pattern in the form of domain stripes oriented parallel to the initial director has been observed [92]. The periodic pattern arises because the response of a liquid crystal placed suddenly far from equilibrium is faster to a spatially periodic director distribution than to a homogeneous orientation. The nonlinear theory of the transient patterns takes into account both the dielectric and the conductivity anisotropies [255,256]. Dynamic Scattering of Light. As is known from the general theory of dissipative dynamic systems, after a finite number of bifurcations a system reaches dynamic chaos. This scenario is also observed in the case of EHD convective motion. With increasing voltage the velocity of the vortices increases rapidly and the periodic flow of the liquid transforms to turbulence. Turbulent motion in nematic liquid crystals results in a nonuniform distribution of the director accompanied by dynamic scattering of light [257, 2581. As the field is increased further, dynamic texturing or secondary dynamic light scattering is observed. This is related to the appearance of disclination loops or/and walls separating regions with different orientations of the director. The light dynamic scattering effect was initially proposed for use in the manufacture of fieldcontrollable shutters and displays, and was the starting point of modern studies of liquid crystals [259, 2601.
highly conductive homogeneously oriented nematics with &,O),the planar texture of a cholesteric liquid crystal in a field parallel to the helical axis is unstable for any sign of E, [263, 2641. The instability is caused by the torque induced by the electrical conductivity acting against the elastic torque of the cholesteric and, although the cause is different from the purely dielectric case (see Sec. 9.3.2.2 of this Chapter), the result obtained is the same; that is, the appearance of a twodimensional periodic pattern for the distribution of the director. Investigation of the EHD instability (E, are spherical harmonics and A,, are coefficients which are nonzero onlY if the corresponding y;" is compatible with the symmetry of the nematic Phase (even 1 ) and that of the surface.
10.2.1 Definitions Both discussing anchoring in more details, it is necessary to define a terminology to describe it (for a more detailed lexicon, see JCrBme [4]). The main concept is the anchoring induced by an interface. The energy x of this interface  also called the anchoring energy  depends, among other things, on the orientation of the director at the surface. This energy has a certain number of minima ob
Figure 2. Some experimentally observed anchorings: (a) monostable planar (on grooved surfaces [ S ] ) ; (b) degenerate tilted, also called conical (at the nematidisotropic interface [6, 71); (c) homeotropic (on surfactantcoated glass @I); (d) tristable planar (on phlogopite mica [9]).
10.2 Macroscopic Alignment of Nematic Liquid Crystals
The term ‘surface’ means here the surface of the other phase in contact with the nematic liquid crystal. The symmetry of this surface (and of y,) is independent of the orientation taken by the nematic phase at the surface. In contrast, the symmetry of the interface depends on this orientation: it is the subgroup of the surface symmetry group containing the symmetry elements which leave invariant the anchoring direction effectively taken by the liquid crystal. If the other phase is a solid or liquid substrate, the surface is simply the surface of this substrate. In the case when the other phase is the gas or isotropic phase, the ‘surface’ is not a physical entity. However, one can still, in principle, distinguish this isotropic surface (C, symmetry) from the interface with the nematic phase, the symmetry of which is C,, C2,,,and C1,,for homeotropic, planar, and tilted anchoring, respectively. The interfaces at which anchoring has been mostly studied are those with crystal surfaces and treatedglass substrates. Glass treatments can be mechanical (rubbing) or chemical (deposition of a layer of surfactant, polymer, inorganic substance, etc.) or a combination of the two (for a review see Cognard [S]). The most commonly obtained anchorings are homeotropic, degenerate, and monostable planar (Fig. 2). Monostable tilted anchorings are less frequent, and multistable anchorings are seldom obtained. The occurrence of multistable or degenerate anchorings raises the issue of the selection of anchoring directions; indeed, at each point of the surface, the director can take only one of the possible anchoring directions characterizing such anchorings. Generally speaking, the selection is made by the history of the sample, for instance cooling from the isotropic phase under a magnetic field [ 1 1,121or spreading [ 131. In general, once the selection has been made, the anchoring direction is preserved by the sur
435
face, even in the case of degenerate anchorings [ 1 1, 141. This appears to come from the adsorption of the surface molecules onto the substrate [12]. Switching between the anchoring directions of a multistable anchoring is, however, possible [15, 161.
10.2.2 Anchoring Directions By minimizing the interfacial energy ys, one can find the anchoring diagram giving the different anchorings induced by a surface depending on the values of the coefficients A,, appearing in Eq. (1) (Fig. 3). These diagrams give a general description of anchoring, independent of the nature of the system. However, the limitation of this macroscopic approach lies in the fact that it is, in general, not possible to establish a relationship between the coefficients A,, and the parameters governing the structure of the interface. Anchoring diagrams show the different ways in which anchoring can change when some parameters are varied. These anchoring transitions follow the same symmetry rules as phase transitions: transitions which do not involve a change of symmetry of the interface must be first order, while when a symmetry change is involved the transition can be first or second order [ 101. Anchoring transitions also appear the same way as phase transitions: nucleation and growth of domains having a new orientation for firstorder transitions [ 191, and director fluctuations for secondorder transitions [ 181. These fluctuations correspond to a divergence of the susceptibility of the system for a force driving the director away from the anchoring directions: indeed, the anchoring strength (see Section 10.2.3) does go to zero at secondorder anchoring transitions [20221. One characteristic of anchoring transitions is that this susceptibility can be
436
10 Surface Alignment
Figure 3. Anchoring diagram corresponding to a surface with C , , symmetry (with mirror plane 0)inducing planar anchorings: y,(cp)=a, cos(2cp)+a4 cos(4cp)+a6 cos(6cp) [17, 181. ys is normalized by the condition a ~ + a ~ + 1, a so ~ =that the anchoring diagram can be represented on a sphere. At each point on the sphere, the color indicates the predicted anchoring direction. The code is given by the background, the surface of which corresponds to the substrate surface. () Firstorder transition; () secondorder transition. C,, Critical endpoint; C,, tricritical point.
anisotropic (i.e. the response to an applied force can depend on the force direction) ~31. There are several examples of experimentally observed anchoring transitions (see JCr6me [4] and Pieranski and JCrbme [lo], and references therein). Since anchoring transitions occurring at the surface of a liquid crystal cell induce a change of director configuration in the cell, these transitions can be used to switch a liquid crystal device between different states [24, 251.
pens is determined the dependence of ‘/s on the orientation of the director n at the surface. Knowledge of this dependence is necessary in order to establish the surface boundary conditions on the director field [26]. Several methods have been developed in order to measure experimentally some characteristics of y,@) [27, 281. Generally speaking, they consist in observing the change in orientation induced at a surface under the action of an external field. Thermodynamically, y, can be defined by the equation [28]:
10.2.3 Anchoring Energy
f =fO
m
+ys[n(zd),zd]+
jfd[n(z)3$(z)]dz ZA
The director at an interface might depart from the anchoring directions induced by this interface under the effect of another orienting field. The way in which this hap
wherefis the total free energy of the system per unit area,fo is the free energy in absence of surface and deformation in the bulk,fd is
437
10.2 Macroscopic Alignment of Nematic Liquid Crystals
the elastic energy density due to deformations of the director field n (z), and zd is the position of the surface above which the nematic phase is considered to have bulklike behavior. From this definition, it is clear that when the director field is not uniform, which is always the case in anchoring energy measurements, ‘/s depends on zd. Unfortunately, the value of zd depends both on the technique used to measure the anchoring energy and on the structure of the interfacial region [28]. Therefore, the results of the anchoring energy measurements interpreted using this approach (as has generally been done until now) are not comparable with each other. The dependence of the interfacial energy ‘/s with the surface director was first considered by Rapini and Papoular [29] who assumed that the dependence of “/s on the tilt angle e was proportional to sin2(ees) where 0, is the tilt of the anchoring direction. The coefficient of proportionality measures the ease with which the surface director can deviate from the anchoring direction and is called the anchoring strength or anchoring energy coefficient. Generally speaking, one defines two anchoring strengths, the polar and the azimuthal one, corresponding to deviations from the anchoring direction ( Q p , ) at constant azimuthal angle cp and tilt angle 6, respectively:
theoretical calculations of ‘/s (6,cp) [30321. It might also come from the orderparameter gradient existing at the interface, giving rise to an orderelectric polarization [33] and to a contribution to [34]: owing to symmetry considerations, this contribution is zero for W , while it is finite for W,. It has also been suggested that the upper limit of the measured anchoring strengths could be due to the fact that, for strong anchorings, the interfacial region would prefer to melt instead of undergoing too strong a distortion WI. The anchoring strengths (Eq. (3)) are useful only when the director remains close to the anchoring directions. For large deviations of the surface director, the whole dependence of ‘/s should be known. With few exceptions [23], measurements of are performed assuming that the 8 and cp variations of ‘/s are independent. Concerning the 8 dependence, neither experiments [36391 nor theoretical calculations [31, 401 (see also JCrBme [4] and references therein) have come to an agreement on whether the expression of ‘/s ( @should contain one or more Fourier components. Part of the discrepancies in the anchoring energy measurements could be due to bulk effects such as ferroelectricity [39] or the presence of ions [27, 41, 421. In addition, in none of these studies was the contribution to the anchoring energy of the adsorption of liquid crystalline molecules onto the substrate [ 121 taken into account. In fact, ‘/s contains two terms [4]:
x
x
Ys(n)=y~f(n)+y,ad(n;a,d) All measurements of anchoring strengths and give values of Wp ranging between lop3J m2 (lOP51 erg cm2) and values of W , one or two orders of magnitude smaller. This inequality might be intrinsic to the anchoring mechanisms, as predicted by some
(4)
gurf is the interfacial energy in the absence of adsorption; f d arises from the adsorption of molecules onto the substrate and has two opposite minima corresponding to the anchoring direction a a d =aa,, initially taken by the liquid crystal. The orienting field felt by the surface director therefore has uniax
438
10
Surface Alignment
ial symmetry, regardless of the symmetry of fUrf. However, gdis not an intrinsic property of the surface and can be subject to changes, depending on the history of the sample [43]. From the above discussion, it is clear that the macroscopic approach is inadequate for describing situations in which the director is forced to depart from anchoring directions. A proper description of these situations should take into account the response of the interfacial region to such distortions. There have been some attempts to describe the interfacial region in a semimacroscopic way, assuming that the nematic order is retained in the interfacial region but with a varying order parameter [22, 34, 44, 451. These semimacroscopic theories define a surface anchoring energy giving the energy of the surface layer as a function of its orientational state defined by the tensorial nematic order parameter. The spatial evolution of this order parameter away from the surface is calculated using the Landaude Gennes [46] theory under the appropriate conditions corresponding to the way, in which the orientation of the director is imposed in the bulk. The main defect in this kind of theory is the assumption that the orientational order is nematic like in the interfacial region, which is generally not true (see Section 10.3.1). Another problem is linked to the fact that the surface anchoring energy is unknown. This surface anchoring energy is difficult to measure directly and the result of any indirect measurement depends on how the response of the system to a disorientation is modeled. One way out is to use the orientational distribution of the molecules in the surface layer as a boundary condition of the nematic order [47] (see also Section 10.3.21.
10.3 Microscopic Surface Order of Nematic Liquid Crystals 10.3.1 Surface Orientational Order An experimental technique has recently been developed to investigate the surface orientational order of liquid crystals: optical secondharmonic generation [48]. Becauseof its high sensitivity to surface polar ordering and its surface specificity, this method is able to probe the orientational distribution of polar monolayers of liquid crystal molecules located at the surface of a substrate, whether they are covered by a bulk liquid crystal or not. So far, such measurements have only been performed on cyanobiphenyl molecules (nCB and nOCB). These molecules exhibit polar ordering (with the cyano groups pointing towards the surface) on hydrophilic substrates such as water, glass, and certain polymer films [49511, but not on hydrophobic layers [52]. On the latter, the molecules orient with their aliphatic chains in contact with the substrate, and arrange following their natural tendency to form apolar ‘dimers’ (two molecules oriented head to head). In all cases where a surface dipolar ordering exists, it is lost after the first molecular layer [49]. The tilt of the hard core of cyanobiphenyl molecules is found to be always approximately the same, namely 70” from the surface normal, resulting from a balance between the dipoledipole interaction of the polar heads and the steric interaction of the biphenyl core with the substrate [49,531. By means of infrared sumfrequency generation, it has also been shown that the aliphatic chains are relatively straight and point away from the surface [54].
10.3 Microscopic Surface Order of Nematic Liquid Crystals
The distribution of azimuthal orientation strongly depends on the substrate [52, 55, 561. On glass and surfactant and polymercoated glass this distribution is isotropic, as would be expected from the isotropy of these surfaces. When polymer films are rubbed by translation in one direction on a piece of cloth, the polymer chains at the surface of the film are oriented along the rubbing direction [57, 581. The liquidcrystal molecules then orient preferentially along the polymer chains (Fig. 4a). As on crystal surfaces, this anisotropic orientational distribution is the result of the direct interaction between the molecules and the substrate. Conversely, monolayers at the surface of rubbed glass, certain rubbed surfactant layers, and evaporated SiO films exhibit an isotropic azimuthal distribution [5 1, 521; despite their anisotropy, these substrates have no shortrange azimuthal orienting action on nematic molecules. The azimuthal orientational distribution of surface liquidcrystal molecules can, in principle, also be obtained by imaging the molecules. However, sufficiently high res
Figure 4. The three main substrate classes: (a) smooth surfaces on which surface molecules have a definite orientational distribution (represented: surface obtained on a rubbed polyimide film [ 5 2 ] ) ;(b) interpenetrable surfaces of dangling chains; (c) topographies (represented: grooved surface) with a favorable (left) and unfavorable director field n. In all cases, a is the macroscopic anchoring direction.
439
olution can only be obtained with scanning tunneling microscopy, which limits the use of imaging techniques to special conducting substrates, such as cleaved pyrolytic graphite [59,60] and MoS crystals [6 11. A feature common to all the images obtained is the high orientational and positional order of the molecules in the surface monolayer. The techniques described above allow for the determination of the orientational order in the surface layer. A complete description of the liquid crystalline ordering close to a surface should also include the evolution of the orientational order in the interfacial region from the one at the surface to the one in bulk. There are, however, no experimental techniques available to measure this evolution directly. Some experimental techniques allow one to measure some integrated quantities over the whole interfacial region, which depend on the evolution of the orientational order in this region (see e.g. [62651). To obtain the order profile from such measurements, one needs to assume the general shape of this evolution and fit the experimental data to obtain the profile parameters. Knowledge of the surface orientational order can, however, guide the choice of model profile.
10.3.2 Microscopic Anchoring Mechanisms at Solid Substrates With the presently known information on the orientational order in surface layers and interfacial regions, it is possible to deduce some of the microscopic origins of the macroscopic anchoring of liquid crystals. One can distinguish three main classes of substrate, giving rise to three main classes of anchoring mechanism: smooth surfaces, interpenetrable layers, and topographies (Fig. 4). It should, however, be emphasized that the macroscopic anchoring is often due
440
10
Surface Alignment
to a combination of effects, some of which are specific to certain substrates. Smooth substrates include crystal and glass surfaces, and polymer films. The direct influence of such a substrate on the liquid crystal is limited to the molecules in the surface layer and is due to the shortrange interaction of these molecules with the substrate (Fig. 4a). Once these microscopic anchoring conditions are known, the configuration of the rest of the liquid crystal (in particular the orientation of the director outside the interfacial region) can be determined from the properties of the liquid crystal regarding propagation of orientational order. The microscopic anchoring conditions can be modeled by the energy of the surface layer as a function of its orientational order. The evolution of the orientational order away from the surface is then calculated by minimizing the sum of this surface energy and of the (orientational order dependent) bulk energy. Since the dependence of the energy of the surface layer on its orientationa1 order is generally unknown, the orientational distribution of the surface molecules, if experimentally available (see Section 10.3.1), can be used as a boundary condition for the order in the rest of the liquid crystal [52, 551. This surface orientational distribution does indeed seem to be strongly enforced by the surface; it is essentially independent of whether this monolayer is covered by a bulk liquid crystal or not, and whether this bulk is in the nematic or isotropic phase [ 5 2 ] . This type of calculation has been performed successfully, both by using a general form of the surface energy [22] and experimentally determined surface orientational distributions [66, 671, in order to explain the anchoring directions and anchoring transitions observed on different substrates. These calculations were made within the framework of the Landaude Gennes
theory [46], the liquid crystalline order at each point in space (including the interfacial region and surface layer) being described by the tensorial order parameter. The evolution of the director and the degree of molecular order in the interfacial region is coupled. This orderparameter/director coupling comes essentially from the L2 term in the Landaude Gennes energy; this term should therefore not be neglected (as is often the case). This implies that, since the degree of order is generally different at the surface and in the bulk, the anchoring direction is different from the mean orientation of the molecules at the surface [66681. This also means that the,degree of surface ordering is a determinant factor in the tilt of the anchoring directions [43,47, 551. The Landaude Gennes theory is, however, not applicable to all surfaces; in particular it is unable to predict the azimuthal orientation of the anchoring directions in the case of multistable anchorings, which occur on substrates with sufficiently symmetry. Indeed, reducing the information on the surface orientational distribution to a nematic tensorial order parameter suppresses the information on the symmetry of the surface. Order parameters of higher order reflecting the surface symmetry should then be included in the description of the orientational order, together with the corresponding terms in the energy of the system. A second class of substrates corresponds to surfaces which are smooth but on which molecules with a long tail (such as surfactants) are grafted, forming a layer that the liquid crystal can penetrate (Fig. 4b). The influence of the substrate on the liquid crystal at a microscopic level can then be separated into two parts: the effect of the surface underlying the surfactant layer and the effect of the chains forming the layer. It seems that the latter always dominates; the liquid crystal adopts the orientation of the chains
10.3 Microscopic Surface Order of Nematic Liquid Crystals
in the layer, which leads to a homeotropic or conical anchoring depending on the orientation of the chains [54, 69, 701. It should be emphasized that not all substrates covered with aliphatic chains belong to this class of substrates. If the chains are closely packed, the liquid crystal molecules cannot penetrate the layer [54] and the substrate can be seen as a smooth surface belonging to the first class described above. The third class of substrates corresponds to those having a surface of a certain topography (Fig. 4c). This topography is generally obtained by rubbing the surface with a hard material (rubbed glass or surfactantcoated glass) or by anisotropic vapor deposition (evaporated SiO films). Each point of such a surface induces a given orientationa1 distribution of liquid crystal molecules. On all the substrates mentioned above, this local orientational distribution is isotropic [5 1,521. However, since the orientation and the height of the surface is not uniform, the microscopic anchoring conditions are not uniform over the surface, introducing distortions along the plane of the surface. The anchoring direction chosen by the liquid crystal is then the one that minimizes these distortions. For instance, grooved surfaces induce an anchoring direction parallel to the grooves. This anchoring mechanism can be modeled by minimizing the FranckOseen elastic free energy associated with director distortions [5]. All the anchoring mechanisms described above are based on the knowledge of the microscopic anchoring conditions. However, a complete understanding of anchoring requires knowledge of the origins of this microscopic anchoring, which should be found in the interactions between the liquid crystal molecules and the substrates. These interactions are basically unstudied.
44 1
10.3.3 The Nematic/Isotropic and NematicNapor Interfaces The case of the interface with an isotropic or vapor phase is relatively simple in that no interaction with a substrate is involved. The molecular ordering and the orientation of the nematic director at these interfaces arise mainly from the change in density and type of order taking place across the interface. Studies of the orientational order at this type of interface concern exclusively nematic/vapor interfaces. No direct measurement of this order has been performed so far, but indirect observations have shown that the order at the free surface can be higher or lower than in the bulk [71731. Excess order occurs when the intermolecular interaction depends on the relative molecular positions (i.e. when the translational and rotational degrees of freedom are coupled) [74, 751. This coupling is also essential for anchoring to occur at the surface (Fig. 5 ) . Since the surface breaks the bulk inversion symmetry, it creates a polarity which, in principle, should give rise to polar ordering near the surface. This ordering has been investigated in asymmetric molecules with a polar head. These molecules prefer to orient with their polar heads pointing in the direction of the more polar medium. This tends to create a polar surface layer with all the heads pointing away from the surface. However, in order to minimize the polar intermolecular interactions, the molecules tend to arrange antiparallel to each other with a partial or total overlap. This effect compensates for any surfaceinduced polar ordering, creating either a nonpolar [76] or an antiferroelectric [49, 77, 781 surface ordering. As far as macroscopic anchoring is concerned, it has been found experimentally that, at the nematic/isotropic interface, the director is tilted (in all the compounds so far studied, including nCB and MBBA), with
442
10 Surface Alignment
planar anchoring
hornentropic anchoring
orienrion 0
I I
excess order
l/bi
no preferred
//uni
I
excess disorder
excess order
*C
1
Figure 5. Anchoring (top) and surface ordering (bottom) at the free surface of a nematic liquid crystal as a function of the strength C of the coupling between translational and rotational degrees of freedom [75]. I,Homeotropic ordering; Iluni and Ilbi, uniaxial and biaxial ordering parallel to the surface.
an angle 19,from the surface normal in the range 5080" [6,7].At the free surface, there are more differences from one liquid crystal to the other: I9,=O0 in nCB and PCHn [79, 801 (because the polar head of these molecules prefers to point away from the surface), 8,=90" in PAA [81], and 0, decreases to 0" as the temperature increases in MBBA and EBBA [82]. The first attempt to account for these results was made by de Gennes using the Landaude Gennes theory [46]. This theory predicts that the tilt angle can only be 0" or 90", depending on the elastic properties of the liquid crystals. In order to account for tilted anchorings in this framework, different effects can be added in the model, such as order electricity arising from orderparameter gradients [ 3 3 ] . Another series of theoretical models is based on molecular interactions, either anisotropic hardcore interactions [40, 8385] or combining different kinds of intermolecular interactions [86, 871 (see also JCrBme [4] and references therein). The results depend greatly on the details of the models, the validity of which still needs to be checked.
10.4 Orientation of Other Liquid Crystals The study of surface orientation of nonnematic liquid crystals is still incomplete.
Here, separate sections are dedicated to polymer liquid crystals and lyotropic liquid crystals, the latter being peculiar in that they are inhomogeneous phases.
10.4.1 Smectic and Chiral Liquid Crystals In smectic A phases where the smectic layers are perpendicular to the molecules, the orientation of the whole structure is, in principle, fixed once the orientation of the molecules is defined by the interface. The surface orientation of achiral smectic A phases is then the same as that of the nematic phase [88, 891. However, since splay deformations of smectic layers (director bend deformations) are forbidden and layer bend deformations (director splay deformations) require a lot of energy, smectic phases tend to adopt uniform configurations, even between two walls inducing two different orientations. In the latter case, the surface orientation of the smectic phase differs from that of the nematic phase, and depends on the layer configuration in the bulk [90,9 I 1. In the case of tilted smectic phases (for instance the smectic C phase), there is a degeneracy in the orientation of the director with respect to that of the layers. If a surface inducing a degenerate planar anchoring is placed perpendicular to the layers, there are two possible orientations of the director that satisfy both the surface and the liquid crystal structural constraints (Fig. 6).
10.4 Orientation of Other Liquid Crystals
Figure 6. Two equivalent orientational states in a smectic C liquid crystal between two walls inducing a degenerate planar anchoring.
This surface bistability is at the basis of chiral smectic C surface stabilized ferroelectric liquid crystal (SSFLC) devices [92]. As their name indicates, these devices are made of thin cells in which the walls, imposing the orientation of the molecules at the surfaces, unwind the spontaneous smectic C* helix and stabilize two uniform configurations of the director in the cell. Switching between these two states can be done by applying an electric field. The preparation of such cells requires both that the director is oriented parallel to the surface and that the layers are oriented perpendicular to the surfaces. Because the walls only have an influence on the orientation of the director, and because of the director/layernormal degeneracy, the alignment of the layers must be achieved in the smectic A* phase, before cooling the system in the smectic C* phase [93]. Due to the positional anchoring of the layers at the surfaces [94], the location of the layers is pinned at the walls. Since the layer thickness dA in the smectic A phase is larger than the thickness dc in the smectic C phase, the layers must tilt in the bulk by an angle 6 , such that dc = dA cos 6, [95]. The combination of tilted orientation of the director at the surface (breaking the inplane isotropy of the surface) and of the surfaceinduced updown asymmetry [96] gives rise to new terms in the energy of the surface layer which favor splay configurations of the director [97, 981. Such config
443
urations have been observed at the free surface of achiral tilted smectic phases. The details of the patterns obtained depend on the type of smectic phase considered: in a smectic C phase, the director can rotate freely on a cone, while in a smectic phase presenting a bondorientational order (smectic I, F, or L) the coupling existing between this order and the director imposes discrete rotations of the director through walls [99, 1001. The surface pattern also depends on whether or not there is a mechanism imposing the sign of the surfaceinduced polarization, and consequently that of the director rotation [ 100 1031. In a chiral compound, the liquid crystalline structure itself possesses a polarity which interacts with the surface. At the surface of a smectic C* liquid crystal, the ferroelectric polarization P points preferably either towards or away from the surface, depending on the material [104, 1051. Conversely, if the surface director of a chiral nematic liquid crystal is tilted, a polarization (dependent on the tilt angle) is created perpendicular to the tilt plane [106]. In principle, the presence of this polarization makes a contribution to the anchoring energy; this chiral contribution is, however, too small to be measured [ 1071. The combination of liquid crystalline chirality and surface polarization is also the origin of the socalled surface electroclinic effect in chiral smectic A phases: if the smectic layers are oriented perpendicular to the surface, the surface electric field tilts the layer normal away from the surface molecular orientation [1081 101 (Fig. 7).
Figure 7. The surface electroclinic effect rotating the smectic layer normal away from the surface molecular orientation in smectic A* liquid crystals.
444
10 Surface Alignment
10.4.2 Polymer Liquid Crystals The macroscopic orientation of polymer liquid crystals at surfaces can formally be described in the same way as that of lowmolecularweight liquid crystals. However, the polymer character of these materials has an influence on the surface behavior at a microscopic level. One can distinguish different aspects: loss of freedom of the mesogenic groups, change in polymer chain entropy due to the steric restriction near the surface, increase of longitudinal persistence length (along the director), and attractionhepulsion of the polymer chain at the surface. When mesogenic groups are part of apolymer chain (in mainchain polymers) or attached by one of their ends to a main chain (in sidegroup polymers), they lose the ability to orient independently of each other. In particular, they might not be able to adopt the surface orientation which they would have if they were free. This effect can lead to a change in anchoring direction with respect to that of the free mesogens, as observed at the free surface of sidechain polymer liquid crystals the sidegroups of which are terminated by a polar head (such as cyanobiphenyl groups) [111, 1121. As mentioned in Section 10.3.3, lowmolecularweight liquid crystalline compounds carrying a polar head orient perpendicularly to their free surface because the head prefers to point away from the surface. In a sidegroup polymer liquid crystal, satisfying this constraint would force the surface polymer molecules to have their main chain confined at the surface and all their sidegroups pointing in the same direction. This is sterically impossible. The system solves this configurational problem by orienting the sidegroups (and the surface director) parallel to the surface. As in any polymer, the presence of a surface limits the number of configurations that the polymer chains are allowed to take in the
vicinity of this surface. Since these chains and the mesogenic groups are mechanically coupled, this loss of chain entropy implies a limitation of the orientations accessible to the mesogenic groups. Moreover, the presence of a polymer chain linking the mesogenic groups increases the longitudinal persistence length along the director. These two effects can make the anchoring strength of polymer liquid crystals considerably larger than that of lowmolecularweight liquid crystals [ 1131. Finally, the polymer chain (the main chain in sidechain polymers or the intermesogen chain in mainchain polymers) interacts directly with the surface and can be either attracted to or expelled from the surface. For instance, sidegroups terminated by a polar head and attached to a chain also carrying polar groups orient parallel to hydrophilic surfaces, instead of being tilted as the corresponding lowmolecularweight liquidcrystal molecules (see Section 10.3.1).
10.4.3 Lyotropic Liquid Crystals The anisotropic micelles forming lyotropic liquid crystals are also oriented by surfaces. Both prolate and oblate micelles orient parallel to flat surfaces [ 1 14, 1 151 probably due to hardcore interactions [116]. Prolate micelles can also be azimuthally oriented by grooved surfaces, or homeotropically oriented by twodimensional topographies [ 1 171. However, one peculiarity of these systems is that the surfactant molecules forming the micelles are surface active and generally adsorb at the surface: this leads a modification of the surface [ 1 151. The presence of anisotropic defects in this adsorbed layer can then induce an azimuthal anchoring of the bulk micelles. The slow reorientation of these surface defects under a mag
10.5 References
netic field induces a slow inplane reorientation  or gliding  of the anchoring directions [ I 181.
10.5 References [I] C. Mauguin, C.R.A.S. 1911, 156, 1246. 121 T. J. Sluckin, A. Poniewierski, in Fluid Interfacial Phenomena (Ed. C. A. Croxton), Wiley, New York 1986, Chap. 5 , pp. 215253. 131 A. A. Sonin, The Surface Physics uf Liquid Crystals, Gordon and Breach, Amsterdam 1995. [4] B. JCrBme, Rep. f r o g . Phys. 1991, 54, 391. [S] D. W. Berreman, Phjs. Rev. Lett. 1972,28, 1683. [6] R. Vilanove, E. Guyon, C. Mitescu, P. Pieranski, J. Phys. Frunce 1974, 35, 153. 171 H. Yokoyama, S . Kobayashi, H. Kamei, Mol. Cryst. Liq. Cryst. 1984, 107, 31 1. [8] J. Cognard, Mol. Cryst. Liq. Cryst. 1982, 1 (SUPPI.), 1. 191 P. Pieranski, B. JCrBme, M. Gabay, Mol. Cryst. Liq. Cryst. 1990, 17Y, 285. [ 101 P. Pieranski, B. JCrBme, Mol. Cryst. Liq. Cryst. 1991, 199, 167. [ I I ] J. Cheng, G. D. Boyd, Appl. Phys. Lett. 1979,35, 444. 1121 Y. Ouchi, M. B. Feller, T. Moses, Y. R. Shen, Phys. Rev. Lett. 1992, 68, 3040. [I31 B. JCrBme, P. Pieranski, J . Phys. France 1988, 49, 1601. [ 141 N. Koshida, S . Kibui,Appl. Phys. Lett. 1982,40, 541. [IS] R. Barberi, M. Boix, G. Durand, Appl. Phys. Lett. 1989, 55, 2506. [I61 R. Barberi, G. Durand, Liq. Cryst. 1991,10,289. [I71 H. S. Kitzerow, B. JCrBme, P. Pieranski, Physic a A 1991, 174, 163. (181 J. Bechhoefer, J. L. Duvail, L. Masson, B. JCrBme, R. M. Hornreich, P. Pieranski, Phys. Rev. Left. 1990, 64, 191 1. 1191 P.Pieranski, B. JCrGme, Phys. Rev. A 1989, 40, 317. [20] P. Chiarelli, S. Faetti, L. Fronzoni, Phys. Lett. 1984, IUIA, 31. [21] G. A. DiLisi, C. Rosenblatt, A. C. Gr Hari, Liq. Cryst. 1990, 7, 353.
527. (241 K. Ichimura, Y. Suzuki, T. Seki, A. Hosoki, K. Aoki, Langmuir 1988, 4. 12 14. [25] W. Gibbons, P. Shanon, S . T. Sun, B. Svetlin, Nature 1991, 351, 49.
445
[26] P. G. de Gennes, J. Prost, The Physics of Liquid Crystals, 2nd edn, Clarendon Press, Oxford 1993. [27] L. M. Blinov, A. Y. Kabayenkov, A. A. Sonin, Liq. Cryst. 1989,5,645. [28] H. Yokoyama, Mol. Cryst. Liq. Cryst. 1988. 165, 265. [29] A. Rapini, M. Papoular, J. P h y ~Coll. . 1969, 30, c 4 54. [30] J. Bernasconi, S . Strassler, H. R. Zeller, Phys. Rev. A 1980,22, 276. [31] K. Okano, N. Matsuura, S . Kobayashi, Jpn. J. Appl. Phys. 1982, 21, L109. 1321 S. Faetti, Phys. Rev. A 1987, 36, 408. 1331 G. Barbero, I. Dozov, J. F. Palierne, G. Durand, Phys. Rev. Lett. 1986, 56, 2056. [34] H. Yokoyama, S . Kobayashi, H. Kamei, J. Appl. Phys. 1987, 61,4501. 1351 G . Barbero, G. Durand, Mo1. Cryst. Liq. Cryst. 1991, 203, 33. [36] K. H. Yang, C. Rosenblatt, Appl. Phys. Lett. 1983, 43, 62. [37] G. Barbero, N. V. Madhusudana, G. Durand, Z. Naturforsch., Teil a 1984, 39, 1066. [38] H. Yokoyama, S . Kobayashi, H. Kamei, Mol. Cryst. Liq. Cryst. 1985, 129, 109. 1391 G. Barbero, G. Durand, J. Phys. France 1986, 47, 2 129. [401 J . D. Parsons, Mol. Phys. 1980,42, 951. [41] G. Barbero, G. Durand, J. Phys. France 1990, 51, 28 I. [42] B. Valenti, M. Grillo, G. Barbero, P. Taverna Valabrega, Europhys. Lett. 1990, 12, 407. [43] B. 0. Myrvold, Liq. Cryst. 1995, 18, 287. [44] G. Barbero, G. Durand, J . Appl. Phys. 1991,69, 6968. [45] M. Nobili, G . Durand, Phys. Rev. A 1992, 46, 6174. [46] P. G. de Gennes, Mol. Cryst. Liq. Cryst. 1971, 12, 193. (471 Y. Zhuang, L. Marrucci, Y. R. Shen, Phys. Rev. Lett. 1994, 73, 15 13. [48J Y. R. Shen, Nature 1989, 337, 519. 1491 P. GuyotSionnest, H. Hsiung, Y. R. Shen, Phys. Rev. Lett. 1986, 57, 2963. [50] C. S . Mullin, P. GuyotSionnest, Y. R. Shen, Phys. Rev. A 1989, 39, 3745. [ S l ] W. Chen, M. Feller, Y. R. Shen, Phys. Rev. Lett. 1989,63,2665. [52] M. B. Feller, W. Chen, Y. R. Shen, Phys. Rev. A 1991,43,6778. 1531 N. A. J. M. van Aerle, Liq. Cryst. 1994,17,585. [54] J. Y. Huang,R. Superfine,Y. R. Shen, Phys. Rev. A 1990,42,3660. [ S S ] M. Barmentlo, R. W. J. Hollering, N. A. J. M. van Aerle, Phys. Rev. A 1982, 46, 4490. [56] B. JCrBme, Y. R. Shen, Phys. Rev. E 1993, 48, 4556. [57] J. M. Geary, J. M. Goodby, A. R. Kmetz, J. S. Patel, J . Appl. P hys. 1987, 62, 4 100.
446
10 Surface Alignment
I581 M. F. Toney, T. P. Russel, J. A. Logan, H. Kikuchi, J. M. Sands, S. K. Kumar, Nature 1995,374, 709. [59] J. S . Foster, J. E. Frornmer, Nature 1988,333,542. [60] D. P. E. Smith, J . K. H. Horber, G. Binnig, H. Nejoh, Nature 1990, 344, 641. [61] M. Hara, Y. Iwakabe, K. Tochigi, H. Sasabe, A. F. Garito, A. Yarnada, Nature 1990,344,228. [62] K. Miyano, Phys. Rev. Lett. 1979, 43, 51. [63] J. P. Nicholson, J. Phys. France 1987, 48, 131. [64] W. Chen, L. J. MartinezMiranda, H. Hsiung, Y. R. Shen, Phys. Rev. Lett. 1989, 62, 1860. [6S] G. P. Crawford, R. Stannarius, J. W. Doane, Phys. Rev. A 1991, 44, 2558. [66] D. Johannsmann, H. Zhou, P. Sonderkaer, H. Wierenga, B. 0. Myrvold, Y. R. Shen, Phys. Rev. E 1993,48, 1889. 1671 B. JCrBme, J. Phys.: Condens. Matter 1994, 6, A269. [68] B. JCrGrne, J. O’Brien, Y. Ouchi, C. Stanners, Y. R. Shen, Phy.7. Rev. Lett. 1993, 48, 4556. [69] G. Porte, J. Phys. France 1976, 37, 1245. [70] K. Hiltrop, H. Stegemeyer, Ber. Bunsenges. Phys. Chem. 1981,85, 582. [71] A. W. Neumann, R. W. Springer, R. T. Bruce, Mol. Cryst. Liq. Cryst. 1974, 27, 23. 1721 D. Beaglehole, Mol. Crvst. Liq. Cryst. 1982, 89, 319. [73] D. Langevh, J. Ph~s.Frunce 1972,33,249. [74) J. H. Thurtell, M. M. Telo da Gama, K. K. Gubbins, Mol. Phys. 1985, 54, 321. [75] B. TjiptoMargo, A. K. Sen, L. Mederos, D. E. Sullivan, Mol. Phys. 1989, 67, 601. 176) E. F. Gramsbergen, W. H. de Jeu, J . Phys. France 1988,49, 363. [77] B. M. Ocko, P. S. Pershan, C. R. Safinya, L. Y. Chiang, Phys. Rev. A 1987, 35, 1868. [78] E. F. Gramsbergen, J. Als Nielsen, W. H. de Jeu, Phys. Rev. A 1988, 37, 1335. [79] M. G. J. Gannon,T. E. Faber, Phil. Mag. A 1978, 37, 117. [80] S . Immerschitt, T. Kohl, W. Stille, G. Strobl, J. Chem. Phys. 1992, 21, 173. [Sl] M. A. Bouchiat, D. LangevinCruchon, Phys. Lett. A 1971, 34, 33 1. [82] S . Faetti, L. Fronzoni, Solid State Commun. 1978.25, 1087. [83] R. Holyst, A. Poniewierski, Phys. Rev. A 1988, 38, 1527. [84] B. G. Moore, W. E. McMullen, Phys. Rev. A 1990,42,6042. [85] M. A. Osipov, S . Hess, J. Chem. Phys. 1993, 99, 4181. [86] J. D. Parsons, Phys. Rev. Lett. 1978, 41, 877. [871 B. ThiptoMargo, D. E. Sullivan, J . Chem. Phys. 1988,88,6620. I881 W. Urbach, M. Boix, E. Guyon,Appl. Phys. Lett. 1974,25, 479. [89] J. E. Proust, L. TerMinassianSaraga, J. Phys. Colloq. 1979,40, C3 490.
[90] S. J . Elston, Liq. Cryst. 1994, 16, 151. [91] J. J. Bonvent, J. A. M. M. van Haaren, G. Cnossen, A. G. H. Verhulst, P. van der Sluis, Liq. Cryst. 1995, 18, 723. [92] N. A. Clark, S . T. Lagerwall, Appl. Phys. Lett. 1980, 36, 899. [93] K. Kondo, F. Kobayashi, A. Fukuda, E. Kuze, Jpn. J . Appl. Phvs. 1981, 20, 1773. [94] M. Cagnon, G. Durand, Phys. Rev. Lett. 1993, 70, 2742. [95] M. A. Handschy, N. A. Clark, Ferroelectrics 1984, 59, 69. [96] Y. Galerne, L. Liebert, Phys. Rev. Lett. 1990, 64, 906. [97] R. B. Meyer, P. S . Pershan, Solid State Commun. 1973, 13, 989. [98] J. V. Selinger, Z . G. Wang, R. F. Bruinsma, C. M. Knobler, Phys. Rev. Lett. 1988, 70, 1139. 1991 S. B. Dierker, R. Pindak, R. B. Meyer, Phys. Rev. Lett. 1986,56, 1819. [loo] J. Maclennan, M. Seul, Phys. Rev. Lett. 1992, 69, 2082. [ l o l l T. J . Scheffer, H. Gruler, G. Meier, Solid State Commun. 1972, 11, 253. [lo21 E. I. Demikhov, Phys. Rev. E 1995, 51, 12. [ 103) J. Pang, N. A. Clark, Phys. Rev. Lett. 1994, 73, 2332. [I041 M. A. Handschy, N. A. Clark, S. T. Lagerwall, Phys. Rev. Lett. 1983, 51, 471. (1051 J. Xue, N. A. Clark, M. R. Meadows, Appl. Phys. Lett. 1988, 53, 2397. [I061 S. Tripathi, M. H. Lu, E. M. Terentjev, R. G. Petschek, C. Rosenblatt, Phys. Rev. Lett. 1991, 67, 3400. [ 1071 K. A. Crandall, C. Rosenblatt, R. M. Hornreich, Liq. Cryst. 1995, 18, 25 1. [ 1081 K. Nakagawa, T. Shinomiya, M. Koden, K. Tsubota, T. Kuratate, Y. Ishii, F. Funada, M. Matsuura, K. Awane, Ferroelectrics 1988, 85, 427. [I091 J. Xue, N. A. Clark, Phys. Rev. Lett. 1990, 64, 307. [ 1101 W. Chen, Y. Ouchi, T. Moses, Y. R. Shen, K. H. Yang, Phys. Rev. Lett. 1992, 68, 1547. [I1 11 S. Immerschitt, W. Stille, G. Strobl, Macrumolecules 1992, 25, 3227. [I121 G. Decher, J. Reibel, M. Honig, I. G. VoigtMartin, A. Dittrich, H. Ringsdorf, H. Poths, R. Zentel, Ber. Bunsenges. Phys. Chem. 1993, 97, 1386. [ 1131 E. M. Terentjev, J. Phys. France 1995, 5, 159. 11141 M. C. Holmes, N. Boden, K. Radley, Mul. Cryst. Liq. Cryst. 1983, 100, 93. [ 1 151 U. Kaeder, K. Hiltrop, Mol. Cryst. Liq. Cryst. Lett. 1991, 7, 173. [ 1 161 A. Poniewierski, R. Holyst, Phys. Rev. A 1988, 38, 372 I . [I171 T. Yoshino, M. Suzuki, J. Phys. Chem. 1987, 91, 2009. [ I 181 E. A. Oliveira, A. M. Figueiredo Neto, G. Durand, Phys. Rev. A 1991, 44, 825.
11 Ultrasonic Properties Olga A. Kapustina Liquid crystal acoustics is an extremely diverse science insofar as the range of the problems that is covers is concerned. In recent years many experimental and applied investigations have been performed which have given rise to new branches of this science. We present here the current state of liquid crystal acoustics and discuss the most important advances in and the future potential of the field. The classical aspects of the subject are outlined briefly, with reference to associated chapters in this book.
11.1 Structural Transformation in Liquid Crystals Since the very beginning of the research on mesomorphism, the influence of ultrasonic fields has been of great importance; only the goals of study have changed with time. The early research on which the later developments were based was done by Lehman [ 11, Zolina [2], Zvereva and Kapustin [ 3 ] , and Fergason [4]. Discussion about the nature of the phenomena observed simulated much work in the pioneering days [5131. The various principles used to interpret the in
fluence of ultrasonic fields on the mesophase were of exceptional theoretical importance. These included interpreting the effects of the field on the molecular arrangement of the liquid crystalline state on the basis of the LeslieErickson hydrodynamic theory or, as Kozhevnikov later demonstrated, using models adapted from nonequilibrium hydrodynamics. This variety of approaches to the problem was a result of the complex nature of the phenomena. The effect of ultrasound on the mesophase is, as a rule, associated mainly with the onset of flows induced by nonlinear phenomena. The flow process is characterized by an essentially stationary velocity distribution in the layer. Calculation and experimental determination of the flow velocity present major difficulties. Flowinduced disturbances in the molecular arrangement can be of several kinds; in particular, they can be both of the threshold or nonthreshold type and modulated or unmodulated. Modulated disturbances always show threshold behavior. Most of the data available at present refer to the nematics, the characteristic properties of which are manifested to certain degree in the smectics and in cholesterics. Ultrasonic field effects are covered in several reviews and monographes [13191.
448
11
Ultrasonic Properties
11.1.1 Orientation Phenomena in Nematics All research on the changes in the macrostructure of nematics when i n an ultrasonic field is done on samples 10360 pm thick and using generally accepted optical methods. Any changes are observed either as a result of the depolarization of light transmitted through the sample or because of light scattering by the inhomogeneous structure [20]. Such experiments have shown three kinds of layer structure disturbance: homogeneous, spatially periodic, and inhomogeneous. Naturally, intermediate states between these three extreme phenomena are possible.
11.1.1.1 Homogeneous Distortion Stage This stage involves longitudinal waves [ 5 , 10, 21, 341 and surface acoustic waves (SAWS) [9, 3540], with wavevectors k = o l c and k , = olc,, respectively, where c and C , are phase velocities and m is the angular frequency of the wave. Typical geometries of the equipment used for experiments on homeotropically aligned nematics are shown in Fig. 1. The wavevector is parallel or perpendicular to the director iz and makes an angle 8 with i z . The measurement ofultrasoundinduced birefringence offers an excellent tool for studying orientational phenomena and checking models. The characteristic properties of the effect that can be elucidated experimentally are [ 5 , 9, 10, 2140]: Ultrasonic longitudinal and surface waves applied to a nematic sample change the birefringence properties of the fluid in the reflective and transmission modes when the ultrasound intensity J e x ceeds a certain minimum value [9, 10,22, 26, 271.
Longitudinal wave
Shear vibration
z $i
3
4
Longitudinal wave
Shear Compression vibration
Figure 1. Equipment geometries used for studying ultrasonically induced structural transformations in liquid crystals: (a) longitudinal waves, k [In;(b) SAW, k , l n : (c) longitudinal waves, kyin, &O; (d) shear vibrations, k , l n : (e) longitudinal waves, k l n : (f) shear and compression vibrations, k s l n , klln.
The conditional clearing threshold of the ultrasound intensity J'hfor birefringence is dependent on the layer thickness as d* 122, 25, 271. The frequency dependence of the threshold Jthis given by Jth~ f  ' '[ 17, ~ 22, 271. The value of the threshold can be reduced by 'biasing' the sample with an electric field [lo]. Above the threshold: the relation between the optical transmission m of the nematic layer and the ultrasound intensity J is nonlinear [lo, 22, 25, 271; the transmission depends on the ultrasound intensity as m=sin2 (const.J2) and shows interference maxima and minima between ordinary and extraordinary light rays for monochromatic light [21, 251; and for small values of the intensity m=J4 [21, 381. The optical transmission properties of nematic samples depend on the acoustic boundary conditions (cells with fixed
1I . 1
Structural Transformation in Liquid Crystals
[22] or free [2 I] edges) and on the molecular orientation at the boundaries (planar or homeotropic configurations [27]). The variation in the orientation of the molecules in the ultrasonic field is observed as a system of alternating light and dark bands, the width and contrast of which depend on the ultrasound intensity. The distance between the centers of the light bands is of the order of the ultrasound wavelength [9, 12, 13, 2 1, 22, 27, 29, 35, 3840]. The band configurations depend on the cell structure, the acoustic boundary conditions and the mutual orientation of the wavevector and director; these clearing patterns may be distorted by nonuniformity of the wave field inside the ultrasonic beam. Several theories aimed at explaining the phenomena have been proposed, each of which is founded on completely different concepts. Sripaipan et al. [21] proposed a nematic layer with free ends, in which the interaction between the longitudinal oscillations (induced by the motion of the free ends of the layer in compression) and the traverse oscillations establishes steady flow of the liquid and, as a result, rotation of the molecules. However, these authors used incorrect dispersion relations and their calculations are not consistent with observed layer compression patterns. Nagai and coworkers [26,27] hypothesized that with normal incidence of an ultrasound beam on the layer the rotation of molecules is attributable to radiation fluxes. Radiation fluxes are the steady acoustic trows caused by radiation forces in a traveling acoustic wave, the only provision being that the width of the ultrasound beam is smaller then the dimensions of the cell. In reality, radiation fluxes can only occur near the boundaries of the beam and produce a compression effect that is smaller than the one that is actually ob
449
served [22, 251. Radiation fluxes are significant when an ultrasound beam is focused so that it is obliquely incident on the layer [28]. Helfrich [ 3 3 ] and Chaban [34] treated molecular rotation as a threshold effect associated with the fact that the equations of motion for nematics contain nonlinear stresses proportional to the angle of molecular rotation and the particle velocity. However, the theoretical values obtained by these authors for the threshold ultrasound intensity are 23 orders of magnitude greater than the intensities usually observed experimentally. Dion and coworkers [4 143] hypothesized that torques created by the sound absorption anisotropy are responsible for rotating the molecules, which tend in turn in such a way as to diminish the losses in the ultrasound wave. This effect is theoretically possible, but is two or three orders of magnitude smaller than what is observed experimentally. Kozhevnikov and coworkers [44461 have developed the most general theory, which is based on LeslieEricksen hydrodynamics. These workers attributed the orientation effects to the steady inhomogeneous acoustic flows that result from the interaction between the periodic compression of the layer in the ultrasound field and the periodic motion of the liquid along the plates confining the layer. Unlike previous theories [27,33,34,41431, Kozhevnikov’s model predicts the effect observed for normal incidence of the ultrasound on the layer. In the case of k 11 n, according to the theory [44, 451, two physical reasons are responsible for the periodic liquid motion that occurs in the cell: vibrations of the cell plates in the layer having free ends [21, 441 and pressure gradients near the border of the beam for an infinitely wide layer [45]. In all instances, the acoustic flow velocity component along the x axis, V ,that initiates the director rotation, satisfies a wellknown
450
11 Ultrasonic Properties
acoustics equation [47]. The equation for the small steadystate angle is [48]
Information on the velocity flows, configuration, scale, velocity distribution and the suitable distortion profiles of the director field of the layer under the action of an ultrasonic field for the qualitatively different situations presented above can be found in the literature [44, 451. The distortion of the layer structure is usually studied by estimating the optical phase differences A, of the light that is polarized in the plane of the sandwichcell plates, or the optical transmission m of the layer. The latter quantity can be calculated from the intensity I of the light transmitted through the layer parallel to the z axis and under crossed polarizers, the initial intensity I,, and A, according to m = I/I, sin2Ao12 [20]. It is useful to introduce the effective clearing threshold Jthas the ultrasound intensity (or displacement amplitude) at which m=0.01 [ 171. Sometimes, in order to compare theoretical prediction with experimental results it is also possible to estimate the ultrasound intensity at which A, = n (i.e. the depth of light modulation is 100%). Many experimental data are presented in some detail and are discussed quite throughly by Kapustin and Kapustina [17, 181. Kozhevnikov’s theory is borne out by the facts. For example, according to Gus’kov and Kozhevnikov [45], in a cell with fixed ends, fh=d2.5f’.The experimental values of Jthobtained by Kapustina and Lupanov [22] and Hatakeyama and Kagawa [25] also follow this law (Fig. 2). Recent data on the qualitative behavior of Jth for some equipment geometries are summarized in Table 1 [44461. It has recently been shown that the flow structure depends on both the inhomogene
6 4
Figure 2. Effective clearing thresholds Jth for a 10126 pm sample of MBBA in the ultrasound frequency range: ( 0 ) 0.4, (0)I , (A) 3.2 MHz.
ity of the wave field in the cell and d/A, where A is the length of the elastic wave (see in [ 181). In the ultrasound frequency range (d/A@1) the efficiency of the flow generation is high if the typical value of the wave inhomogeneity length lcis in the vicinity of A. In this case J1O0%= (4 I . / K ~ ~ ) J A ~ ~ ~ , where is the value of JIo0% for the wave field with K f A; 6= ( p d 2 q)%is the wave number in a viscous wave. At hypersonic frequencies ( d l b l), when the sound absorption in nematics is sufficiently high, J’oo” = (4 a 2 n ~ 6 d ) J ~ In ~ ~nematics ” . the sound absorption coefficient a is usually about 20 dB cm’. The preceding discussion is summarized in Table 2 using the terminology of Russian physists for the comparison of the flow efficiency [ 181. Information concerning the ultrasoundinduced birefringence in homeotropic nematics when the k makes an angle with n (see Fig. 1 c) can be found in the literature [19, 28, 301. The theoretical aspects of the problem cannot be detailed here and the reader is referred to the paper by Zhukovskaya et al. [46], wherein the flow mechanism of the aligning effect of an ultrasound wave or beam on a sample layer is discussed. In this case the flow is induced by nonline
11. I
45 1
Structural Transformation in Liquid Crystals
Table 1. Effective clearing thresholds 0 (")
Boundary conditions
Equipment geometry
Compression wave
0
Acoustically rigid
Cell of radius R
Compression wave
0
Acoustically soft
Infinitely wide cell; ultrasound beam of radius R
Type of wave
Effective threshold jth2d2.Sfl
.Ith=&'5 f  0 5 jlh2d2
Sf0 5
Remarks 
thick layer thin layer
x exp [8,(Rr)l
Compression wave
0
Acoustically soft
Infinitely wide cell; beam in the form of a strip
Compression wave
0#0
Acoustically soft
Infinitely wide cell; beam of radius R
90
Acoustically soft
SAW
Jth=d2'f
O'
Jth=d' 25 jth=dO7

first maximum second maximum two cell eigenmodes
~
Here value of R is the radius of a ultrasonically irradiated circular zone: an ultrasonic beam of radius R is incident on the layer of infinite width or an ultrasonic wave is incident on the layer of radius R pressed between a transparent plate and a thin wafer or elastic film; the value of r is a component of a cylindrical coordinate system (r, cp, z) with zaxis directed along the normal to the layer plane, while the boundary of the layer have the coordinates z = +d/2; the value of &=W 26d is the coefficient of attenuation of longitudinal waves in the layer; the source of these waves in the layer is nonuniform compression near the boundaries of the ultrasonic beam or it is the nonuniformity of compression of the layer as a result of bending of the thin wafer or film at the edges. So that the value of &(Rr) describes the attenuation of longitudinal waves during propagation along the width of the liquid crystal layer in the radial direction both into and outside of the ultrasonically irradiated region; the value oft:", is the threshold of displacement amplitude of SAW.
Table 2. Values of J'OO" versus the frequency and order of the inhomogeneity of the field. Jll"'" Layer Frequency Order of thickness inhomogeneity, ( P I (Hz) K (mW cm2)
10 10 10
1o6
1o6 1 o9
h 2h
10 20

1
ar boundary forces due to the interaction between the longitudinal and viscous waves. According to this theory, the maximum of the effect corresponds to the maximum of the acoustic transparency of the cell, while the relationship between Jthand d depends on the angle of incidence of the ultrasound wave or beam (see Table 1 ) . This the
ory correlates with the experimental results reported by Hareng and coworkers [ 19,301. There have been unanimously verified reports of steadystate distortion of a homotropically aligned nematics in a SAW field [9,35401. In this case the wave field in the layer is caused by the mixing of several cell eigenmodes that have different phase velocities excited in the layer when a SAW propagates in one of the bounding plates. Thus the number of modes depends on d/A. Earlier work concentrated more on the phenomena themselves rather than their interpretation [9, 391. Calculated values obtained using theories based on viscoelastic effects and the parametric instability [34371 show considerable discrepancy with experimental data. Miyano and Shen [38] have inves
452
11
Ultrasonic Properties
tigated flows in a nematic layer with the SAW propagation along the substrate (see Sec. 11.2 of this chapter).
11.1.1.2 Spatially Periodic Distortion Stage Domains of different nature in homeotropically and planar oriented layers may appear under the action of longitudinal or shear waves only above a certain threshold. The directions of the domains, their width, and the threshold value depend on the type of the wave, the wave frequency, and the layer thickness. Russian physists were the first to observe ultrasonically induced domains in nonoriented samples [5]. Later, Italian and Japanese physists investigated the appearance of domains in a homeotropic layer subjected to shear vibrations, created by the ac motion of one of the cell plates in its plane (see Fig. 1 d) [49521. The domain lines always aligned perpendicular to the shear direction. A theoretical attempt to describe the domains [53] was concerned with a periodic shear strain, but this model does not fit what is observed experimentally: in particular, the threshold values of the shear amplitude to not fit the experimental values in terms of magnitude, do not exhibit the experimentally observed dependence on the frequency and layer thickness, and fail to give the domain dimensions. Kozhevnikov [54] has analyzed the effect on the basis of the equations of the hydrodynamics of nematics, retaining the quadratic terms proportional to the product of the angle of rotation of the molecules and the velocity of the liquid. The model leads to the following picture of the effect. A periodic shear, in the case of a random slowly varying and periodic (along the layer) deviation of the molecules from the normal, creates eddies oscillating at the shear fre
quency. The interaction of the eddies with the initial shear field gives rise to an average moment which increases the deflection of the molecules. The threshold amplitude and domain size are given by
where p = nld, q = nlL, and qo is the wavenumber at the threshold of the effect; for information concerning the form of function F ( q , p ) see Kozhevnikov [54]. Figure 3 shows the theoretical and experimental dependences of the threshold shear amplitude on the frequency for various values of d [49, 52,551. It is evident that in the range of validity of the calculations, Kozhevnikov’s theory and the experimental data agree well. According to Kozhevnikov [54], the theory considers the frequenciesf satisfying the inequalities 7rK312 y, d2 f 4pc’I2 R 17 and f < 1712 npd2. Russian physists [56,57] have performed systematic investigations of the condition
+
k\
L
+04
40 f
i

40”
(Hz)
Figure 3. Calculated (lines 1 and 2) and measured
(symbols) threshold displacements 1 , the amplitude of the threshold particle velocity is virtually independent of temperature and follows the law: u ~ ~ = A T  ~ [58]. This agrees with the experimentally observed data (Fig. 5 b). The foregoing discussion illustrates that the new approach proposed by Russian physists is valid.
11.1.1.3 Inhomogeneous Distortion Stage
Figure 4. Diagram of a cell with domains in crosssection: (1) Ultrasound, (2) system of oscillatory vortex flow with the velocity v ~ = c o s q i ,(3) stationary flows, (4) profile of distortion of the nematic orientation, ( 5 ) nematics molecule, (6) acoustically rigid boundary, (7) acoustically soft boundary.
This stage involves the phenomena corresponding to higher excitation: at a definite threshold the nematic layer exhibits orientational turbulence, corresponding to observable light scattering. Kapustin and Dmitriev [ 5 ] were the first to observe this effect on a nonoriented sample in a field of longitudinal waves. Later, Kessler and Sawyer [7] found that the intensity of this scattering depends nonlinearly on the excitation level. By analogy with a similar phe
454
11
Ultrasonic Properties
IGO
5
h
420
Y
4
80
40
(b)
Nemdtic
pease
I s o t o p i c pRwse
I
30
20
\
10
0
AT#( "C)
Figure 5. Ultrasonically induced orientational instability in planar nematics. (a) Spatial period of domains versus layer thickness,f= 3.2 MHz, T = 30.2 "C. (b) Calculated and measured threshold parameters characterizing the wave field in the layer versus temperature of the nematics; the running values of Urh(tension) and uth are normalized to the values of U,': and u,", corresponding to the lower limit of the test temperature interval (T= 22.8 "C), AT= TN, T.
nomenon in an electric field, this effect is called the acoustic dynamic scattering mode (DSM). The characteristic properties of this effect are as follows [22, 56, 59, 601: The intensity and angular distribution of the scattered light are independent of the wavelength and polarization of the incident light, and the scattering is directed mainly forward. The intensity and frequency of the ultrasound play an important role. Instability begins just above a threshold value J:h. Sometimes domains appear first, and then
gradually switch over to the DSM with increasing intensity of the ultrasound. The effect reaches maximum scattering (saturation) at an excitation level of about 68 times J:h.The threshold value is virtually independent of the substance, and hardly varies from the thickness of the layer (J:h= 1/d2) [22]. The initial orientation of the molecules in relation to k and to the boundary surfaces does not play a critical role, but it does have importance in technical application [22, 56, 591. The rise and decay times are influenced by many parameters (viscosity, sample thickness, intensity, etc.) [ 17, 591. This problem has not yet been studied theoretically. However, the progress made to date in the area of experimental research clearly foreshadows rapid advances in the future. The flows generated by ultrasound create optical inhomogeneities in the layer that act as individual scattering centers. Bertolotti and coworkers [50, 601 have measured the coherence length of scattered light on the hometropic samples. The transition to the disordered state is accompanied by a drop in the coherence length to a rather small value, and the sample behaves as a thermal source containing a large number of statistically independent scattering centers. The sample thickness and observation angle do not play a critical role. Many features of the acoustic DSM have been studied with regard to technical applications [59]; this applies in particular to rise and decay times [ 17,591. Several technical studies have been concerned with contrast ratio [ 17, 591. Kapustina [61] has recently reported on the acoustic DSM induced by ultrasound (1.5 MHz) in a polymerdispersed nematic film.
11.1
Structural Transformation in Liquid Crystals
11.1.2 Cholesterics in an Ultrasonic Field The behavior of cholesterics in an ultrasonic field has generally been far less well researched than that of nematics. Only a few aspects of the problem have been examined since the systematic investigations done by Russian and Italian physists [ I7,58,6265]. It may therefore seem to be somewhat stretching a point to draw an analogy with the phenomena in nematics, but this is a valuable way to obtain an overview of the following rather complex phenomena: 




periodic twodimensional distortion, analogous to nematic domains (k parallel to the helical axis); excitation of the storage mode via turbulent flow, analogous to acoustic DSM in nematics ( k parallel or perpendicular to the helical axis); erasing of the storage mode ( k parallel to the helical axis); focalconic texture transformation into a planar one (k parallel to the normal to the layer); bubble domains texture formation ( k perpendicular or parallel to the helical axis); fingerprint texture transformations ( k parallel to the normal to layer).
455
independent of frequency. By analogy with nematics, Kozhevnikov [62] described this phenomenon within the framework of an approach based on nonequilibrium hydrodynamics, but introduced the added assumption of an initial deformation of the layered systems in the crystal axis direction. The threshold amplitude ahhand the size of the domains L in the equilibrium layers or the layers extended along the crystal axis are determined. As with nematics, two frequency bands (limiting value of B = 38 77 n2/pw2z d 2 ) appear here also to be due to dissimilar behaviors of the threshold and domain size relative to d, p , , f , etc. In particular, for COT& 1 ( B e 1, high frequency) the value of ahh= (p, d)x ( ll)%, whereas in the case of wz+ 1 ( B & 1, low frequency) the value of z9Ah is also independent of frequency and follows the law: 8hh=(d/pJX (1l)%. Here 1 = A/A, is a relative value of the layer extension (A, is the critical extension of the layered system when the domains appear under static deformation [48, 661 and A is the extension of the layer). According to the theory [ 5 8 ] , the domain size L is approximately ( p o d ) %over all the frequency range. The correlation between the experimental data and this theory is satisfactory only if the initial deformation of the layered system is taken into account; the relative value of the layer extension is then found to be close to 0.80.9.
11.1.2.1 Periodic Distortion An ultrasonic field applied parallel to the helical axis h (k llh) can cause a square gridlike pattern deformation of the planar texture [17, 58, 621. This can be observed in nematic/cholesteric mixtures with a helix of large pitch. According to experimental data, the spatial period of distortion follows the equation L  ( p , d ) % and tends to decrease slightly with frequency. The threshold particle velocity in the wave Ohh is practically
11.1.2.2 Storage Mode The interest in this area is due more to the possibilities of technical application than theoretical considerations. Gurova, Kapustina, and Lupanov were the first to transform the uniform planar texture of a nematidcholesteric mixture sample into a focalconic one by means of an ultrasound field [ 17,591. The helical structure is still present in this state, having the same pitch on a microscop
456
11
Ultrasonic Properties
ic level. Macroscopically, the sample is broken up into a myriad of randomly oriented domains with the size of a few micrometers, and consequently it strongly scatters visible light of all wavelengths. Such a texture is said to be stable for up to several days, during which time it gradually reverts to the planar one. The initial texture can be restored at any time by applying an ac pulse (20 kHz) 159,641. Russianphysists have described the ultrasonically initiated storage effect 1641. Their data for the contrast ratio and for the rise and decay times have not as yet been improved upon. As mentioned above, the stored information slowly decays, but it persists in certain mixtures for several days after ultrasound excitation has been removed. Thickness, pitch and boundary conditions were found to play a crucial role in the memory properties of the planar to focalconic texture transformations [ 17, 591.
mensurate with the pitch of the helix, is accompanied by the formation of a bubble domain, which is a strong light scatterer. These data and the mechanism of the formation and stabilization of bubble domains have been discussed within the framework of the Akahane and Tako model 1681. This model attributes the formation and high stability of the bubble domains to the presence of defects (disclinations) in the sample, which pin the domains. The model does not take into account the interaction of the domains, and is thus valid in the case of low density domain packing. Test bubble domains have provided the first possibility for a quantitative analysis of the model, since they have a rather low packing density. The correlation of the theory with the experimental data is fully satisfactory (Fig. 6).
JC
11.1.2.3 FocalConic to Planar Texture Transition Ultrasound waves may also create an oriented structure. This effect was observed in a sample with a focalconic texture subjected to ultrasound (0.4 and 3.2 MHz [ 17,671). According to Hiroshima and Shimizu [67], the transmission of a sample (a nematickholesteric mixture) increases with increasing ultrasound intensity tending towards a value characteristic of a planar texture.
11.1.2.4 Bubble Domain Texture Gurova and Kapustina were the first to describe ultrasonically induced bubble domains in large pitch nematickholesteric mixtures 117, 631. It was found that relaxation of an ultrasoundinduced perturbation at a critical layer thickness, which is com
Figure 6. Comparison of Akahane and Tako's model and the experimental data. The calculated bubble domain diameter D and the free energy F,,,,, normalized to the layer thickness d and the free energy of the homeotropic structure F,, respectively, versus the ratio dip, (curves I and 11). Pitches (pm): ( 0 ) 3, (B) 4.2, (A) 10.5, (x) 48 (f=0.2 MHz). Frequency (MHz): (0) 0.5, (n) 3 (P=48 pm).
11.2
11.1.2.5 Fingerprint Texture Transition Bertolotti et al. [65] have studied the behavior of a wellknown fingerprint texture [69] formed in a sample (a nematickholesteric mixture) due to periodic compression in the frequency range 0.1 Hz to 130 kHz (freeedge cell). All the data obtained were analysed within the framework of PressArrot’s model [70].
11.1.3 Smectic Phase in an Ultrasound Field There has been no systematic study of this area because at present no potential technological applications of smectics in conjunction with ultrasound are known. Thus we have only a fragmentary picture from the few isolated investigations that have been made of smectic phases in ultrasound fields [ 5 , 59, 71, 721. Visual observations have shown that the optical transparency of a nonoriented sample of a smectic A phase under the action of longitudinal waves is diminished as a result of light scattering due to fluctuations in the refractive index [73]; transparency is not restored to its initial value when the disturbance is removed [ 5 ] . Italian physists have performed experiments on homeotropic smectic A layers and observed an ultrasonically induced spatially periodic structure distortion, including the formation of domains with relaxation times of up to several hours [71]. Russian physists have acknowledged the ability of smectic A phases to preserve remanent strain [72]. They investigated the behaviour of a homeotropic sample under the action of longitudinal waves. According to these data the smectic A phase exhibits an ultrasonically induced storage mode, where the remanent optical transparency barely differs from the value observed at the onset of the action of
Wave Interactions in Nematics
457
the ultrasound waves. It this case the storage effect is highly pronounced. The thickness of the sample and the method of preparation of the plate cell surfaces were found to affect both the contrast ratio and the efficiency of the transition from the transparent to the opaque structure. As in cholesterics, recovery of the initial orientation in smectic phases is realized by the application of an electric pulse (20 kHz, 200 V) [72]. All the abovedescribed studies were concentrated more on the phenomena themselves than on their interpretation.
11.2 Wave Interactions in Nematics All meaningful contributions i n this area are relatively recent because, without the support of Vuzhva’s theory [40], earlier observations have remained partly inexplicable [35, 36, 42, 741. Since the systematic studies done by Miyano and Shen [38], only a few aspects of the problem have been examined. Three simple cases can be differentiated: the interaction of two nematic cell eigenmodes with different phase velocities [401;  the interaction of the nematic cell eigenmode and the viscous wave [75];  the interaction of the elastic and viscous waves [76]. 
The mathematical models proposed by Kozhevnikov and coworkers [44461 paved the way for the development of a general wave interaction theory based on the unified concept: steadystate inhomogeneous acoustic flows. The validity of this theory [40, 751 is borne out by the following observations related to the traditional geome
458
11
Ultrasonic Properties
try. A homeotropically oriented nematic, several tenths of a micrometer thick, was placed between the substrate ( I ) and a glass plate (2) and observed under a microscope (Fig. 7). In a first scenario (Fig. 7 a), an interdigital transducer (3) generated the SAW at the substrate (1). Within the range of frequences that satisfy the inequalities d < A and d$&, the SAW excites only two nematic cell eigenmodes with phase velocities c i and c2=c/2. The velocity components of the modes obey the following conditions: 191xD,>D,,,) disagrees with theoretical predictions, and the alternation is opposite to that predicted by calculations using the ChuMoroi model [8] (Eqs (6a) and (6b)).
a1 clearing points T,, the diffusivity components show an oddeven alternation parallel to the clearing temperature, which changes to a n'= 036 alternation also exhibited by the nematic activation energies if compared at constant temperture T [50]. In the first case one has Dll>D, and, surprisingly,
The most striking distinction from nematic diffusivities is that NMR pulsefieldgradient measurements [24, 561 of smectic mesophases show Arrheniustype behavior of D, and Dllwith strongly different activation energies, namely El< Ell.As a consequencs, the two plots can cross [24], either within the smectic phase or outside by extrapolation, and with decreasing temperature the anisotropy ratio CT can change from 20
5CB, 4’hpentylPAA, 4,4’dinbialkoxyazoxybenzene;MBBA, 4methoxybenzylidene4’nbutylaniline; 4cyanobiphenyl; 5OCB, 4’npentoxy4cyanobiphenyl; TBBA, terephthalylidenebis(4nbutylaniline); C 12BAA,C I 2benzylideneaminoazobenzene; PL, potassium laurate; DPPC, dipolmitoylphosphatidylcholine.
490
13
Diffusion in Liquid Crystals
ly. In the easy direction diffusion constants are of similar order of magnitude as in thermotropics, namely typically about lo' I to 1010
m2 sl
13.4.7 Selected Diffusion Constants Table 1 lists a few pulsedfieldgradient measurements of diffusion constants for some familiar mesophases considered in the text. Extensive data have been collected by Kruger [24] and by Lindblom and Oradd [ 2 5 ] ; further more recent references have been summarized by Karger et al. [38].
13.5 References [ I ] G. Vertogen, W. H. de leu, Thermotropic Liquid
Crystals, Fundamentals, Springer Verlag, Berliln 1988, 201. [2] P. de Gennes, J. Prost, The Physics of Liquid Crystals, Clarendon Press, Oxford 1993, 250. [3] L. M. Blinov, V. G. Chigrinov, Electrooptic Effects in Liquid Crystal Materials, Springer Verlag, Berlin 1994, 89. [4] W. Jost, K. Hauffe, Diffusion, Methoden der Messung und Auswertung, Dr. Dietrich Steinkopff Verlag, Darmstadt 1972, I. [5] H. J. V. Tyrrel, K. R. Harris, Diffusion in Liquids, a Theoretical and Experimental Study,Butterworths, London 1984, 56. [6] A. Ferrarini, P. L. Nordio, G . J. Moro in The Molecular Dynamics of Liquid Crystals (Eds. G. R. Luckhurst, C. A. Veracini), Kluwer, Dordrecht 1994, 4 1. [7] R. Blinc, M. Burgar, M. Luzar, J. PirS, L. Zupanc'ic', S. Zumer, Phys. Rev. Lett. 1974, 33, 1192. [8] K. S . Chu, D. S. Moroi, J. Phys. Colloq. 1975, 36, C199. [9] K. S . Chu, D. S . Moroi, Mol. Cryst. Liq. Cryst. 1981, 67, 109. [ l o ] A. J. Leadbetter, F. P. Temme, A. Heidemann, W. S. Howells, Chem. Phys. Lett. 1975, 34, 363. [ 1 I ] F. Volino, A. J. Dianoux, A. Heidemann, J. Phys. Lett. 1979, 40, L583. [ 121 G. Moro, P. L. Nordio, U.Segre, Mol. Cryst. Liq. Cryst. 1984, 114, 113.
[I31 S. Hess, D. Frenkel, M. Allen, Mol. Phys. 1991, 74, 765. [14] W. Franklin, Phys. Rev., Sex A 1975, 11, 2156. [I51 S. Tang, G. T. Evans, J. Chem. Phys. 1993, 98, 728 1. [ 161 M. E. Moseley, A. Loewenstein, Mol. Cryst. Liq. Cryst. 1982, 90, 117. [17] A. Kozak, D. Sokolowska, J. K. Mosciki, Proc. ECLC, Bovec, Slovenia 1995, 178. [I81 R. M Clegg, W. L. C. Vaz in Progress in ProteinLipid Interactions (Eds. A. Watts, J. J. H. H. M. De Pont), Elsevier, Amsterdam 1985, 173. [I91 M. H. Cohen, D. Turnbull, J. Chem. Phys. 1959, 31, 1164. [20] M. P. Allen, D. J. Tildesley, Computer Simulations o f l i q u i d s , Clarendon Press, Oxford 1989, 182. [21] A. Alavi, D. Frenkel, Phys. Rev. 1992, 45, R5355. [22] G. Kromer, D. Paschek, A. Geiger, Bev. Bunsenges. Phys. Chem. 1993, 97, 1 188. [23] T. Svedberg, Kolluidzeitschrift 1918, 22, 68. [24] G. J. Kriiger, Phys. Rep. 1982, X2, 229. [25] G. Lindblom, G. Oradd, Prog. NMR Spectrosc. 1994, 26,483. [26] C. K. Yun, A. G. Fredrickson, Mol. Cryst. Liq. Cryst. 1970, 12, 73. [27] A. V. Chadwick, M. Paykary, Mol. Phys. 1980, 39, 637. [28] F. Rondelez, SolidState Commun. 1974,14,815. [29] H. Hakemi, M. M. Labes, J. Chem. Phys. 1975, 63, 3708. [30] M. Daoud, M. Gharbia, A. Gharbi, J. Phys. I I (France) 1994,4, 989. [31] T. Moriyama, Y. Takanishi, K. Ishikawa, H. Takezoe, A. Fukuda, Liq. Cryst. 1995, 18, 639. [32] P. A. Egelstaff, An Introduction to the Liquid State, Clarendon Press, Oxford, 1992, 217. [33] J. A. Janik, Acta Phys. Pol. 1978, AS4, 513. [34] J. Topler, 8. Alefeld, T. Springer, Mol. Cryst. Liq. Cryst. 1973, 26, 297. [35] M. Bee, A. J. Dianoux, J. A. Janik, J. M. Janik, R. Podsiadly, Liq. Cryst. 1991, 10, 199. [36] A. Abragam, The Principles of Nuclear Magnetism, Clarendon Press, Oxford 1961, 265. [37] J. H. Freed, A. Nayeem, S. B. Rananavare in The Molecular Dynamics of Liquid Crystals (Eds. G. R. Luckhurst, C. A. Veracini), Kluwer, Dordrecht, 1994, 71. [38] J. Karger, H. Pfeifer, W. Heink, Adv. Magn. Reson. 1988, 12, I . [39] I. Chang, F. Fujara, B. Geil, G. Hinze, H. Sillescu, A. Tolle, J. NonCryst. Sol. 1994, 172, 674. [40] R. Blinc, J. PirS, I. Zupanc'iE, Phys. Rev. Lett. 1973, 30, 546. (411 S. Miyajima, A. F. McDowell, R. M. Cotts, Chem. Phys. Lett. 1993,212,277. [42] G. Rollmann, Thesis, University of Stuttgart 1984.
13.5 [43] J. 0. Mager, Thesis, University of Stuttgart 1993. [44] N. A . P. Vaz, G. Chidichimo, Z. Yaniv, J. V. Doane, Phys. Rev. 1982, A26, 637. [45] R. Stannarius, H. Schmiedel, J. Magn. Reson. 1989, 81, 339. [46] R. Blinc, V. Dimic, Phys. Lett. 1970, 3IA, 531. [47] K. Otnes,R. Pynn, J. A. Janik, J. M. Janik, Phys. Lett. 1972, 38A, 335. [48] W. Wolfel, Thesis, University of Stuttgart 1978. [49] S. Ghosh, T. Tettamanti, Chem. Phys. Lett. 1980, 69, 403. [50] F. Noack, Mol. Cryst. Liq. Cryst. 1974, II3,247. [51] G. Kruger, H. Spiesecke, Z. Naturjorsch. Teil a 1973, 28, 964. [52] 1. Zupantit, J. PirS, M. Luzar, R. Blinc, Solid State Commun. 1974, 15,227. [53] H. Hakemi, M. M. Labes, J . Chem. Phys. 1974, 61, 4020. [54] H. Hervet, W. Urbach, F. Rondelez, J. Chem. Phys. 1978,68,2725.
References
49 1
[55] F. Noack in Proc. AMPERE Summer Institute on Magnetic Resonance (Eds. R. Blinc, M. Vilfan), J. Stefan Institute, Ljubliana, Slovenia 1993, 18. [56] M. Hara, S . Ichikawa, H. Takezoe, A. Fukuda, Jpn. J . Appl. Phys. 1984, 23, 1420. [56a]G. J. Kruger, H. Spiesecke, R. van Steenwinkel, F. Noack, Mol. Cryst. Liq. Cryst. 1977,40, 103. [57] H. Hakemi, Mol. Cryst. Liq. Cryst. 1983, 95, 309. [58] R. T. Roberts, Nature 1973, 242, 348. [59] A. L. Kuo, C. G . Wade, Biochemistry 1979, It?, 2300. [60] P. Ukleja, J. W. Doane in Ordering in Two Dimensions (Ed. S. K. Sinha), Elsevier, Amsterdam 1980,427. [61] G. Lahajnar, S. h m e r , M. Vilfan, R. Blinc, L. W. Reeves, Mol. Cryst. Liq. Cryst. 1984, 113, 8592. [62] R. Homan, H. J. Pownall, Biochim. Biophys. Acta 1988, 938, 155.
This Page Intentionally Left Blank
Index
absorption, optical 1 19, 21 9 ac calorimetric techniques, phase transitions 2 14 achiral polyphilics, polar 406 acoustics 273,458 ff acoustoelectrical interactions 460 f acoustooptical effect 460 adiabatic calorimetry 2 13 AkahaneTako model 456 alignment  local molecular 304  nematics 32 alkyl groups  evenoddeffect 233  phase stability 298 AMBER force field 77 anchoring 12  directorfield interactions 398  elastic properties 158  external fields 390  flowiviscosity 365  instabilities 421  nematics 30  solid substrates 439  surface alignment 434 f  textures 308 AndereckSwift theory 283 anhydrous soaps, density measurements 24 1 anisotropic fluids, dielectric properties 133 f anisotropic interactions 44 surface alignment 433 anisotropic materials, tensor properties 871 0 1 anisotropic modes 419, 425 anisotropy  external fields 381  magnetic 102  orientational 151 ultrasonic properties 460 anisotropy ratios, diffusion 489 antiferroelectrics 406, 41 1 argon saturation, phase transitions 257 Arrhenius law 147,483 associations, defectsitextures 346 atomistic simulations, bulk systems 83 

backflow effect directorfield interactions 388  flowiviscosity 361  smectics 408 balance laws, nematics 35 band configuration, ultrasonic properties 449 barometric method, highpressure experiments 26 I BeerLambert law, optical properties 119 bend deformation directors 442 elastic properties 154, 165 benzenes, reentrants 289 biaxial nematics flowiviscosity 366  transitions 181 biaxial smectics, torsional elasticity 156 biaxial structures, meanfield model 200 biaxiality induced 381  molecular 42, 56 bicritical behavior, phase transitions 268 bilayers atomistic simulations 85  textures 307 birefringence  elastic constants 169  external fields 382  ultrasonic properties 448 Bloch walls, defects 3 13 blue phases cholesterics 40 I , 475 external fields 383 transitions 223 BMAB, density measurements 240 body forcesimoments, nematics 28 Bohr magneton 104 Boltzmann distribution, modelling 74 Boltzmann factor, diffusion 482 bond ordering, phase transitions 191 bond stretches, molecular modelling 73 bookshelf structures, external fields 404 boundary conditions clearing thresholds 45 1 molecular modelling 77 nematics 30  twisted periodic 85 boundary effects, ultrasonic properties 463 







B distortions, extcrnal fields 387 BSmBSmA transtions, fluctuations
283
494
Index
bouyancy method, density measurements 232 BPI,,isotropictransitions, fluctuations 284 Bragg law, external fields 384 Bridgman flexible bellows 269 bubble domains, ultrasonic fields 455 bulk fluids, molecular modelling 77 bulk second harmonic generation, optical properties 475 bulk systems, largescale simulation 83 Burgers vectors 323,345 calamitics definitions 19  density measurements 236.240  flowiviscosity 352  magnetic properties 107 calorimeter 2 13, 2 16 calorimetric data, phase transitions 208, 22 1 f Canada balsam 335 capacitance method, elastic constants 168 capillary flow alignment 357 carbon tetrachloride, vortex formation 41 8 CarnahanStarling equation, nematics 55, 64 CarrHelferichOrsay approach 414 f, 419 Cartesian representation, tensor properties 96 caustics, textures 328 5CB (4npentyl4'cyanobiphenyl) 8 I , 85, 89  optical properties 12 I phase shifts 470 CBs (cyanobiphenyls) enthalpy curves 22 1 external fields 378 photoacousticiphotopyroelectric data 229 f reentrants 294 surface alignment 438  texturesidefects 342 f CCH5 (4(truns4npentylcyclobexyl)cyclohexylcarbonitrile) 81 f central core, definitions I9 CHARMM force field 77 ChenLubensky model 189 chevrons external fields 404 instabilities 414, 419  textures 337 chiral ferroelectrics 406 chiral liquid crystals 442 chiral lyotropicsidiscotics 412 chiral nematics, Frederiks transitions 170 chiral smectics 2 1 chirality 192 f, 223 cholesteric flexoelectric domains 402 cholesteric helix 399 cholesteric textures 336, 340 cholestericsmectic A transitions 281 cholesterics 223  blue phases 383 electrohydrodynamic behavior 424 f flowiviscosity 364 f 






ultrasonic field 455 Volterra process 3 16 cholesteryl nonanoate (CN) 223 circular dichroism 127 ClarkLagerwall effect 407 classification, liquid crystals 1723 ClausiusClapeyron equation calamitic compounds 240 external fields 379, 385 highpressure experiments 255 clearing parameters, definitions 23 clearing temperatures diffusion 488 phase transitions 258 clearing threshold, ultrasonic properties 450 ColeCole plots 131 ColeDavidson equation 132 columnar phases 98, 15 I competing fluctuations, reentrants 300 computer simulations  elastic properties 176  molecular theories 40 concurrence, singular points 347 condis crystals, definitions 23 conductivity CamHelferich mode 422 phase transitions 214 tensor properties 90 conformation  molecular modelling 79  optical properties 473 conical interfaces, surface alignment 434 conjugation, singular points 347 constitutive hydrodynamic equations 352 f continous defects, cholesterics 321 continuum theory 2539, 15 1 cooling runs, scanning calorimetry 2 13 core disjunctions 325 correlation lengths  fluctuations 277 phase transitions 182 Cotter approach 55 Coulomb gauge 187 Coulomb interaction, diffusion 483 Coulomb potentials, molecular modelling 73 coupling constants, external fields 377 critical point 187, 209 critical point fluctuations 284 crossover behavior 2 11,225 crystal phases, definitions 18 cubic crystals 23 Curie law 104 CurieWeiss law 106, 141 curvature elasticity, 3dimensional I6 1 f cyano compounds, reentrants 289 cyano mesogens, molecular modelling 78 cyanobiphenyls see: CBs cybotactic groups phase transitions 240  fluctuations 278 









Index dangling chains, anchoring 439 de Gennes theory fluctuations 279 IN transitions 221 phase transitions 184 f de Vries equation 125 Debye equations  dielectric properties 13 1 f  rotational diffusion 145 DebyePellat equation 132 defect crystals 348 defects 30435 1 elastic properties 157 ff  ultrasonic properties 456 deformations  Dupin cyclides 331  elastic properties 151, 162  external fields 389  smectics 442  strong 311 deformed helix ferroelectric effect 401, 408 density, phase transitions 232 f density functional approach 58 density wave vector 32 diamagnetic compounds 102 diamagnetic liquid crystals 106 diamagnetic susceptibility 28 diamgnetism 104 dielectric anisotropy, ultrasonic properties 460 dielectric losses, DTA measurements 258 dielectric permittivity, nematics 28 dielectric properties 129150, 273 dielectric regime, CamHelfrich mode 422 differential scanning calorimetry (DSC) 2 12, 254, 258 differential thermal analysis (DTA) 254 diasion 480491 diffusion constants 84, 489 diffusivity, phase transitions 220 dilatometers 232 dimers  mesogens 81  reentrants 294 surface alignment 438 dipole moments dielectric properties 129 f molecular modelling 44, 80 tensor properties 87 dipoledipole interactions phase transitions 239  surface alignment 438 direct current Kerr effect 469 directions, easy 3 12 director defects 304 director deformations 442 director distribution 375 elastic properties 157 f director fields, surface alignment 433 director gradients, nematics 3 1 director helix, chiral nematics 155 

director orientation, flowiviscosity 353, 369 director reorientation, optical properties 469, 472 directorfield interactions, distortions 386 directors  largescale simulation 82  molecular theories 43  nematics 26 torsional elasticity 156 Dirichlet problem, defects 345 disclination pairs, core disjunction 325 disclination pointsilines 342 disclinations  defects 312, 327  elastic properties 158 f  ultrasonic properties 456  Volterra process 3 17 discontinous defects, cholesterics 32 1 discotic ferroelectrics 4 12 discotics  density measurements 24 1  external fields 403 f, 412  flowiviscosity 352, 362  highpressure experiments 261  reentrants 298 dislocationloop melting theory 188, 281 dislocations  phase transitions 191  Volterra process 3 17 dispersion, molecular theories 44 dissipation, nematics 36 distortions directorfield interactions 386 elastic properties 160 ultrasonic properties 448, 455 DOBAMBC 406 domain mode, smectics 410 DPPC, diffusion 489 Dupin cyclides 328 dynamic scattering mode (DSM) 454 dynamics  molecular modelling 74 f  nematics 35 f 







easy directions, defects 3 12 EBBA anchoring 442 atomistic simulations 83 density measurements 240 metabolemeter 248  pVTdata 270 EDA complex formation 239 edge dislocations, Volterra process 3 17 effusivity 220 Einstein diffusivityviscosity law 483 Einstein relation 84 Einstein summation convention 90 elastic constants  external fields 408 Frederiks transitions 168 


495
496
Index
elastic constants nematics 26 twistisplayibend 172 elastic properties 15 1180, 27.3 elastic torques flowiviscosity 358  optical properties 470 elastomers  definitions 20  fluctuations 279 electric field induced deformations 163 electric field SHG (EFSHG) 475 electric fields 3 7 5 4 3 2  ultrasonic properties 460 electric permittivity 1 13 f electroclinic effect  smectics 409  surface alignment 443 electroclinic response, cholesteric helix 402 electrohydrodynamic instabilities 4 13 f electrokinetic coefficients 41 8 electrolytic mode, instabilities 4 17 electromagnetic radiation, optical properties 467 f electronic response, optical properties 474 electronic structures 102 electrooptical properties 273, 375 electrostatic interaction 44 elementary pinch, defects 346 enantiomer mixtures, blue phase transitions 223 energy profiles, molecular modelling 74, 79 enthalpy, phase transitions 208,232 enthalpy curve, hexylcyanobiphenyl 22 1 equilibrum equations  nematics 26 f  smectics 32 f EricksenLeslie viscous coefficients 281 Euler angles flowiviscosity 367 tensor properties 88 Euler equations, instabilities 414 EulerLagrange equations  elastic properties 171  nematics 30  smectics 35 eutectic mixture, Tait parameters 27 I eutetic point formation, metabolemeter 25 I expansivity, thermal 233 experimental techniques diffusion 483 f  phase transitions 208 ff extinction coefficients 119 



FabryPerot resonator 477 fan textures 334 Faraday balance 11 1 ferrielectric phases (FIP), external fields 41 1 ferroelectric compounds, phase transitions 259 ferroelectric liquid crystals (FLC) 406 ferroelectric smectics, chiral 406
ferroelectric TGB, external fields 385 ferroelectric transitions 273, 378 ferromagnetism 102, 106, 110 Fick diffusion law 480 field untwisting, cholesteric helix 399 fingerprint textures 326  ultrasonic fields 457 first order transitions 209, 377 f flexoelectric effects  cholesteric helix 401 f  external fields 391 f flexoelectric structure 156 flow 352374 flow alignment  nematics 356, 368  SmCphase 371 flow distribution, ultrasonic properties 447 fluctuations  elastic properties 157 ff  phase transitions 182,208,277 fluid layers 332 fluidfluid phase transition 252 fluidity, reentrants 289 focal conics 328, 333 focal curves, defects 344 focal domains, textures 334 foggy phases  cholesteric helix 401  external fields 383 force field, molecular modelling 72 Fourier series, surface alignment 434 fractional volume changes, phase transitions 233 Frank elastic constants  cholesteric helix 401  molecular theories 60 Frank energy, field interactions 387, 393 FrankOseen approach, optical properties 125 FrankOseen energy  anchoring 441  nematics 26, 36  phase transitions 185 Franklin relations 482 Frederiks transitions  elastic properties 164 ff  external fields 386, 395  smectics 403 f  ultrasonic properties 460 freeze etching technique, textures 3 11 frequency  electric permitivities 143  ultrasonic properties 448 frustrated smectics 196 frustration reentrants R l 290 gauche conformation, molecular modelling 79 Gaussian model, phase transitions 182,203 GayBeme interaction  diffusion 483  phase transitions 241
Index GelbhartBarboy expansion, nematics 55 GelbhartBenSbaul theory 172 de Gennes theory  fluctuations 279  IN transitions 221  phase transitions 184 f giant optical nonlinearity (GON) 470 Gibbs free energy  elastic properties 172  molecular theories 48 phase transitions 210 Ginzburg criterion 2 11 Ginzburg temperature 182 GinzburgLandau parameter 28 1 Goldstone modes, dielectric properties 142 Gouy balance 111 grain boundaries 337 Grandjean textures  cholesteric helix 403  electrohydrodynamic behavior 424 external fields 396 GrandjeanCano wedge 325 groups, definitions 19 gyromagnetic ratio, diffusion 485 

HalperinNelsonYoung concept, bond ordering 191 Hamiltonian molecular theories 5 I  phase transitions 182 f hard core repulsion, Maier function 56 hard particles theory, elastic properties 175 hard rod fluid, phase diagram 63 harmonic potentials, bond stretches 73 HBA, atomistic simulations 83 HBPD, thermobarogram 250 heat capacity 208 heating modes, scanning calorimetry 2 13 Helfrich model, ultrasonic properties 460 HelfrichHurault mechanism, elastic properties 171 helical axis, cholesterics 364 helicity 18 helicoidal structures, optical properties 124 helium saturation 257 Helmholtz energy 172 heptyl, Tait parameters 271 heringbone structure 283 hexagonal smectic phases 405 hexatic properties, fluctuations 283 high pressure experiments 253 f historical developments 11 6 homeotropic nematics 393 homogeneous distortions, ultrasonic properties 448 homologues, nematic 487 Hooke law 152 Hiickel model, freeelectron 469 hybrid aligned cells, elastic properties 170 hydrogen bond formation 240 hyperpolarizability 468 
497
incompressibility nematics 27 smectics 34 indicatrix, optical 114 f inertia tensor, atomistic simulations 83 inertial mode, instabilities 423 inhomogeneous distortions, ultrasonic properties 453 injection modes 416 instabilities electrohydrodynamic 375, 413 f planar cholesteric textures 397 interaction types  diffusion 483  molecular theories 44 interdigitated smectic phases, reentrants 293 interface defects 3 13 interface deformation, elastic properties 162 interfaces  nematic 30, 441  surface alignment 433 intermolecular interactions 40, 65, 15 1 phase transitions 210 intermolecular potentials, molecular modelling 8 1 interpenetrable layers, anchoring 439 isotropic fluids, dielectric properties 129 f isotropic instabilities 41 7 isotropic interfaces, nematic 441 isotropic modes, electrohydrodynamic behavior 425 isotropicnematic transitions 179 f, 221 f IUPAC, liquid crystal nomenclature 17 



jogs, defects 327 Joule heating, tensor properties
90
KapustinWilliam domains (KPD) 414 f, 419 Kawasaki mode coupling, fluctuations 28 1 Kernpunkt, Lehmann convention 3 14 Kerr cell, cholesteric helix 401 Kerr effect direct current 469  external fields 382 f kinks 327 Kirkwood correlation factor 130 KirkwoodFrohlich equation I30 Kobayashi model 61 Konvergenzpunkt, Lehmann convention 3 14 KosterlitzThoules mechanism 191 Kozhevnikov theory 449 f KramersKrohnig relation 12 1, 143 KrautKennedy equation 259 Kronecker delta 92 
Landau theory 210,227,376 Landaude Gennes theory 179 ff anchoring 440 IN transitions 221  optical properties 472

498
Index
LandauGinzburg coefficients 182 LandauGinzburg Hamiltonian, critical 203 LandauKhalatnikov mechanism 462 LandauLifshitz theory, phase transitions 266 LandauPeierls instabilities 185 LangmuirBlodgett film, atomistic simulations 85 Laplace equation 343 largescale simulation, molecular modelling 82 lattice models, elastic properties 175 layers 305 f, 332 leaks, scanning calorimetry 2 13 leapfrog algorithm, molecular modelling 75 Legendre functions flowiviscosity 363  molecular theories 4 1  tensor properties 93 Lehmann convention, defects 3 14 LennardJones interaction, diffusion 483 Leslie viscosities  diffusion 482  external fields 388  flows 353,363 LeslieErickson theory  flow/viscosity 352 f  ultrasonic properties 447 f lettering scheme, nomenclature 17 LeviCivita tensor  flowiviscosity 354  molecular theories 43 Lifshitz point 228, 399 light band centers, ultrasonic properties 449 light scattering, instabilities 423 linear dichroism 98 linking groups 19 Liouville theorem, reentrants 297 liquidgas type transitions 2 10 liquidnematic transition, isotropic 377 London penetration depth 185 f LorenzLorentz equation low frequency permittivity 133 Lubensky model, fluctuations 282 lyotropic systems, external fields 391 lyotropics 11  chiral 412  density measurements 24 1  diffusion 489 elastic properties 162 nomenclature 18  surface alignment 444 textures 307 


macroscopic structures 375 macroscopic surface alignment 434 f macroscopic tensor properties 92 magnetic field induced deformations 163 magnetic fields 3 7 5 4 3 2 magnetic properties 28, 88, 102113 magnetic resonance 484 magnetometers 1 11
Maier function, hardcore repulsion 56 MaierMeier equations, dielectric properties 134 f MaierSaupe theory 44 f, 179 f, 232  optical properties 472 main chain liquid crystalline polymers (MCLCP) 20 Maltese cross 308 Mauguin behavior, defects 326 Maxwell equations  instabilities 415  optical properties 1 13,467 f MBBA (4'methoxybenzylidene4butylaniline) anchoring 442 bulkSHG 475 clearing thresholds 450 conformational effects 473 defects 304 diffusion 486 metabolemeter 248 polygonal textures 309 Tait parameters 270  volumechanges 235  vortex formation 4 18 MBBAiCanada balsam, textures 336 2MBCB ((+)4(2methylbutyI)4'cyanobiphenyl) 83 McMillan theory 61,279 f  fluctuations 279 meanfield theory 47 f  elastic properties 175  fluctuations 277  NSmA transition 60  NSmASmC 193 phase transitions 199, 210 measuring cell, photoacoustic 2 18 mechanics, molecular modelling 72 f Meissner effect I85 f  fluctuations 280 f melting point equation 259 mesogens, definitions 19,78 f mesophases  defects 341  density measurements 232 diffusion 486 lamellar 335 MET(MNT) mixture, thermobarogram 252 metabolemeter 248 f metal containing liquid crystals 74 methylene 237 Metropolis algorithm, molecular modelling 76 microscopic anchoring mechanism 439 microscopic preparations, defects 304 microscopic structures 375 microscopic surface order, nematics 438 f microscopic tensor properties 92 microtomy methods, textures 31 1 Miesowitz notation, flowhiscosity 354 miscibility 17 mixtures  molecular theories 41 reentrants 289, 292 Mobius strips, defects 324 










499
Index model potentials, molecular theories 46 modelling defects, nematics 32 modelling software 72 modulated structures, meanfield model 201 molecular interactions, phase transitions 239 molecular modelling 7286 molecular properties 80 molecular shapes, reentrants 298 molecular structures 78 molecular theories 407 1 elastic properties 172 f refractive indices 115 f monitoring boundary effects 463 monocrystals, textures 308 Monte Carlo simulation, molecular modelling i'4 f MOPAC, molecular modelling 80 mosaic textures 338 MPP theory, flowiviscosity 352 multicritical point  phase transitions 228, 267  reentrants 291 myelin textures 307 

NA transitions, external fields 379 NI transitions 47, 59,22 1 density changes 233  external fields 377  fluctuations 278 optical fields 472 NSm transitions, fluctuations 279 NSmA transitions 183 f, 224 NSmASmC point multicritical 228 phase transitions 189 NrcSmCSmA multicritical point 267 NAC multicritical point, fluctuations 285 NavierStokes theory  flowiviscosity 352  instabilities 415, 421 Nee1 walls 313 neighbor lists, molecular modelling 77 nematic biaxiality, induced 38 I nematic mesophase, diffusion 486 nematic phases 17 ff, 47  dielectric properties 133  order parameters 41 nematics  directorfield interactions 386  flowiviscosity 352 instabilities 413 surface alignment 433 Volterra process 3 16 Neumann principle 99 Newton equations, molecular modelling 74 nitrogen saturation 257 nomenclature 1723 nonadiabatic scanning calorimetry 2 17 nonergodic systems, reentrants 297 nonlinear optical properties 4 6 7 4 7 9 




normalmetalsuperconducting transitions NoseeHoover thermostat 75 nuclear magnetic resonance (NMR) 111  diffusion 484  phase transition 262  tensor properties 98 nucleation, defects 346 nuclei textures 3 15
280
OBBA, volumeidensity changes 237 nOCB (4alkoxy4'cyanobiphenyl) 83 octylcyanobiphenyl 248 oily streaks, textures 308 Onsager theory 44 f  flowiviscosity 353, 369  nematics 37  phase transitions 179 f OPLS parameters, molecular modelling 77 optical absorption coefficient, phase transitions 2 19 optical activity, highpressure experiments 263 optical contrast, defects 326 optical harmonic generation 475 optical methods, highpressure experiments 255, 260 optical path, smectic structures 124 optical power limiting (OPL) 477 optical properties 1 131 28  nonlinear 467479 optical second harmonic generation 438 optical transmission nematics 459  ultrasonic properties 448 order parameterdirector coupling 440 order parameters 4 1  defects 304  external fields 380  largescale simulation 82  phase transitions I80 f, 239  tensor properties 92  viscosity coefficients 362 order types, phase transitions 236 ordoelectric polarization, external fields 392 organic liquid crystals 74 orientational anisotropy, elastic properties 15 I orientational correlations, shortrange 5 I orientational order, opticalfieldinduced 472 orientations nematics 448  surface alignment 433, 442 OrnsteinZernike equation 58 Orsay energy, smectics 32 orthogonal phases, definitions 22 Oseen theory, diffbsion 482 

PAA (pazoxyanisole) density measurements 240  diffusion 486 packing, thermotropic nematics 54 paramagnetic liquid crystals I08 
500
Index
paramagnetism 102 PariserPamPople model 469 Parodi equation, flowiviscosity 353, 363 Parsons approximation 60 ParsonsLee approximation 54 pattern formation, optical 472 PCH3 (4(truns4npropylcyclohexyl)benzonitrile))  energy minima 80 molecular modelling 78 PCH5, atomistic simulations 83 Peierls argument 280 penetration depth, phase transitions 185 pentyl, Tait parameters 271 PercusYevick approximation 55 periodic distortions, ultrasonic properties 452 periodic structures, external fields 390 permittivity, dielectric 129 f, 404 pertubation theory tensor properties 89 timedependent 468 phase diagrams hardrod fluid 63 NSmA transition 224 NSmASmC multicritical point 228 reentrants 289 phase sequences, reentrants 290 f phase structures 121 phase symmetry 115 f phase transitions 20, 181276 highpressure experiments 256 optical properties 122 temperature shifts 376 ultrasonic properties 46 1 underpressure 266 phases 17 ff optical properties 1 16 pHB, atomistic simulations 83 phlogopite mica, interfaces 434 phospholipids, textures 307 photoacoustic methods, phase transitions 2 18 photoacoustic spectroscopy 463 photopyroelectric method 220 physical properties orientationdependent 87 f underpressure 273 piezocoefficient, external fields 377 piezoelectric tensor 89 piston displacement, phase transitions 270 plages a noyaux, textures 3 15 planar textures 332 . external fields 397  walls 338 plastic crystals, definitions 23 platelet textures 338 plugflow 365 Pockels modulator, optical properties 477 Poiselle flow 365 polar achiral polyphilics, external fields 406 polar interactions, phase transitions 240 polar smectics, phase transitions 32, 196 








polarity, nematics 26 polarizability anisotropic 51  dielectric properties 129 f  mesogens 1 I8 polarization 468 magnetic 104  optical properties 114 f ordoelectric 392 photopyroelectric method 220 tensor properties 88 polarizing microscopy 308 polygonal textures 333 polymer dispersed liquid crystal (PDLC) 12 polymer liquid crystals 20 external fields 386  ferroelectric 410 surface alignment 444 polymers density measurements 24 1 external fields 383 polyphilics, external fields 406 PoniwierskiSluckin theory 68 potentials, molecular modelling 73 Potts model 284 pressure, flow/viscosity 360 pressure transducer, metabolemeter 249 pressuretemperature phase diagram, calamitics 240 pressurevolumetemperature behavior 269 pretransition behavior, density measurements 239 propyl, Tait parameters 271 Prost model, phase transitions 197 pseudowalls, textures 337 pycnometers, density measurements 232 pyroelectric transducer, phase transitions 220 






quantum mechanical techniques, molecular modelling 78 quasielastic neutron scattering (QENS) 484


R1 reentrants 291 f R3 reentrants 300 radiation fluxes, ultrasonic properties 449 rank, tensor properties 87 f reentrant behavior high pressure experiments 263  mctabolemetcr 249 reentrant phase transitions 204,289303 reentrants, definitions 23 red shifts, external fields 384 reflectivity, optical properties 122 refraction, phase transitions 273 refractive indices fluctuations 160  mesogens 118  optical properties I13128,474 

Index relaxation dielectric properties 143 f  ultrasonic properties 461 relaxation times  ac calorimetry 215  dipole reorientation 130  external fields 383 RennLubensky model, fluctuations 282 renormalization group 188, 2 1 1 reorientation directors 163  opticalfieldinduced 470 resistivity, tensor properties 90 Reynolds number, instabilities 415 rotational viscosity 354, 368 

Sdistortions 387 salicylaldimine complexes 108 Saupe ordering matrix 95 SaupeNehring theory 175 scaling, phase transitions 187 f scanning calorimetry 213 Schiff base mixtures, reentrants 292 Schiller theory 352 schlieren textures 3 15 nematic 344 screw dislocations 3 17 second harmonic generation (SHG) 475 second order transitions 209 external fields 376 segregation, elastic properties 162 selective reflection, phase transitions 261 selfdiffraction, optical properties 47 1 SHAKE procedure, molecular modelling 75 shear gradients, flowiviscosity 364 shear stress 151 shear viscosity flowphenomenon 353  nematics 367 shifts, phase transitions 376 shortrange dipoledipole interactions 138 side group liquid crystalline polymers (SGLCP) 20 silicone oil, vortex formation 418 Simon equation 257 SimonGlatzel equation 258 singular pointsilinesiwalls 3 11 f SmA phases  flow/viscosity 372  interdigitated 293 SmAAmA critical point, isolated 202 SmAC* transitions, ferroelectric 379 SmAhexatic smectic B transition 19 1 f SmASmC transition 65, 189 f, 226, 375 SmATGB,cholesteric, multicritical behavior 268 SmA,SmA point, critical 202 SmA,/SmA, transitions, fluctuations 284 SmC*SmATGB,, multicritical behavior 268 SmC/C* phases, flowiviscosity 368 smectic mesophase, diffusion 488 


50 1
smectic phases 17,43, 60 dielectric properties 137 electrohydrodynamic behavior 425 order parameters 41 ultrasonic field 457 smectics 21  electrohydrodynamic behavior 424 external fields 403 f  Frederiks transitions 171  surface alignment 442  torsional elasticity 156 Volterra process 3 16 smooth surfaces, anchoring 439 soft crystals 20 solid state, description 20 solutes, diffusion 488 specific volume 232 spherical harmonics, tensor properties 95 spinglas, reentrants 297 spinspin interactions 106 spirals origin, textures 340 splay deformation directors 442 elastic properties 165 torsional elasticity 154 splay Frederiks distortion 396 splaybendtwist deformations, external fields 389 SQUID magnetometer 111 stability, mechanical 151 stability exchange 41 7 states, definitions 18 statistical mechanics 40 statistical molecular theory 58 steadystate patterns, external fields 390 stepped drops, textures 328 stereochemistry 23 steric energy, molecular modelling 72 stochastic dynamics, molecular modelling 75 storage model, ultrasonic fields 455 strain 151 f strain tensor 37 stress 151 f stress matrix 35 stress tensor 353 strong anchoring, elastic properties 158 structural properties, TGB phases 194 structural transformations, ultrasonic properties 447 f structures 78 magnetic/electric field influences 375 periodic 390  supertwist 395  ultrasonic properties 462 superconductor analogy, phase transitions 184 f superconductors fluctuations 277 reentrants 291 superfluid helium analogy, phase transitions 189 superposition, defects 347 supertwist structures 395 surface acoustic waves (SAW) 448 








502
Index
surface alignment 4 3 3 4 4 6 surface conditions, continuum theory 25 surface extrapolation length, distortions 387 surface orientational order, nematics 438 surface second harmonic generation 476 surface stabilized ferroelectric liquid crystals (SSFLC) 407,443 surface stabilized ferroelectrics, flowiviscosity surfaces, textures 307, 328 susceptibility diamagnetic 107 dielectric 134 elastic 163 external fields 377 magnetic 102 molecular 42, 107  nonlinear 468 phase transitions 180 . tensor properties 88 symmetry, reentrants 289 symmetry changes, external fields 381


37 1




Tdistortions, external fields 387 Tait equation, phase transitions 270 TBBA (terephthalbisbutylaniline) 488 TBDA, volumeidensity changes 238 temperature dependence density 233  phase transitions 209  refractive indices 122 temperature effect, viscosity coefficients 362 temperature independent paramagnetism (TIP) 105 tensor properties 42, 87101 torsional elasticity 152 f terminal groups, definitions 19 texture transformations 342 f ultrasonic fields 455 texture transitions, smectics 404 textures 30435 1 electrohydrodynamic behavior 424 Grandjean 396 thermal characteristics, phase transitions 208 thermal effects, optical properties 473 thermal expansion coefficients 232 thermal methods, phase transitions 208 f thermistors 2 15 thermobarograms, phase transitions 248 f thermobarometric analysis (TBA) 249 thermotropic mesogens, magnetic properties 107 thermotropic nematics, packing effects 54 thermotropic properties, notation 18 ff thermotropic systems, external fields 391 thermotropic textures 305 f THE5, atomistic simulations 83 third harmonic generation (THG) 475 threads, thinithick 3 I6 tiltpolarization coupling 377 tilted chiral phases 21 




tiltedorthogonal smectic transitions 282 topographies, anchoring 439 torque elastic properties 157  flowiviscosity 355 generation under flow 366 torsional elasticity 151 f torsional energy barriers, molecular modelling 75 tracer technique, diffusion 483 transconformation, molecular modelling 79 transient patterns, external fields 39 I transition temperatures 20 transitions external fields 376  fluctuations 278 translation dislocations 345 transmission, optical properties 123 transmission techniques, highpressure experiments 258 transport properties, phase transitions 208 transverse pressure, flowiviscosity 360 tricritical behavior, phase transitions 266 tricritical point anchoring diagram 436 external fields 380  fluctuations 277 phase transitions 228 tumbling, flowiviscosity 357 tungsten tip surface scanning by screw spindle 269 turbidity measurements, phase transitions 259 twist bend distortions, elastic properties 160 twist deformation  elastic properties 165 torsional elasticity 154 twist dischation, defects 327 twist grain boundary (TGB) 22 external fields 383 fluctuations 282 highpressure experiments 260 phase transitions 186, 194 twist transitions, opticalfieldinduced 471 twisted nematicsicholesterics, external fields 395 twisted phases 383 twodimensional approach, instabilities 42 I 




ultrasonic properties 4 4 7 4 6 6 ultrasound absorption 462 intensity 448 phase transitions 273 studies 461 uniaxial nematic transitions 180 uniaxial nematics, flowiviscosity 352 uniaxial structures, meanfield model 199 uniaxialbiaxial nematic transitions 279 united atom model 77, 82 untwisting dynamics, cholesteric helix 400

Index van der MeerVertogen model 68 van der Waals interaction  elastic properties 172 f  molecular theories 44  nematics 55 vapor interfaces, nematic 441 variable grating mode, external fields 394 virtual work, nematics 27 viscosities 151 ff, 352374  diffusion 482  external fields 388  temperature effect 362 transitions under pressure 273 viscous coefficients  fluctuations 281 nematics 36 VogelFulcher model 147 voltagetemperature phase diagram 386 Volterra process 3 16 volume changes, phase transitions 233 volume effects, Onsager theory 52 vortex formation, instabilities 416 f vortex patterns, twodimensional 42 1 de Vries equation 125 Vuzhva theory 459
walls, textures 337 wave interactions, nematics 457 f weak anchoring elastic properties 158 flowiviscosity 365 wedge disclination 327 Wigner rotation matrices 94 Wulf model, smectic AC transition

67
Xray measurements, highpressure experiments 262


503
.v expansion elastic properties 173 hardcore energy 55 YpmaVertogen approach 55 
Zscan method, optical properties 474
This Page Intentionally Left Blank